This new edition of the well-received introduction to solid-state physics provides a comprehensive overview of the basic

*1,020*
*192*
*12MB*

*English*
*Pages 536
[543]*
*Year 2009*

Solid-State Physics

Advanced Texts in Physics This program of advanced texts covers a broad spectrum of topics which are of current and emerging interest in physics. Each book provides a comprehensive and yet accessible introduction to a field at the forefront of modern research. As such, these texts are intended for senior undergraduate and graduate students at the MS and PhD level; however, research scientists seeking an introduction to particular areas of physics will also benefit from the titles in this collection.

Springer Berlin Heidelberg New York Hong Kong London Milan Paris Tokyo

Harald Ibach

l

Hans Lu¨th

Solid-State Physics An Introduction to Principles of Materials Science

Fourth Extensively Updated and Enlarged Edition With 286 Figures, 18 Panels and 104 Problems

13

Professor Dr. Harald Ibach Professor Dr. Dr. h.c. Hans Lu¨th Institut fu¨r Bio- und Nanosysteme Forschungszentrum Ju¨lich GmbH, 52425 Ju¨lich and Rheinisch-Westfa¨lische Technische Hochschule 52062 Aachen, Germany e-mail: [email protected] e-mail: [email protected]

Title of the German original edition: H. Ibach, H. Lu¨th: Festkorperphysik. Einfu¨hrung in die Grundlagen (Siebente Auflage) ¨ # Springer-Verlag Berlin Heidelberg 1981, 1988, 1990, 1995, 1999, 2002, 2009

ISBN 978-3-540-93803-3 e-ISBN 978-3-540-93804-0 DOI 10.1007/978-3-540-93804-0 Springer Dordrecht Heidelberg London New York Library of Congress Control Number: 2009926968 # Springer-Verlag Berlin Heidelberg 1993, 1995, 2003, 2009 This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable to prosecution under the German Copyright Law. The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Cover design: eStudio Calamar S.L. Printed on acid-free paper Springer is part of Springer Science+Business Media (www.springer.com)

Preface to the Fourth Edition

The Nobel Prize awarded to Albert Fert and our colleague Peter GruÈnberg has drawn the attention to the remarkable progress that has been achieved in the field of magnetism concerning both its understanding and its applications. Adding a section on the giant magneto resistance (GMR) eect was therefore necessary. As the GMR-eect is observed in magnetic thin-film systems, it was natural to combine the treatise on the GMR- eect with a brief summary of the specific magnetic properties of thin films; and we did so with a new panel. The wealth of phenomena encountered in thin-film magnetism is intimately related to the interplay of various sources of magnetic anisotropy. We therefore had to pay attention to the most common source of magnetic anisotropy, the crystalline anisotropy and to the phenomena that go along with it, such as magnetic hysteresis and domain walls. The GMR-eect is only one of the many new eects that one encounters when the dimensions of solids shrink into the nanometer range. For example, the semi-classical approach to electron transport fails in small dimensions, and normal electric current flow is replaced by ballistic or diusive transport giving rise to quantum eects such as Aharonov-Bohm oscillations, Altshuler-Aronov-Spivak-oscillations, weak localization, and universal conductance fluctuations. A new section on quantum transport is devoted to these phenomena. One of the intellectually most appealing fields in the realm of dielectric properties of matter is that of materials with negative index of refraction. While no natural material with that property exists, composite materials involving lattices of electric and magnetic resonance circuits, so called metamaterials, have been made and exhibit most unusual optical properties. With further progress in the preparation of artificial structures of nanometer dimensions application of metamaterials for optics in the visual range is at hand. We have devoted a new panel to this exciting field. Here, as well as in nearly all other fields of current interest, progress largely depends on the progress in the preparation of nanostructures. We have included a new panel on various preparation techniques. We have also updated the panels on photoemission and neutron diraction. We gratefully acknowledge the many comments and suggestions by colleagues and students that have helped to improve this volume. JuÈlich and Aachen, February 2009

H. Ibach . H. LuÈth

Preface to the Third Edition

Our German textbook ``FestkoÈrperphysik'' has meanwhile appeared in its 6th edition, extensively revised and extended in comparison to the latest 2nd English edition. Presently, the book has been translated into Japanese, Korean and Polish and is used as a standard text in many universities around the world. It is therefore high time to carefully revise the English text and bring it up to par with the latest 6th German edition. The sections on ``High Temperature Superconductors'' as well as Panel XVI on ``Shubnikov-de Haas Oscillations and Quantum Hall Eect'' are completely revised according to the present deeper understanding of the phenomena. This 3rd English edition has furthermore been expanded by several chapters to meet the educational requirements for recent fields of research. We let ourselves be guided by the idea that modern teaching of solid state physics emphasizes aspects of material science and its applications, in particular in solid state electronics. Accordingly, deviations from the ideal periodic solid have gained more weight in the text: we now consider phase diagrams of alloys, some basics of defect physics and amorphous solids. Because of the importance of strained layer systems in device physics, inclusion of the fundamentals of crystal elasticity theory seems (again) necessary, so a new chapter is devoted to this topic. The additional chapter on the excitation spectrum of a superconductor is intended to further the understanding of modern research on superconductor/normal conductor interfaces as well as on applications in superconductor electronics. For similar reasons, sections on the metal/semiconductor Schottky-contact and on the basic concepts of important semiconductor devices have been included in the new edition. With all of these additions we have tried to maintain the spirit of the book, namely to put the phenomena into a general frame of an atomistically founded understanding of solid state physics. We thank Dr. Klaus Dahmen, Dr. Arno FoÈrster, Dr. Margret Giesen, Dr. Michel Marso, Prof. Dr. Angela Rizzi and Dr. Thomas SchaÈpers for discussions on special topics and many suggestions for improving the presentation. We express our thanks to Dr. H. J. Koelsch, Dr. T. Schneider and Mr. C.-D. Bachem of Springer-Verlag for the pleasant collaboration. JuÈlich and Aachen, January 2003

H. Ibach . H. LuÈth

Preface to the Second Edition

Our German textbook ``FestkoÈrperphysik'' has become rather popular among German-speaking students, and is currently produced in its 4th edition. Its English version has already been adopted by many universities in the United States and other countries. This new 2nd edition corresponds to the 4th edition in German. In addition to correcting some typographical errors and making small improvements in the presentation, in the present edition some chapters have been revised or extended. Panel V, for example, has been extended to include a description of angle-resolved photoemission and its importance for the study of electronic band structures. Section 10.10 on high-temperature superconductors has been completely rewritten. This active field of research continues to progress rapidly and many new results have emerged since the publication of the first edition. These results shed new light on much of the fundamental physics. The new version of Sect. 10.10 has been developed in discussions with colleagues who are themselves engaged in superconductivity research. We thank, in particular, Professor C. Calandra from the University of Modena and Dr. R. WoÈrdenweber of the Institute of Thin Film and Ion Technology at the Research Centre JuÈlich. The revision of the problems was done with the help of Dr. W. Daum, Dr. A. FoÈrster, A. Leuther and Ch. Ohler. We would like to thank them for their eorts. We also thank Dr. Margret Giesen for numerous improvements to the manuscript as well as Dr. Angela Lahee for the competent translation of the revised or new sections. JuÈlich and Aachen, April 1995

H. Ibach . H. LuÈth

Preface to the First Edition

In recent decades solid state physics has seen many dramatic new developments and has become one of the largest independent branches of physics. It has simultaneously expanded into many new areas, playing a vital role in fields that were once the domain of the engineering and chemical sciences. A consequence of this explosive development is that no single university lecturer can today be expected to have a detailed knowledge of all aspects of this vast subject; likewise, it is impossible to conceive of a course that could oer students a comprehensive understanding of the entire discipline and its many applications. In view of this situation, it is particularly valuable to have a textbook that gives a concise account of the essential elements of the physics of solids. In this book the fundamental aspects of solid state physics are presented according to the scheme: Chemical bonding, structure, lattice dynamics, and electronic properties. We believe that this sequence is the optimum choice for tutorial purposes. It enables the more dicult concepts to be introduced at a point where a basic understanding of fundamental ideas has already been achieved through the study of simple models and examples. In addition to this carefully structured exposition of classical solid state theory based on the periodic solid and the one-electron approximation, the book also includes comprehensive descriptions of the most active areas in modern research: magnetism, superconductivity and semiconductor physics. The chapter on magnetism discusses the exchange coupling of both localized and delocalized electrons, and will even guide the reader to the point when he or she can appreciate modern thin-film experiments. The standard picture of superconductivity is elucidated by means of a simplified presentation of BCS theory. A section is also devoted to the novel high-temperature superconductors. This field, however, remains in such a state of flux that it was necessary to confine the treatment to some selected experimental results and a few central ideas about this fascinating phenomenon. The chapter on semiconductors contains, in addition to a general introduction to these materials and their properties, detailed descriptions of semiconductor heterostructures, superlattices, epitaxy, and the quantum Hall eect. In solid state physics, the interaction between theory and experiment has always played, and continues to play, a vital role. We have thus attempted throughout this book to steer a middle course in which both theory and experiment are adequately represented. Where a theoretical approach is

Preface to the First Edition

ix

helpful and not too cumbersome, we have not hesitated in challenging the reader with the necessary abstract concepts. Furthermore, we have tried to include theoretical methods and concepts, for example, those of group theory, that are indispensible for an understanding of contemporary original publications dealing with solid state theory. The concise presentation of the essential theoretical aspects is complemented by the inclusion of selected experimental methods and examples, summarized in the form of self-contained panels. These oer the reader the opportunity to test and consolidate the material already studied and may prove helpful in stimulating further study in areas of particular interest. Students will also benefit significantly from working through the extensive series of problems that relate to each chapter. These examples are not restricted to calculations based on the methods described in the text; in many cases they lead into areas that lie outside the scope of the main presentation. All of the examples have been put to the test in our own lecture courses. Nonetheless, the student may often need a helping hand or some preparatory instruction from a lecturer. The problems will be useful to both students and lecturers; they are designed to stimulate further study and to illustrate the connections between dierent disciplines. This book is a translation of the third edition of the original German text. The authors consider it their immensely good fortune to have been supported by Dr. Angela Lahee in the translation and editing of this work. We are also grateful to numerous colleagues who over the years have oered valuable suggestions about the presentation of the book or have supplied the experimental material described herein. For her critical reading of parts of the manuscript and the page proofs we thank in particular Dr. Angela Rizzi. Other valuable contributions were made by Dr. W. Daum, Mr. Ch. Stuhlman, Dr. M. Wuttig and Mr. G. Bogdanyi. The figures were prepared with great care and patience by Mrs. U. Marx-Birmans and Mr. H. Mattke. The German manuscript was typed by Mrs. D. KruÈger, Mrs. JuÈrss-Nysten and Mrs. G. Oermann. We express our thanks to Dr. H. Lotsch and Mr. C.-D. Bachem of Springer-Verlag for the pleasant collaboration. JuÈlich, January 1991

H. Ibach . H. LuÈth

Contents

1 Chemical Bonding in Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 The Periodic Table of the Elements . . . . . . . . . . . . . . . . . . . . . . 1.2 Covalent Bonding . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3 Ionic Bonding . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4 Metallic Bonding . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5 The Hydrogen Bond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6 The van der Waals Bond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

1 1 4 9 13 15 15 16

2 Structure of Solid Matter . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 The Crystal Lattice . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Point Symmetry . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 The 32 Crystal Classes (Point Groups) . . . . . . . . . . . . . . . . . . . . 2.4 The Significance of Symmetry . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5 Simple Crystal Structures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6 Phase Diagrams of Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.7 Defects in Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

21 22 25 27 28 31 36 45 48

3 Diraction from Periodic Structures . . . . . . . . . . . . . . . . . . . . . . 3.1 General Theory of Diraction . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Periodic Structures and the Reciprocal Lattice . . . . . . . . . . . . . . 3.3 The Scattering Conditions for Periodic Structures . . . . . . . . . . . 3.4 The Bragg Interpretation of the Laue Condition . . . . . . . . . . . . 3.5 Brillouin Zones . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.6 The Structure Factor . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7 Methods of Structure Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Panel I: Diraction Experiments with Various Particles . . . . . . . . . . . . Panel II: X-Ray Interferometry and X-Ray Topography . . . . . . . . . . .

51 51 57 58 60 63 64 67 70 72 78

4 4.1 4.2 4.3

83 84 85 86

Dynamics of Atoms in Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . The Potential . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . The Equation of Motion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . The Diatomic Linear Chain . . . . . . . . . . . . . . . . . . . . . . . . . . . .

XII

Contents

4.4

Scattering from Time-Varying Structures ± Phonon Spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 91 4.5 Elastic Properties of Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . 94 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 104 Panel III: Raman Spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 107 5 Thermal Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1 The Density of States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2 The Thermal Energy of a Harmonic Oscillator . . . . . . . . . . . . . 5.3 The Specific Heat Capacity . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4 Eects Due to Anharmonicity . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5 Thermal Expansion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.6 Heat Conduction by Phonons . . . . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Panel IV: Experiments at Low Temperatures . . . . . . . . . . . . . . . . . . . .

113 113 116 118 120 121 124 129 131

6 6.1

135

``Free'' Electrons in Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . The Free-Electron Gas in an Infinite Square-Well Potential . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2 The Fermi Gas at T = 0 K . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3 Fermi Statistics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 The Specific Heat Capacity of Electrons in Metals . . . . . . . . . . . 6.5 Electrostatic Screening in a Fermi Gas ± The Mott Transition . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6 Thermionic Emission of Electrons from Metals . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

136 140 142 145 150 152 156

7 The Electronic Bandstructure of Solids . . . . . . . . . . . . . . . . . . . . 7.1 General Symmetry Properties . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2 The Nearly Free-Electron Approximation . . . . . . . . . . . . . . . . . 7.3 The Tight-Binding Approximation . . . . . . . . . . . . . . . . . . . . . . . 7.4 Examples of Bandstructures . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5 The Density of States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.6 Density of States in Non-Crystalline Solids . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Panel V: Photoemission Spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . .

159 159 163 167 173 177 179 182 184

8 8.1 8.2 8.3 8.4 8.5

191 191 196 199 201

8.6

Magnetism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Diamagnetism and Paramagnetism . . . . . . . . . . . . . . . . . . . . . . The Exchange Interaction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Exchange Interaction Between Free Electrons . . . . . . . . . . . . . . The Band Model of Ferromagnetism . . . . . . . . . . . . . . . . . . . . . The Temperature Behavior of a Ferromagnet in the Band Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Ferromagnetic Coupling for Localized Electrons . . . . . . . . . . . .

205 209

Contents

XIII

8.7 Antiferromagnetism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.8 Spin Waves . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.9 Crystalline Anisotropy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Panel VI: Magnetostatic Spin Waves . . . . . . . . . . . . . . . . . . . . . . . . . . Panel VII: Magnetism in Thin-Film Systems and GMR-Eect . . . . . . .

211 215 219 225 227 233

9 Motion of Electrons and Transport Phenomena . . . . . . . . . . . . . . 9.1 Motion of Electrons in Bands and the Eective Mass . . . . . . . . 9.2 Currents in Bands and Holes . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.3 Scattering of Electrons in Bands . . . . . . . . . . . . . . . . . . . . . . . . 9.4 The Boltzmann Equation and Relaxation Time . . . . . . . . . . . . . 9.5 The Electrical Conductivity of Metals . . . . . . . . . . . . . . . . . . . . 9.6 Thermoelectric Eects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7 The Wiedemann-Franz Law . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.8 Electrical Conductivity of Localized Electrons . . . . . . . . . . . . . . 9.9 Quantum Transport in Nanostructures . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Panel VIII: Quantum Oscillations and the Topology of Fermi Surfaces . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

241 241 245 247 251 255 261 264 266 268 282

10 10.1

291

285

Superconductivity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Some Fundamental Phenomena Associated with Superconductivity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.2 Phenomenological Description by Means of the London Equations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.3 Instability of the ``Fermi Sea'' and Cooper Pairs . . . . . . . . . . . . 10.4 The BCS Ground State . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.5 The Excitation Spectrum of a Superconductor . . . . . . . . . . . . . . 10.6 Consequences of the BCS Theory and Comparison with Experimental Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.7 Supercurrents and Critical Currents . . . . . . . . . . . . . . . . . . . . . . 10.8 Coherence of the BCS Ground State and the Meissner-Ochsenfeld Eect . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.9 Quantization of Magnetic Flux . . . . . . . . . . . . . . . . . . . . . . . . . 10.10 Type II Superconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.11 ``High-Temperature'' Superconductors . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Panel IX: One-Electron Tunneling in Superconductor Junctions . . . . . Panel X: Cooper-Pair Tunneling ± The Josephson Eect . . . . . . . . . . .

324 329 333 340 349 352 362

11 11.1 11.2 11.3

371 371 374 377

Dielectric Properties of Materials . . . . . . . . . . . . . . . . . . . . . . . . The Dielectric Function . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Absorption of Electromagnetic Radiation . . . . . . . . . . . . . . . . . The Dielectric Function for a Harmonic Oscillator . . . . . . . . . .

291 296 299 304 312 317 321

XIV

Contents

11.4 Longitudinal and Transverse Normal Modes . . . . . . . . . . . . . . . 11.5 Surface Waves on a Dielectric . . . . . . . . . . . . . . . . . . . . . . . . . . 11.6 Reflectivity of a Dielectric Half-Space . . . . . . . . . . . . . . . . . . . . 11.7 The Local Field . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.8 The Polarization Catastrophe and Ferroelectrics . . . . . . . . . . . . 11.9 The Free-Electron Gas . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.10 Interband Transitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.11 Excitons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.12 Dielectric Energy Losses of Electrons . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Panel XI: Novel Optical Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . Panel XII: Infrared Spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Panel XIII: The Frustrated Total Reflection Method . . . . . . . . . . . . . .

379 382 384 385 387 389 391 398 400 403 407 414 417

12 12.1 12.2 12.3 12.4 12.5 12.6

419 420 424 428 432 437

Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Data of a Number of Important Semiconductors . . . . . . . . . . . . Charge Carrier Density in Intrinsic Semiconductors . . . . . . . . . . Doping of Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . Carrier Densities in Doped Semiconductors . . . . . . . . . . . . . . . . Conductivity of Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . The p±n Junction and the Metal/Semiconductor Schottky Contact . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.7 Semiconductor Heterostructures and Superlattices . . . . . . . . . . . 12.8 Important Semiconductor Devices . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Panel XIV: The Hall Eect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Panel XV: Cyclotron Resonance in Semiconductors . . . . . . . . . . . . . . . Panel XVI: Shubnikov-de Haas Oscillations and Quantum Hall Eect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Panel XVII: Semiconductor Epitaxy . . . . . . . . . . . . . . . . . . . . . . . . . . Panel XVIII: Preparation of Nanostructures . . . . . . . . . . . . . . . . . . . .

443 459 472 486 489 492 495 504 510

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 517 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 527

1 Chemical Bonding in Solids

Solid-state physics is the physics of that state of matter in which a large number of atoms are chemically bound to produce a dense solid aggregate. The emphasis in this statement is placed on the large number of atoms involved, since that number is of the order of 1023 cm±3. At first sight it would seem to be a hopeless task to try to apply traditional scientific methods for the description of such a vast number of atoms. However, it is exactly the large number of atoms involved that in fact makes a quantitative description possible by means of new models, applicable specifically to solids. A prerequisite, though, for the success of these models, is that the participating atoms are not simply chosen at random from the periodic table of elements; the solid must be composed of a limited number of dierent elements whose atoms are arranged in space with a certain order. Thus, for the solid state physicist, the showpieces are the ``elementary'' crystals, i.e., three-dimensional periodic arrangements of atoms of one type, or chemical compounds of two elements. An understanding of solids and of their characteristic properties thus requires that we first achieve a fundamental understanding of two particular phenomena: the first is that of the forces that hold together the atoms of a solid, in other words, the chemical bonding between atoms. The second important aspect is the structural ordering of the atoms within the solid. A consideration of these two basic questions forms the content of the first two chapters. In both cases it will only be possible to give a short introduction and for a more detailed discussion of these phenomena the reader is referred to textbooks on quantum chemistry and crystallography.

1.1 The Periodic Table of the Elements By way of introduction to the topic of chemical bonding, we will take a brief look at the construction of the periodic table of the elements. The electronic states of an atom are classified according to the one-electron states of the radially symmetric potential. Thus we have 1 s, 2 s, 2 p, 3 s, 3 p, 3 d, 4 s, 4 p, 4 d, 4 f, . . . states where the numbers give the principal quantum number, n, and the letters s, p, d, f correspond to the values of the electron's orbital angular momentum (l = 0, 1, 2, 3, . . .). This classification stems from the picture in which the potential for each electron includes the eect of all other electrons by representing them as a continuous fixed charge distribution H. Ibach, H. LuÈth, Solid-State Physics, 4th ed., DOI 10.1007/978-3-540-93804-0_1, Ó Springer-Verlag Berlin Heidelberg 2009

2

1 Chemical Bonding in Solids

Table 1.1. The build-up of the periodic table by successive filling of the electronic energy shells. Indicated on the left of each column is the outer electron level that is being progressively filled, and in brackets is its maximum allowed occupation number. See also cover page 1s 2s 2p 3s 3p

(2) H, He (2) Li, Be (6) B ? Ne (2) Na, Mg (6) Al ? Ar

4s 3d 4p 5s 4d

(2) (10) (6) (2) (10)

K, Ca Transition metals Sc ? Zn Ga ? Kr Rb, Sr Transition metals Y ? Cd

5 p (6) In ? Xe 6 s (2) Cs, Ba 4 f (14) Rare earths Ce ? Lu 5 d (10) Transition metals La ? Hg 6 p (6) Tl ? Rn

which, to a greater or lesser extent, screens the potential of the bare nucleus. In addition to the principal quantum number n and the orbital angular momentum quantum number l, there is also a magnetic quantum number m which can take (2 l+1) dierent values (ranging from ±l to +l ). According to the Pauli exclusion principle, each state can be occupied by at most two electrons of opposite spin. As a function of increasing nuclear charge this then leads to the periodic tables whose structure is outlined in Table 1.1. From the order of the energy levels of the hydrogen atom, one would expect that after the 3 p-states are filled, the next states to be occupied would be the 3 d. But in fact, as can be seen from Table 1.1, this is not the case; following the 3 p-levels those next occupied are the 4 s. The subsequent filling of the 3 d-states gives rise to the first series of transition metals (the 3 d-metals). Similarly, one also finds 4 d- and 5 d transition metals. The same eect for the f-states leads to the so-called rare earths. The reason for this anomaly is that the electrons in s-states have a nonvanishing probability of being located at the nucleus thereby reducing for them the screening eect of the other electrons. Hence the s-electrons possess lower energy. If one considers a thought experiment in which several initially isolated atoms are gradually brought closer together, their interaction with one another will lead to a splitting of each of their energy levels. If a very large number of atoms are involved, as in the case of a real solid, then the energy levels will lie on a quasicontinuous scale and one therefore speaks of energy bands (Fig. 1.1). The width of the band (i.e., the broadening) depends on the overlap of the wavefunctions concerned. Thus for the deep lying levels the broadening is small, and these ``core levels'' retain their atomic shell-like character even in the solid. For the highest occupied levels, on the other hand, the broadening is so large that the s-, p- and where present, d-levels merge into a single band. It is the electrons in this uppermost band that are responsible for the chemical bonding between atoms, and hence one speaks of the valence band. The ultimate source of the chemical bonding is the reduction in electronic energy which results from the level broadening. This, despite the increase in repulsion between the nuclei, leads to a decrease in the total energy as a function of atomic separation until the point where the equilibrium separation is reached ± i.e., the point of minimum total energy. The type of bonding in a solid is determined essentially by the degree of overlap between the electronic wavefunctions of the atoms involved. At the

1.1 The Periodic Table of the Elements

3

Fig. 1.1. Broadening of the energy levels as a large number of identical atoms from the first row of the periodic table approach one another (schematic). The separation r0 corresponds to the approximate equilibrium separation of chemically bound atoms. Due to the overlap of the 2 s and 2 p bands, elements such as Be with two outer electrons also become metallic. Deep-lying atomic levels are only slightly broadened and thus, to a large extent, they retain their atomic character

one extreme, this overlap may be limited to neighboring atoms; in other cases the wavefunctions may be spread over many atoms. In the former case, the degree of overlap, and thus the strength of the bonding, is dependent not only on the separation of neighboring atoms, but also on the bond angles. This is referred to as directional bonding or covalent bonding. In its purest form, covalent bonding is realized between a few elements of equal ``valence'', i.e. elements with the same outer electronic configuration. However, an equal electronic configuration is neither a necessary nor a sucient condition for covalent bonding. What is important is simply the relative extent of the wavefunctions in comparison to the interatomic separation. If the extent of the wavefunctions is large compared to the nearest-neighbor distance, then the exact position of the nearest neighbors plays an insignificant role in producing the greatest possible overlap with many atoms. In this case, the packing density is more important than the position of the next neighbors. Here one speaks of non-directional bonding. This regime in which the wavefunctions spread over a distance that is large in comparison to the atomic separation is characteristic of metallic bonding. However, there is a further type of non-directional bonding with extremely small overlap of wavefunctions; this is the ionic bond. It occurs in cases where the transfer of an electron from one atom to another is suciently

4

1 Chemical Bonding in Solids

energetically favorable. A prerequisite for ionic bonding is thus a dissimilarity of the atoms involved. In the following sections we will explore the various types of bonding in greater detail.

1.2 Covalent Bonding We have characterized covalent bonding in solids as a bonding for which the interaction between nearest neighbor atoms is of prime importance. It is therefore possible to derive many of the essential properties of covalent solids using the quantum chemistry of molecules. For our discussion we shall refer to the simplest model for bonding, namely of a diatomic molecule with a single bonding electron. The Hamiltonian for this molecule contains the kinetic energy of the electron and the Coulomb interaction between all partners (Fig. 1.2 a).

Fig. 1.2 a±c. The simplest model of a covalent bond (the H+ 2 molecule). (a) Definition of the symbols in (1.1). (b) Bonding and antibonding combinations of atomic orbitals. The bonding combination leads to an accumulation of charge between the nuclei which in turn gives rise to a reduction in the Coulomb energy. (c) The splitting of the atomic energy level into the bonding and antibonding states. The greatest gain in energy is achieved when the bonding state is fully occupied ± i.e., contains two electrons ± and the antibonding state is empty (covalent bonding)

1.2 Covalent Bonding

H

h2 D 2m

Z 0 e2 ZZ0 e2 : 4 p e0 rB 4 p e0 R

Z e2 4 p e0 rA

5

1:1

The appropriate molecular orbital wmo for the electron would be the solution to the SchroÈdinger equation

H wmo E wmo :

1:2

However, even in this simple case, it is necessary to rely on approximate solutions. The expectation value of the ground-state energy may be calculated using such an approximate solution, according to w H wdr 0 :
1:3 E w w dr The approximate solution w may be set equal to a linear combination of states of the two separate atoms: w cA wA cB wB :

1:4

Here the wavefunctions and their coecients are real. It is possible to show that any trial function such as w always leads to an energy E ' that lies above the true value E (see Problem 1.8). The best values for the coecients cA and cB are those which lead to a minimum value of E '. With the abbreviations S wA wB dr
overlap integral) ;
1:5 a
1:5 b HAA wA H wA dr ; HAB wA H wB dr ;
1:5 c one obtains the following expression for E ', which then has to be minimized E0

c2A HAA c2B HBB 2 cA cB HAB : c2A c2B 2 cA cB S

1:6

For the minimum with respect to cA and cB we require @ E0 @ E0 0; @ cA @ cB

1:7

which leads to the following secular equations cA
HAA cA
HAB

E 0 cB
HAB 0

E 0 S 0 ;

E S cB
HBB

0

E0:

1:8 a
1:8 b

Their solution is given by the condition that the determinant vanishes, i.e.,
HAA

E 0
HBB

E 0

HAB

E 0 S2 0 :

1:9

6

1 Chemical Bonding in Solids

For simplicity, we consider a molecule with two identical nuclei (for example, H + 2 ) for which we have HAA = HBB. With the single atomic eigenvalue HAA = HBB of the individual free atoms, we then obtain two new molecular orbitals with the energies E < E 0 e

HAA HAB : 1S

1:10

When the two nuclei are infinitely far apart we have S = 0 on account of (1.5 a), whereas when the nuclear positions coincide, we have S = 1. From (1.10) it follows that the spatial overlap of the wavefunctions wA and wB leads to a splitting of the original energy level HAA = HBB into a higher and a lower molecular energy level (Fig. 1.2 c). The molecular orbital corresponding to the higher energy level is known as antibonding, and the other is bonding. In the molecule the electron occupies the lower-lying bonding orbital thereby giving rise to a reduction in the total energy. This reduction corresponds to the binding energy of the covalent bond. From the foregoing discussion one sees that only partially occupied single-atomic orbitals, i.e., those containing less than two electrons, can participate in covalent bonding: Since the bonding molecular orbital can contain only two electrons (the Pauli principle allows two opposite spin states), any further electrons would have to occupy the higher-lying antibonding orbital, which would counteract the original gain in energy (cf. Problem 1.7). For the diatomic molecules considered here the bonding molecular orbital consists of an additive combination of wA and wB, i.e. wmo = wA+wB [in (1.4) we have cA = cB for identical nuclei]. As shown in Fig. 1.2, this leads to an increase in the electronic charge density between the nuclei. The antibonding combination wmo = wA±wB, on the other hand, results in a decrease of this charge density. One sees that covalent bonding is associated with a ``piling-up'' of charge between the atoms that form the molecule or solid concerned. It is the spatial overlap of the wavefunctions that is responsible for this bonding and which also determines the energy gain of the bonding orbitals of the molecule or solid, and thereby the binding energy. As shown in Fig. 1.3, for particular atomic orbitals (s, p, d, etc.) there are some orientations that favor the overlap and others that are unfavorable. This is the underlying reason for this strongly directional character of the covalent bonding, which is particularly evident in the covalently bound crystals of diamond (C), Si and Ge with their tetrahedral coordination (Fig. 1.4). Let us take a closer look at this tetrahedral bonding for the example of diamond. From a consideration of its electronic configuration 1 s 2, 2 s 2, 2 p 2, one would expect a carbon atom to be able to participate in only two covalent bonds (corresponding to the two 2 p-orbitals each occupied by one electron). However, when these atoms form part of a crystal it is clear that a larger reduction in total energy is produced if four bonding orbitals can overlap. In a one-electron picture this may be understood in terms of the

1.2 Covalent Bonding

7

Fig. 1.3 a, b. Pictorial representation of the spatial overlap between an s- and a p-wavefunction of hydrogen. The ``size'' of the wavefunction is illustrated by a surface of constant wavefunction amplitude. (a) A situation in which the overlap cancels due to sign reversal of the pz-wavefunction. (b) Nonvanishing overlap between s- and px-wavefunctions

Fig. 1.4. The tetrahedral configuration of nearest neighbors in the lattice of C, Si, Ge and a-Sn. This structure is favored because its periodic repetition fills three-dimensional space, and because it enables the formation of sp 3 hybrid orbitals from the s, px py and pz states. The figure displays the orbitals of diamond (C). The orbitals of Si, Ge, and aSn possess additional nodes

following simplified description: One of the electrons from the 2 s-orbital is excited into the empty 2 p-orbital. Each of the 2 p-orbitals and the single 2 sorbital now contains one electron and thus each of these can participate in a covalent bond. The overlap with the wavefunctions of the nearest neighbors is maximized if four new wavefunctions are formed by a linear combination of the original 2 s, 2 px, 2 py, and 2 pz-orbitals. These new molecular orbitals are known as sp 3 hybrids and their creation is called hybridization (Problem 1.9). The gain in energy that is produced by the overlap in the tetrahedral configuration is more than enough to compensate for the energy needed to promote the 2 s-electron into the 2 p-orbital. If one now considers carbon atoms arranged in the diamond structure, in which each atom is surrounded by four other atoms positioned at the corners of a tetrahedron (Fig. 2.12), one finds that in the sp 3 hybridized state all the available electrons can be shared with the neighbors such that only the bonding orbitals are occupied. This leads to a fully occupied valence band that is separated from the next highest (antibonding) band by

8

1 Chemical Bonding in Solids

an energy gap. Energy can only be supplied in large quanta that are sucient to promote an electron across this band gap. At low temperature such covalently bonded solids are therefore nonconducting. If the bandgap is not too large, however, electrons can be promoted by thermal excitation leading to a measurable conductivity. In this case one speaks of semiconductors. A more precise definition of these will be given in Chaps. 9 and 12. Instead of the sp 3 hybrid orbital carbon can also form a planar hybrid orbital from one 2 s and two 2 p functions (Problem 1.10). These orbitals yield a planar 120 ° star called sp 2. An additional pz orbital containing one electron lies perpendicular to the plane of the star. The overlap between pz orbitals of neighboring C atoms leads to a further bonding, the so-called p bonding. This type of bonding is found within the layers of the graphite structure of carbon. The bonding between the covalently bound layers of graphite is of the van der Waals type (Sect. 1.6) and is thus relatively weak. An interesting spatial structure involving sp 2 orbitals is that of the fullerenes, whose most prominent member is C60 (Fig. 1.5). Their structure includes pentagons. For topological reasons, 12 pentagons are necessary to produce a closed structure. In addition to the 12 pentagons, the C60 cluster also contains 20 hexagons. Even larger molecules can be produced by the inclusion of more hexagons. C60 clusters can also form the basis of threedimensional crystal structures, for example when other atoms such as alkali or alkaline earth metals are included. A complete saturation of the covalent bonding is possible for the group IV elements C, Si, Ge and a-Sn in the three-dimensional space-filling tetrahedral configuration. The group V elements P, As, Sb, demand a three-fold coordination for saturation; they form planar layer structures. Correspondingly, the group IV elements Te and Se occur in a chain-like structure with two-fold coordination. Covalently bonded solids can, of course, also be produced from combinations of dierent elements. As an example, we consider boron nitride. The two elements involved have the electronic structure: B (2 s 2, 2 p 1);

Fig. 1.5. The structure of C60

1.3 Ionic Bonding

9

N (2 s 2, 2 p 3). These elements can also bind in the diamond structure with tetrahedral coordination. Each boron atom is thereby surrounded by four nitrogen atoms and vice versa. The shared bonding electrons are comprised of five electrons from the nitrogen atom and three from boron. The total number of electrons per atom is thus the same as in the case of the carbon diamond structure. However, because two dierent elements are involved, the bonding has an ionic character. This will be discussed in the next section. Typical examples of binding energy for purely covalently bonded crystals are: C (diamond): Si: Ge:

7.30 eV per atom (712 kJ/mol); 4.64 eV per atom (448 kJ/mol); 3.87 eV per atom (374 kJ/mol).

1.3 Ionic Bonding To understand ionic bonding one needs to consider the ionization energies and electron anities of atoms. The ionization energy I is defined as the energy that must be supplied in order to remove an electron from a neutral atom. The electron anity A is the energy that is gained when an additional electron is added to a neutral atom. Ionic bonding is produced whenever an element with a relatively low ionization energy is combined with an element with a high electron anity. As an example we consider the combination of sodium and chlorine. The ionization energy of sodium is 5.14 eV, and the electron anity of chlorine 3.71 eV. Thus in order to transfer one electron from a sodium atom to a chlorine atom requires an energy expenditure of 1.43 eV. The electrostatic attraction between the two ions leads to an energy gain that increases as they approach closer to one another, with a minimum separation that is determined by the sum of their two ionic radii. This electrostatic attraction contributes an energy gain of 4.51 eV thus giving an overall gain in energy of 3.08 eV. It is therefore possible for sodium and chlorine to form a diatomic molecule with a strongly ionic character. Threedimensional crystals can also be produced in this way. In the structure so formed, each chlorine atom is surrounded by sodium neighbors, and vice versa. The exact structure is determined by the optimal use of space for the given ionic radii, and by the condition that the Coulomb attraction between oppositely charged ions should be greater than the repulsion between ions of the same sign. Figure 1.6 shows two structures that are typical for twoion crystals; the sodium-chloride and the cesium-chloride structures. The ionic radii are the essential factor in determining the minimum separation because, if the ions were to approach still closer, a strong overlap between the ionic electron clouds would occur. For fully occupied electron shells such as these (Sect. 1.2), the Pauli principle would then require that

10

1 Chemical Bonding in Solids

Fig. 1.6. The two structures typical for ionic bonding in solids: (a) NaCl structure; (b) CsCl structure

higher lying antibonding orbitals should become occupied. This should lead to a steep increase in the energy and therefore a strong repulsion. Whereas this repulsive contribution to the total energy, like the covalent bond, can only be derived from a quantum mechanical calculation, the attractive Coulomb contribution to the ionic bond can be described simply as a sum over the Coulomb potentials ion sites. For the potential energy between two singly charged ions i and j at a separation rij one writes uij

e2 B ; 4 p e0 rij rnij

1:11

the second term describes the repulsion between the two electron clouds. It is an heuristic term containing two free parameters n and B. It should, of course, be possible to determine these parameters from an exact quantum mechanical treatment of the problem. However, a commonly used approach is to derive the values of these parameters from a fit to measured experimental quantities (ionic separation, compressibility, etc.); this yields values of n mainly in the range 6 to 10. The form of a typical potential energy curve is depicted in Fig. 1.7. The total potential energy due to all other ions j at the site of ion i is given by the summation X ui uij :
1:12 i6j

If r is the separation of nearest neighbors one can write rij r pij ;

1:13

where the pij depend on the particular crystal structure. If the crystal contains N ion pairs, then its total potential energy is given by

1.3 Ionic Bonding

11

Fig. 1.7. Potential energy as a function of the separation of two ions

U N ui N

e2 X 1 B X 1 n : 4 p e0 r i6j pij r i6j pnij

1:14

For each possible structure one has the characteristic quantity X 1 A pij i6j

1:15

which is known as the Madelung constant. For the sodium-chloride structure A = 1.748 and for the cesium-chloride structure A = 1.763. Some typical binding energies are NaCl: NaI: KrBr:

7.95 eV per ion pair (764 kJ/mol); 7.10 eV per ion pair (683 kJ/mol); 6.92 eV per ion pair (663 kJ/mol).

In ionic crystals, it is not possible for the electrons to move about freely between ions unless a large amount of energy (*10 eV) is supplied. Solids with ionic bonding are therefore nonconducting. However, the presence of Table 1.2. The electronegativity of selected elements [1.1] H 2.1 Li 1.0

Be 1.5

B 2.0

C 2.5

N 3.0

O 3.5

F 4.0

Na 0.9

Mg 1.2

Al 1.5

Si 1.8

P 2.1

S 2.5

Cl 3.0

K 0.8

Ca 1.0

Sc 1.3

Ge 1.8

As 2.0

Se 2.4

Br 2.8

Rb 0.8

Sr 1.0

Y 1.3

Sn 1.8

Sb 1.9

Te 2.1

I 2.5

12

1 Chemical Bonding in Solids

Fig. 1.8. Density of valence electrons in a typical ionic crystal (NaCl) and in a typical covalently bound crystal (Si) [1.2, 3]. One clearly sees the concentration of charge along the bond between Si atoms, whereas in the ionic bonding, the electrons are almost spherically distributed around the ions

defects means that at high temperatures the ions themselves can move around, giving rise to ionic conduction. Ionic bonding and covalent bonding are two limiting cases, of which only the latter can exist in solids composed of a single type of atom. In the majority of cases the bonding is of an intermediate nature representing a mixture of the two extremes. A qualitative measure of the ionicity of a bond is made possible by the electronegativity scale. This scale was first developed

1.4 Metallic Bonding

13

by Pauling as a result of observations of bond energies. Subsequently Millikan made use of the physical quantities ionization energy, I, and electron anity, A, to derive the following definition of the electronegativity of an element: X 0:184
I A :

1:16

If the ionization energy and electron anity are expressed in electron volts one obtains the Pauling electronegativity scale of Table 1.2. The higher the ionization energy and electron anity of an atom, the greater is its tendency to draw the electrons of a bond towards itself. In a bond between two atoms it is therefore always the atom with the higher electronegativity that is the anion. The dierence in the electronegativity of the two atoms is a measure of the ionicity of the bond. The dierence between ionic bonding and covalent bonding, in particular the dierent electron density distributions, is illustrated in Fig. 1.8. This shows contours of constant electron density which may be deduced for example from X-ray diraction studies. For ionic bonding (NaCl) the electrons are concentrated around the atoms, whereas for covalent bonding (Si) there is an accumulation of electrons between the atoms.

1.4 Metallic Bonding It is possible to regard metallic bonding as an extreme case of bonding in which the electrons are accumulated between the ion cores. However, in contrast to covalent bonding, the electrons now have wavefunctions that are very extended in comparison to the separation between atoms. As an example, Fig. 1.9 shows the radial part of the 3 d and 4 s wavefunction of nickel in the metallic state. The 4 s wavefunction still has significant amplitude even at a distance half way to the third nearest neighbors; thus many neighbors are involved in the bonding. This leads to a strong screening of the positive ion core, and to a bonding that has certain similarities to covalent bonding. However, due to the strong ``smearing out'' of the valence electrons over the whole crystal, the bonding is not directional as in the case of covalent crystals. The crystal structure of metals is thus determined, to a large extent, by the desire for optimum filling of space (Sect. 2.5). Unlike the s-electrons, the d-electrons of transition metals are localized, and the overlap is correspondingly smaller. The d-electrons form a kind of covalent framework in transition metals and produce the main contribution to the binding energy. The valence band of metals, comprising the outer s-, p- and sometimes d-electrons, is not fully occupied (Table 1.1). As a consequence of the quasicontinuous distribution of states on the energy scale for a large number of

14

1 Chemical Bonding in Solids

Fig. 1.9. The amplitude of the 3 dzz-wavefunction and the 4 s-wavefunction of Ni [1.4]. The half-distances to the first, second and third nearest neighbors (r1, r2 and r3) are shown for comparison

atoms, one can supply energy to the electrons in infinitesimally small portions; in particular, they can be accelerated by an externally applied electric field. A particular feature of metals is thus their high electrical conductivity, which is related to their similarly high thermal conductivity. In this sense, the metallic bond is a feature that is peculiar to solids, i.e., to aggregates of many atoms. A glance at Table 1.1 indicates that the partially filled valence band of metals can arise in various ways. The alkali metals (Li, Na, K, Rb, Cs) clearly have the necessary prerequisite since the outer atomic s-state is only singly occupied. For the alkaline earth metals (Be, Mg, Ca, Sr, Ba) one might initially expect a full valence band formed from the doubly occupied atomic s-states. However, because of the overlap in energy with the bands stemming from the (empty) atomic p-states of the same shell, the net result is a partially occupied joint sp-band. The transition metals represent a special case. Here the s- and p-states again form a broad common band. As mentioned previously, the d-electrons have a relatively small spatial extent (Fig. 1.9) and, due to the correspondingly small overlap with the neighboring atoms, the d-band of the transition metals has a smaller energy width than the sp-band. The large spreading of the wavefunction of valence electrons in metals makes it particularly dicult to theoretically predict their binding energy. On the other hand, the valence electrons are free to move between the atoms. This simplifies the description of the electrical conductivity and the specific heat of the electrons, as will become clear in Chap. 6.

1.6 The van der Waals Bond

15

1.5 The Hydrogen Bond One speaks of a hydrogen bond when a hydrogen atom is bound to two other atoms. At first sight, it is surprising that such a bond can exist since hydrogen has only one electron. However, one can imagine the hydrogen bond as follows: when hydrogen takes part in a covalent bond with a strongly electronegative atom, for example, oxygen, its single electron is almost completely transferred to the partner atom. The proton which remains can then exert an attractive force on a second negatively charged atom. Because of the extended electron cloud of the electronegative atom and the extremely small size of the proton with its strongly reduced electron screening, it is not possible for a third atom to be bound. The hydrogen atom is thus always doubly coordinated in a hydrogen bond. Such bonds are most common between strongly electronegative atoms, but are not limited to this case alone. They can be of a symmetric A±H±A type or of an asymmetric A±H . . . B type. A criterion for the existence of a hydrogen bond is that the observed separation of the atoms A and B is smaller than it would be if only van der Waals bonding (Sect. 1.6) were present. A further indication of the presence of hydrogen bonds may be obtained from infrared spectroscopy, in which the band corresponding to hydrogen vibrations shows a strong shift, and is often broadened, too. Generally, speaking, the phenomena associated with hydrogen bonding are quite diverse, and this type of bonding is harder to characterize than most other types. The binding energies of hydrogen bonds are of the order of 0.1 eV per bond. It is hydrogen bonds that are responsible for linking the two chains of the double helix in the DNA molecule and, as such, these bonds play a crucial role in the mechanism of genetic reproduction. The best-known example from the realm of inorganic chemistry is water, in particular when it is in the form of ice. Each oxygen atom in ice is surrounded by four further oxygen atoms in a tetrahedral configuration and the bonding is provided by hydrogen atoms. Hydrogen bonds are also present in the liquid form of water, which leads, for example, to the anomaly in the expansion coecient: water has its highest density at 4 °C. The reason for this is that the liquid form of water also contains complexes of H2O molecules that are held together by hydrogen bonds. In comparison to H2O molecules without hydrogen bonds, the former occupy a larger volume. As the temperature increases the hydrogen-bonded aggregates melt, leading to an increase in the density. Above 4°C one finds the usual thermal expansion, i.e., the density decreases with further increasing temperature.

1.6 The van der Waals Bond This is an additional type of bond that, in principle, is always present. However, the van der Waals bond is only significant in cases where other

16

1 Chemical Bonding in Solids

types of bonding are not possible, for example, between atoms with closed electron shells, or between saturated molecules. The physical source of this bonding is charge fluctuations in the atoms due to zero-point motion. The dipole moments which thereby arise cause an additional attractive force. Van der Waals forces are responsible for the bonding in molcular crystals. The bonding energy is dependent on the polarizability of the atoms involved and is mostly of the order of 0.1 eV. Typical atomic bonding radii for van der Waals bonding are considerably larger than for chemical bonding. The attractive part of the potential between atoms that interact only via van der Waals forces varies as r ±6, where r is the separation of the atoms (or molecules). This can be readily understood as a consequence of the dipole interaction. A dipole moment p1 resulting from a momentary charge fluctuation gives rise to an electric field at distance r of strength E *p1/r 3. A second atom of polarizability a situated at distance r is polarized by this electric field and acquires an induced dipole moment of p2*a p1/r 3. Since the potential of this dipole in the field is proportional to E and to p2, it follows that the attractive part of the van der Waals interaction varies as r ±6 (Problem 1.11).

Problems 1.1 a) Calculate the Madelung constant A for a linear ionic chain. b) Make approximate numerical calculations of the Madelung constant (A = 1.7476) for the NaCl lattice. Use two dierent approaches: First, a cubic geometry where 2 ma is the length of a side of the cube and a the separation of nearest neighbors, and, second, a spherical geometry where ma is the radius of the sphere. In both cases the reference ion is located at the center. Carry out the calculation for m-values of m = 97, 98, and 99 and compare the results. What is the cause of the discrepancy? 1.2 Determine the isothermal bulk modulus @p jV @V T and the lattice energy per ion pair for NaCl using the expression for the lattice energy of N ion pairs: e2 BX 1 U
r N A n : r i6j p nij 4 p e0 r Using the value n = 9, calculate B from the condition that U (r) is a minimum at the equilibrium separation.

Problems

17

1.3 It is well known that common salt (NaCl) is easily dissolved in water. In the solution Na and Cl atoms are present as positive and negative (``solvated'') ions. Show that, due to the high dielectric constant of water and the resulting screening of the Coulomb potential, the binding energy of a NaCl crystal in water is smaller than the mean thermal energy of the free ions. Calculate the equilibrium separation of the ions of a hypothetical NaCl crystal in water and show that this separation is larger than the van der Waals radius of a water molecule, thereby justifying the approximate approach used here to discuss the solubility of NaCl. 1.4 Discuss the ionicity of alkali halides with the help of Table 1.2. 1.5 Take the CsCl structure and assume that the cation radius becomes smaller while the anion radius remains constant. What happens to the binding energy? Show that for small cations the NaCl lattice becomes the preferred structure. For an even smaller cation radius the ZnS lattice has the largest binding energy (Madelung constant A = 1.638). Give examples. 1.6 Calculate approximately the zero-point entropy of ice. In the ice structure the oxygen atoms form a wurtzite lattice which is stabilized by hydrogen bonds between the nearest neighbor oxygen atoms. The zero-point entropy results from the possible ways of distributing the two hydrogen atoms per oxygen atom over the four bonds to the nearest neighbors. 1.7 Discuss the electron configuration of the oxygen molecule. Why is the bond strength equivalent to a chemical double bond? Why is O2 paramagnetic? Give an argument to explain why O+ 2 is a stable ion. 1.8 Prove that the estimate of the ground-state energy obtained with the help of an approximate wavefunction using the Ritz procedure, E

w; H w ;
w; w

is always greater than or equal to the exact eigenvalue E0. To do this, expand the approximate function in terms of the exact eigenfunctions wi (exact eigenvalue Ei ). 1.9 The carbon atom in its tetrahedral bonding configuration in diamond can be approximately represented by four 2sp 3 wavefunctions, which are linear superpositions of the four hydrogenic 2s, 2px, 2py, 2pz atomic wavefunctions fj : wi

X j

aij fj ; with i; j 1; 2; 3; 4

18

1 Chemical Bonding in Solids

and where the possible functions fj appear in spherical coordinates as follows: f1 f
2 s c e f2 f
2pz c e

R

1

R

R ;

R cos h ;

R

f3 f
2px c e R sin h cos u ; f4 f
2 py c e R

Zr 2a0

R

R sin h sin u ;

and

a0 Bohr radius, Z=nuclear charge, here that of carbon).

One demands of the wi that, like the fj, they are orthonormal, i.e. R wi wk dr dik : a) Plot the contours of f (R = const, h, u ) for the 2s and one of the 2p states on a polar diagram. b) Prove that the orthonormality requirement for the wi (2sp 3) wavefunctions leads to the condition X aij akj dik with aij aji : j

c) Determine four possible wi functions which fulfill the orthonormality requirement with aij = 12 or aij = ± 12. d) Show that the maxima of |wi |2 are located in tetrahedral directions and draw these by means of vectors pointing to the corners of a cube whose edges are parallel to the x, y and Pz axes. e) Show that the electron density 4i = 1 |wi |2 has spherical symmetry. f) Discuss possible reasons why the real valence electron density in a diamond crystal is nevertheless not spherical around a carbon atom but is concentrated in tetrahedral bonding directions. 1.10 a) In analogy to the sp3 hybridization of carbon in the diamond lattice, discuss the possibility of the carbon atom forming sp 2 hybrid orbitals with three planar bonding directions. Plot a qualitative picture of the three bonding sp 2 orbitals and the remaining unpaired pz orbital and give their electron occupation. b) Assuming sp 2 hybridization for the carbon atoms explain the chemical bonding in the benzene molecule C6H6. What is the origin of the p bonding system parallel to the hexagonal ring skeleton of the six carbon atoms. c) Assuming sp 2 hybridization explain the highly anisotropic properties of the planar hexagonal graphite lattice of carbon (quasi-metallic properties parallel to the carbon planes). How are these anisotropic properties exploited in every-day life?

Problems

19

1.11 As a simple quantum mechanical model for the van der Waals interaction consider two identical harmonic oscillators (oscillating dipoles) at a separation R. Each dipole consists of a pair of opposite charges whose separations are x1 and x2 , respectively, for the two dipoles. A restoring force f acts between each pair of charges. a) Write down the Hamiltonian H 0 for the two oscillators without taking into account electrostatic interaction between the charges. b) Determine the interaction energy H 1 of the four charges. c) Assuming |x1| R, |x2| R approximate H 1 as follows

H1

2 e2 x1 x2 : R3

d) Show that transformation to normal coordinates 1 xs p
x1 x2 ; 2 1 xa p
x1 x2 2 decouples the total energy H = H 0 + H 1 into a symmetric and an antisymmetric contribution. e) Calculate the frequencies xs and xa of the symmetric and antisymmetric normal vibration modes. Evaluate the frequencies xs and xa as Taylor series in 2e 2/( f R 3) and truncate the expansions after second order terms. f) The energy of the complete system of two interacting oscillators can be expressed as U = ± 12 h (xs + xa). Derive an expression for the energy of the isolated oscillators and show that this is decreased by an amount c/R 6 when mutual interaction (bonding) occurs. 1.12 Calculate how the van der Waals bonding of a molecule depends on its distance, d, from a solid surface. For simplicity, choose a simple cubic lattice. Show that the result does not depend on the structure of the crystal.

2 Structure of Solid Matter

When atoms are chemically bound to one another they have well-defined equilibrium separations that are determined by the condition that the total energy is minimized. Therefore, in a solid composed of many identical atoms, the minimum energy is obtained only when every atom is in an identical environment. This leads to a three-dimensional periodic arrangement that is known as the crystalline state. The same is true for solids that are composed of more than one type of element. In this case, certain ``building blocks'' comprising a few atoms are the periodically repeated units. Periodicity gives rise to a number of typical properties of solids. Periodicity also simplifies the theoretical understanding and the formal theory of solids enormously. Although a real solid never possesses exact three-dimensional periodicity, one assumes perfect periodicity as a model and deals with the defects in terms of a perturbation (Sect. 2.7). Three-dimensional periodic arrangements of atoms or ``building blocks'' are realized in many dierent ways. Basic elements of the resulting crystal structures are described in Sects. 2.1±2.5. The counterpart to the crystalline state of solids is the amorphous state. This is a state in which no long-range order exists; however, a degree of short-range order remains. Examples of amorphous solids are glasses, ceramics, gels, polymers, rapidly quenched melts and thin-film systems deposited on a substrate at low temperatures. The investigation of amorphous materials is a very active area of research. Despite enormous progress in recent years, our understanding of amorphous materials still remains far from complete. The reason is the absence of the simplifications associated with periodicity. Nonetheless, from comparison of the properties of materials in a crystalline and an amorphous state we have learned the essential features of the electronic structure, and thereby also macroscopic properties, are determined by short-range order. Thus these properties are similar for solids in the amorphous and crystalline state. In the context of this book we focus on a few structural and electronic properties of amorphous solid in Sects. 3.1, 7.6 and 9.8. Materials of practical use are nearly always composites. Examples, some of them known to mankind since early ages, are the bronzes (alloys of copper and tin), brass (copper and zinc) or steel (in its simplest form iron with a few per cent of carbon). Modern material science has supplemented these classical, mostly binary alloys with many multi-component systems including composite materials. In the framework of this textbook,

H. Ibach, H. LuÈth, Solid-State Physics, 4th ed., DOI 10.1007/978-3-540-93804-0_2, Ó Springer-Verlag Berlin Heidelberg 2009

22

2 Structure of Solid Matter

particular attention will be paid to semiconductor alloys (Chap. 12). Alloys typically do not exist as a homogenous crystalline phase; they rather consist of microcrystallites, whose composition depends on temperature, pressure, and the percentage of the constituting elements. Phase diagrams of simple binary alloys are discussed in Sect. 2.6.

2.1 The Crystal Lattice A two-dimensional lattice is spanned by two vectors a and b. Every point on the lattice can be reached by a lattice vector of the form r n n1 a n2 b

2:1

where n1 and n2 are integers. Depending on the ratio of the lengths of the vectors a and b, and on the angle c between them, lattices of various geometries can be constructed. The most general lattice, with no additional symmetry, is obtained when a=b and c=90 ° (Fig. 2.1). A planar crystal structure would be produced if every point of this ``parallelogram lattice'' were occupied by one atom. In this case, each elementary (or unit) cell with sides a and b would contain one atom. Such elementary cells are termed primitive. It is also possible for crystal structure to contain more than one atom per unit cell. In such cases the lattice points of Fig. 2.1 correspond to points in the crystal which all have identical environments. Such points may, but need not necessarily, lie at the center of an atom. Other planar lattices of higher symmetry are obtained when c, a and b take on certain special values. The rectangular lattice is obtained when c = 90 8 (Fig. 2.2). When additionally a = b, this becomes a square lattice. The two-dimensional plane can also be filled with a regular array of hexagons. The unit cell is then given by a = b and c = 60 8. A hexagonal close packing of spheres has this unit cell. The condition a = b with c arbitrary also produces a new type of lattice. However, this lattice is more conveniently described as a ``centered'' rectangular lattice with a=b and c = 908 (Fig. 2.2). One thereby obtains the advantage of an orthogonal coordinate system; the lattice, however, is no longer primitive. It is easy to see that the description in terms of a centered unit cell is only useful for a rectangular lattice. If centering is introduced into a square, parallelogram or hexagonal lattice, it is always possible to describe

Fig. 2.1. A plane oblique lattice

2.1 The Crystal Lattice

23

Fig. 2.2. Further two-dimensional lattices: square, rectangular, centered rectangular and hexagonal (c = 60 8, a = b)

the new lattice in terms of an alternative set of smaller basis vectors. In other words, the only result is that one has obtained a larger than necessary unit cell. The discussion so far has concerned two-dimensional lattices, but the principles can be extended to lattices in three dimensions. Instead of the five possible systems of basis vectors in the plane, one now has seven possibilities (Table 2.1). These correspond to the seven distinct crystal systems of crystallography. With the addition of centering, one can construct from these basis vector systems all the possible lattices of three-dimensional space. As well as face centering, one now has the additional possibility of body centering (Fig. 2.3). As was the case in two dimensions, one can readily convince oneself that only certain

Table 2.1. The seven dierent basis-vector systems or crystal systems. Most elements crystallize in a cubic or hexagonal structure. For this reason, and also because of their high symmetry, the cubic and hexagonal coordinate systems are particularly important Basis vectors/crystal axes

Angles

Crystal system

a=b=c a=b=c a=b=c a=b=c a=b=c a=b=c a=b=c

= b = c = 90 ° = c = 90 ° b = 90 ° = b = c = 90 ° = b = c = 90 ° = b = 90 ° c = 120 ° = b = c = 90 ° = b = c = 90 °

triclinic monoclinic orthorhombic tetragonal hexagonal rhombohedral cubic

24

2 Structure of Solid Matter

Fig. 2.3. The 14 three-dimensional Bravais lattices. The hexagonal lattice and the two centered cubic lattices are particularly important in solid state physics

centerings are useful. For example, it would not make sense to employ a tetragonal base-centered lattice because this is equivalent to a primitive tetragonal lattice with a smaller unit cell.

2.2 Point Symmetry

25

2.2 Point Symmetry Every point of the lattices just discussed represents an atom, or a more-orless complicated group of atoms, each of which has particular symmetry properties. The symmetries and the corresponding notation will be presented in the following. Reflection in a Plane This symmetry is expressed mathematically by a coordinate transformation. For example, mirror symmetry about the yz-plane is represented by the transformation y ' = y, z ' = z, x ' = ±x. The presence of a mirror plane in a crystal structure is indicated by the symbol m. An example of a molecule possessing two perpendicular mirror planes is the water molecule (Fig. 2.7). One of the mirror planes is the plane defined by the atoms of the molecule; the other is perpendicular to this and passes through the oxygen atom, bisecting the molecule. Inversion Inversion symmetry is described by the coordinate transformation x ' = ±x, y ' = ±y, z ' = ±z. Thus in a sense this might be described as reflection in a point. The symbol representing inversion symmetry is 1. An example of a molecule possessing inversion symmetry is cyclohexane (Fig. 2.4). Homonuclear diatomic molecules also have inversion symmetry and, of course, mirror planes. Rotation Axes Rotational symmetry is present if a rotation through a particular angle about a certain axis, leads to an identical structure. The trivial case is, of

Fig. 2.4. The cyclohexane molecule (C6H12). The principal symmetry element is the 3-fold axis of rotation C3. The molecule also has a center of inversion, three mirror planes and, perpendicular to the main axis, three 2-fold rotation axes at 120 ° to one another. The point group is denoted by D3 d (Table 2.2)

26

2 Structure of Solid Matter

course, rotation by 360 ° which inevitably leads to the same structure. The number of intermediate rotations that also result in indistinguishable arrangements is called ``the order'' of the rotation axis. Thus one can have 2-, 3-, 4- and 6-fold rotation axes, corresponding to invariance under rotations of 180 °, 120 °, 90 °, and 60 °. For single molecules it is also possible to have 5-fold, 7-fold, etc., axes. Small solid aggregates (clusters) may also display 5-fold rotational symmetry. An example is the particularly stable icosohedron composed of 13 atoms. Icosohedra are formed in the rapid quenching of melts. The solid which is thus formed has a quasi crystalline structure and produces sharp X-ray diraction spots that reflect the local 5-fold symmetry [2.1]. For strictly periodic crystals, however, only 2-, 3-, 4- and 6-fold rotation axes are possible. All other orders of rotation are incompatible with the required translational symmetry. The notation describing the possible axes of rotation is given simply by the numbers 2, 3, 4 and 6. The cyclohexane molecule shown in Fig. 2.4 has a 3-fold rotation axis. A molecule with a 6-fold axis is benzene (C6H6), whose carbon skeleton consists of a planar regular hexagon. Rotation-Inversion Axes Rotation with simultaneous inversion can be combined to give a new symmetry element ± the rotation-inversion axis. It is symbolized by 2, 3, 4, or 6. Figure 2.5 illustrates a 3-fold rotation-inversion axis. From this it is evident that a 3-fold rotation-inversion axis is equivalent to a 3-fold rotation together with inversion. The 6-fold rotation-inversion axis may alternatively be represented as a 3-fold rotation axis plus a mirror plane.

Fig. 2.5. Representation of a 3-fold rotation-inversion axis. The effect can also be described by the combination of other symmetry elements

2.3 The 32 Crystal Classes (Point Groups)

27

2.3 The 32 Crystal Classes (Point Groups) The symmetry elements discussed in the previous section may be combined with one another in various ways. Conversely, every crystal may be described by a particular combination of point-symmetry elements. To be complete, the description must satisfy a number of conditions. For example, if two successive symmetry operations are applied, the result must be a further symmetry element: A6B = C. Three (or more successive symmetry operations must obey the so-called associativity rule: (A6B )6C = A6 B6C). There is an identity element E, corresponding to no operation or to a rotation about 360 °, such that A6E = A. Furthermore, every symmetry element A possesses an inverse A ±1, which corresponds to the reverse operation, so that A ±16A = E. These properties are the mathematical definition of a group. There are 32 distinct crystallographic point groups. If the translational symmetry is also taken into account then one obtains the 230 possible space groups. Although not necessarily true in general, we should note that for translations A6B = B6A (the property of Abelian groups). The 32 crystallographic point groups are most commonly represented by so-called stereographic projections. These projections were developed by crystallographers in order to obtain a systematic classification of the exposed surfaces of naturally grown crystals. The point at which each surface normal intersects a sphere is marked and then projected onto the plane perpendicular to the highest order symmetry axis. Intersection points above this plane are marked by a full circle, and those on the lower half sphere by an open circle or a cross. Hence, in the systematic representation of the point groups, the highest order axis lies in the center. Stereographic projections of two point groups are shown in Fig. 2.6. A particular point group may be denoted in three dierent ways: 1) by specifying a system of generating symmetry operations; 2) by specifying the international point group symbol; 3) by the SchoÈnflies symbol. The notation based on the generating symmetry operators is common in crystallography, whereas the SchoÈnflies symbols have largely been adopted in group theory and spectroscopy. The SchoÈnflies notation consists of a

Fig. 2.6. Representation in stereographic projection of the symmetry elements of two point groups. The symbols 0, s and n denote 2-, 3-, and 4-fold rotation axes. The full lines are mirror planes. When the outer circle is also drawn as a full line, this indicates that the plane of the drawing is also a mirror plane

28

2 Structure of Solid Matter

Table 2.2. The SchoÈnflies point group symbols

Classification according to rotation axes and principal mirror planes

Symbol

Meaning

Cj Sj Dj

( j = 2, 3, 4, 6) j-fold rotation axis j-fold rotation-inversion axis j two-fold rotation axes ^ to a (j-fold) principal rotation axis 4 three- and 3 two-fold rotation axes as in a tetrahedron 4 three- and 3 four-fold rotation axes as in an octahedron a center of inversion a mirror plane horizontal = perpendicular to the rotation axis vertical = parallel to the main rotation axis diagonal = parallel to the main rotation axis in the plane bisecting the 2-fold rotation axes

T O

Additional symbols for mirror planes

Ci Cs h v d

main symbol that characterizes the axes of rotation (if any) of the system, and a subsidiary symbol that gives the positions of the symmetry planes. The symbols and their meanings are summarized in Table 2.2. As an example, we consider the water molecule, for which the highest order rotation axis is a 2-fold axis. The symmetry planes are vertical, i.e. they lie parallel to the main axis of rotation. The corresponding SchoÈnflies symbol is C2 v . A cube has three 4-fold rotation axes, four 3-fold rotation axes and symmetry planes perpendicular to the 4-fold axes. Its SchoÈnflies symbol is Oh .

2.4 The Significance of Symmetry To the uninitiated, the correct assignment and symbolization of symmetry often seems complicated and confusing. It will thus be useful to give a brief overview of the importance of symmetry in the description of a solid. For this purpose, we base our discussion on quantum mechanics. As we have seen, the water molecule, for example, has two mirror planes. The presence of these two mirror planes must somehow be reflected in all the physical properties of the molecule. When the electronic or vibrational properties of the molecule are described by a Hamiltonian, then this has 2-fold mirror symmetry, i.e., it remains invariant under the corresponding coordinate transformation. This invariance can also be expressed in other ways. An operator r is assigned to the reflection. When r operates on the Hamiltonian H , on an eigenstate w or on R, the result should describe H , w or R in the transformed (mirror image) coordinates. Such operators are represented as matrices. Thus the reflection of coordinates in the yz-plane is represented by the matrix operation

2.4 The Significance of Symmetry

0

1 @ 0 0

0 1 0

10 1 0 1 0 x x 0 A@ y A @ y A : 1 z z

29

2:2

This is a three-dimensional representation. The same operation can also be expressed in terms of three one-dimensional matrices,
1x;
1y;
1z
x; y; z ; each of which acts on only one coordinate component. In this case the three-dimensional representation is known as ``reducible'', whereas the corresponding one-dimensional representation is called ``irreducible'' since it cannot be further simplified. It is easy to see that the irreducible representation of a rotation through 180 ° (a 2-fold rotation axis) is also one-dimensional: for a suitable choice of coordinates, it can be expressed simply by a sign reversal. However, for 3-, 4- and 6-fold rotation axes, except for the case of a 360 ° rotation, the operations always involve two coordinate changes. The irreducible representation is therefore two-dimensional. If the Hamiltonian operator possesses a particular symmetry, for example mirror symmetry, then it makes no dierence whether the reflection operation appears before or after the Hamiltonian operator, i.e., the two operators commute. As is well known from quantum mechanics, such operators have a common set of eigenstates. Thus the possible eigenstates of H can be classified according to their eigenvalues with respect to the symmetry operators. In the case of mirror symmetry and that of a 2-fold rotation axis C2, one has r 2 = 1 and C 22 = 1 and thus the eigenvalues can only be 1: r W W ;

C2 W W ;

rW

C2 W

W ;

2:3

W :

The eigenstates of H may therefore be either symmetric or antisymmetric with respect to these operators. This is often expressed by saying that the eigenstates have even or odd ``parity''. We have already met an example of even and odd parity in our discussion of the chemical bonding between hydrogen atoms (Sect. 1.2). The bonding state was a symmetric combination of atomic wavefunctions and therefore a state of even parity. As seen in this example, the eigenstates W+ and W± belong to distinct eigenvalues of H . The corresponding energy levels are thus nondegenerate. From this we may conclude, for example, that the water molecule can possess only nondegenerate energy states (we ignore here any accidental degeneracy of energy levels or normal mode vibrations). To illustrate the above discussion we will apply these ideas to the normal mode vibrations of the water molecule. Accordingly, the atoms can move symmetrically or antisymmetrically with respect to the two mirror planes of the molecule. For atoms that lie in a mirror plane, antisymmetric motion with respect to the plane implies motion perpendicular to the plane, since only then can reflection reverse the motion. The corresponding sym-

30

2 Structure of Solid Matter

metric vibrations of such atoms must involve motion in the mirror plane. One of the two mirror planes of the H2O molecule is the plane containing the three atoms (Fig. 2.7). The motions that are antisymmetric with respect to this plane are two rotations of the molecule and its translation perpendicular to the plane. The six symmetric modes with motion in the plane of the molecule are two translations, a rotation about an axis perpendicular to the plane, and the three normal mode vibrations (Fig. 2.7). Of these vibrations two are symmetric and one is antisymmetric with respect to the mirror plane perpendicular to the molecular plane. For more complex molecules too, it is possible to perform such a classification of the vibrational modes and/or electronic states. However, the process becomes rather more involved for operators that have two-dimensional irreducible representations, such as C3. If C3 commutes with H , then together with the state W, the state C3 W is also an eigenstate of H . There are now two possibilities: 1) Apart from a numerical factor, which, for suitable normalization can be made equal to 1, the state C3 W is identical to W. Thus, in this case W is totally symmetric with respect to C3 and the operation C3 has a one-dimensional (numerical) representation. The state W is then ± at least with respect to the operation ± nondegenerate. 2) C3 W produces a new, linearly independent state W ', which however, due to the commutivity of C3 and H , must also be an eigenstate of H with the same eigenvalue E. The states W and W ' are thus degenerate. Since the rotation C3 always aects two coordinates, its irreducible representation is a two-dimensional matrix. Every eigenstate of C3 may then be constructed as a linear combination of two functions that

Fig. 2.7. The two symmetric and the antisymmetric vibrations of the water molecule. Together with the three rotations and three translations these give the nine normal modes corresponding to the nine degrees of freedom

2.5 Simple Crystal Structures

31

can be selected to be orthonormal. The energy levels are therefore 2fold degenerate. Such degenerate levels are found for all point groups possessing more than a 2-fold rotation axis. Particularly important in solid state physics are the diamond lattice and the face-centered and body-centered cubic lattices. These belong to the point groups Td and Oh , respectively, the former displaying tetrahedral and the latter octahedral symmetry (Figs. 2.8, 10, 12). The representations of such symmetries aect three coordinates and thus Td and Oh have three-dimensional irreducible representations. They are associated accordingly with 3fold degeneracy. We will meet such states when we deal with the normal modes of these lattices (Sect. 4.5) and their electron states (Sect. 7.4). Besides symmetry-determined degeneracy, one also finds degeneracy that results from the specific form of H . The degeneracy associated with the angular momentum quantum number l of the hydrogen atom is well known to be a result of the 1/r potential, whereas the degeneracy with respect to the magnetic quantum number m stems from symmetry. The crystal symmetry also determines the number of independent components of the tensors describing macroscopic material properties. We note here for later use that second-rank tensors, such as the thermal expansion or susceptibility, have only one independent component in cubic crystals, and two in hexagonal crystals. The symmetry of the fourth rank elastic tensor is discussed in Sect. 4.5.

2.5 Simple Crystal Structures The Face-Centered Cubic Structure The simplest crystal structures are those in which each point of the lattice is occupied by one atom. In this case, the face-centered cubic lattice produces a face-centered cubic crystal. Each atom in this structure is surrounded by 12 nearest neighbors. The number of nearest neighbors in a particular structure type is known as the coordination number. The coordination number 12 represents the highest possible packing density for spheres. In a single plane of close-packed spheres the number of nearest neighbors is 6. In three dimensions there are an additional 3 nearest neighbors in each of the planes below and above. If the lattice constant of the face-centered structure is by a, then the separation of nearest pdenoted neighbors is given by a/ 2 as is readily seen from Fig. 2.8. The closestpacked planes are sketched in Fig. 2.8 b. They lie perpendicular to the main diagonal of the cube. If one moves away from a particular close-packed plane along the main diagonal, another identical plane is reached only after passing through two dierently positioned close-packed planes. This packing sequence is illustrated more clearly by Fig. 2.9. A close-packed layer has two sorts of hollow sites (visible in layer A). The second layer is obtained by placing further spheres on one of the two possible sites, and the third-

32

2 Structure of Solid Matter

Fig. 2.8 a, b. The face-centered cubic structure showing the primitive rhombohedral unit cell (a). The close-packed planes are illustrated by dotted lines in (b). The number of nearest neighbors (the coordination number) is 12

Fig. 2.9. The close-packed layers of the fcc structure with the stacking sequence ABCABC . . .

layer spheres lie above the other type of site. Thus the face-centered cubic structure is composed of close-packed layers in the stacking sequence ABCABC . . . . Each of these layers alone has hexagonal (6-fold) symmetry; however, stacked above one another in this manner the symmetry is reduced to a 3-fold rotation axis (Fig. 2.9). The face-centered cubic structure therefore has four 3-fold rotation axes as well as a mirror plane perpendicular to the 4-fold axis. It therefore belongs to the point group Oh. The face-centered cubic structure is usually denoted by the abbreviation fcc. Examples of fcc crystals are the metals Cu, Ag, Au, Ni, Pd, Pt and Al. Despite their relatively high melting points these metals are fairly soft. The reason for this is that the close-packed layers are able to slide over one another. This sliding motion occurs in the plastic deformation of these crystals. However, it does not involve an entire layer; it is limited to regions associated with dislocations (Sect. 2.7). Hexagonal Close Packing The hexagonal close-packed (hcp) structure results when close-packed planes are stacked in the sequence ABAB . . . . In contrast to the fcc structure, the

2.5 Simple Crystal Structures

33

smallest possible unit cell now contains two atoms. Thus the main axis of rotation is again 3-fold rather than 6-fold. As can be seen by considering only the layers A and B of Fig. 2.9, there exist three 2-fold rotation axes perpendicular to the 3-fold axis. Furthermore, the close-packed layer also lies in a mirror plane. The point group corresponding to these symmetry elements is D3 h. As with the fcc structure, the coordination number is 12. Important metals that crystallize in the hcp structure include Zn, Cd, Be, Mg, Re, Ru and Os. The Body-Centered Cubic Structure The body-centered cubic (bcc) structure is shown in Fig. 2.10. For this structure the coordination number is only 8. Thus for nondirectional bonding the bcc structure would appear to be less favorable. Nonetheless, all alkali metals as well as Ba, V, Nb, Ta, W, and Mo, are found to crystallize in this structure, and Cr and Fe also possess bcc phases. At first sight this is hard to understand. However, it is important to note that in the bcc structure the 6 next-nearest neighbors are only slightly farther away than the 8 nearest neighbors. Thus, depending on the range and the nature of the wavefunctions contributing to the bonding, the eective coordination number of the bcc structure can be higher than that of the fcc structure. Figure 2.11 shows the probability functions for the positions of the lithium electrons relative to the atomic nucleus. Also shown are the half distances to the nearest (r1), the next-nearest (r2) and the third-nearest (r3) neighbors for the actually occurring bcc structure and for a hypothetical fcc structure with the same nearest-neighbor separation. When the next-nearest neighbors are taken into account, it is easy to see that the bcc structure leads to a greater overlap of wavefunctions and thus an increase in the strength of the chemical bonding. This eect is enhanced by the fact that the p-orbitals in a cubic structure are oriented along the edges of the cube, thereby contributing significantly to the bonding with the next-nearest neighbors. The picture

Fig. 2.10. The body-centered cubic structure with coordination number 8

34

2 Structure of Solid Matter

Fig. 2.11. Absolute square of the radial part of the electron wavefunctions of lithium as a function of distance from the nucleus. For the bcc structure, both the 8 nearest and the 6 next-nearest neighbors lie in a region of relatively high density. Hence for non-directional metallic bond it is possible for the bcc structure to be energetically favorable with respect to fcc. Examples of bcc metals are the alkali metals Li, Na, K, Rb, Cs and Fr. This curve may be compared with Fig. 1.9 which shows the wavefunction amplitude rather than the probability density. The decay at large distances then becomes weaker

changes, however, when d-electrons become involved in the bonding. The dorbitals are directed both along the cube edges and along the diagonals of the faces. Since the d-orbitals are localized relatively strongly on the atoms (Fig. 1.9), they can only contribute to the bonding when they are directed towards the nearest neighbors. The fcc structure enables exactly this, which is the reason why metals with a large number of d-electrons often crystallize in the fcc structure. The Diamond Structure The diamond structure belongs to the crystal class Td . It allows threedimensional covalent bonding (Sect. 1.2) in which every atom is surrounded by four nearest neighbors in a tetrahedral configuration (Fig. 2.12). Thus the coordination number is 4. The diamond structure takes its name from the structure of the carbon atoms in diamond. Other elements that crystallize with the same structure are Si, Ge and a-Sn. The diamond structure can be described as two interpenetrating fcc structures that are displaced relative to one another along the main diagonal. The position of the origin of the 1 1 1 second fcc structure, expressed in termspof the basis vectors, is 4, 4, 4. This leads to a nearest-neighbor distance ofp 3a=4. Since the separation of closepacked layers in the fcc structure is 3a/3, the distance of a central atom from the base of its tedrahedron of neighbors is 14 of the total height of the tetrahedron.

2.5 Simple Crystal Structures

35

Fig. 2.12. The diamond structure. It consists of two interpenetrating fcc structures which are displaced relative to one another by 1/4 of the long diagonal of the cube. This type of structure is typical of the elements of group IV of the periodic table (C, Si, Ge, a-Sn) and also for III±V compounds in which the sites (000) and 14 14 14 are occupied by different types of atom (ZnS-type structure)

The Zinc Blende Structure The zinc blende (ZnS) structure is closely related to the diamond structure, but now the two interpenetrating fcc structures contain dierent atoms. The ZnS structure is found in the most important of the compounds of group III with group V elements. Examples are GaAs, GaP and InSb. The compound ZnS which gives its name to this structure is of course also of the ``zinc blende structure''. The choice of name for this structure is actually slightly unfortunate, since the compound ZnS also crystallizes in a hexagonal phase with the so-called wurtzite structure. This structure, in common with the ZnS type, has tetrahedral coordination; however, the stacking sequence of the close-packed (111) planes is no longer ABCABC . . ., but ABAB . . ., thereby giving it a hexagonal structure. The wurtzite structure is also adopted by other compounds between group II and group VI elements (ZnO, ZnSe, ZnTe, CdS, CdSe). As well as the ordered packing sequences ABAB . . . and ABCABC . . . it is also possible to find mixed forms with random stacking or very long period repeats. The best-known example of these so-called ``polytypes'' is SiC. Ionic Structures Typical ionic structures, exemplified by the CsCl and NaCl structures, have already been introduced in Sect. 1.3 (Fig. 1.6). The CsCl structure is derived from the bcc structure by replacing the ion at the center of the cube by an ion of a dierent element. The NaCl structure is the result of placing one fcc structure within another. The coordination numbers are 8 for the CsCl structure and only 6 for the NaCl structure. As we have seen in Sect. 1.3, for equal ionic separations, the Madelung constant and thus also the ionic energy are greater for the CsCl structure. Although the dierences are relatively small, it is perhaps surprising that the majority of ionic crystals prefer the NaCl structure. The explanation for this is as follows: In most cases, the radius of the cations is much smaller than that of the anion. For example,

36

2 Structure of Solid Matter

rNa 0:98 A ;

rCl 1:81 A :

The cesium ion however is a large cation:

rCs 1:65 A : As the cation becomes smaller, the anions of a CsCl-type structure approach one another and eventually overlap. This occurs at a radius ratio of r +/r ± = 0.732. For still smaller cations the lattice constant could not be further reduced and the Coulomb energy would remain constant. In this case the NaCl-type structure is favored since anion contact does not occur until a radius ratio of r +/r ± = 0.414 is reached. Yet smaller radius ratios are possible for the ZnS-type structure. Indeed, for ZnS itself, the ratio is r +/r ± = 0.40. This can be regarded as the reason why ZnS does not crystallize in the NaCl structure. This is a somewhat simplified view as it neglects the strong covalent contribution to the bonding (see also Problem 1.2).

2.6 Phase Diagrams of Alloys Modern functional materials consist of many elements in dierent phases. The term phase denotes a domain of homogeneous concentration and structure on a length scale that is large compared to atomic dimensions. Separate phases can be observed even with simple binary alloys. Figure 2.13 displays the scanning electron microscope image of the polished surface of an Ag/Cu alloy. The dark and light sections represent copper- and silver-rich fcc-phases, respectively. As a rule, the various constituting phases of modern composite materials are not in thermal equilibrium. Nonetheless,

Fig. 2.13. Scanning electron microscope image of a polished specimen of an Ag/Cu alloy with 30% Agand 70% Cu-atoms. The dark and light areas consist of fcc-phases with about 95% Cu-atoms and about 86% Ag-atoms, respectively

2.6 Phase Diagrams of Alloys

37

the equilibrium properties are basic to the understanding. Equilibrium properties are described with the help of phase diagrams. In a phase diagram, the temperature is plotted vs. the concentration of one component (at the expense of another). For a particular temperature and composition, the material possesses a particular equilibrium structure. The boundaries between dierent structures are marked by lines. In the simplest case the lines describe the boundary between the solid and the liquid state. Phase diagrams for all important alloys have been determined experimentally by thermodynamic measurements [2.2]. In the following, we consider only the simple phase diagrams of substitutional binary alloys. A substitutional alloy consists of two types of atoms A and B, which as pure materials crystallize in the same structure. If in addition the chemical bonding is similar and the lattice constants of the pure phases are not too dierent, atoms A and B will assume the same lattice sites in the composite system. A number of different states exist even in this simple case: the liquid state with a complete mixture of the two components, a mixture of liquid phase and a solid phase in which atoms of either type A or B are enriched, a solid phase with micro-crystals in which either A or B are enriched, or a continuously miscible solid phase. Alloys that are continuously miscible in the solid phase have the simplest phase diagrams. The SiGe alloy is an example. Its phase diagram is displayed in Fig. 2.14. Depending on the temperature and the relative Si-concentration, the alloy exists either as a homogeneous liquid (` for liquidus), as a homogeneous solid (s for solidus) or as a two-phase

Fig. 2.14. Phase diagram for the continuously miscible alloy Ge/Si. In the range bounded by the liquidus and solidus curves a Ge-rich liquid phase coexists with a Si-rich solid phase

38

2 Structure of Solid Matter

system with liquid and solid parts (`+s). The realms of existence are marked by the so-called liquidus and solidus lines. Another substitutional alloy is AgCu. Here, the phase diagram is much more complex (Fig. 2.15). The reason is that the solid phase of AgCu is not completely miscible. Cu is soluble in Ag only up to a particular percentage that depends on the temperature (-phase, left side of Fig. 2.15). Likewise is Ag in Cu only soluble up to a temperature-dependent percentage (b-phase, right side of Fig. 2.15). In the intermediate range in the so-called miscibility gap the solid phase consists of microcrystalline domains of an Ag-rich -phase and a Cu-rich bphase (see Fig. 2.13). In real systems, the size and shape of the microcrystals are nearly always determined by kinetics rather than by thermodynamic equilibrium. A defined equilibrium size of the crystallites nevertheless exists. It is determined by the minimum of the interfacial energy between the dierent crystallites and the elastic strain energy due to the mismatch of the lattice constants between the crystals of dierent composition. The strain energy decreases as the crystal size becomes smaller. On the other hand the interfacial area and thus the interfacial energy increases so that one has a minimum of the total energy for a particular crystal size. In the course of this section we want to come to an understanding of the origin of the dierent phase diagrams of the two substitutional alloys SiGe and AgCu based on thermodynamic reasoning. As seen above, the crucial dierence between the two systems is the possibility, respectively impossibility of a continuous mixture in the solid phase. Our thermody-

Fig. 2.15. Phase diagram for the binary alloy Ag/Cu. The system is not continuously miscible in the solid phase. Rather the alloy has a wide miscibility gap in which a Ag-rich fcc-phase (a-phase) co-exists with a Cu-rich fcc-phase (b-phase) (see Fig. 2.13)

2.6 Phase Diagrams of Alloys

39

namic considerations therefore focus on the free enthalpy associated with a mixture. The free enthalpy of a system G is a linear combination comprising of the internal energy U, the entropy S and mechanical (or other) work. In the simple case of a homogeneous, liquid or gaseous matter G is GU

TS pV ;

2:4

in which T is the temperature, p the pressure and V the volume. In addition to the work against the external pressure one needs to consider the mechanical work associated with the internal degrees of freedom of the system (see discussion above). This part is rather dicult to deal with (see also Sect. 4.5). Fortunately, the contributions of energy and entropy of mixture prevail. We therefore consider only those two contributions in the following and neglect contributions of mechanical, electrical or magnetic work. In a first step we likewise neglect thermal contributions. One further approximation is needed for the purpose of calculating the energy and entropy of mixture: this is that we admit only homogeneously mixed phases, that is we exclude spatial and temporal fluctuations. This corresponds to a mean field approximation, an approximation that we encounter quite frequently in the theory of solid matter. In the present context, the approximation is also known as the Bragg±Williams approximation. The variation in the enthalpy associated with mixing Gmix consists of a variation of the internal energy Umix, which is the heat of solution, and the variation of the entropy due to mixing Smix Gmix Umix

T Smix :

2:5

In a first step we calculate the variation of the internal energy under the assumption that the binding energies of the involved atoms can be represented by nearest neighbor pair interactions. This simple ansatz does not conform with reality but must suce here. We denote the number of atoms of type A and B as NA and NB, and the number of nearest-neighbor bonds between atoms of type A, of type B, and between atoms A and B as NAA , NBB, and NAB, respectively. Correspondingly, the binding energies of the atom pairs AA, BB and AB are denoted as VAA , VBB and VAB. The coordination numbers (number of nearest-neighbors) in the two structures of interest here, the diamond structure (Si, Ge) and the fcc-structure of Ag and Cu, are z = 4 and z = 12, respectively. The variation of the energy due to mixing Umix is Umix

NAA VAA NBB VBB NAB VAB 1
z NA VAA z NB VBB : 2

2:6

The sum of the first three terms is the energy after mixing and the sum of the last two terms is the energy before mixing. The factor 1/2 occurs because there are z/2 bonds per atom. Note that the definitions of binding energy and internal energy imply an opposite sign: a higher binding energy

40

2 Structure of Solid Matter

corresponds to a lower internal energy! The numbers of atom pairs NAA, NBB and NAB can be expressed in terms of the concentrations xA NA =N xB NB =N with

2:7

N NA NB and one obtains NAA NA xA z=2 N x2A z=2 NBB NB xB z=2 N x2B z=2

2:8

NAB NA xB z=2 N xA xB z=2 : With that the energy of mixing Umix becomes Umix N z xA xB WAB

2:9

with 1 WAB
VAA VBB 2

VAB :

2:10

If WAB < 0 then the alloy has a higher binding energy and the internal energy of the alloy is lower than the sum of the internal energy of the constituents. Since xA+xB = 1 the energy of mixing has the form of a parabola. Umix N z xA
1

xA WAB :

2:11

Associated with a mixing of two components is always an enlargement of the entropy. This is because microscopically a mixture can be realized in many dierent ways. The dierent microscopic realizations originate from the exchange of atoms A with atoms B. The number of possibilities for an exchange of all atoms N = NA+NB is N!. The exchange of atoms A and B among themselves, however, does not constitute a discernibly dierent microscopic state. The number of discernible states is thus N!/(NA! NB!). With that the entropy of mixing becomes Smix k ln

N! N! k ln : NA ! NB !
N xA !
N xB !

With Stirling's approximation for large numbers N ln N! N ln N one obtains Smix

N k xB ln xB
1

xB ln
1

2:12 N; N 1

xB :

2:13

The entropy Smix is zero for xB = 0 and xB = 1 and positive for intermediate xB. The free enthalpy of mixing is Gmix Umix T Smix Nfz xB
1 xB WAB k T xB ln xB
1 xB ln
1 xB g :

2:14

2.6 Phase Diagrams of Alloys

41

The function has an extreme at xB = 0.5. Whether it is a minimum or a maximum depends on the ratio of WAB and k T. One has a minimum for z WAB =k T < 0:5 ;

2:15

a maximum for z WAB =k T > 0:5 :

2:16

Examples for zWAB/k T = 0.5, 2.5 and 3 are displayed in Fig. 2.16. For negative values of WAB the free enthalpy of mixing is always smaller than the sum of the free enthalpies of the separate components. In that case the alloy is continuously miscible. The same holds for any system, only if the temperature is high enough (2.14). The system becomes unstable if the free enthalpy has a maximum at xB = 0.5. It decomposes into two separate phases, one with a concentration of the B-component x0B < 1=2 and the other one with x00B > 1=2. This is independent of the sign of the free enthalpy of mixing. For the special case when Gmix(xB) is symmetric around xB = 1/2 (Fig. 2.16) it is easy to see that the instability exists not only at xB = 1/2 but in the entire range between the two minima of Gmix(xB). Figure 2.17 displays the more general case of an asymmetric shape of Gmix(xB). The two concentrations x0B and x00B of the two phases into which the system separates are determined by the condition that the system as a hole must remain in equilibrium, that is, the chemical potentials of the two phases must be equal. The chemical potentials of the atoms of type B in the two phases are

Fig. 2.16. The free enthalpy of a solid mixture according to a simple model (2.14). The solid line corresponds to the limiting case in which an intermediate maximum is not yet present. If an intermediate maximum occurs, the system is unstable against phase separation into two phases, one depleted of NB atoms and one enriched with NB atoms. Phase separation occurs independent of whether the enthalpy of mixing is gained in the alloying process (dotted line) or not (dashed line for concentrations around 0.5)

42

2 Structure of Solid Matter

l 0B l 00B

@G0 1 @ G0 @ NB N @ xB 00

2:17

00

@G 1 @G : @ NB N @ xB

Hence the system decomposes into two phases for which the slope of the free enthalpy (Fig. 2.17) is equal. Of all (the infinite number of) points on the curve G(xB) that fulfil the condition of an equal slope the total free enthalpy is minimal for the particular pair of concentrations x0B and x00B through which a common tangent to G(xB) can be drawn. This common tangent condition uniquely determines the two concentrations and x0B and x00B . A few simple geometrical considerations demonstrate that the system indeed separates into two phases with concentrations x0B and x00B , and that an alloy is unstable in the entire concentration range between x0B and x00B . Consider an arbitrary intermediate concentration xB0. Conservation of mass during the process of phase separation requires that the numbers of Batoms in the two phases N0B N0 x0B and N00B N00 x00B obey the relation N 0 x 0B N 00 x 00B
N 0 N 00 xB0 :

2:18

The ratio of the total number of atoms in the two phases becomes therefore equal to the ratio of the concentration dierences N0 x 00B N 00 xB0

xB0 : x 0B

2:19

Fig. 2.17. Free enthalpy of an alloy with an intermediate maximum and two minima of a different depth. The system is unstable in the concentration range between the two points of tangency at x0B and x00B , and the system separates into two phases with the concentrations x0B and x00B . The free enthalpy of the two-phase system is described by the common tangent

2.6 Phase Diagrams of Alloys

43

A corresponding relation holds for the component A. This simple relation resembles the lever principle in mechanics and is therefore known as the lever rule of phase diagrams. It holds for any phase separation, regardless of its nature. After phase separation the free enthalpy of the system becomes G
x 0B ; x 00B G
x 0B N 0 =N G
x 00B N 00 =N :

2:20

By substituting (2.20) into (2.19) and after a suitable rearrangement the enthalpy can be written as G
x 0B ; x 00B G
x 0B G
x 00B

G
x 0B

xB0 x 00B

x 0B ; x 0B

2:21

which is precisely the equation describing the y-coordinate in x0 of the common tangent. Thus, the common tangent is simply the free enthalpy after phase separation. Between x0B and x00B all values of the common tangent are below the free enthalpy of the system before phase separation (Fig. 2.17). The system is therefore unstable with respect to phase separation in the entire gap between x0B and x00B . In the context of binary alloys this gap is known as the miscibility gap. As can be seen from the phase diagram (Fig. 2.15) a miscibility gap does exist for the Ag/Cu alloy. If a melt of 40 atom% silver and 60 atom% copper is cooled below the temperature of solidification, the solid crystallizes in the b-phase containing about 95% Cu. The remaining melt becomes enriched with Ag, until the Cu-rich -phase (95.1% Cu) and the silver-rich b-phase (85.9% Ag) solidify together at the so-called eutectic point, which corresponds to 39.9% Cu in the melt at a temperature of 779 8C. Upon further cooling the concentrations of the two solid phases should continue to vary in principle (Fig. 2.15). However, the equilibrium state can be achieved only for an extremely low cooling rate because of the low diusivity of atoms in the solid phase. The concentrations in the darker and lighter areas in Fig. 2.15 therefore practically correspond to the equilibrium concentrations of the - and b-phase at the eutectic point. Thermodynamic reasoning can also be applied to the phase transition between the liquid and the solid phase in the case of a completely miscible alloy. Consider the free enthalpy of such a system in the liquid and solid phases (Fig. 2.18). The system is completely miscible since the free enthalpy is now represented by a function with a positive curvature in the entire concentration range. Liquid and solid phases coexist if the minima of the free enthalpies for the liquid and the solid state occur at dierent concentrations which is generally the case. The curves in Fig. 2.19 approximately represent the system Ge/Si. We consider first a high temperature T > 1412 8C. There, the free enthalpy of the melt is below that of the solid for all concentrations. This is because of the entropic contribution to the free enthalpy. At high temperatures, the entropy of the liquid phase is higher than that of the solid phase. The reason is that a liquid has more states of low quantum energy

44

2 Structure of Solid Matter

Fig. 2.18. Free enthalpy of the solid and liquid phase of a completely miscible alloy in the temperature range between the liquidus and solidus curves (schematic)

Fig. 2.19. Free enthalpies for the system Ge/Si at different temperatures as a function of the Si-concentration xSi (schematic)

than a solid. Simply speaking, the degrees of freedom of the transverse sound waves of the solid become free translations in the melt. At a temperature of 1412 8C the free enthalpies of the melt and the solid become equal for the concentration xSi = 1. Melt and the solid coexist: we have reached the melting point of pure silicon. For even lower temperatures, e.g. at 1150 8C, one has, according to the common tangent construction, a coexistence of a Si-depleted, liquid phase with a Si-enriched solid phase. Below 940 8C finally, only the solid phase exists for all mixing ratios. If the cooling process is performed using a melt with a mixing ratio of 50 atom% Ge and 50 atom% Si, e.g., crystallites with 80% Si will solidify first at a temperature of about 1270 8C. In the temperature range between the liquidus and solidus curve the equilibrium concentrations of Si in the

2.7 Defects in Solids

45

liquid and the solid state are given by the corresponding values for the concentrations of the liquidus and solidus curves. The ratio of the atom numbers in the two phases obey the lever rule (2.19). With decreasing temperature the solidified fraction of the melt increases, and the Si-concentration in the crystalline phase decreases. It is therefore not possible for continuously miscible alloys to grow a crystal out of a melt that has a homogeneous concentration ratio, unless one confines the crystallization to a small fraction of the melt. One can utilize, however, the dierent equilibrium concentrations in the melt and the solid to purify a crystal of undesirable impurities. This is the basis of purification by zone melting: One begins by melting a narrow zone of a crystal rod at one end. In this molten zone the impurity concentration necessarily is as it was in the solid. Then, the molten zone is slowly pulled over the rod. If the liquidus and solidus curves are as in Fig. 2.14 with regard to an impurity (with Si as the base material and Ge as an impurity) then the re-crystallized rod in the cooling zone has a lower concentration of impurities than the (respective) melt. Hence, the impurities are enriched at that end of the rod that is molten last. A large section of the crystal can very eectively be purged of impurities by repeating the process many times.

2.7 Defects in Solids Mechanical and electrical properties of solids are largely controlled by defects in the periodic structure. This section briefly reviews various known defects. In the previous section we have already learned about a special defect: In a diluted substitutional alloy, minority atoms may assume the sites of the majority atoms. In the context of semiconductors replacing majority atoms by atoms of another kind, preferably by atoms of a higher or lower valence is known as ``doping''. Doping varies the electrical conductivity of a semiconductor by many orders of magnitude (see Sect. 12.3). Defects consisting only of one or a few atoms, as in the case of doping, are known as point defects. Point defects do not necessarily involve foreign atoms. The so-called Frenkel defect consists of an atom displaced from its regular site to an interstitial site. The atom in the interstitial site and the vacancy in the regular site together are named ``Frenkel pair''. Since the bond energy of the atom is lower at the interstitial site the formation of a Frenkel pair requires energy. Nevertheless, Frenkel pairs do exist in equilibrium at higher temperatures because the formation of a Frenkel pair increases the entropy. That increase arises from the fact that the atom as well as the vacancy may sit in any possible interstitial or lattice site, respectively, thereby enjoying many distinguishable microscopic realizations. The number of possibilities to distribute nv vacancies on N regular atom sites is N!/[nv!(N±nv)!]. Similarly, the number of possibilities to

46

2 Structure of Solid Matter

distribute nint interstitial atoms on N' interstitial sites is N0 !=nint !
N0 nint !. For a Frenkel pair the number of interstitial atoms nint necessarily equals the number of vacancies nv . With n = nint = nv one obtains for the entropy S (comp. 2.12) S k ln

N! N0 ! k ln n!
N n! n!
N 0 n!

k N ln NN0 ln N 0
N0

2n ln n

N n ln
N n

2:22

n ln
N 0 n :

In equilibrium the system is in the state of lowest free energy F = n D E ±TS, in which DE is the energy required to create a Frenkel pair. The corresponding equilibrium concentration hni is obtained by dierentiating the free energy with respect to n dF 0 D E k T ln dn
N 0

hni2 hni
N

hni

:

2:23

Since the concentration of defects is small
hni N; N0 hni is approximately p DE=2 k T hni N N 0 e :
2:24 Hence, the concentration rises exponentially with the temperature according to an Arrhenius law. The activation energy in the Arrhenius law is half the energy required for the creation of a Frenkel-pair. The factor of two in the denominator of the exponent arises because vacancies as well as interstitial atoms are distributed independently in the crystal. One therefore has two independent contributions to the entropy. If the atom that is displaced from the regular site diuses to the surface or into an interface (``Schottky defect''), the full energy of creation for the defect appears in the Arrhenius law. The reason is that for a macroscopic solid the number of available sites on the surface or in an interface are infinitely small compared to the number of sites in the bulk. In that case only the vacancies in the regular crystal sites contribute to the entropy. Defects of the next higher dimension are line defects. A common intrinsic line defect is the dislocation. A simple example is shown in Fig. 2.20, which displays a cross section of a crystal with a dislocation. Around the core of the dislocation atoms are displaced from their regular lattice positions because of the elastic stresses. Most of the energy required to create a dislocation is actually in the elastic strain that decays rather slowly as one moves away from the core. Dislocations are described by the Burgers vector. The Burgers vector is constructed by considering the positions of atoms after completing a closed loop of an arbitrary size around the dislocation core for a lattice with and without a dislocation (Fig. 2.20). If the Burgers vector is oriented perpendicular to the dislocation line as in Fig. 2.20, the

2.7 Defects in Solids

47

b A

B

Fig. 2.20. Sectional drawing of a crystal with an edge dislocation (schematic). The dashed line represents a loop around the core of the dislocation. The loop begins with atom A. It would close at atom B if the dislocation were not present. The Burgers vector b points from atom A to atom B. The same Burgers vector is obtained for any arbitrary loop that encloses the dislocation

dislocation is called an ``edge dislocation''. If the Burgers vector is oriented along the dislocation line, then the dislocation is called a ``screw dislocation'', since by moving along a closed loop around the dislocation one climbs from one lattice plane onto the next. Edge dislocations and screw dislocations represent two limiting cases of a general, intermediate form of a dislocation. Furthermore, the angle between the orientation of the Burgers vector and the dislocation line may vary as one moves along the dislocation line. The modulus of the Burgers vector is equal to the distance of an atom plane for the common screw or edge dislocations. However, dislocations for which the modulus of the Burgers vector is only a fraction of a distance between an atom plane also exist. Such a partial dislocation is generated, e.g., if all atoms in a section of an fcc-crystal are displaced along a direction in a densely packed plane so as to produce a stacking fault (Fig. 2.9). Dislocations play a crucial role in plastic deformation of crystalline material. Consider a shear force acting parallel to an atom plane. It is not feasible to make all the atoms glide simultaneously since the shear force works against the atomic bonds of all atoms in the glide plane at once. A step wise glide is energetically much more favorable. Firstly an edge dislocation is generated at the surface and then the dislocation is shifted through the crystal. Then gliding is eectuated by displacing the atoms row-by-row until the dislocation line has moved through the entire crystal. The required forces are much lower since fewer atoms are aected and bonds need not be broken but must merely be strained and re-oriented. Plastic deformations of a crystalline solid are therefore connected with the generation and wandering of dislocations. In a pure, ideally crystalline material dislocations can move easily, provided the temperature is not too low. For many metals,

48

2 Structure of Solid Matter

e.g., room temperature suces. Such materials have little resistance to plastic deformation. Examples are rods or wires consisting of annealed copper and silver. If the material is polycrystalline, e.g., after cold working, then the wandering of dislocations is hindered by the grain boundaries between the crystallites, and the material resists plastic deformation more eectively.

Problems 2.1 The phase transition from graphite to diamond requires high pressure and high temperature in order to shift the equilibrium in favor of diamond and also to overcome the large activation barrier. Suggest a method of producing diamond (layers) without the use of high pressure. 2.2 Below 910 °C iron exists in the bcc structure (a-Fe). Between 910 °C and 1390 °C it adopts the fcc structure (c-Fe). Assuming spherical atoms, determine the shape and size of the octahedral interstitial sites in c-Fe (a = 3.64 AÊ) and in a-Fe (a = 2.87 AÊ). Sketch the lattices and the interstitial sites. For which phase would you expect the solubility of carbon to be higher? (Hint: The covalent radius of carbon is 0.77 AÊ.) When molten iron containing a small amount of carbon (91%) is cooled, it separates into a more-or-less ordered phase containing a-Fe with a small concentration of carbon atoms on interstitial sites (ferrite) and a phase containing iron carbide (cementite, Fe3C). Why does this occur? Why does cementite strengthen the medium against plastic deformation? (Hint: Fe3C, like many carbides, is very hard and brittle.) 2.3 Copper and gold form a continuous solid solution with the copper and gold atoms statistically distributed on the sites of an fcc lattice. For what relative concentrations of copper and gold atoms do you expect ordered alloys and what would they look like? Draw the unit cells of these alloys and identify the corresponding Bravais lattices. Can you suggest an experiment which would determine whether the alloy is ordered or not? 2.4 Draw and describe the symmetry elements of all Bravais lattices. 2.5 Draw the primitive unit cell of the fcc lattice and determine the lengths of the primitive lattice vectors a ', b ', c ' (in units of the conventional lattice constant a ) and also the angles a ', b', c' between the primitive lattice vectors. (Hint: Express the primitive lattice vectors as a linear combination of the lattice vectors a, b, c of the face-centered cubic lattice and use elementary vector algebra.) What distinguishes this unit cell from that of the rhombic Bravais lattice?

Problems

49

2.6 Determine the ratio of the lattice constants c and a for a hexagonal close packed crystal structure and compare this with the values of c/a found for the following elements, all of which crystallize in the hcp structure: He (c/a =1.633), Mg (1.623), Ti (1.586), Zn (1.861). What might explain the deviation from the ideal value? 2.7 Supposing the atoms to be rigid spheres, what fraction of space is filled by atoms in the primitive cubic, fcc, hcp, bcc, and diamond lattices? 2.8 Give a two-dimensional matrix representation of a 2-, 3-, 4-, and 6-fold rotation. Which representation is reducible? 2.9 Show that the rhombohedral translation lattice in Fig. 2.3 is equivalent to a hexagonal lattice with two atoms on the main diagonal at a height of c/3 and 2 c/3. Hint: Consider the projection of a rhombohedral translation lattice along the main diagonal into the plane perpendicular to this main diagonal. The main diagonal of the rhombohedral lattice is parallel to the c-axis of the hexagonal lattice. How are the a and the c axis of the corresponding hexagonal lattice related to the angle a = b = c and the length a = b = c of the rhombohedral lattice? 2.10 Take a piece of copper wire and anneal it by using a torch! Demonstrate that the wire is easily plastically deformed. Then pull the wire hard and suddenly or work it cold using a hammer. How is the plastic behavior now? Explain the observations!

3 Diraction from Periodic Structures

A direct imaging of atomic structures is nowadays possible using the highresolution electron microscope, the field ion microscope, or the tunneling microscope. Nonetheless, when one wishes to determine an unknown structure, or make exact measurements of structural parameters, it is necessary to rely on diraction experiments. The greater information content of such measurements lies in the fact that the diraction process is optimally sensitive to the periodic nature of the solid's atomic structure. Direct imaging techniques, on the other hand, are ideal for investigating point defects, dislocations, and steps, and are also used to study surfaces and interfaces. In other words, they are particularly useful for studying features that represent a disruption of the periodicity. For performing diraction experiments one can make use of X-rays, electrons, neutrons and atoms. These various probes dier widely with respect to their elastic and inelastic interaction with the solid, and hence their areas of application are also dierent. Atoms whose particle waves have a suitable wavelength for diraction experiments do not penetrate into the solid and are thus suitable for studying surfaces. The same applies, to a lesser extent, to electrons. Another important quantity which diers significantly for the various probes is the spatial extent of the scattering centers. Neutrons, for example, scatter from the nuclei of the solid's atoms, whereas X-ray photons and electrons are scattered by the much larger (*104 times) electron shells. Despite this and other dierences, which will be treated in more detail in Sect. 3.7, it is possible to describe the essential features of diffraction in terms of a single general theory. Such a theory is not able, of course, to include dierences that arise from the polarization or spin polarization of the probes. The theory described in Sect. 3.1 below is quasi classical since the scattering itself is treated classically. The quantum mechanical aspects are treated purely by describing the probe particles as waves. For more detailed treatments including features specific to the various types of radiation, the reader is referred to [3.1±3.3].

3.1 General Theory of Diraction In our mathematical description of diraction we will make the assumption of single scattering: the incoming wave induces the emission of spherical H. Ibach, H. LuÈth, Solid-State Physics, 4th ed., DOI 10.1007/978-3-540-93804-0_3, Ó Springer-Verlag Berlin Heidelberg 2009

52

3 Diraction from Periodic Structures

waves at all points r of the target material. A fixed phase relationship is assumed between the primary wave and each of the emitted spherical waves (coherent scattering). Further scattering of the spherical waves, however, is neglected. This is also known as the ``kinematic'' approximation and corresponds to the first Born approximation of the quantum mechanical scattering theory. The approximation is valid for neutrons and X-rays, and within certain limits also for the scattering of high energy electrons. For highly perfect single crystals, it is possible to observe ``nonkinematic'' (``dynamical'') eects in the scattering of X-rays. For the derivation of the scattering amplitudes we make use of Fig. 3.1. Here Q is the location of the source of radiation, P is the position of the scattering center, and B the point of observation. As an example of a source we shall take the spherical light waves emitted in conjunction with an electronic transition in an atom. At suciently large distances from the source the spherical waves can be approximated as plane waves. The amplitude (or for X-rays more accurately the field strength vector) at position P and time t may thus be written AP A0 ei k0
Rr

i x0 t

:

3:1

If we follow this wave back to the source Q (R + r = 0), then its amplitude here as a function of time behaves as *exp (±ix0t), i.e., it has a well-defined phase at all times. The reasoning, however, can only be applied to a single emission process. In real light sources photons are emitted with uncorrelated phases from many atoms (an exception to this is the laser). For other types of incident particle the phases are likewise uncorrelated. Thus, when we use expression (3.1), we must keep in mind that the result for the observed intensity arises by averaging over many individual diraction events.

Fig. 3.1. Schematic representation of scattering indicating the parameters used in deriving the scattering kinematics. The source Q is assumed to be sufficiently far away from the target that the spherical waves reaching the target can be well approximated by plane waves. The same condition is assumed for the point of observation relative to the scattering centers

3.1 General Theory of Diffraction

53

The relative phases of the wave at points P at time t are given by the position-dependent factor in (3.1). We now allow the primary wave to be scattered by the material. Every point P in the scattering material is caused by the primary wave to emit spherical waves, whose amplitude and phase relative to the incident (primary) wave are described by a complex scattering density R
r. The time dependence of these spherical waves is determined by the time dependence in (3.1) (forced oscillation). The spherical waves observed at B are therefore described by 0

AB AP
r; t R
r

ei k j R rj : jR 0 rj

3:2

For a fixed position P, the wave vector k is in the direction R '± r. Thus we can also write 0

AB AP
r; t R
r

ei k
R r : jR 0 rj

3:3

At large distances from the scattering center AB is then given by AB AP
r; t R
r

1 i k
R 0 e R0

r

3:4

where k now has the same direction for all positions P in the target material. Inserting (3.1) into (3.4) we obtain AB

A0 i
k0 Rk R 0 e e R0

i x0 t

R
r ei
k0

k r

:

3:5

The total scattering amplitude is given by integration over the entire scattering region:
3:6 AB
t / e i x0 t R
r ei
k0 k r dr : For scattering from a rigid lattice, R
r is time independent and the time dependence of AB only contains the frequency x0. In the quantum mechanical picture this corresponds to energy conservation. We thus have elastic scattering. This form of scattering is important for structural analyses. If instead we allow the scattering density R
r to vary with time, then we also obtain scattered waves with x = x0 . This inelastic scattering will be dealt with in Sect. 4.4. In diraction experiments for structure determination, it is not the amplitude but the intensity of the scattered waves that is measured: I
K / jAB j2 / j R
r e i K r dr j2 :
3:7 In this equation we have introduced the scattering vector K = k± k0. We see that the intensity is the absolute square of the Fourier transform of the scattering density R
r with respect to the scattering vector K. From this we establish an important fact: The smaller the structures to be resolved in the diraction measurement, the larger is the required value of K, and thus

54

3 Diraction from Periodic Structures

also of the k-vector of the incident radiation. In studies of the atomic structures of solids the wavelengths should thus roughly correspond to the lattice constants. For such waves it is impossible to measure their amplitude as a function of position and time ± only the intensity can be measured. This leads to considerable complications in structural analysis. If it were actually possible to measure the amplitude instead of the intensity, then one could make use of inverse Fourier transformation to obtain the spatial distribution of the scattering density directly from the diraction pattern. However, since in reality one can only observe the intensities, the information about the phases is lost and the scattering density cannot be calculated directly. To determine a particular structure it is therefore necessary to do the calculation in reverse: One chooses a feasible model structure, calculates the diraction pattern that it would produce, and then compares this with the experimentally observed diraction pattern. The structural parameters of the model are varied until optimal agreement with experiment is found. The analysis of unknown structures is facilitated by invoking the socalled Patterson function, which is the Fourier transform of the intensity. In order to elucidate the meaning of the Patterson function we rewrite (3.7) for the intensity 0 I
K / R
r e i K r dr R
r 0 ei K r dr 0 :
3:8 Since both integrals extend over the entire space the variable r' in the second integral can be replaced by r + r'. Hence, one obtains 0 I
K / ei K r dr 0 R
rR
r 0 r dr :
3:9 The auto-correlation function of the scattering density P
r 0 R
r R
r 0 rdr

3:10

is the Patterson function. The function has its peaks where r' corresponds to a vector between two atoms of the crystal structure. A peak is particularly strong if the vector connects two atoms with a large scattering cross section. The interatomic distances in an unknown structure are therefore easily obtained by inspection of the Patterson function. Scattering from disordered systems, i.e. liquids and amorphous solids is most suitably described with the help of the Patterson function P(r'). We decompose the scattering density R(r) into contributions from individual atoms. For simplicity we assume that the material is made up of a single type of atoms. The scattering density centered at the position ri is denoted as Rat(r±ri). X R
r Rat
r ri :
3:11 i

The Patterson-function P(r') can be split into two contributions: one describing the correlation of one atom with itself and the other one describing the correlation of an atom with all other atoms.

3.1 General Theory of Diffraction

P
r0

X

Rat
r

ri Rat
r

rj r0 dr

Rat
r

ri Rat
r

ri r0 dr

i; j

X i

X

X

Rat
r

55

ri

i

Rat
r

rj r0 dr :

3:12

j6i

The second term in (3.12) contains the information on the structure. We assume now that the scattering density is localized at the centers of the atoms. This assumption is particularly well fulfilled for neutron scattering (see also Sect. 3.7 and I.3). In that case, the first integral in (3.12) contributes only at r0 0. The integral can therefore be replaced by f 2 d0 ;r0 where d0;r0 denotes the Kronecker symbol and f the ``atom factor'', which is a measure of the magnitude of the scattering amplitude of an atom. The sum over all (identical) atoms i in the first term can be replaced by a multiplication with the number of atoms N. The second integral in (3.12) vanishes for r 0 0 since the probability to have a second atom j at the position of any other atom i is zero. We assume the system to be disordered, but homogeneous on a coarse scale. Because of the disorder, the mean scattering density around each atom is identical and independent of angle. Thus, the mean value of the sum X R
r Rat
r rj j6i

depends only on the distance r from the atom whose environment is being considered. The Patterson function is then P
r 0 Nf 2 d0;r 0 N R
rR
r r0 dr :
3:13 It is useful to introduce a function g
r0 that is a measure of the pair correlation of atoms, independent of their scattering amplitude and density. The limiting value of g
r0 for r0 ! 1 is one. For large distances away from any particular atom considered the scattering density is lim R
r r0 Nf=V with V the volume. We therefore define the function 0

r !1 0

g
r by N 2 f g
r 0 R
r R
r r 0 dr : V

3:14

After inserting (3.14) and (3.13) in (3.9) one obtains for the scattering intensity I(K) N I
K / S
K 1
3:15 g
r e i K r d r : V S
K is known as the structure factor. The pair correlation function g(r) can be calculated from the Fourier transform of S
K 1. Here, however, one

56

3 Diraction from Periodic Structures

Fig. 3.2. Pair correlation function for amorphous silicon and liquid iron at a temperature of T = 1833 K [3.4, 3.5]. The distances of the nearest, next-nearest, and third nearestneighbors for crystalline silicon are marked as r1(Si), r2(Si) and r3(Si), the corresponding distances for crystalline iron (fcc structure) as r1(Fe) and r2(Fe)

encounters a technical diculty: The contribution to g
r that arises from the homogeneous part of the scattering density at large r leads to a forward scattering at K 0. This contribution cannot be separated from the primary beam. One therefore extracts a function h
r g
r 1 from the experimental data that does not include the forward scattering. The function h
r is therefore the Fourier transform of the structure factor without the forwardscattering contribution (see Problem 3.7). Figure 3.2 shows two examples for the pair correlation function g
r. The dashed and full lines represent g
r for liquid iron and amorphous silicon, respectively. The first peak corresponds to the distance of nearest-neighbors. The sharpness of the peak indicates that the distance to the nearest-neighbor is well defined even for structurally disordered systems. The mean distances of further neighbors are likewise discernible. Here, we encounter a characteristic dierence between the amorphous state and the liquid state of matter. In the amorphous state, the distance to the next nearest-neighbor is nearly the same as in the crystalline state. The lower density of the amorphous state is reflected only in the distance to the third nearest-neighbor. In liquids, the second peak is approximately at twice the distance of the nearest-neighbor peak, hence at a significantly larger distance than, e.g., in a close-packed solid. This larger distance of second nearest-neighbors is an essential feature of the liquid state. Only with a larger distance of second nearest-neighbors can a liquid state be realized, as is easily demonstrated in a model in which the atoms are represented as hard spheres (see also Problem 3.7b).

3.2 Periodic Structures and the Reciprocal Lattice

57

3.2 Periodic Structures and the Reciprocal Lattice For periodic structures, R
r can be expanded in a Fourier series. We first consider a one-dimensional example in which R
x repeats with period a R
x R
x n a

n 0; 1; 2; ::: :

The corresponding Fourier series then reads X R
x Rn ei
n 2 p=a x :

3:16
3:17

n

It is readily seen that a displacement by an arbitrary lattice vector xm = m a leads to an identical R
x, hence satisfying the required translational invariance. The extension to three dimensions is straightforward and yields X R
r RG ei G r :
3:18 G

The vector G must fulfill certain conditions in order to preserve the translational invariance of R with respect to all lattice vectors r n n1 a1 n2 a2 n3 a3 :

3:19

The conditions are expressed by G rn 2 p m

3:20

where m is an integer for all values of n1, n2, n3. We now decompose G in terms of three as yet undetermined basis vectors gi , G h g1 k g2 l g3

3:21

with integer h, k, l. The condition (3.20) now implies for the example of n2 = n3 = 0
h g1 k g2 l g3 n1 a1 2 p m :

3:22

For an arbitrary choice of n1 this can only be satisfied if g1 a1 2 p

and

g2 a1 g3 a1 0 :

3:23

Expressed in general terms this requirement becomes gi aj 2 p dij :

3:24

The basis set g1, g2, g3 that we have thus defined spans the so-called reciprocal lattice. For every real lattice there is a corresponding and unambiguously defined reciprocal lattice. Its lattice points are denoted by the numbers h, k, l. The rules for constructing this lattice are given directly by (3.24): the reciprocal lattice vector g1 lies perpendicular to the plane containing a2 and a3 and its length is 2 p/a1 [cos E 0F (Fig. 6.5). The spherical form of the Fermi surface E0F (k) at T ? 0 K leads immediately to a simple relationship between the electronic density n and the Fermi radius kF or Fermi energy E0F:

6.2 The Fermi Gas at T = 0 K

141

Fig. 6.5 a±c. Description of the quasi-free valence electrons of a metal at T = 0. (a) f
E is a step function. (b) The concentration n of valence electrons is given by the area under the density of states curve up to the Fermi energy E0F. (c) In k-space the Fermi sphere E (k) = E 0F separates occupied from unoccupied states

nL3 E0F

L3 k3F ; 3p2

6:15

2 h
3p2 n2=3 : 2m

6:16

The magnitude of the Fermi energy can thus be estimated by using the number of valence electrons per atom to determine the electron concentration n. A few values of E0F are listed in Table 6.1. From these we see that at normal temperatures the Fermi energy is always very large compared to k T. To make this more obvious one can define a Fermi temperature TF = E0F/k ; this temperature lies about two orders of magnitude above the melting point of the metals.

Table 6.1. Fermi energy E0F, radius of the Fermi sphere in k-space k F, Fermi velocity v F = h kF/m, and Fermi temperature TF = E0F/k for a few typical metals. n is the concentration of conduction electrons deduced from the structural data of the elements [6.2]. It should be noted that the electron configuration of Cu, Ag and Au is 3d 10 4s 1 and so every atom contributes one free electron (Fig. 7.12). The characteristic radius rs is also often used in this context. It is defined via the volume of a hypothetical sphere containing ±1 one electron, 4 pr 3s/3 = a ±3 0 n , where a0 is the Bohr radius so that rs is dimensionless. Values for rs lie between 2 and 6 for typical metals Metal

n (1022 cm±3)

rs

kF (108 cm±1)

v F (108 cm/s)

E0F (eV)

TF (104 K)

Li Na Cs Al Cu Ag Au

4.62 2.53 0.86 18.07 8.47 5.86 5.9

3.27 3.99 5.71 2.07 2.67 3.02 3.01

1.11 0.91 0.63 1.75 1.36 1.20 1.20

1.29 1.05 0.74 2.03 1.57 1.39 1.39

4.70 3.14 1.53 11.65 7.03 5.50 5.52

5.45 3.64 1.78 13.52 8.16 6.38 6.41

142

6 ``Free'' Electrons in Solids

An interesting consequence of the Pauli exclusion principle is that the Fermi gas, in contrast to a classical gas, has a nonvanishing internal energy at T = 0 K. It is well known that the internal energy density U of a system is the average value over all states; thus at T = 0 K we obtain E0F

U

D
EE dE 0

3 nE0F : 5

6:17

As has already been established, this value lies many orders of magnitude above the internal energy of a classical gas at T = 300 K. In order to treat the conduction electrons in a metal it is therefore sucient for many purposes to use a zero-temperature description (Fig. 6.5).

6.3 Fermi Statistics We now move on to consider the Fermi gas at finite temperatures. We shall need to derive the distribution function or occupation probability f
E; T for non-zero temperatures. This is a thermodynamical problem, since we are inquiring about the distribution that arises when various quantum mechanical states are in equilibrium with one another. To derive the distribution f
E; T we must therefore apply some basic concepts of thermodynamics. We consider an atomic system with single-particle energy levels Ej. We assume that the energy levels Ej lie very close to one another as in a solid. We can then consider new energy levels Ei each of which consists of many Ej. The degeneracy of these new levels is denoted by gi and their occupation number by ni where both gi and ni are large numbers. On account of the Pauli principle we must have ni gi. From thermodynamics we know the conditions that the system must fulfill in order for all energy levels to be in equilibrium: the free energy F of the total system must be stationary with respect to a variation in the relative occupation numbers of the levels. In other words we must have dF

X @F i

@ni

dni 0

with the subsidiary condition of conservation of particle number X dni 0 :

6:18

6:19

i

For the specific case of exchange of electrons between two arbitrary levels k and l the equilibrium conditions read

6.3 Fermi Statistics

143

@F @F dnk dnl 0 ; @nk @nl

6:20

dnk dnl 0 :

6:21

From this it follows immediately that the derivatives of the free energy with respect to the occupation numbers must be equal @F @F : @nk @nl

6:22

Since the two levels were selected at random, at equilibrium all @F/@ni must be equal and we denote this quantity by a new constant, l, defined as the ``chemical potential'' of the electrons. We will now calculate the free energy of the system of electrons. From thermodynamics we have the relation FU

6:23

TS

with the internal energy U X U ni E i

6:24

i

and the entropy S. The entropy is given by S k ln P ;

6:25

where P represents the number of possible ways of distributing the electrons among the states. The number of ways of accommodating one electron in the level Ei is gi. For a second electron, also in level Ei, the number of possibilities is gi ±1, and so on. There would therefore be gi
gi

1
gi

2 . . .
gi

ni 1

gi !
gi ni !

6:26

possible ways of accommodating ni electrons at definite positions within the energy level Ei. However, arrangements which dier only in the exchange of electrons within the energy level are not distinguishable. Since there are ni ! such possibilities, the total number of distinguishable ways of accommodating ni electrons in the level Ei is given by gi ! : ni !
gi ni !

6:27

The number of ways P of realizing the total system is then the product over all possibilities for occupying each level: Y gi ! P :
6:28 n !
g ni ! i i i Thus the entropy can be expressed as

144

6 ``Free'' Electrons in Solids

S k

X

ln gi !

ln ni !

ln
gi

ni ! ;

6:29

i

where the factorials can be replaced by using Stirling's approximate formula ln n! n ln n

n
for large n :

6:30

It now becomes a straightforward matter to calculate the chemical potential, i.e., the derivative of the free energy F with respect to the occupation number of an arbitrary level i : l

@F ni Ei k T ln : @ni gi ni

6:31

We can rearrange this expression to obtain the occupation number ni : ni gi
e

k

Ei l= T

1

1

:

6:32

The probability that a quantum mechanical state (degenerate states are also considered distinct here) is occupied is given by the distribution function f
E; T, which, from (6.32), can be seen to be (Fig. 6.6) 1

f
E; T e

k

E l= T

1

:

6:33

This function is also known as the Fermi distribution. It is the distribution function for particles, only one of which may occupy each quantum state. For electrons and all particles with half-integral spin, i.e., fermions, this distribution function guarantees that the Pauli principle is obeyed. However, it

Fig. 6.6. The Fermi distribution function at various temperatures. The Fermi temperature TF = E 0F/k has been taken as 5 104 K. The tangent at the point of inflection (± .. ±) intersects

the energy axis at 2 kT above E0F at all temperatures

6.4 The Specific Heat Capacity of Electrons in Metals

145

would be wrong to claim that the Fermi distribution is only valid for particles with spin 12; it is equally valid for atoms or molecules that are distributed among predetermined fixed positions, whenever only one atom or molecule can occupy such a position. Corresponding situations arise in the thermodynamics of defects (Sect. 2.7), the solubility of gases in solids, and adsorption processes. The significance of the chemical potential l in the Fermi distribution is most readily seen in the limiting case of T = 0 K. At zero temperature the Fermi function becomes identical with the step function introduced previously. It has a value of 1 for E < l and of 0 for E > l. Thus at T = 0 K the chemical potential of the electrons is equal to the Fermi energy: l
T 0 K E0F :

6:34

Because of this equality, one often speaks of the ``Fermi level'' in place of the chemical potential and uses the symbol EF. This Fermi level, however, is then a temperature-dependent quantity! At higher temperatures the sharp edge of the Fermi distribution becomes more rounded; states below EF have a finite probability of being unoccupied, while those slightly above EF may be occupied (Fig. 6.6). The size of the region, over which the Fermi function deviates significantly from the step function, is of the order of 2 k T to each side, as shown by the tangent to f
T; E at EF drawn in Fig. 6.6. One sees that as the temperature is raised, only a small fraction of the electrons is able to gain energy. This has important consequences, e.g., for the specific heat capacity of the electron gas (Sect. 6.4). If one is interested in the occupation probability for energies or temperatures in the range |E±EF| 2 k T, it is possible to use approximations to the Fermi function (6.33). The condition E±EF 2 k T is often fulfilled, for example for the conduction electrons in semiconductors (Sect. 12.2). In this regime, with energies E far above the Fermi edge, the Fermi function f
E; T can be approximated by the classical Boltzmann distribution, f
E; T exp
EF E=k T; see (12.5).

6.4 The Specific Heat Capacity of Electrons in Metals The application of the square-well potential model to the conduction electrons allows a very simple description of the specific heat capacity cv of these metal electrons. In fact this is an age-old problem, and one which seemed insoluble prior to the development of quantum mechanics. For a typical conduction electron density of n = 1022 cm±3 one would have expected, in addition to the lattice specific heat, an electronic contribution according to the equidistribution law of c = 3 n k/2, at least at elevated temperatures. Experiments on metals, however, showed no deviation from the Dulong-Petit

146

6 ``Free'' Electrons in Solids

value. The reason is simple: electrons, in contrast to a classical gas, can only gain energy if they can move into free states in their energetic neighborhood. The number of such electrons, expressed as a fraction of the total density n, is only of the order of 1/100, as demonstrated by the following simple estimate: The ``smeared out'' region of the Fermi function has a width on the order of 4 k T, i.e., according to Fig. 6.7, the Pauli principle dictates that only a fraction of about 4 k T/EF of all ``free'' electrons (density n ) can absorb thermal energy. The energy per electron is around k T and so the total energy of these thermally excited electrons is on the order of U 4
k T2 n=EF :

6:35

With TF = EF/k as the Fermi temperature, one obtains the following order of magnitude estimate for the specific heat of the electrons cv @U=@T 8 k nT=TF :

6:36

As seen in Table 6.1, the Fermi temperatures are typically on the order of 105 K and this, on account of the factor T/TF in (6.36), explains the vanishingly small contribution of the conduction electrons to the specific heat capacity. The exact calculation to determine the specific heat capacity of the gas of free electrons is as follows: Upon heating the Fermi electron gas from 0 K to a temperature T, the internal energy per unit volume is increased by an amount U given by E0F

1

U
T

dE ED
E f
E; T 0

dE ED
E :

6:37

0

Fig. 6.7. Explanation of the specific heat capacity of quasi-free metal electrons. The eect of raising the temperature from 0 K to T is to allow electrons from 2 k T below the Fermi energy to be

promoted to 2 k T above EF . The tangent (± ± ±) intersects the energy axis at EF + 2 kT

6.4 The Specific Heat Capacity of Electrons in Metals

We also have the relation 1
EF n EF dE D
E f
E; T ;

147

6:38

0

where n is the total concentration of free electrons. Dierentiating (6.37) and (6.38) yields 1
cv @U=@T E D
E
@f=@TdE ;
6:39 0 1

0 EF
@n=@T

EF D
E
@f=@TdE :

6:40

0

Subtracting (6.40) from (6.39), the specific heat capacity cv of the electrons is obtained as 1
cv @U=@T dE
E EF D
E
@f=@T :
6:41 0

The derivative @f/@T (Fig. 6.7) has significant values only in the ``smeared out'' region of 2 k T about EF. The density of states D (E) does not vary a great deal in this region and may be approximated by D (EF), i.e., 1
6:42 cv D
EF dE
E EF
@f=@T ; 0

where the temperature derivative of the Fermi function (6.33) is given by exp
E EF =k T @f E EF : 2 @T k T fexp
E EF =k T 1g2 With the abbreviation x
E EF =k T we then have 1
cv k 2 TD
EF dx x2 exp x
exp x 1 2 :

6:43

6:44

k

EF = T

Since the factor of exp x in the integrand is negligible for x ±EF/k T, the lower integration limit can be extended to minus infinity. The resulting integral 1
dx x2 exp x
exp x 1 2 p2 =3
6:45 1

is a standard integral whose value can be found in tables.

148

6 ``Free'' Electrons in Solids

One thus has the following general result for the specific heat capacity of the ``free'' electrons in metals: cv

p2 D
EF k 2 T : 3

6:46

In deriving (6.46) no use has been made of the explicit form of the density of states D (E). Equation (6.46) is therefore also valid for cases where the density of states deviates from that of the free electron gas, as indeed is expected in the majority of cases. For metals, measurements of the electronic heat capacity are therefore used as a method of determining the density of states D
EF at the Fermi level. In the free electron gas model D
EF can be very simply expressed in terms of the electron concentration. In the case of metals, the validity of the relation T TF implies E
F

n

D
EdE ;

6:47

0

and the density of states for this case can be written D
E D
EF
E=EF 1=2 :

6:48

It follows that 2 n D
EF EF ; 3

6:49

and from (6.46) we have cv

k T p2 p2 T nk nk : TF 2 2 EF

6:50

Thus the only dierence between this exact calculation and the previous rough estimate (6.36) is the appearance of the factor p 2/2 in place of the factor 8. The predicted linear dependence of the electronic specific heat capacity on temperature is well confirmed experimentally. For low temperatures, where the phonon contribution to cv displays the Debye T 3 dependence, one expects to observe cv cT bT3 ;

c; b const:

6:51

The experimental results in Fig. 6.8 show the linear dependence expected from (6.51) for a plot of cv/T against T 2. For the transition metals in particular, the experimentally determined values of c bear little resemblance to those calculated from the electron gas model, as is seen in Table 6.2.

6.4 The Specific Heat Capacity of Electrons in Metals

149

Fig. 6.8. Plot of cv/T against T 2 for copper. The experimental points (* and `) stem from two separate measurements [6.3] Table 6.2. Comparison of experimentally determined values of the coecient c of electronic specific heat with values calculated using the free-electron-gas model. At low temperatures one has cv = cT+bT 3 for the combined electronic (!T ) and (!T 3) contributions to the specific heat Metal

cexp (10±3 J/Mol K2 )

cexp =ctheo

Li Na K Cu Ag Al Fe Co Ni

1.7 1.7 2.0 0.69 0.66 1.35 4.98 4.98 7.02

2.3 1.5 1.1 1.37 1.02 1.6 10.0 10.3 15.3

Fig. 6.9. Qualitative behavior of the density of states D
E for the conduction band of a transition metal. The strong contribution of the d-electrons in the vicinity of the Fermi level lies on top of that of the s-band (partially dashed )

150

6 ``Free'' Electrons in Solids

The large deviations for Fe, Co, and Ni are attributed to the partially filled d-shells of these transition metals, whose d-bands thus lie at the Fermi energy. Because of the strong localization of the d-electrons at the atoms, the overlap of their wavefunctions is small. This means that the corresponding energy band is relatively narrow and therefore yields a large contribution to the density of states as shown in Fig. 6.9.

6.5 Electrostatic Screening in a Fermi Gas ± The Mott Transition If an electric charge is introduced into a metal, e.g. by the inclusion of a charged defect, then in the vicinity of this charge there is a perturbation in the otherwise homogeneous electron concentration which compensates or screens the electric field of the charge. This problem can be treated approximately using the model of a quasifree electron gas in a potential well: A local perturbation potential dU (assumed to obey |e dU| EF) produces a local raising of the density of states parabola D
E by an amount e dU (Fig. 6.10). If one imagines the perturbation potential to be switched on, it is clear that some electrons must immediately leave this region in order for the Fermi level to remain constant throughout the crystal. This homogeneity is necessary since the Fermi level is a thermodynamic function of state (equal to the electrochemical potential). For not too large dU the change in the electron concentration is given in terms of the density of states at the Fermi level (in analogy to the specific heat capacity) by dn
r D
EF jejdU
r :

6:52

Except in the immediate vicinity of the perturbation charge, one can assume that dU (r) is caused essentially by the induced space charge. Thus dn (r) is related to dU via the Poisson equation:

Fig. 6.10. Eect of a local perturbation potential dU on the Fermi gas of ``free'' electrons. Immediately after the perturbation is switched on, dn electrons must move away such that the Fermi level EF is homogeneous throughout the crystal in thermal equilibrium

6.5 Electrostatic Screening in a Fermi Gas ± The Mott Transition

D

2

dU

dR e e2 dn D
EF dU ; e0 e0 e0

151

6:53

where e0 is the dielectric constant. With k2 = e 2 D (EF)/e0, this dierential equation for the screening potential dU has a nontrivial solution in spherical coordinates 1 @ 2 @ 2 r
dU :
dU 2 r @r @r D

dU
r e

kr

=r :

6:54

Spherical coordinates are the obvious choice when dealing with a point-like defect. For a point charge e one would have e=
4pe0 since for k ? 0 the screening eect would disappear and one must obtain the Coulomb potential of this point charge (Fig. 6.11). The quantity rT F = 1/k is known as the Thomas-Fermi screening length: rTF e2 D
EF =e0

1=2

:

6:55

For the special case of the free electron gas model, (6.49) and (6.16) give 3 D
EF n=EF 2

and

EF

2 h
3 p2 n2=3 ; 2m

i.e. D
EF

1 2m
3 p2 n1=3 : 2 2p2 h

6:56

For the Thomas-Fermi screening length in the square-well model it follows that 1 r2TF

k2

1=3 me2 4 2 1=3 2 1=3 n
3 p
3 p n ; p a0 p2 h2 e 0

6:57

Fig. 6.11. Screened (ÐÐ) and unscreened (± . ±) Coulomb potential of a positive unit charge in a Fermi gas of free electrons. The distance r is given as a multiple of the Thomas-Fermi screening length rT F

152

6 ``Free'' Electrons in Solids

1 rTF

'2

n1=6 1=2

a0

or

rTF

n ' 0:5 3 a0

1=6

;

6:58

h2 e0 =
m e2 is the Bohr radius. Copper, for example, with an where a0 4 p electron concentration of n = 8.5 1022 cm±3, has a screening length of rTF = 0.55 AÊ. The screening process described here is responsible for the fact that the highest energy valence electrons of a metal are not localized. These electrons cannot be held in the field of the ion core potential. As the electron density decreases, the screening length rTF becomes even larger. Using arguments related to screening, it is possible to understand the sharp transition between metallic and insulating or semiconducting properties known as the Mott transition [6.4]. Above a certain critical electron density nc the screening length rTF becomes so small that electrons can no longer remain in a bound state; this produces metallic behavior. Below this critical electron concentration the potential well of the screened field extends far enough for a bound state to be possible. The electron is then localized in a covalent or ionic bond. Such localized states correspond, by definition, to insulating properties where the highest occupied states form localized bonds. To make a simple estimate of when a bound state becomes possible in a screened potential, we assume that the screening length must be significantly larger than the Bohr radius a0, i.e., that the potential well of a positive center extends suciently far to bind an electron: 1 a0 a20 ; 4 n1=3

6:59

4a0 :

6:60

r2TF ' i.e. n

1=3

This estimate, originally proposed by Mott, predicts that a solid will lose its metallic character when the average electron separation n ±1/3 becomes significantly larger than four Bohr radii. One then expects an abrupt transition to insulating properties. It is today believed that sharp jumps observed in the conductivity of transition metal oxides, glasses, and amorphous semiconductors, may be explicable in terms of the above mechanism.

6.6 Thermionic Emission of Electrons from Metals If a metal is made suciently hot it is found to emit electrons. This phenomenon is exploited in all electron tubes. In the circuit shown in Fig. 6.12 a one observes a saturation current js in the current-voltage characteristic (Fig. 6.12 b) that is dependent on the cathode temperature T.

6.6 Thermionic Emission of Electrons from Metals

153

Fig. 6.12. (a) Schematic drawing of a diode circuit for observing thermionic emission of electrons from the heated cathode C (A = anode). (b) Qualitative behavior of the currentvoltage curve at two dierent temperatures T1 and T2 > T1. As a consequence of their thermal energy, electrons can even overcome a countervoltage (A negative with respect to C)

The existence of this eect demonstrates that the assumption of an infinite square well to describe metal electrons is too simple. The potential well clearly has only a finite barrier height. The energy dierence Evac±EF = U is known as the work function. This is the energy barrier that an electron must overcome in order to reach the energy level of the vacuum (far away from the metal) from the ``Fermi sea''. If the electron also possesses a sucient momentum perpendicular to the surface, it can leave the metal and will contribute to the saturation current js. We will calculate the temperature-dependent saturation current for the free-electron-gas model. If the drift velocity v of the charge carriers is homogeneous, the current density is given by j = n e v, where n is the concentration of charge carriers. (Strictly speaking a minus sign is also required, but this can be omitted for our present purposes.) We can generalize this expression to the case where the electron velocity is a function of the wave vector k :
eX e jx v x
k v x
k dk :
6:61 V k
2p3 E>EF U v x
k>0

This form includes the fact that the density of states in k-space is V/(2 p )3. Both the summation and the integral extend only over occupied states, as dictated by Fermi statistics. This condition can be included explicitly by multiplying by the occupation probability given in (6.33). Thus jx

2e h
2 p3 m

1

1

dkx kx f
E
k; T :

dky dkz 1

6:62

kx min

h kx, and have taken into account that for a Here we have written mv x = free-electron gas all states are doubly degenerate. Since the work function U is large compared to k T, we can approximate the Fermi statistics by Boltzmann statistics:

154

6 ``Free'' Electrons in Solids

e h jx 3 4p m 1

1

dky e

k

h2 k2y =2m T

1

1

dkx kx e

dkz e

k

h2 k2z =2m T

1

k

k

h2 k2x =2m T EF = T

e

:

6:63

kx min

The integrals are thus factorized and can be readily evaluated. In the third integral we must also take into account that the kinetic energy in the +x-direction must be greater than EF + U : 1

dkx kx e

k

k

h2 k2x =2m T EF = T

e

1

1 2 dk e 2 x

k

k

h2 k2x =2m T EF = T

e

EF U2m=h2

kx min

m kT 2 h

e

k

U= T

:

6:64

One thus arrives at the so-called Richardson-Dushman formula for the saturation current density: js

4pme
k T2 e h3

k

U= T

:

6:65

The universal factor 4 p m e k 2 =h3 has the value 120 A/(K2 cm2). In this derivation we have made the simplifying assumption that electrons arriving at the surface with an energy h2 k2x =2m5EF U have a 100% probability of escaping from the solid. Even in the free-electron-gas model this assumption is not correct. The well-known quantum mechanical treatment of the reflection and transmission of electrons at a potential step tells us that electrons whose energy exactly equals the energy of the potential step have zero probability of transmission. q The eect of the potential step can be included by introducing a factor p k T=
EF U, which significantly reduces the saturation current density. The Richardson-Dushman formula can also be applied to the ballistic transport of charge carriers in semiconductor multilayer structures (cf. Sect. 12.7). In the particular case of thermionic emission, it is also necessary to consider the dependence of the work function on the external field E . The appropriate correction is the replacement of the constant U in the exponent by the field-dependent quantity s e3 E U0 U U DU :
6:66 4 p e0

The correction term DU is derived simply by assuming that essential contributions to the work function stem from the Coulomb force due to the image charge of an electron lying outside the surface and the eect of the external

6.6 Thermionic Emission of Electrons from Metals

155

Fig. 6.13. Schematic representation of the thermionic emission of free electrons (density n ) from a metal. An electron in the potential well must overcome the work function barrier U = Evac±EF in order to reach the energy level Evac of the vacuum and escape from the crystal. An important part of the work function is assumed to be the Coulomb potential between the escaping electron and its positive image charge in the metal (image potential ± . ±). If an external electric field is applied, then U is reduced by an amount DU. Reductions of the work function of *1 eV as shown here can only be achieved with extremely strong external fields of 107±108 V/cm

field in reducing the potential barrier. This is illustrated by the superposition of the external applied potential E x and the Coulomb image potential as shown in Fig. 6.13. The Richardson-Dushman formula can be used in this extended form to determine the work functions of metals. In order to do this, one must first determine the saturation emission current js 0 for E = 0 by extrapolating the measured current js at finite fields E . A semi-log plot of js 0 /T 2 against 1/T yields the work function. Work functions of the elements (polycrystalline) are listed in Table 6.3. Table 6.3. Work functions of elements in eV (polycrystalline samples, after Michaelson [6.5]) Li 2.9

Be 4.98

B C 4.45 5.0

Na Mg 2.75 3.66

Al Si P 4.28 4.85 ±

K Ca Sc 2.30 2.87 3.5

Ti V 4.33 4.3

Cr 4.5

Rb Sr Y 2.16 2.59 3.1

Zr Nb 4.05 4.3

Mo Tc 4.6 ±

Cs Ba 2.14 2.7

Hf 3.9

La 3.5

Mn Fe 4.1 4.5

Co 5.0

Ni Cu Zn Ga 5.15 4.65 4.33 4.2

Ge 5.0

S ±

As Se 3.75 5.9

Ru Rh Pd Ag Cd In Sn Sb Te 4.71 4.98 5.12 4.26 4.22 4.12 4.42 4.55 4.95

Pt Au Ta W Re Os Ir 4.25 4.55 4.96 4.83 5.27 5.65 5.1

Hg Tl Pb Bi Po 4.49 3.84 4.25 4.22 ±

156

6 ``Free'' Electrons in Solids

As a concluding remark we note that the work function depends strongly on the crystallographic orientation of the surface and on the degree of contamination.

Problems 6.1 a) Calculate the density of states for a two-dimensional gas of free electrons in a so-called quantum well. The boundary conditions for the electronic wavefunction are: w (x,y,z) = 0 for |x|>a, where a is of atomic dimensions. b) Calculate the density of states for a one-dimensional gas of free electrons in a so-called quantum wire with the boundary conditions: w (x, y, z) = 0 for jxj > a and jyj > b, where a and b are of atomic dimensions. c) Can such electron gases be realized physically? 6.2 Calculate to lowest order the temperature dependence of the chemical potential for a gas of free electrons whose electron concentration remains constant. Hint: Write down an expression for the electron concentration at finite temperature. You will encounter an integral 1

F
x 0

p y dy : 1 ey x

For x 1.5 F
x 2=3x

3=2

p2 1 2 8x

is a good approximation. 6.3 The bulk modulus j is given by the second derivative of the total energy Etot with respect to the volume: j = V ±1 @ 2 Etot/@V 2. Estimate the bulk moduli of alkali metals by assuming that the total energy is equivalent to the kinetic energy of the Fermi gas. What has been neglected in this estimate? 6.4 At what temperature T0 does the specific heat of the free electrons become larger than the specific heat of the lattice. Express this temperature in terms of the Debye temperature H and the electron concentration. Calculate T0 for copper. 6.5 The benzene molecule C6H6 exhibits characteristic optical absorption bands near to the wavelengths 180, 200 and 256 nm. These are explained in terms of p ? p * transitions of the carbon ring skeleton. The occupied p orbitals in the LCAO picture have, respectively: one and the same sign around

Problems

157

the C-ring (1st p orbital); one node line through two opposite C±C bonds (2nd p orbital); and one node line through two opposite C atoms (3rd p orbital). From the equal C±C bond length around the ring (*1.39 AÊ) it is inferred that the 6 p electrons are not localized in a particular bond but delocalized around the ring. As a simple model for the electronic properties of the p-system a closed, ring-like, one-dimensional electron gas consisting of the 6 p electrons is assumed (periodic boundary conditions). Calculate the possible energy eigenvalues En for this p system. a) Successively fill the states with six electrons and determine the optical absorption as the transition between the highest occupied and the lowest unoccupied state. Compare the result with the experimental absorption bands. b) Sketch the wavefunctions of the free electrons in the p-orbitals and match these to the LCAO orbitals. c) Discuss reasons why the calculated optical absorption deviates from experimental values. 6.6 A free electron plasma fills the half-space (z < 0) up to the surface z = 0, where it is bounded by vacuum. Show that the surface wave f f0 exp
kjzj exp i
kx

xt

is a solution of the Laplace equation Df = 0 and that the Maxwell boundary conditions for the E and D fields can be fulfilled at the surface z = 0, thus giving the condition e (xsp) = ±1 for the existence of the surface plasma wave with frequency xsp. Derive the dielectric function e (x ) for the undamped free electron plasma and find a relation between the frequencies xp and xsp of the bulk and surface plasmons. 6.7 Normal (main sequence) stars are stabilized by a balance between gravitational pressure and radiation pressure arising from nuclear fusion processes occurring in the interior. After burn out and exhaustion of the nuclear fuel a new equilibrium state, that of a white dwarf, can be reached following some loss of mass and a gravitational contraction of the residual star. This contraction is accompanied by the production of a large amount of heat, which causes disintegration of atoms. A plasma of free electrons and positive H and He nuclei is formed whose internal (Fermi) pressure counteracts further gravitational contraction. a) Calculate in the non-relativistic limit (electron velocity c ) the average energy of an electron and the average pressure in the electron plasma as a function of electron density n. b) Making use of the equilibrium between Fermi pressure and gravitational pressure, calculate for the non-relativistic case the mass spectrum M
R of possible white dwarfs (R is the density of the star). Hint: It is easy to see that the gravitational energy is proportional to G M 2/R where G is the gravitation constant. However, since the distribu-

158

6 ``Free'' Electrons in Solids

tion of density in a star is very inhomogeneous, a better approximation for the gravitational pressure at the center of the star is pGR(R = 0) ^ 2±1/3 G M 2/3 R 4/3. c) Investigate whether white dwarfs for which the mass-density relationship of part (b) holds are stable. Plot the total energy for a fixed mass and particle-number against the radius. At which masses is the white dwarf stable? d) With decreasing radius, the Fermi velocity of the electrons increases. For the relativistic case (v % c) calculate the average energy per electron and the pressure of the electron plasma as a function of the electron density. Hint: When the kinetic energy becomes significantly larger than the restmass energy, then E % pc = h k c. e) For the relativistic case calculate, in analogy to part (b), the equilibrium between Fermi pressure and gravitational pressure and determine the mass Mcrit for which this is possible. How does Mcrit compare to the mass of the sun Ms = 2 1030 kg? f) Describe explicitly what happens to stars that have masses M > Mcrit, M = Mcrit, and M < Mcrit. For each of the three cases plot the total energy at fixed mass and particle number as a function of the radius. g) Calculate the electron density nc at which the non-relativistic approximation must be replaced by the relativistic. This can be achieved with good accuracy by equating the relativistic and non-relativistic electron momenta at the Fermi edge: prel
n pnon-rel
n : F

c

F

c

Compare the mean separation of electrons at this density with their compton wavelength kc = h/mc. What star mass (expressed as a multiple of the sun's mass, Ms) corresponds to this density? Remark: Realistic calculations give an upper limit for the mass of white dwarfs of Mcrit & 1.4 Ms. This upper limit is named the Chandrasekhar limit after the Indian-American astrophysicist Subrahmanyon Chandrasekhar (Nobel prize 1984). 6.8 When the gravitational collapse of a burnt out star leads to even higher interior temperatures, inverse b decay processes (e + p ? n ) cause the generation of neutrons (n ). In its final state such a star consists only of neutrons (mass mn). These form a Fermi gas similar to that of the electrons in a white dwarf. Apply the stability criterion derived in Problem 6.7 (Chandrasekhar limit) to the neutron Fermi gas of a neutron star and estimate the critical mass Mcrit, the critical density Rcrit, and the critical radius Rcrit of a neutron star. Compare these with the values for the sun.

7 The Electronic Bandstructure of Solids

Despite the success of the free-electron-gas model in describing electrons in crystals (Chap. 6), it must be recognized that the assumptions of the one-electron approximation and of a square-well potential, are oversimplifications. Thus one cannot expect this model to explain, for example, the fundamentally important optical and electronic properties of semiconductors. If one imagines, as discussed briefly in Chap. 1, that a solid is created by allowing initially free atoms to gradually approach one another, then the discrete nature of the energy levels of the isolated atoms should clearly be reflected in the properties of the solid. Indeed, discrete energy levels must be present in order to explain, e.g., the sharp resonance-like structures observed in the optical spectra of solids. An explanation of such features is beyond the scope of the free-electron-gas model. Furthermore, this model is unable to shed any light on the nature of semiconductors and insulators. To make further progress one has to take into account that the electronic states in solids form so-called bands. One can think of these as deriving from the states of the free atom. In our present approximation, all deviations from perfect periodicity, be they static perturbations of the lattice or dynamic vibrations of the atoms, will be neglected. The assumption of an infinitely extended potential also means the neglect of all surface eects. To arrive at a finite crystal, i.e., one with a finite number of degrees of freedom, that is compatible with the infinite periodicity, one again makes use of the periodic boundary conditions introduced in Sect. 5.1.

7.1 General Symmetry Properties We are now faced with the task of solving the time-independent SchroÈdinger equation for a single electron under the assumption that the potential V
r is periodic: h2 2 H w
r r V
r w
r Ew
r ;
7:1 2m where V
r V
r rn ; rn n1 a1 n2 a2 n3 a3 : H. Ibach, H. LuÈth, Solid-State Physics, 4th ed., DOI 10.1007/978-3-540-93804-0_7, Ó Springer-Verlag Berlin Heidelberg 2009

7:2

160

7 The Electronic Bandstructure of Solids

As in Sect. 3.2, rn represents an arbitrary translation vector of the threedimensional periodic lattice, i.e., rn consists of multiples (n1, n2, n3) of the three basis vectors a1, a2, a3 of the real-space lattice. Since the potential V
r has the same periodicity as the lattice, it can be expanded in the following Fourier series: X VG eiG r ;
7:3 V
r G

where the vector G must be a reciprocal lattice vector G hg1 kg2 lg3 ; h; k; l integers:

7:4

(in the one-dimensional case G ? G = h 2 p/a ). The most general plane-wave expansion of the required wavefunction w
r is X w
r Ck eik r :
7:5 k

Here k is a point in reciprocal space that is compatible with the periodic boundary conditions (Sects. 5.1 and 6.1). Substituting the expansions (7.3) and (7.5) into the SchroÈdinger equation (7.1) we obtain: X h2 k 2 k

2m

Ck eik r

X 0

kG

0

Ck0 VG ei
k G r E

X

Ck eik r :

7:6

k

After renaming the summation indices this becomes " # X X h2 k2 ik r E Ck e VG Ck G 0 : 2m k G

7:7

Since this condition is valid for every position vector r, the expression in brackets, which is independent of r, must vanish for every k, i.e., 2 2 X h k E Ck VG Ck G 0 :
7:8 2m G This set of algebraic equations, which is simply a representation of the SchroÈdinger equation (7.1) in reciprocal space, couples only those expansion coecients Ck of w
r (7.5), whose k-values dier from one another by a reciprocal lattice vector G. Thus Ck is coupled to Ck±G, Ck±G', Ck±G'', . . . . The original problem thus separates into N problems (N = number of unit cells), each corresponding to a k-vector in the unit cell of the reciprocal lattice. Each of the N systems of equations yields a solution that can be represented as a superposition of plane waves whose wave vectors k dier only by reciprocal lattice vectors G. The eigenvalues E of the SchroÈdinger equation (7.1) can thus be indexed according to Ek = E
k, and the wavefunction belonging to Ek is

7.1 General Symmetry Properties

wk
r or wk
r

X

Ck

G

ei
k

Ck

G

e

G r

161

7:9

G

X

i G r i k r

e

uk
r ei k r :

7:10 a

G

The function uk
r introduced here is a Fourier series over reciprocal lattice points G and thus has the periodicity of the lattice. The wave vector k, which, for periodic boundary conditions, can take the values (Sect. 6.1) kx 0; 2 p=L; 4 p=L; . . . ; 2 p nx =L ky 0; 2 p=L; 4 p=L; . . . ; 2 p ny =L

7:10 b

kz 0; 2 p=L; 4 p=L; . . . ; 2 p nz =L (L = macroscopic dimension of the crystal), yields the correct quantum numbers kx , ky , kz or nx , ny , nz, according to which the energy eigenvalues and quantum states may be indexed. In other words, we have shown that the solution of the one-electron SchroÈdinger equation for a periodic potential can be written as a modulated plane wave wk
r uk
r ei k r

7:10 c

with a modulation function uk
r uk
r rn

7:10 d

that has the periodicity of the lattice. This result is known as Bloch's theorem, and the wavefunctions given in (7.10 a±d) are called the Bloch waves or Bloch states of an electron (Fig. 7.1). The strict periodicity of the lattice potential has further consequences that follow directly from the properties of the Bloch states. From the general representation of a Bloch wave (7.10 a), and by renaming the reciprocal lattice vectors G '' = G '±G, it follows that X 0 wkG
r CkG G 0 e iG r ei
kG r G0

X G

00

! Ck

G 00

e

i G 00 r

ei k r wk
r ;

7:11 a

i.e. wkG
r wk
r :

7:11 b

Thus Bloch waves whose wave vectors dier by a reciprocal lattice vector are identical. The SchroÈdinger equation (7.1):

H

wk E
k wk

and that for the same problem displaced by G:

7:12

162

7 The Electronic Bandstructure of Solids

Fig. 7.1. Example of the construction of a Bloch wave wk
r uk
reikr from a lattice-periodic function uk
r with p-type bonding character and a plane wave

H

wkG E
k GwkG

7:13

together with (7.11 b) then yield

H

wk E
k Gwk :

7:14

Comparing (7.12) with (7.14) we see that E
k E
k G :

7:15

Thus the energy eigenvalues E
k are a periodic function of the quantum numbers k, i.e., of the wave vectors of the Bloch waves. Similar to the case of phonons, whose x
q can be described by dispersion surfaces in reciprocal q-space, the one-electron states of a periodic potential can be represented by energy surfaces E = E
k that are a periodic function of the wave vector (quantum number) in reciprocal k-space. Taken together, these energy surfaces form the electronic bandstructure of the crystal. Since both wk (r) and E (k) are periodic in reciprocal space, one only needs to know these functions for k-values in the first Brillouin zone

7.2 The Nearly Free-Electron Approximation

163

(Sect. 3.5). A periodic continuation of the functions then provides the values throughout the whole of k-space.

7.2 The Nearly Free-Electron Approximation To understand the general concept of electronic bands it is particularly instructive to consider the limiting case of a vanishingly small periodic potential. We therefore imagine that the periodic potential starts at zero and is gradually``switched on''. What happens then to the energy states of the free electrons which, in the square-well potential, were described by the energy parabola E = h 2 k 2/2 m? In the extreme case where the potential is still zero, i.e., where all Fourier coecients VG (7.3) vanish, one must nonetheless consider the symmetry requirements of the periodicity, since the requirements will be a decisive factor even for the smallest nonvanishing potential. This general demand of periodicity immediately implies, from (7.15), that the possible electron states are not restricted to a single parabola in k-space, but can be found equally well on parabolas shifted by any G-vector: E
k E
k G

2 h jk Gj2 : 2m

7:16

For the one-dimensional case (G ? G = h 2 p/a) this is depicted in Fig. 7.2. Since the behavior of E
k is periodic in k-space, it is sucient to represent this in the first Brillouin zone only. To achieve this one simply displaces the part of the parabola of interest by the appropriate multiple of G = 2 p/a. This procedure is called ``Reduction to the first Brillouin zone ''. In three dimensions, the E
k bands are already more complicated, even in the case of a vanishing potential, since in (7.16) one now has G contributions in all three coordinate directions. Figure 7.3 shows the E
k curves along kx in the first Brillouin zone for a simple cubic lattice with vanishing potential. The eect of a finite but very small potential can now be discussed with reference to Figs. 7.2 and 7.3. In the one-dimensional problem of Fig. 7.2 there is a degeneracy of the energy values at the edges of the first Brillouin zone, i.e., at +G/2 = p/a

Fig. 7.2. The parabolic energy curves of a free electron in one dimension, periodically continued in reciprocal space. The periodicity in real space is a. This E
k dependence corresponds to a periodic lattice with a vanishing potential (``empty'' lattice)

164

7 The Electronic Bandstructure of Solids

Fig. 7.3. Bandstructure for a free electron gas in a primitive cubic lattice (lattice constant a ), represented on a section along kx in the first Brillouin zone. The periodic potential is assumed to be vanishing (``empty'' lattice). The various branches stem from parabolas whose origin in reciprocal space is given by the Miller indices h k l. (ÐÐ) 000; (± ± ±) 100, 100; (± . ±) 010, 010, 001, 001; ( . . . ) 110, - -- - 101, 110, 101, 110, 101, 110, 101

and ±G/2 = ±p/a, where two parabolas intersect. The description of the state of an electron with these k-values is necessarily a superposition of at least two corresponding plane waves. For a vanishing potential (zeroth-order approximation) these waves are eiG x=2

and ei
G=2

Gx

e

i G x=2

:

7:17

Equation (7.8) implies that waves with G-values larger than 2 p/a must also be taken into account. However, on dividing (7.8) by [(h 2 k 2/2 m )±E ], it follows that Ck is particularly large when Ek and Ek±G are both approximately equal to h 2 k 2/2 m, and that the coecient Ck±G then has approximately the same absolute magnitude as Ck. This is precisely the case for the two plane waves at the zone boundaries (7.17), and thus, to a first approximation, one can neglect contributions from other reciprocal lattice vectors. The appropriate expressions for a perturbation calculation of the influence of a small potential are therefore of the form x
7:18 a w
ei G x=2 e i G x=2 cos p ; a x w
ei G x=2 e i G x=2 sin p :
7:18 b a These are standing waves possessing zeros at fixed positions in space. As seen in the discussion of diraction from periodic structures (Chap. 3), these standing waves can be represented as a superposition of an incoming wave and a counter-propagating ``Bragg-reflected'' wave. The probability densities, corresponding to w+ and w±, x
7:19 a R w w cos2 p ; a x R w w sin2 p ;
7:19 b a

7.2 The Nearly Free-Electron Approximation

165

Fig. 7.4. (a) Qualitative form of the potential energy V (x) of an electron in a one-dimensional lattice. The positions of the ion cores are indicated by the points with separation a (lattice constant). (b) Probability w for the standing density R w wave produced by Bragg reflection at k p=a (upper edge of band in Fig. 7.5). (c) Probability density R ww for the standing wave at the lower edge of band (Fig. 7.5) at k p=a

are depicted in Fig. 7.4 together with a qualitative sketch of the potential. For an electron in the state w+, the charge density is maximum at the position of the positive cores and minimum in between; for w± the charge density is maximum between the cores. In comparison with the travelling plane wave ei kx, which is a good approximation to the solution further away from the zone boundary, w+ thus has a lower total energy (particularly potential energy), and w± a higher energy than that of a free electron on the energy parabola (zero potential case). This increase and decrease in the energy of the states at the zone boundary represents a deviation from the free-electron energy parabola (Fig. 7.5). Having gained insight into the problem from this qualitative discussion, it is now easy to carry out a formal calculation of the magnitude of the socalled band splitting or energy gap shown in Fig. 7.5. Starting from the general representation of the SchroÈdinger equation in k-space (7.8), translation by a reciprocal lattice vector yields

Fig. 7.5. Splitting of the energy parabola of the free electron (± ± ±) at the edges of the first Brillouin zone k p=a in the one-dimensional case). To a first approximation the gap is given by twice the corresponding Fourier coecient VG of the potential. Periodic continuation over the whole of k-space gives rise to continuous bands and , shown here only in the vicinity of the original energy parabola

166

7 The Electronic Bandstructure of Solids

E

2 h jk 2m

Gj

2

Ck

X

G

G0

X

G0

P Ck

G

G0

VG 0

VG 0

G G0

G Ck G 0

;

7:20 a

i:e:

G Ck G 0

:

2 h jk 2m

E

VG 0 Ck

7:20 b

2

Gj

For small perturbations, a first approximation to the calculation of Ck G can be made by setting the true eigenvalue E that we are seeking equal to the energy of the free electron ( h 2 k 2/2 m ). Furthermore, in this first approximation, only the largest coecients Ck G are of interest; in other words, we expect the greatest deviation from free-electron behavior when the denominator in (7.20 b) vanishes, i.e., for k2 ' jk

Gj2 :

7:21

This is identical to the Bragg condition (3.32). The strongest perturbations to the energy surface of the free electron (spheres in k-space), produced by the periodic potential, occur when the Bragg condition is satisfied, i.e., for the k-vectors at the edge of the first Brillouin zone. It follows from (7.20 b), however, that besides Ck G , the coecient Ck is equally important. Thus, in the system of (7.20 a), for this approximation we only need to consider two relations (V0 = 0): E E

2 2 h k Ck 2m 2 h jk 2m

Gj

VG Ck

0

G

2

(7.22) Ck

V

G

G Ck

0:

We thus obtain the secular equation for the energy value 2 h k2 E 2m V G

VG

2 h jk 2m

2

Gj

0: E

7:23

With E 0k±G = ( h2/2 m) | k±G | 2 as the energy of the free electrons, the two solutions to this secular equation may be written E 12
Ek0

0 G Ek

h

1 0 4
Ek G

Ek0 2 jVG j2

i1=2

:

7:24

7.3 The Tight-Binding Approximation

167

Fig. 7.6. Energy dispersion curves E (k) for a one-dimensional lattice (lattice constant a ) in the extended zone scheme. As can be seen, the quasi-free-electron approximation gives rise to forbidden and allowed energy regions due to the opening of band gaps, as shown in Fig. 7.5 (cf. the vanishing potential case of Fig. 7.2). The parts of the bands corresponding to the free-electron parabola are indicated by the thick lines

Therefore, at the zone boundary itself, where the contributions of the two waves with Ck and Ck G are equal ± see (7.21) ± and where E 0k±G = E 0k, the energy gap has a value DE E

E 2jVG j ;

7:25

i.e., twice the G th Fourier component of the potential. Near to the zone boundary, the form of the two energy surfaces that are separated by this gap is described by (7.24) (in which one again sets E 0k = h 2 k 2/2 m ). Figure 7.5 illustrates this for the one-dimensional case near to the zero boundary at k = G/2. The correspondence between the energy parabola of the free electrons and the periodic bandstructure, with its energy gaps due to the realistic potential, is depicted in Figs. 7.5 and 7.6, in both cases for the one-dimensional problem.

7.3 The Tight-Binding Approximation The electrons that occupy the energetically low-lying core levels of a free atom are strongly localized in space. They naturally retain this strong localization when the atom participates in the formation of a crystal. It thus appears that the description of a solid's electronic structure in terms of

168

7 The Electronic Bandstructure of Solids

quasi-free electrons must be inadequate. Since these core electrons largely retain the properties that they had in the free atom, an obvious approach is to describe the crystal electrons in terms of a linear superposition of atomic eigenfunctions. This procedure, also known as the LCAO method (Linear Combination of Atomic Orbitals), was already discussed qualitatively in Chap. 1 in relation to chemical bonding, in order to explain the existence of electronic bands in solids. In formulating the problem, one assumes that the solutions to the SchroÈdinger equation for the free atoms that form the crystal

H A
r

rn ui
r

rn Ei ui
r

rn

7:26

are known. H A (r± rn) is the Hamiltonian for a free atom at the lattice position rn = n1 a1 + n2 a2 + n3 a3 and ui
r rn is the wavefunction for an electron in the atomic energy level Ei. One imagines the entire crystal to be built up of single atoms, i.e., the Hamiltonian for an electron (one-electron approximation!) in the total potential of all the atoms can be written:

H H A v

2 h D VA
r 2m

rn v
r

rn :

7:27

The influence of atoms in the neighborhood of rn, where the electron of interest is relatively strongly localized, is described by a perturbation v
r rn to the potential VA of the free atom. This perturbation can thus be expressed as X v
r rn VA
r rm
7:28 m j n

i.e., as a sum over the potentials of all atoms apart from that at rn, at the position r of the electron (Fig. 7.7). We now seek solutions of the SchroÈdinger equation

H wk
r E
kwk
r ;

7:29

where H is the Hamiltonian of (7.27) for the crystal electron and wk (r) are Bloch waves with the general properties discussed in Sect. 7.1. Multiplying (7.29) by wk and integrating over the range in which wk is defined, one readily obtains hwk jH jwk i ;
7:30 hwk jwk i where hwk jwk i dr wkwk and hwk jH jwk i dr wkH wk (cf. Sect. 1.2 and Problem 1.8). If, instead of the true wavefunction, one inserts a trial wavefunction Uk into (7.30), then one obtains an energy E ' that is always larger than E
k. The better Uk approximates the true wavefunction, the closer E '
k lies to E
k. This circumstance provides the basis for the Ritz procedure. E
k

7.3 The Tight-Binding Approximation

169

Fig. 7.7. Cross section of the potential used in the tight-binding approximation along the x-direction. The lattice potential Vlatt (ÐÐ) is obtained by summing the potentials VA of the free atoms (± ± ±). The perturbation potential v
r rn used in the approximate calculation is given by the dash-dotted line in the lower part of the figure

In the present case, when we want to calculate the crystal electron energy states E
k that derive from the energy level Ei of the free atom, we assume that a good approximation to wk is provided by a linear combination of atomic eigenfunctions ui
r rn ; i:e:; X X an ui
r rn ei k rn ui
r rn :
7:31 wk Uk n

n

The expansion coecients are determined as an = exp (i k . rn ) by the requirement that Uk should be a Bloch wave. It can easily be shown that Uk in (7.31) possesses all the required properties of Bloch waves (Sect. 7.1), e.g., X ei k rn ei G rn ui
r rn Uk :
7:32 UkG n

An approximate calculation of E
k can now be made by inserting in (7.30) the trial function of (7.31); the denominator in (7.30) becomes:
X i k
rn rm ui
r rm ui
r rn dr : hUk jUk i e
7:33 n; m

For a suciently localized electron, uk
r rm only has significant values in the vicinity of rm. Thus, to a first approximation, we only retain terms in (7.33) with n = m, and obtain

170

7 The Electronic Bandstructure of Solids

hUk jUk i '

X
n

ui
r

rn ui
r

rn dr N ;

7:34

where N is the number of atoms in the crystal. Making use of the fact we know the solutions to (7.26) for the free atom, we write
1 X i k
rn rm E
k e
7:35 ui
r rm Ei v
r rn ui
r rn dr N n; m where Ei is the energy eigenvalue of the isolated atom. In the term containing Ei we have again neglected the overlap between nearest neighbors (i.e., only terms with n = m are considered). For the term containing the perturbation v
r rn , overlap is included only up to nearest neighbors. In the simple case when the relevant atomic state ui possesses spherical symmetry, i.e., s-character, the result can be readily represented with the help of the following two quantities: A u
r rn v
r rn u
r rn dr ;
7:36 a i

B

i

ui
r

rm v
r

and reads E
k Ei

A

B

X

rn ui
r

ei k
rn

rm

rn dr

:

7:36 b

7:37

m

The sum over m includes only values for which rm denotes a nearest neighbor of rn. In the present case, A is positive since v is negative. Equation (7.37), applied to the case of a primitive cubic lattice with rn

rm
a; 0; 0 ;
0; a; 0 ;
0; 0; a ;

gives, for an atomic s-state, E
k Ei

A

2B
cos kx a cos ky a cos kz a :

7:38

When the atoms are brought together to form a crystal (with primitive cubic lattice), the atomic energy level Ei therefore becomes an electronic band whose center of gravity is reduced by an amount A with respect to Ei and whose width is proportional to B. This situation is illustrated in Fig. 7.8. The important consequences can be summarized as follows: i) Since the cosine terms vary between +1 and ±1, the width of the energy band is 12 Bi . For small k-values, the cosine terms can be expanded such that near to the C-point (center of the first Brillouin zone at k = 0) one obtains E
k Ei

A

6B B a2 k2 ;

7:39

7.3 The Tight-Binding Approximation

171

Fig. 7.8 a±c. Qualitative illustration of the result of a tight-binding calculation for a primitive cubic lattice with lattice constant a. (a) Position of the energy levels E1 and E2 in the potential V
r of the free atom. (b) Reduction and broadening of the levels E1 and E2 as a function of the reciprocal atomic separation r ±1. At the equilibrium separation a the mean energy decrease is A and the width of the band is 12 B. (c) Dependence of the oneelectron energy E on the wave vector k (1, 1, 1) in the direction of the main diagonal [111]

where k 2 = k 2x + k 2y + k 2z . This k 2-dependence corresponds to that which results from the quasi-free-electron approximation (Sect. 7.2). ii) From (7.36 b) it follows that the energy width of the band becomes greater as the overlap between the corresponding wavefunctions of neighboring atoms increases. Lower lying bands that stem from more strongly localized states are thus narrower than bands originating from less strongly bound atomic states whose wavefunctions are more extended. iii) In the framework of the present one-electron approximation, the occupation of the one-electron band states is obtained by placing two of the available electrons of every atom into each band, beginning with the lowest energy band, until all electrons have been accommodated. The Pauli principle allows the double occupation because of the two possible spin states of the electron. If a crystal with a primitive cubic lattice contains N atoms, and thus N primitive unit cells, then an atomic energy level Ei of the free atom will split, due to the interaction with the other (N±1) atoms, into N states. These then form the corresponding quasi-continuous band. This band can thus be occupied by 2 N electrons. We obtain the same result by considering this problem in terms of the quasi-free-electron model: In k-space each electron state corresponds to a volume (2 p )3/V (where V is the macroscopic crystal volume). The volume of the first Brillouin zone, however, is (2 p )3/Vc

172

7 The Electronic Bandstructure of Solids

(where Vc is the volume of the unit cell). Thus the part of the band within the first Brillouin zone contains V/Vc = N states, which, when the two spin states are considered, yields 2 N states available for occupation by electrons. The existence of a bandstructure arising from the discrete energy levels of isolated atoms upon their joining together to form a crystal was illustrated qualitatively in Fig. 1.1. For sodium, for example, the atomic 3 s- and 3 p-levels give rise, in the crystal (equilibrium atomic separation r0), to bands that overlap. Since the occupied levels of atomic sodium are 1 s 2, 2 s 2, 2 p 6, 3 s 1, the atomic 3 s-level only contributes one electron per unit cell to the 3 s-band of the crystal, which could, however, accommodate two electrons per unit cell. Thus, even without the 3 s-3 p overlap (analogous to the 2 s±2 p overlap in Fig. 1.1), the 3 s band of Na would only be half full. In Sect. 9.2 we will see that this partial occupation of a band is the source of the metallic conductivity of Na. Qualitative arguments concerning the conductivity have already been presented in Sect. 1.4. It is well known that isolated carbon atoms have the electronic configuration 1 s 2, 2 s 2, 2 p 2. However, in the diamond crystal, as a result of the forma-

Fig. 7.9. Schematic behavior of the energy bands as a function of atomic separation for the tetrahedrally bound semiconductors diamond (C), Si, and Ge. At the equilibrium separation r0 there is a forbidden energy gap of width Eg between the occupied and unoccupied bands that result from the sp 3 hybrid orbitals. For diamond, the sp 3 hybrid stems from the 2 s and 2 p 3 atomic states, for Si from the 3 s and 3 p 3, and for Ge from the 4 s and 4 p 3. One sees from this figure that the existence of a forbidden energy region is not tied to the periodicity of the lattice. Thus amorphous materials can also display a band gap. (After [7.1])

7.4 Examples of Bandstructures

173

tion of the sp 3 hybrid (a mixture of 2 s and 2 p wavefunctions with tetrahedral bonding; Chap. 1), there is a modification of the s- and p-levels which manifests itself in a further splitting of the sp 3 hybrid band into two bands, each of which (including spin) can accommodate four electrons (Fig. 7.9). The four electrons of the atomic 2 s- and 2 p-states thus fill the lower part of the sp 3 band, leaving the upper part unoccupied. Between the two sp 3 subbands there is a forbidden energy gap of width Eg. This is the origin of the insulating property of diamond, as will be shown in Sects. 9.2 and 12.1. The semiconductors Si and Ge are similar cases (Chap. 12). The form of the bandstructure shown in Fig. 7.9 cannot be derived using the simple approach outlined here. More complex methods are necessary for this calculation and these require the use of modern computing facilities. For further information about such calculations the reader is referred to theoretical reviews and more advanced text books.

7.4 Examples of Bandstructures In the preceding sections, the origin of the electronic bandstructure, i.e., the existence of allowed and forbidden energy regions for a crystal electron, was attributed to the presence of Bragg reflections, which cause certain regions of the continuous spectrum of free-electron states to become forbidden. The alternative, but equally important, approach starts from the discrete energy levels of the free atom and explains the evolution of bands as a quasi-continuous splitting of the atomic levels due to the interaction with the other atoms of the crystal. In this picture, each band corresponds to an energy level of the free atom and may thus be classified as an s-, p-, or d-band etc. Having given a qualitative picture of a typical metal and a typical insulator in the examples of Figs. 1.1 and 7.9, in this section we will examine a few further examples of realistic bandstructures. Figure 7.10 shows how the highest occupied bands of the ionic crystal KCl can be imagined to evolve from the energy levels of isolated K+ and Cl± ions as they approach one another until they reach the equilibrium separation in the crystal. Even at this equilibrium separation, which is known from X-ray diraction data, the occupied bands are extremely narrow. This indicates that there is relatively little overlap between the charge clouds of the individual ions. If theoretical results such as those shown in Fig. 7.10 are in good agreement with experimental data, then they allow important conclusions to be drawn about the form of the chemical bonding. The entire information about the one-electron states in the periodic potential is of course contained in a representation of the complete E
k surfaces in wave-vector space. In order to simply portray the often complicated surfaces, one considers cross sections through the energy surfaces along directions of high symmetry in the first Brillouin zone. This is illustrated in Fig. 7.11 a for the example of an Al crystal. The definitions of the

174

7 The Electronic Bandstructure of Solids

Fig. 7.10. The four highest occupied energy bands of KCl calculated as a function of the ionic separation in Bohr radii (a0 = 5.29 10±9 cm). The energy levels in the free ions are indicated by arrows. (After [7.2])

symmetry directions and symmetry points in the first Brillouin zone of a face-centered cubic lattice are indicated in Figs. 3.8 and 7.11 b. A striking feature of the Al bandstructure is that it can be described very well by the parabolic dependence of a free-electron gas (dotted lines). The energy gaps at the Brillouin zone edges are relatively small and the

Fig. 7.11. (a) Theoretical bandstructure E
k for Al along directions of high symmetry (C is the center of the Brillouin zone). The dotted lines are the energy bands that one would obtain if the s- and p-electrons in Al were completely free (``empty'' lattice). After [7.3]. (b) Cross section through the Brillouin zone of Al. The zone edges are indicated by the dashed lines. The Fermi ``sphere'' of Al (ÐÐ) extends beyond the edges of the first Brillouin zone

7.4 Examples of Bandstructures

175

complexity of the bandstructure stems largely from the fact that the energy parabolas are plotted in the reduced-zone scheme, i.e.,``folded'' back into the first Brillouin zone. This type of bandstructure is characteristic for simple metals. The similarity to the free electron gas is particularly pronounced for the alkali metals Li, Na and K. The filling of the bands with the available electrons continues up to the Fermi energy EF (indicated in Fig. 7.11). It can be seen that the corresponding constant energy surface, the so-called Fermi surface E (k) = EF , intersects several bands. Thus, even for Al, the Fermi surface is not a simple continuous surface: whereas the Fermi surfaces of the alkali metals are almost spherical and are contained wholly within the first Brillouin zone, the ``Fermi sphere'' of Al extends just beyond the edges of the first Brillouin zone. The Bragg reflections occurring at these edges cause a slight deviation from the spherical form in these regions. This is shown qualitatively in Fig. 7.11 b in a cross section through three-dimensional k-space. In comparison to the simple metals, the band structures of the transition metals are considerably more complicated, due to the significant influence

Fig. 7.12. Bandstructure E (k) for copper along directions of high crystal symmetry (right ). The experimental data were measured by various authors and were presented collectively by Courths and HuÈfner [7.4]. The full lines showing the calculated energy bands and the density of states (left ) are from [7.5]. The experimental data agree very well, not only among themselves, but also with the calculation

176

7 The Electronic Bandstructure of Solids

of the d-bands. Together with the bands that originate from s-levels and resemble the parabolic form of the free-electron gas, there are also very flat E (k) bands, whose small energy width (low dispersion) can be attributed to the strong localization of the d-electrons. This is readily seen for the example of copper, whose bandstructure is illustrated in Fig. 7.12. For transition metals such as Pt, W, etc., where the Fermi level intersects the complex dbands, the Fermi surfaces possess particularly complicated forms. Other interesting phenomena, such as semiconducting properties (Chap. 12), occur when the bandstructure possesses an absolute gap, i.e., a so-called forbidden region: in this particular energy range and for all k-directions in reciprocal space, there are no available electron states. A typical bandstructure of this type is that of germanium (Fig. 7.13). Like diamond and silicon, germanium crystallizes in the diamond structure, whereby the tetrahedral bonding of the individual atoms is a consequence of the formation of sp 3 hybrid orbitals. As was mentioned at the end of Sect. 7.3, the formation of sp 3 hybrids leads to the existence of sp 3 sub-

Fig. 7.13. Theoretically derived bandstructure E (k) for germanium along directions of high symmetry (right), and the corresponding electronic density of states (left). A number of critical points, denoted according to their position in the Brillouin zone (C, X, L ), can be seen to be associated with regions of the bandstructure where E
k has a horizontal tangent. The shaded region of the density of states corresponds to the states occupied by electrons [7.6]

7.5 The Density of States

177

bands. The lower of these (below the forbidden gap) are fully occupied whereas the higher-lying sp 3 subbands above the gap are unoccupied. The Fermi energy must therefore lie within the forbidden gap, a fact that will be important when we come to discuss the semiconducting properties of this crystal in Chap. 12.

7.5 The Density of States In analogy to the thermal properties of the phonon system (Chap. 5), one finds also in the case of electronic states, that a knowledge of the density of states is sucient to describe e.g. the energy content of the electron system. For certain electronic excitation mechanisms (e.g. non-angle-resolved photoemission spectroscopy; Panel V), in which the experiment eectively integrates over all k-directions, one can often interpret the spectra simply in terms of the number of electron states per energy interval dE. Once the energy surfaces E
k of the bandstructure are known, then in analogy to (5.4), the density of states is obtained by integrating over an energy shell {E
k, E (k) + dE } in k-space: dZ

EdE

V
2 p3

dk ;

7:40

E

where V/(2 p ) is the density of states in k-space. If the volume element dk is separated into an area element dfE on the energy surface and a component dk^ normal to this surface (Fig. 5.1), i.e., dk = dfE dk^, then with dE = |gradk E| dk^ one has 0 1
1 B dfE C D
EdE
7:41 AdE : 3@ jgradk E
kj
2 p 3

E
kconst

This density of states D (E) is given here in relation to the real volume V of the crystal in order to obtain a crystal-specific quantity. It should be remembered that, due to spin degeneracy, each state can accommodate two electrons. The main structure in the function D (E) is again yielded by those points in k-space for which |gradk E| vanishes, i.e., where the energy surfaces are flat. These points are known as van Hove singularities or critical points. In three dimensions D (E) does not become singular near to these critical points because an expansion of E
k about the extremum (E * k2) implies that |gradk E|±1 has a k ±1 singularity. Thus the integration of the E (k) surface (7.41) yields a linear k dependence. In three dimensions the density of states near to a critical point therefore has the form shown in Fig. 7.14. For onedimensional bandstructures, which, to a good approximation, can be used

178

7 The Electronic Bandstructure of Solids

Fig. 7.14. Form of the density of states D (E) in the vicinity of the four possible types of critical point in three dimensions. The energy of the critical points is denoted by Ec and the corresponding k-space position by kciP(i = 1, 2, 3). In the parabolic approximation, the energy band has the form E (k) = Ec + i i . (ki±kci)2 in the vicinity of a critical point, where i = const. The quantities D0 and C in the figure are also constants

to describe one-dimensional organic semiconductors, the density of states diverges at the critical points, although its integral remains finite. (See discussion of density of states of lattice vibrations for a linear chain; Sect. 4.3.) Theoretical densities of states may be obtained by integrating in k-space over the first Brillouin zone for a calculated bandstructure, and may then be compared with experimental data, for example from photoemission spectroscopy (Panel V). As such, they provide an important point of connection between calculated bandstructures and the experimental data. In the integration over k-space the main contributions to the density of states are derived from the critical points. Since the critical points usually occur along lines of, or at points of high symmetry in k-space, this lends further justification for the preferred representation of bandstructures along lines of high symmetry, e.g., CK, CX, C L, etc. In the intermediate regions one can expect only minor contributions, and it is sometimes possible to make use of simple mathematical interpolation to obtain the bandstructure there. The relationship between a calculated bandstructure and the corresponding density of states is nicely demonstrated by the case of the semiconductor germanium as shown in Fig. 7.13. Important contributions, i.e., maxima in the density of states, are clearly correlated with flat portions of the E
k curves along directions of high symmetry. Also evident is the absolute band gap between the fully occupied valence band states and the (at low temperatures) unoccupied conduction band states. This forbidden region has a width of about 0.7 eV for germanium. As an example for a transition metal, Fig. 7.12 shows the calculated density of states for copper. The density of states is obtained by integrating

7.6 Density of States in Non-Crystalline Solids

179

over the bandstructure E
k, which is also shown in the figure. The sharp structures seen between ±2 and ±6 eV below the Fermi level can be readily attributed to critical points of the relatively flat d-bands. In the E
k plot (Fig. 7.12) one can also recognize the parabola-like shape of the s-band with its minimum at the C-point. This s-band is responsible for the structureless contribution to the density of states beginning at about ±9.5 eV. Below ±6 eV one cannot fail to notice the distinct similarity to the ``free-electron-gas'' parabolic density of states. At the Fermi level it is again the s-electrons that produce the density of states. This explains why the model of a free-electron gas in a box (Chap. 6) yields relatively good results for copper. However, as shown in Sect. 6.4, this is far from true for Fe, Ni, Co and the other transition metals. For these metals the Fermi level intersects the high density of states of the d-bands, which are therefore only partially filled. For the ferromagnets Fe, Ni and Co there is an additional complication, which will be dealt with in detail in Sect. 8.3. In these metals there is a ferromagnetic phase at T < TC (Curie Temperature) in which the atomic spins are aligned. One then has two distinct densities of states ± one for electrons whose spin is parallel to the spontaneous magnetization M and one for the electrons with antiparallel spin orientation. Figure 8.6 shows these two densities of states for Ni. To derive such densities of states requires a calculated bandstructure E
k in which the electron±electron interaction is explicitly included.

7.6 Density of States in Non-Crystalline Solids A crystalline solid is translationally invariant with respect to a lattice vector and the electronic states can be classified according to the components of the wave-vector kx , ky , and kz. Only then are the eigen-values of the electronic states described by a band structure E(k). However, the concept of a density of states per energy and volume and of allowed and forbidden bands does not require translational invariance. Thus, a non-crystalline solid possesses a defined density of states, just as the crystalline solid, provided that the non-crystalline solid is suciently homogeneous in composition and structure on a mesoscopic length scale. Many materials exist in a crystalline as well as non-crystalline phases, as under-cooled melts (glasses). Examples are SiO2 and Al2O3. As is well known, these two materials are optically transparent in either phase. Both phases must therefore have an energy gap between occupied and unoccupied states larger than 3 eV. Thus it seems that the magnitude of the energy gap does not depend on the existence of crystalline order. The amorphous phases of SiO2 and Al2O3, and likewise the amorphous phases of Si and Ge dier from the crystalline phases only by the missing long-range order. The nearest and next nearest neighbor configuration is rather similar. In Si and Ge the local order is

180

7 The Electronic Bandstructure of Solids

determined by the sp3-bonding to the nearest-neighbors. Since the electronic structure is dominated by the local bonding, the magnitude of the energy gap is nearly equal for the crystalline and the amorphous phases. Likewise the densities of states for other electron energies are rather similar. Only the sharp features in the band structure resulting from the critical points (Fig. 7.13) are absent in the amorphous phases. Amorphous phases of Si and Ge can be fabricated by growth at (relatively) low temperatures. At these temperatures long-range order, which requires diusion of material, is not established and the state of lowest free enthalpy which is the crystalline phase, is not reached. In order to saturate nevertheless as many bonds as possible the sp3-tetraeders of the local bonding configuration must be slightly distorted. Hence, instead of defined nearest-neighbor bond angles and bond distances the amorphous phase possesses a (narrow Gaussian) distribution of bond angles and distances. As shown in Fig. 7.9 the magnitude of the energy gap depends on the distance between the nearest-neighbors. The fuzzy distribution of bond distances in amorphous solids therefore leads to a fuzzy band gap: the density of states acquires exponential tails that extend into the forbidden zone (Fig. 7.15). The magnitude of the density of states at any energy reflects the probability for the realization of a particular bond distance and bond angle. States that reach far into the forbidden zone (forbidden in crystals) are due to structural configurations that are realized only rarely. The mean distance between such configurations is therefore large and consequently the wave functions of these states do not overlap. Electronic states deeper in the for-

Fig. 7.15. Schematic density of states of an ideal amorphous material with saturated tetrahedral bonds to the nearest-neighbors (full line). The numbers for the density of states correspond to amorphous silicon. Compared to crystalline silicon (dashed line) the density of states possesses exponential tails into the band gap. Non-saturated bonds in the amorphous network lead to additional states in the forbidden zone. For practical applications of amorphous silicon (e.g. in solar cells) one attempts to reduce the number of unsaturated bonds by adding hydrogen

7.6 Density of States in Non-Crystalline Solids

181

Fig. 7.16. Calculated energy terms below the Fermi level for cubic Ni-clusters consisting of 13, 43, and 79 atoms and non-cubic clusters of the symmetry D2h with 20 and 28 atoms [7.7]. The energy scale refers to the vacuum level. States displayed as thick lines consist of several, nearly degenerate states. The work function of the solid (5.2 eV [6.5]) as well as the high density of d-states at the Fermi level is quite well represented by the cluster with 79 atoms

bidden zone are therefore localized in space. Electrons in these states are not free to move about, unlike the electrons in Bloch states (see also Sect. 9.8). The calculation of electronic states in ``amorphous'' solids is significantly more dicult than for crystalline solids. This is in part due to the fact that the characterization of a solid as being amorphous is not a welldefined one. While the atom positions in a crystal are unique, an infinite number of dierent realizations of an amorphous solid exist. A calculation of the electronic density of states of an amorphous solid requires the input of a particular distribution of bond angles and distances. With that input, one may compose a structure of an amorphous solid and treat this agglomeration of atoms as a large molecule. Such molecules consisting of many atoms or atomic units of the same type are named ``clusters''. The electronic states of clusters are discrete because of the finite number of atoms that make up the cluster. With increasing number of atoms in the cluster a continuous density of states can be defined. Technically, a density of states is frequently calculated by broadening the individual states artificially (Fig. 7.16). Theoretical methods to extend clusters into all three dimensions in a non-periodic way have also been developed. Initially, clusters were merely a construct of the theorists to calculate the electronic properties of amorphous solids. Since the experimental realization of clusters with a defined size and composition [7.8], research on clusters has become a field of its own, situated between Moleculer Physics, Solid State Physics, and Material Science.

182

7 The Electronic Bandstructure of Solids

Problems 7.1 Solve the SchroÈdinger equation for the potential 1; x < 0 V
x; y; z 0; x 0 and calculate the charge density X R
x; y; z
2 e jW k j2 ; kx ; ky ; kz

where the maximum k value is determined by the Fermi energy EF . Sketch R (x) and discuss the result (Friedel oscillations). Consider the cases of a typical metallic electron density of 1022 cm±3 and of a weakly doped semiconductor with a density of 1016 cm±3. 7.2 A two-dimensional electron gas is described in reciprocal space by a two-dimensional lattice whose Brillouin zone is a primitive square. a) Show that the kinetic energy of a free electron in a corner of the first Brillouin zone is a factor of two larger than that of an electron with k vector in the middle of the Brillouin-zone edge. b) How large is the corresponding factor for a primitive lattice in three dimensions? c) Show that band overlap can occur even in a two-dimensional lattice. Do this by drawing the following dispersion relations for the case of free electrons that are perturbed by a weak periodic potential: E
ky

kx 0 ; p E
ky for kx ; a E
k for kx ky : for

7.3 As a simple model of a crystal consider a one-dimensional chain of 2N atoms at distances a0 from each other. Let fi (x±n a0) be the correct wavefunction for an electron with energy Ei at the atom located at n a0 (eigenvalue for a single-isolated atom). Under what conditions can the one-electron wavefunction W (x ) for an electron delocalized over the whole chain of atoms be approximated by a linear combination of atomic orbitals (LCAO) W
x

N X

cn fi
x

n a0 ?

n N

Choose the coecients cn such that for N ? ? the wave-function W (x ) is a Bloch wave.

Problems

183

7.4 a) Consider points in the vicinity of the minimum of an electronic band at suciently small k values that E (k ) can be written in parabolic approximation as ! k2y k2z h2 k2x E
k Ec ; 2 mx my mz with mx , my and mz as positive constants. Show that the density of states D (E ) is proportional to (E±Ec)1/2 around the critical point Ec (k = 0). b) Consider the density of states in the neighborhood of a saddle point, where ! k2y k2z h2 k2x E
k Ec 2 mx my mz with positive mx, my, mz. Show that the density of states can be written near Ec as const for E > Ec D
E / D0 C
Ec E1=2 for E < Ec : Sketch D (E) in the vicinity of (a) a minimum and (b) a saddle point of E
k. 7.5 On the basis of the electronic bandstructure and corresponding density of states, explain why copper, in contrast to many other metals, appears colored, i.e., exhibits pronounced spectral structure in its optical constants in the visible spectral range. 7.6 Explain why and how, for diamond and silicon, the energy of the forbidden band Eg changes with increasing temperature. 7.7 Consider an angle resolved UV photoemission spectroscopy (ARUPS) experiment, where UV photons of energy 40.8 eV are incident on the (100) surface of a cubic transition metal with a work function of 4.5 eV. Photoemitted electrons from d-states at 2.2 eV below the Fermi level are detected at an angle of 45° to the surface normal and in the [100] azimuth. a) Calculate the wave vector k of the emitted electrons. b) What problem arises in deriving the wave vector ki of the electronic state from which the electron is released. Consider the components k|| and k^ (parallel and normal to surface) separately.

Panel V

Panel V Photoemission Spectroscopy

Experiment Photoemission electron spectroscopy is the most important experimental method to acquire information on electronic states in solids [V.1]. The possibility to vary energy, incident angle and polarization of the incident photon and to observe kinetic energy and angle of emerging electrons provides means to probe for all occupied electronic states of solids and characterize their properties. Here we focus on experiments concerned with the valence band structure. A typical experimental setup consists of a combination of an energy analyzer and a lens system as shown in Fig. V.1. The sample is mounted on a goniometer that defines the polar and azimuthal angles of electron emission with respect to the surface orientation. Energy analysis is performed with a hemispherical electrostatic deflector. When equipped with corrections for the fringe fields at the entrance and exit apertures by a suitable grading of the aperture potential (Fig. V.1), energy resolutions down to 1 meV can be realized. To keep the resolution constant during energy scans the analyzer operates at constant pass energy while a lens system provides energy retardation or acceleration to match the kinetic energy of photoemitted electrons to the pass energy. The lens system also defines the angular aperture. The combination of exit slit and electron multiplier as shown in Fig. V.1 is frequently

Rotatable sample

Lens system

hν

Fringe field correction

Hemispherical deflector

Electron multiplier

Fig. V.1. Experimental setup for photoemission spectroscopy

185

replaced by a position-sensitive detector for parallel detection of electrons of dierent energy. Special analyzers even combine (moderate) energy analysis with a display of emission angles on a position-sensitive detector. Light Sources Depending on the photon energy of the light sources, one distinguishes between Ultraviolet Photoemission Spectroscopy (UPS) and X-ray Photoemission Spectroscopy (XPS). The distinction between these two regimes is according to the traditionally available light sources. Ultraviolet radiation is provided by open, dierentially pumped gas discharge lamps. Mostly used are the sharp and intense spectral lines of helium at photon energies of 21.22 eV (HeI) and 40.82 eV (HeII). Less common but occasionally also used are neon and argon at 16.85/16.67 eV (NeI), 26.9 eV (NeII), 11.83 eV (ArI) and 13.3/13.48 eV (ArII). Standard laboratory sources for X-rays are the Mg-Ka1,2 and Al-Ka1,2 emission lines at 1253.6 eV and 1486.6 eV, respectively. The traditional sources have lost some of their importance as synchrotron sources became available for the entire spectral range between 10 eV and several keV. The advantage of synchrotron sources, in particular of undulator beam lines is that they combine high photon fluxes with tunability in a wide spectral range. By varying photon energy and pass energy of the analyzer simultaneously, one can e.g. optimize the cross section for photoemission out of particular electron states and even learn about the unoccupied parts of the band structure. Synchrotron light is polarized, linear-horizontal in the synchrotron plane, left circular and right circular below and above the plane of the ring, respectively, if electrons in the ring circulate clockwise in top view. The polarization oers additional possibilities. By using selection rules, the symmetry of electron orbitals can be determined with linear polarized light, and with circular polarized light, one can distinguish between spin-up and spin-down states via the eect of magnetic circular dichroism. Fig. V.2 displays the experimental set-up at one of the undulator beam lines (beam line 7) of the Advanced Light Source (ALS) at Berkeley, USA [V.2]. With three dierent gratings, the monochromator covers the photon energy range between 60 and 1200 eV. The resolving power of the monochromator E/E is about 8000. The energy resolved photon flux is between 1012 and 1013 s±1. As far as UV-light is concerned these figures of merit are not much better than for the HeI-lamp (%1012 photons per second, E = 3 meV, hence E/E = 7000). Thus, the HeI discharge lamp is still competitive in performance, and orders of magnitude lower in operational cost, if a fixed photon energy of 21.2 eV suces and polarization is not required. The Photoemission Process A simple although not exact way of looking upon photoemission is to consider photoemission as a three-step process: Absorption of electromagnetic radiation and the resulting photoexcitation of an electron from an occupied into an

Panel V

Panel V Photoemission Spectroscopy

Panel V

186

Panel V Photoemission Spectroscopy

8.5 m

13.5 m

18.5 m

28 m 6° 4°

Position monitors

Diffraction grating R = 70 m Entrance slit

Exit slit 5° 4°

R=∞

R = 107 m

R = 57.5 m 1.40 m

Floor

1.33m

Floor

Fig. V.2. The set-up of a the undulator beam line 7 at the Advanced Light Source (ALS) at Berkeley, USA that is commissioned to extended UV-light and soft X-rays. The synchrotron is not drawn to scale. (After Warwick et al. [V.2])

unoccupied state, transport of that electron to the surface, and crossing the potential barrier at the surface (Fig. V.3). In the latter process, the electron looses an a priori unknown amount of momentum perpendicular to the surface, whereby information about the perpendicular component of the wave vector is lost. The valence band regime is mostly probed with ultraviolet light and occasionally with soft X-ray light. The kinetic energy of photo-excited electrons is therefore between a few eV and about 1-2 keV. The information depth of photoemission spectroscopy in solids is given by the mean free path of those electrons and ranges between 3AÊ and 30AÊ depending on the energy. Photoemitted electrons therefore carry information on bulk electronic states as well as on electronic states that are localized to the surface atoms. The wavelength of photons in the UV-regime amounts to a few hundred Angstroms. All atoms within the information depth therefore experience electromagnetic radiation of nearly the same phase. An alternative way of expressing this fact is that the light contributes nearly no momentum and the transitions between the initial and final electron states E(k) are vertical (Fig. V.3a). The photon energy is furthermore outside the regime of collective excitations of the electron gas and outside the regime of extremely strong absorption. The modifications of the electromagnetic field at the surface may then be disregarded. In that case, the absorption of the electromagnetic radiation and therefore the intensity of the photoemission current is proportional to the square of the matrix element of the dipole moment ex, i.e. the vector x* parallel to the electric field with the initial and final Most treatments here formulate ``momentum operator p '' which is correct; leads however, save for a factor, to an identical result in the case of a homogeneous electric field.

*

(a)

187

Panel V

Panel V Photoemission Spectroscopy

(b)

E E (f)(k) k (ext) Ekin Evac hν

k||(ext)= k||(int) EF E(i)(k) k (int)

k Fig. V.3. Illustration of the photoemission process. (a) A photon of energy h excites an electron from the initial state E(i)(k) to the final state E(f)(k) above the vacuum level Evac. The kinetic energy of the photoemitted electron is Ekin = E(f)(k) ± Evac. (b) The wave vectors of the electron inside k(int) and outside k(ext) have the same parallel components since the spatial phase irjj kjj has to be identical to make the wave function continuous at any given point rjj of the surface

state (see Sect. 11.10). The current carried by electrons of a particular ki
el netic energy Ekin into a particular direction given by the wave vector kjj is proportional to: E 2 X X D
el Iph
kjj ; Ekin / j; kjj ; kz jxji; kjj ; kz i; j kz
V:1
Ekin Evac

E
i
kjj ; kz

h
kjj

el

kjj :

Here, i, j denote the initial and final bands, k||, kz are the components of the wave vector in the initial and the final state, and E(i), Evac are the energies of the initial state and the vacuum level. The matrix element is an integral over the unit surface cell and over the information depth along the z-coordinate. The kinetic energy of the photoemitted electron therefore carries the information on the energy of the initial state by virtue of the energy conservation term in (V.1), Ekin

Evac E
i
kjj ; kz h:

V:2

The parallel component of the k-vector is conserved for periodic surfaces, as the electron wave function inside has to phase-match to the wave function outside in order to have the wave function continuous at the surface. The k||-vector of surface states is therefore fully determined by the k||-vector of

Panel V Photoemission Spectroscopy

Panel V

188

1] [11

k||

Photoemission intensity (arb. units)

35.3°

52.5°

[110]

(110) surface

(111) surface [111] direction

(110) surface θ = 35.3° ([111])

(110) surface θ = 52.5°

0 –4 –3 –2 –1 Binding energy of electrons E − EF (eV)

Fig. V.4. Photoemission spectra of Cu(111) and Cu(110) surfaces [V.3] serving to establish the wave vector k111 for bulk electronic states: the two prominent peaks appearing in the spectra along [111] on Cu(111) are found at an angle of = 52.58 in the [110] zone on Cu(110). The magnitude of k111 is determined by considering k|| conservation (V.3). (After Courts and HuÈfner [V3])

the photoemitted electron (Fig. V.3b). The vertical component of the k-vector of bulk states which is lost in the transgression of the surface potential barrier may be recovered by special techniques. One technique is triangulation as illustrated with Fig. V.4. A series of photoemission spectra from a Cu(110) surface in the [110] zone as function of angle with respect to surface normal is compared to the emission spectrum in the [111] direction on a Cu(111) surface. In the latter case, the internal k vector of the emitting electron states is along [111] because of k|| conservation. While on the Cu(110) surface the [111] direction makes an angle of = 35.28 with the surface normal, peaks at the same initial state energies as on Cu(111) are found at = 52.58 (Fig. V.4) because of the refraction of the electrons when they traverse the surface (insert in Fig. V.4).
int We now calculate the modulus of the k vector of the initial states k111 making use of the conservation of the parallel component of the wave vector (Fig. V.3, insert in Fig.V.4):

int

kjj

ext

kjj

int

) k111 sin 35 k
ext sin 52:5 :

V:3

189

The moduli of the wave vectors outside k(ext) are calculated from the kinetic energies of the photoemitted electrons. Thus, the peaks observed at ±2.7eV and ±3.7eV binding energy belong to dierent k111 vectors. Selection Rules in UPS The photoemission process obeys certain selection rules that follow from the matrix element in (V.1). Consider for example a surface with a mirror plane. The electron eigenstates belong to either the odd or the even representation. The final state of electrons with trajectories in the mirror plane is even. The matrix element in (V.1) is then nonzero for s-polarized light (polarization in plane of incidence) and even initial electron states and for p-polarized light (polarization perpendicular to the plane of incidence) and odd initial electron states. Hence, by orienting the sample with respect to the polarization plane of the synchrotron light and by observing electrons emitted in the mirror plane one can immediately determine the symmetry of the initial state. For atomic orbitals with vector character, the p-states, one can furthermore determine the orientation of the orbitals in space from the intensity profile with reference to the polarization of light. Since the vector x in the matrix elements is oriented as the electric field E 0 (s) of the UV-light at the surface, the photoemission intensity from a pz-orbital is proportional to |E z(s)|2, from a px-orbital proportional to |E x(s)|2 and from a py-orbital proportional to |E y(s)|2. By changing the polarization such that either |E x(s)|2, |E y(s)|2 or |E z(s)|2 become zero and looking for the disappearance of the intensity, the orientation of p-orbitals is easily determined. The flux of electrons that are photoemitted from localized orbitals also shows an interesting dependence on the energy of the final state, which follows directly from the matrix element. If, for example, the initial state is an s-orbital the intensity goes through a minimum when the wavelength of the electron in the final state matches approximately the spatial extension of the initial state since positive and negative contributions to the matrix element cancel. Such minima have been discussed first by J. W. Cooper [V.4] and are therefore named Cooper minima.

References V.1 S. HuÈfner: Photoelectron Spectroscopy, 2nd ed., Springer series in Solid-State Sci. Vol. 82 (Springer, Berlin, Heidelberg, New York 1996) H. LuÈth: Solid Surfaces, Interfaces and Thin Films, 4th. edn., (Springer, Berlin, Heidelberg, New York 2001) H. Ibach: Physics of Surfaces and Interfaces (Springer, Berlin, Heidelberg, New York 2005) V.2 T. Warwick, P. Heimann, D. Mossessian, W. McKinney, H. Padmore: Rev. Sci. Instr. 66 (1995) 2037 V.3 R. Courts, S. HuÈfner: Physics Reports 112, 55 (1984) V.4 J. W. Cooper: Phys. Rev. Lett. 13, 762 (1964)

Panel V

Panel V Photoemission Spectroscopy

8 Magnetism

In our previous discussions of the electronic structure of materials we have assumed the one-electron approximation. The energy levels and the bandstructure were calculated for an electron in an eective potential consisting of the potential of the ion cores and an average potential due to the other electrons. Within this model quite acceptable bandstructures can be calculated. However, another aspect of the one-electron model is more important than the qualitative agreement with experiment and the (in principle) simple calculational method: Within the one-electron model it is also possible to understand conceptually the excited states of the electronic system, resulting for example from the interaction with photons and other particles or from thermal excitation. Just as the energy levels of the hydrogen atom serve as a model for describing the energy levels of all elements, so the one-electron model is the basic model for our understanding of the solid state. Furthermore, there are phenomena associated with the collective behavior of the electrons which can nonetheless be tackled within this framework; for example, Thomas-Fermi screening (Sect. 6.5) or the excitation of charge density waves (Sect. 11.9). In the case of magnetic phenomena in solids, in particular ferromagnetism and antiferromagnetism, the one-electron and many-electron aspects are mixed in such a way that it is dicult to formulate a simple basic model. We will consider, for instance, excited states in which one electron spin is flipped but in which all valence electrons take part (spin wave). In addition, the electronic theory of magnetism is complicated by the fact that it contains both collective and local aspects. A particularly important topic in this chapter is the ferromagnetism of the 3 d metals Ni, Co and Fe, which exists due to the exchange interaction between the largely delocalized 3 d electrons. A local description is suitable for most magnetic compounds and particularly for the 4 f transition metals and their compounds. Antiferromagnetism and spin waves can also be described relatively easily in terms of an exchange interaction between localized electrons.

8.1 Diamagnetism and Paramagnetism The physical quantities magnetic field strength, H, and magnetic induction, B, in vacuum, are related by the equation H. Ibach, H. LuÈth, Solid-State Physics, 4th ed., DOI 10.1007/978-3-540-93804-0_8, Ó Springer-Verlag Berlin Heidelberg 2009

192

8 Magnetism

B l0 H

8:1

where l0 = 4 p 10 Vs/Am is the permeability of free space. The magnetic state of the system (Sommerfeld system) will be specified by the magnetization M, which is related to B and H by ±7

B l0
H M :

8:2

It is bewildering that the magnetization M and the magnetic field H have the same dimensions in the SI-system although they are conceptually dierent quantities. One awkward consequence is that the conversion factors from Gaussian units are dierent: For HGaussian into HSI it is 1 Oe = 1 G > 1000/4p Am±1; for MGaussian into MSI it is 1 emu cm±3= 1 G > 1000 A m±1. This may cause confusion since nearly all material constants are tabulated in Gaussian units. Furthermore, original papers concerning the physics of magnetism nearly always refer to the Gaussian system. For the conversion between SI units and Gaussian units an article of Arrot is quite useful [8.1]. The magnetization M of a solid may be understood as the density of magnetic dipole moments m, Mm

N : V

8:3

Because of the conceptual problem discussed above it is useful to replace the magnetic field H by the magnetic flux density B0 = 0H and call B0 the (external) magnetic field. B0 has the units Vs/m2 = T (Tesla). In most cases there is a linear relation between the ``field'' B0 and the magnetization M: l0 M vB0

8:4

where v is the magnetic susceptibility. If v is negative, then the induced magnetic polarization is opposite in sign to the applied field. Such behavior is denoted diamagnetic, while the reverse behavior is termed paramagnetic, and is characterized by v > 0. In general, the susceptibility of atoms, and therefore of solids, comprises a dia- and a paramagnetic component, which we will denote as vd and vp. The paramagnetic component is related to the orientation of intrinsic magnetic moments, which originate from the angular momentum and the spin of the electrons. For instance, the magnetic dipole moment of an electron due to its angular momentum is e X m ri pi lB L
8:5 2m i P with h L = i ri pi and the Bohr magneton lB = (eh/2m) (= 5.7884 .10±5 eV/T = 9.2741.10±24 J/T; 1 T = 1 Tesla = 1 Vs/m2). The negative sign in (8.5) follows from the fact that the electric current has the opposite sense to that of the particle current because of the negative charge of the electron. (The elementary charge e is treated throughout this book as a positive number.) Besides a magnetic moment due to angular

8.1 Diamagnetism and Paramagnetism

193

momentum, the electrons also possess a magnetic moment due to spin, and these add up to give the spin moment of the whole atom X m lB g0 si lB g0 S :
8:6 i

Here g0 is the electronic g factor (g0 = 2.0023) and si are the (negative) electron spins. As already stated (8.5, 6), L and S can, without further ado, be treated as operators. The choice of sign of the spin operator is best made so that the spin operator and the magnetic moment have the same sign. By evaluating the expectation values of the operators L and S for atoms, it can be seen that a nonvanishing expectation value results only for open shells. For closed shells the sum of the angular momentum and spins is 0. In solids, we have open shells for transition metals and rare earths. Paramagnetic behavior is thus expected for both. Besides this paramagnetism due to the electrons, one must also consider diamagnetism. The latter results from the induction of eddy currents by an external magnetic field. According to Lenz's rule, the magnetic moment of these induced currents is opposed to the applied field. The susceptibility thereby acquires a negative, diamagnetic contribution. To calculate this diamagnetic contribution, we must replace the momentum operator in the SchroÈdinger equation, , by +e A. Here A is the vector potential, which is related to the field B0 by

p

p

B0 rot A

divA 0 :

and

8:7

For a homogeneous field B0, a possible choice of vector potential is A

1 2r

B0 :

8:8

It is easy to show that (8.8) fulfills the conditions (8.7). We can now write the kinetic component of the Hamiltonian as 2 1 X 1 X e H kin ri B0
i e A i 2 i 2m i 2m i 2

p

1 X 2m i

p

p 2em 2 i

X e2 B20z X 2
ri i z B0z
xi y2i : 8m i i

p

8:9

In the second step of the calculation we have assumed that B0 is parallel to the z axis, and have used the commutation rule to exchange terms in the triple product. The sum index runs over all electrons. The second term in the above expression is nothing other than the paramagnetism due to the angular momentum, which was discussed above. By comparing (8.9) with (8.5), one sees that the expectation value of the magnetic moment in a state u is m

@hujH jui @B0z

lB hujLz jui

X e2 B0z huj
x2i y2i jui : 4m i

8:10

The first term in (8.10) represents a magnetic moment that exists even in the absence of a magnetic field. This term, together with the occupation statistics

194

8 Magnetism

of the energy levels for dierent orientations of the magnetic moment in an external magnetic field, yields the temperature dependence of the paramagnetism. The second term is responsible for diamagnetism. Due to the spherically symmetric charge distribution of atoms, we can set hujx2i jui hujy2i jui 13 hujr2i jui ;

8:11

and therefore for the susceptibility we obtain (in the SI system) v

e2 n X l hujr2i jui ; 6m 0 i

8:12

where n is the number of atoms per unit volume. In the sum over the matrix elements the electrons in the outer shells are naturally of greatest importance because their mean square distance from the nucleus is largest. If the number of outer electrons is Za, and we insert in place of r2i the square of the ionic or atomic radius ra , then we obtain v

e2 l n Za r2a : 6m 0

8:13

The measured values of the diamagnetic susceptibility for atoms and ions with closed shells are indeed found to be in good agreement with Za r 2a (Fig. 8.1). However, the values indicate that the above estimate should be multiplied by a prefactor of approximately 0.35. From Fig. 8.1 we can see that for typical solid state densities of 0.2 mol/cm3, the susceptibility is about 10±4 (SI), i.e. small compared with 1. A similar order of magnitude results for paramagnetic contributions. We therefore find that, apart from the case of ferromagnetism, to be discussed below, the magnetic susceptibility of solids is small. In contrast, the electric susceptibility is of the order of one or larger. This explains why, in solid state spectroscopy with electromagnetic radiation, which is one of the most important experimental methods, one usually considers only electric eects (Chap. 11). So far we have treated only electrons that are bound to atoms. For free electrons in a metal, (8.10) is not applicable. To calculate the diamagnetism of free electrons, one must solve the SchroÈdinger equation for free electrons in a magnetic field (Panel VIII), and from the energy levels, one can then calculate the free energy in a magnetic field, and from that the susceptibility. This last part, however, is mathematically rather tedious and brings few new insights, and in any case the free electron gas model is only a very crude approximation. It should nonetheless be remarked that the diamagnetism of free electrons does represent a genuine quantum eect. For a classical gas of free electrons, the free energy does not depend on the magnetic field, and thus the diamagnetic susceptibility vanishes. This is already evident in (8.9): the magnetic field shifts the momentum by e A. If one then integrates over all states, and thus over all momenta, the result does not depend on A, and is therefore independent of the magnetic field.

8.1 Diamagnetism and Paramagnetism

195

Fig. 8.1. Molar diamagnetic susceptibility (in cgs units) of atoms and ions with closed shells as function of Za r 2a. In order to obtain the susceptibility of a material, e.g. a gas composed of these atoms or ions, one has to multiply by the density in mol cm±3. If one inserts the value of the ionic radius ra in [AÊ], then the value of Za r 2a immediately provides an estimate for v in units of 10±6 cm3/mol. To convert v to SI units one must simply multiply by 4 p

Besides diamagnetism due to their angular momentum, free electrons also exhibit paramagnetism (Pauli paramagnetism). This part is easy to calculate and we do not even need to involve the free energy. In the absence of a magnetic field, states with dierent spin quantum numbers have the same energy (they are degenerate). In a magnetic field the spins adopt one of two alignments. Electrons with spins parallel to the field lines of B0 are in states whose energy is lowered by 12 g0 lB B0 with respect to the field-free condition. Electrons with spins antiparallel to the field lines have an energy raised by 1 2 g0 lB B0. The energy parabola D
E (Fig. 6.4) splits into two parabolas (Fig. 8.2), which are separated on the energy axis by g0 lB B0. From Fig. 8.2 it follows that, in the approximation k T EF, the volume density of electrons with uncompensated spins is approximately 12 D (EF)g0 lB B0 (crosshatched region in Fig. 8.2). Each of these electrons contributes a magnetic moment of 12 g0 lB, and the resulting magnetization is M 12 D
EF g0 lB B0 12 g0 lB :

8:14

We thereby obtain a temperature-independent paramagnetic susceptibility vp given by vp l0

g20 2 l D
EF l0 l2B D
EF : 4 B

8:15

196

8 Magnetism

Fig. 8.2. Paramagnetism of free electrons. The density of states D
E splits in a magnetic field B0 into two parabolas which are shifted with respect to one another. This leads to a net a magnetic moment due to the excess (uncompensated) electron spins parallel to B0 (cross-hatched area )

If we include the diamagnetic component, which we have not calculated here, we find 1 m 2 v l0 l2B D
EF 1 :
8:16 3 m Here m is the so-called eective mass of the charge carriers, which takes account of the fact that the electrons are moving in a crystal lattice and not in vacuum (Sect. 9.1). According to the value of the eective mass, the charge carriers may show paramagnetic or diamagnetic behavior. We can also estimate the order of magnitude of the susceptibility of the conduction electrons. Values of the density of states at the Fermi level can be obtained from the electronic specific heat (Table 6.2). If m = m, then we obtain, e.g. for the molar susceptibility of sodium, vm = 1.96 10±4 cm3/mol or v = 8.6 10±6 when one multiplies by the density of metallic sodium. Thus even Pauli paramagnetism does not lead to large values of the susceptibility. It is of the same order of magnitude as the diamagnetism of closed shells. One could now close the chapter on magnetic eects in solids and ``file it away'', were it not for the phenomenon of the collective coupling of electron spins which will now be addressed.

8.2 The Exchange Interaction To describe the exchange interaction between localized electrons we return to the hydrogen molecule as the prototype of covalent bonding. The oneelectron approximation has already been discussed in Sect. 1.2. Considering both electrons (labelled 1 and 2), the Hamiltonian operator H (1, 2) can be decomposed into three parts

H
1; 2 H

1 H
2 H w
1; 2 :

8:17

Here H (1) and H (2) are the Hamiltonian operators as in (1.2) expressed in terms of the coordinates of electrons 1 and 2 respectively, and H int (1, 2)

8.2 The Exchange Interaction

197

describes the residual interaction between the electrons. We can recover the one-electron approximation from (8.17) if we neglect H int (1, 2) and set the total wavefunction (without spin) equal to the product of the one-electron solutions. For the ground state this would be W
1; 2 uA
1 uB
1uA
2 uB
2

8:18

where uA and uB are the atomic wavefunctions. It is immediately clear that the eigenvalue problem is separable and the calculation proceeds as in Sect. 1.2. Carrying out the multiplication, (8.18) reads W
1; 2 uA
1uB
2 uB
1uA
2 uA
1uA
2 uB
1uB
2 :

8:19

One sees that states in which both electrons are located on one atom (``ionic states'') are equally represented. This is quite acceptable provided we neglect the repulsive Coulomb interaction or at least absorb it into an eective potential of the ions. For a Hamiltonian with electron-electron interactions, (8.19) is a poor postulate, particularly for nuclei which are far from one another. It is then better to omit the ionic states completely. This leads to the Heitler-London approximation W
1; 2 uA
1uB
2 uB
1uA
2 :

8:20

This formula is symmetric with respect to the coordinates of the electrons. Because the total wavefunction, including the spin function, must be antisymmetric (generalized Pauli principle), the spins in this state must be antiparallel (singlet state). A triplet state with parallel spin orientation is described in space coordinates by the antisymmetric wavefunction W
1; 2 uA
1uB
2

uB
1uA
2 :

8:21

With these two electron wavefunctions we can calculate the expectation value of the energy and, after a few intermediate steps, we obtain: E

hW
1; 2jH jW
1; 2i CA 2 EI 1S hW
1; 2jW
1; 2i

8:22

where EI is the ionization energy of the hydrogen atom, C the so-called Coulomb integral, A the exchange integral, and S the overlap integral. The + sign in (8.22) corresponds to the singlet state.
h2 e2 D1 EI uA
1
8:23 u
1dr1 ; 2m 4p e0 rA1 A C

e2 4 p e0

e2 A 4 p e0

1 1 RAB r12

1 1 RAB r12

rA2

1 juA
1j2 juB
2j2 dr1 dr2 ; rB1

8:24

1 rA1

1 u
1uA
2uB
1uB
2dr1 dr2 ; rB2 A

8:25

1

198

8 Magnetism

S uA
1uA
2uB
1uB
2dr1 dr2 :

8:26

The result for the energy levels in the two-electron model (8.22) is quite different from that in the one-electron model. The interpretation of the energy levels (8.22) is also dierent. We shall examine these dierences with the aid of Fig. 8.3. In the one-electron model, the energy levels can be occupied by either two or one electron(s). Within this model, an excited state corresponds, for instance, to the occupation of the lowest level with one electron and the next higher level with the second electron. The excited state can be a singlet or a triplet state, and the energies are necessarily degenerate. The degeneracy of these two states is easy to see in the formula by neglecting the electron-electron interaction and forming the expectation value of the Hamiltonian (8.17). In the two-electron picture, however, the energy of a single electron is not defined, only a total energy for both. The ground state is, as in the one-electron model, a singlet state but the first excited state is necessarily a triplet state. We see from this example that the energy levels of the calculated band structures in Chaps. 6 and 7 only have meaning within the one-electron picture. In a many-body model the energy of the ground state can only by symbolized by a single total energy, or single eigenvalue. This dierence between single-body and many-body models will be met again in Chap. 10. The energy dierence between the triplet and singlet state is obtained from (8.22) as Et

Es

J2

CS A : 1 S2

8:27

The quantity J gives the separation of the energy levels for parallel and antiparallel spins and is called the exchange constant. For the hydrogen molecule it is always negative and the singlet state is therefore the lower energy state. Using the exchange constant, a model Hamiltonian can be introduced which only aects the spin functions and produces the same splitting be-

Fig. 8.3. Energy levels for a pair of electrons in the one-electron and two-electron models

8.3 Exchange Interaction Between Free Electrons

199

tween the energy levels for parallel and antiparallel orientations (for proof see e.g. [8.1], or textbooks on quantum mechanics)

H spin

2Jr1 r2 :

8:28

The operators r can be represented by the Pauli spin matrices. Ferromagnetic coupling between the electrons is obtained for J > 0. This Heisenberg Hamiltonian is the starting point of many modern theories of magnetism, in so far as the magnetism can be understood within a model that treats only pairwise coupling between electrons. This is not always the case, however, and particularly for typical ferromagnetics such as the 3 d transition metals Ni, Co and Fe, this model is insucient. Besides the Heisenberg Hamiltonian, we require a description of the collective exchange interaction. As an example we will study the free electron gas.

8.3 Exchange Interaction Between Free Electrons Although the exchange interaction for an electron pair in a bond is negative, for free electrons it is positive. This can be shown by considering two free electrons i and j and their pair wavefunction Wij. For electrons with the same spin, the pair wavefunction must be antisymmetric in space coordinates. From this requirement we obtain 1 W ij p
ei ki ri ei kj rj ei ki rj ei kj ri 2V 1 i
ki ri kj rj p e
1 e i
ki kj
ri 2V

rj

:

8:29

The probability that electron i is to be found in volume element dri and that electron j is to be found in volume element drj is then equal to |wij|2 dri drj: jW ij j2 dri drj

1 1 V2

cos
ki

kj
ri

rj dri drj :

8:30

This expression shows all of the crucial features: the probability of finding two electrons with the same spin at the same place vanishes for every ki and kj. As a result, for a particular spin-up electron, the other electrons with the same spin cannot screen the Coulomb potential of the ion cores so well locally, which leads to a reduction of the energy of the spin-up electron. This energy reduction is reinforced if the highest possible percentage of all the electrons have the same spin as the spin-up electron. The net eect is thus a gain in the electronic energy for parallel spins and a collective exchange interaction with positive sign. Before we expand these ideas into a model description of ferromagnetism, it is quite useful to consider the spatial correlation (8.30) further. From (8.30), we can obtain a k-averaged probability if we integrate over the

200

8 Magnetism

Fermi sphere. We introduce relative coordinates between the electrons i and j with r = ri±rj. We then ask what is the probability that a second spin-up electron is at a distance r in a volume element dr. This probability is then P
r"" dr n" dr1

cos
ki

kj r

8:31

with n: the concentration of electrons with the same spin, which is half as large as the total concentration n of electrons. Instead of the probability we can also speak of an eective electron density acting on the spin-up electron, we denote this by Rex (r), because of its origin in the exchange interaction en 1 cos
ki kj r with n" n=2 :
8:32 Rex
r 2 If we now take the average over the Fermi sphere, we obtain en 1 cos
ki kj r Rex
r 2 2

en6 6 61 2 4

1 i
k 2 dki dkj
e i 2 4p 3 k 3 F 1

kj r

0 Rex
r

enB B B1 2 @

e

1
C 1 C ik r dkj ei kj r C : 2 dki e i A 4p 3 k 3 F

i
ki kj r

3 7 7 7 : 5
8:33 a

8:33 b

These integrals may be solved analogously to (3.40): en Rex
r 1 2

9

sin kF r

kF r cos kF r2
kF r6

! :

8:34

The total charge density seen by a free electron is the sum of the charge density of electrons with the same spin and the homogeneous charge density e n/2 of the electrons with opposite spin, for which the spatial part of the wavefunction remains symmetric and thus unaltered, ! 9
sin kF r kF r cos kF r2 Reff
r e n 1 :
8:35 2
kF r6 This charge density is plotted in Fig. 8.4. The charge density at r = 0 is reduced as a result of the exchange interaction. This creates an ``exchange hole'', whose size is approximately equal to twice the reciprocal Fermi vector. According to Table 6.1 the radius is about 1±2 AÊ. We can use the eective charge density Re (r) to form a new (``renormalized'') SchroÈdinger

8.4 The Band Model of Ferromagnetism

201

Fig. 8.4. Effective charge density seen by an electron in an electron gas. Due to the exchange interaction, the density of electrons with the same spin orientation in the neighborhood of a particular electron is reduced (``exchange hole''). If this electron moves, it must drag the exchange hole with it and thus its effective mass is raised. Furthermore, the existence of an exchange hole implies a positive exchange coupling. From this we can obtain a model for the ferromagnetism of band electrons

equation for the free electron gas and this leads us to the Hartree-Fock approximation. We note that (8.35) does not properly reproduce the electronelectron correlation because the Coulomb interaction in fact forbids the presence of two electrons with the same spin at the same place. Furthermore, the correlation (8.30) between two electrons that are arbitrarily far apart is an unrealistic result of the assumption of plane waves.

8.4 The Band Model of Ferromagnetism We now wish to construct a simple band model of ferromagnetism using the qualitatively derived renormalization of the one-electron levels due to correlation of electrons bearing the same spin. The model is due to Stoner and Wohlfarth. For the renormalized electron energies we make the ansatz E"
k E
k

I n" =N ;

E#
k E
k

I n# =N ;

(8.36)

E (k) are the energies in a normal one-electron bandstructure, n: and n; are the number of electrons with corresponding spin, and N is the number of atoms. The Stoner parameter I describes the energy reduction due to the electron correlation. Its dependence on the wave vector will be neglected in this model. We now introduce the relative excess of electrons of one spin type

202

8 Magnetism

R

n"

n# N

:

8:37

This quantity is, apart from a factor lB (N/V), equal to the magnetization M (8.3). Furthermore, to simplify the formula, we subtract I (n: + n;)/2 N from the one-electron energies and obtain, in place of (8.36), ) E"
k E~
k I R=2 with E~
k E
k I
n" n# =2N :
8:38 E#
k E~
k I R=2 The pair of equations (8.38) corresponds to a k-independent splitting of the energy bands with dierent spin. The k-independence of the exchange splitting is, of course, only an approximation. Theory nevertheless indicates that it holds to within a factor of about two. The value of the splitting depends on R, that is on the relative occupation of the sub-bands, which in turn is given by Fermi statistics. We therefore arrive at the self-consistency condition: R

1X f"
k N k 1X N

k

e

f#
k 1

1

k

E~
k I R=2 EF = T

1

e

k

E~
kI R=2 EF = T

1

:

8:39

Under certain conditions this equation has a non-zero solution for R, that is to say, a magnetic moment exists even in the absence of an external field, thus leading to ferromagnetism. It is possible to find a criterion for the appearance of ferromagnetism. For this purpose we expand the right-hand side of the equation for small R. Making use of the relation Dx Dx 2 Dx 3 000 0 f x f
x
8:40 f x f
xDx 2 2 3! 2 we obtain R

1 X @f
k IR N k @E~
k

1 1 X @ 3 f
k
I R3 : ~
k3 24 N k @E

8:41

In this formula, the first derivative of the Fermi function is negative, while the third derivative is positive. The condition for ferromagnetism (R > 0) is therefore I X @f
k 1 >0:
8:42 ~
k N k @E The derivative of the Fermi function @f=@E~ obviously has its largest value for T ? 0 (Fig. 6.6). If the condition (8.42) is to be fulfilled at all, then it will be easiest at T = 0. For the case of T = 0 it is a straightforward matter to perform the summation over all k values:

8.4 The Band Model of Ferromagnetism

1 X @f
k V @f dk ~ N k @E~
k
2 p3 N @E
V 1 1V dk d
E~ EF D
EF : 3 N 2N
2 p

203

8:43

Here we have taken account of the fact that at T = 0, the Fermi function is ~ is equal to the d-function a step function and the first derivative @f=@E ~ EF . The factor 1/2 originates from the fact that, according to (8.39) d
E and (8.41), the sum over k and also the integral over the electrons is taken over only one spin type, while the usual definition of the density of states considers the number of electrons with positive and negative spins per unit volume. The sum is thus equal to half the density of states for electrons at the Fermi level, in relation, however, not to the volume but to the number of atoms. We introduce the density of states per atom and spin as V D~
EF D
EF : 2N

8:44

The condition for ferromagnetism to occur at all is then simply ID~
EF > 1 :

8:45

This is the so-called Stoner criterion for the existence of ferromagnetism. Under the assumption that this criterion is fulfilled, (8.42) also yields the temperature at which the magnetic moment disappears (Curie temperature). The Curie temperature is the point at which (8.42) becomes an equality instead of an inequality. This will be considered in the next section. Figure 8.5 shows the Stoner parameter, the density of states and their product from a theoretical treatment by Janak [8.2]. The theory correctly predicts that ferromagnetism exists only for the elements Fe, Co, and Ni. For the elements of the 4 d series, the density of states and the Stoner parameter are too small to achieve the ferromagnetic state. Nevertheless, there is a considerable enhancement of the magnetic susceptibility due to the positive exchange interaction of the band electrons. For an external magnetic field B0, (8.39) contains, in addition to the exchange splitting of I R/2, a splitting of lB B0. In a first approximation for R at T = 0, (8.41) then becomes R D~
EF
I R 2lB B0 : For the magnetization M one thus obtains N N M lB R D~
EF I M 2l2B B0 V V ~ N D
EF M 2l2B B0 : V 1 I D~
EF

8:46

8:47

204

8 Magnetism

Fig. 8.5. (a) Integral of the exchange correlation (Stoner parameter) I as a function of the atomic number (after [8.2]). (b) Density of states per atom D~ (EF); (c) the product of the density of states D~ (EF) and the Stoner parameter I. The elements Fe, Co and Ni with values of ID~ (EF) > 1 display ferromagnetism. The elements Ca, Sc and Pd come very close to achieving ferromagnetic coupling

The numerator is just the normal Pauli susceptibility of band electrons (8.15), which is now considerably enhanced, however, by the denominator. If we denote the Pauli susceptibility by v0, we obtain v

1

v0 : I D~
EF

8:48

Janak [8.2] has calculated the factor v/v0 and obtained values as large as 4.5 (Ca), 6.1 (Sc) and 4.5 (Pd). Thus, together with the rather high density of states, one also finds relatively large values for the susceptibilities of these elements. A direct comparison with experiment, however, must also take into account the magnetism due to angular momentum. It turns out that the previous assertion that v1 always remains valid.

8.5 The Temperature Behavior of a Ferromagnet in the Band Model

205

8.5 The Temperature Behavior of a Ferromagnet in the Band Model We now turn to the temperature dependence of the saturation magnetization of a ferromagnet. For this purpose one could, in principle, evaluate (8.39) with the aid of a one-electron bandstructure calculation. However, the associated mathematical eort would not be rewarded: the k-independent and delocalized treatment of the exchange interaction does not provide any quantitatively significant results. A qualitative, but for our purposes quite sucient, picture of the temperature behavior can be obtained from a highly simplified density of states model, which keeps the amount of mathematics to a minimum. Let us look at the density of states of Ni (Fig. 8.6 a), taken from a bandstructure calculation by Callaway and Wang [8.3]. The

Fig. 8.6. (a) Calculated density of states of nickel (after [8.3]). The exchange splitting is calculated to be 0.6 eV. From photoelectron spectroscopy a value of about 0.3 eV is obtained. However the values cannot be directly compared, because a photoemitted electron leaves a hole behind, so that the solid remains in an excited state. The distance D between the upper edge of the d-band of majority spin electrons and the Fermi energy is known as the Stoner gap. In the bandstructure picture, this is the minimum energy for a spin flip process (the selectrons are not considered in this treatment). (b) A model density of states to describe the thermal behavior of a ferromagnet

206

8 Magnetism

largest contribution to the density of states at the Fermi level is provided by the d electrons, firstly because of their high number (9 per atom, or, more precisely, 9.46 per atom; see below), and secondly because the d band is only 4 eV wide (in contrast to the s band). In addition, the exchange splitting for s electrons is small. It is thus the diering occupation of the d bands for majority and minority spins that leads to the magnetization. For nickel at T = 0, this is given simply by the number of unoccupied d states in the minority band. From the measured magnetization at T = 0, the number of d holes is found to be 0.54 per atom in the case of nickel, i.e., the eective magnetic moment is lBe*0.54 lBe per atom. The variation of the magnetization with temperature and the existence of the Curie point at which the magnetization vanishes, result from the interplay of the exchange splitting, the Fermi statistics and the density of states near the Fermi level, according to (8.39). For a qualitative discussion of (8.39), we do not need the actual functional behavior of the density of states, and it is sucient to replace the sharp peak in the density of states at the upper edge of the d band with a dfunction in energy (Fig. 8.6 b). If, in addition to the exchange splitting, there is also a field splitting as in (8.46), our model density of states would be D~
E

lBeff d
E lB

EF

lB B0

IR=2 d
E

EF lB B0 IR=2 :
8:49

Since the states for majority and minority spin have equal weight in this model, the Fermi level always lies midway between these two levels, a feature that is already included in the above expression. In place of (8.39) we obtain ! lBeff 1 1 R :
8:50 lB
lB B0 IR=2=k T
lB B0 IR=2=k T e 1 e 1 We now look for ferromagnetic solutions to this equation, i.e., solutions ~ = lB / with R 0 at B0 = 0. With the abbreviations Tc = I lBe /lB 4 k and R lBe R, equation (8.50) becomes R~

1 e

2R~ Tc =T

1 1

e2R~ Tc =T

1

tanh

~T c R T:

8:51

In limiting cases this equation has the solutions R~ = 1 for T = 0 and R~ = 0 for T = Tc . Thus Tc is identical to the previously introduced Curie temperature, above which the spontaneous magnetization vanishes. The behavior over the whole temperature range is shown in Fig. 8.7. Because the magnetization M is proportional to R, Fig. 8.7 should reproduce the temperature dependence of the spontaneous magnetization of a ferromagnet. The agreement with the experimental observations is quite acceptable (Fig. 8.7). For the limiting cases T Tc and T*Tc , the right-hand side of (8.51) can be expanded to give

8.5 The Temperature Behavior of a Ferromagnet in the Band Model

207

Fig. 8.7. Magnetization of a ferromagnet below the Curie temperature Tc. Experimental values for nickel from [8.4, 8.5]

R~ 1 R~

2e

p 3 1

2Tc =T

T Tc

T Tc ;

1=2

T Tc ; R~ 1 with

8:52 tanh x x

1 3 x ... : 3
8:53

However, neither of these equations is confirmed by experiment. The critical exponent in the vicinity of the Curie point is 13 (Fig. 8.8) and not 12. The behavior at low temperature is likewise incorrectly described by (8.52). This is due to the fact that, in addition to the spin-flip accompanying the excitation from one band to another, other elementary excitations with smaller quantum energy are possible in a ferromagnet, and these can also cause spin-flip (Sect. 8.8). Above the Curie temperature, (8.50) yields a magnetization only when the field B0 is non-zero. We can expand the Fermi function for small R and B0 to give l Tc ~ R~ B B0 R T kT l R~ B

k

1 T

Tc

B0 :

or

8:54

8:55

As T approaches Tc from above the paramagnetic susceptibility should thus diverge according to the law

208

8 Magnetism

Fig. 8.8. Magnetization in the vicinity of the Curie temperature. The experimental values for nickel are from [8.4, 8.5]. The critical exponent in the vicinity of the transition to the paramagnetic phase above the Curie temperature is 1/3 and not 1/2 as predicted by the simple model

v

C T

Tc

:

8:56

This is the so-called Curie-Weiss law in which C is the Curie-Weiss constant. The Curie-Weiss law is experimentally fulfilled for T Tc. As Tc is approached, one observes deviations from this law, and a better description is a decrease proportional to (T±Tc)±4/3. According to our model the CurieWeiss constant C is related to the saturation magnetization at T = 0. This interrelation, however, gives a value for C which is too small. We could also try to use the relationship between the Stoner parameter I and the Curie temperature Tc (in this model Tc = I lBe /4 lB k ) to estimate a value of Tc from the measured values of the exchange splitting. This approach yields values of Tc that are much too large. The failure of our simple model in these respects does not, however, lie in the simple bandstructure. It is due to the fact that the model does not correctly treat excited states. The Curie-Weiss law and the temperature dependence of the spontaneous magnetization are often derived in a mean field approximation, in which the exchange interaction is replaced by an average ``internal'' field. The derivation chosen here, whose principles are due to E. C. Stoner, is equivalent to the mean field approximation in that it allows no spatial variation of the spin distribution. Our treatment illustrates the role of the bandstructure more clearly than the conventional mean field approximation.

8.6 Ferromagnetic Coupling for Localized Electrons

209

8.6 Ferromagnetic Coupling for Localized Electrons Whereas the magnetic behavior of d-band transition metals is well described in the band model, the approach developed in Sect. 8.2 based on the exchange interaction between two localized electrons is particularly well suited to the rare earths with their partly filled f shells and to many ionic compounds of the d and f transition metals. The starting point is the Heisenberg Hamiltonian introduced in (8.28) for the exchange interaction between two electrons. In the following model treatment of ferromagnetism, we assume a primitive lattice of atoms each having one unpaired electron with zero angular momentum. This model of a spin lattice illustrates the essential consequences of the exchange interaction in a lattice. Taking into account an additional external magnetic field B0 , we obtain the Hamiltonian X XX H Ji d Si Si d g lB B0 Si :
8:57 i

i

d

The index i runs over all atoms and the index d over all the neighbors of an atom that participate in the exchange interaction. Unfortunately, the Heisenberg operator is a non-linear operator. Solutions can only be found in special cases or by introducing a linearizing approximation. One such approximation is the mean field approximation which will be discussed now. In the mean field approximation the operator product in (8.57) is replaced by the product of the spin operator Si and the expectation value of the spin operators of the neighbors hSi di. In the mean field approximation the Hamiltonian therefore becomes ! X X H MF Si Ji d hSi d i g lB B0 :
8:58 i

d

The exchange interaction thus acquires the character of an internal field BMF

1 X Ji d hSi d i : g lB d

8:59

For homogeneous systems (without a surface), h Si di is the same for all atoms. The average value h Si di = hSi can be expressed in terms of the magnetization M g lB

N hSi V

8:60

with N/V the number of atoms per unit volume. We therefore obtain for the mean field BMF BMF

V mJM ; Ng2 l2B

8:61

210

8 Magnetism

where the exchange interaction is restricted to the m nearest neighbors. The Hamiltonian in the mean field approximation (8.58) is now mathematically identical to the Hamiltonian of N independent spins in an eective magnetic field Be = BMF + B0. Its eigenvalues are E 12 g lB Beff

8:62

for each electron spin. We denote the number of electrons in states with spin parallel and antiparallel to the B-field by N: and N;. In thermal equilibrium one has N# e N"

k

g lB Beff = T

8:63

and the magnetization is thus 1 N" N# 1 N 1 g lB tanh g lB Beff =k T : M g lB 2 V 2 V 2

8:64

This equation together with (8.61) has non-zero solutions for the magnetization (even without an external magnetic field) provided J > 0, i.e., whenever there is ferromagnetic coupling of the spins. With the abbreviations Ms

N1 gl V2 B

8:65

and

Tc 14 m J=k

8:66

we obtain from (8.61, 8.64), and with no external magnetic field B0 Tc M M
T=Ms tanh : T Ms

8:67

This equation is equivalent to (8.51). It means that the temperature behavior of the magnetization in the band model and in the model of localized electrons is the same. Therefore, for T ? 0 and T & Tc one finds M
T Ms
1

2e p M
T=Ms 3 1

2Tc =T

T Tc

; 1=2 ;

T Tc

8:68

T Tc :

8:69

Tc is therefore the critical temperature at which the spontaneous magnetization vanishes. It depends on the strength of the exchange coupling and on the number of nearest neighbors. Interestingly, the critical exponent in (8.69) does not depend on the dimensionality of the system. A planar lattice has the same critical exponent in the mean field approximation as a 3 d lattice, but its Tc is smaller because of the reduced number of nearest neighbors. This leads to an interesting behavior for the magnetization near the surface of a ferromagnet.

8.7 Antiferromagnetism

211

In the mean field approximation not only the magnetization, but also the short-range order of the magnetic moments vanishes at Tc. In reality a certain degree of short-range order survives. The Curie temperature is merely the temperature at which the magnetic order vanishes on a large length scale. For temperatures above Tc, we can once again derive the Curie-Weiss law for the susceptibility. With an external field B0, and using the series expansion (8.68), we obtain from (8.64) M
T

g2 l2B N 1 B0 : T Tc 4Vk

8:70

8.7 Antiferromagnetism Up until now we have assumed ferromagnetic coupling of the electron spins, i.e., J > 0. A number of compounds, for example, the oxides of Fe, Co and Ni, display antiferromagnetic coupling between the transition metal d electrons. They possess the NaCl lattice structure, i.e., the lattices of the paramagnetic d metal ions and of the O2± ions each form a face-centered cubic sub-lattice. In the antiferromagnetically ordered structures, the metal ions form a magnetic elementary cell which is no longer face centered, but possesses a complicated magnetic superstructure. The magnetic behavior of an antiferromagnet will be treated within the mean field approximation for a simple magnetic superstructure. This superstructure should be constructed in such a way that all nearest neighbors have antiparallel spins (Fig. 8.9). In a model treatment with antiferromagnetic coupling (J < 0) we can now apply (8.60±8.64) to each magnetic sub-lattice separately. We note that the

Fig. 8.9. (a) A model crystal with antiferromagnetic orientation of the nearest neighbor spins. (b) An equally simple spin structure, but with a tetragonal lattice, is observed for the compounds MnF2, FeF2 and CoF2. In this case the atoms along the c axis are the nearest neighbors. If the transition metal ions form a face-centered cubic lattice, it is topologically impossible to have only antiferromagnetic orientation between nearest neighbors. The magnetic superstructures become correspondingly more complex

212

8 Magnetism

mean field for the sub-lattice with positive spin orientations is created by the sub-lattice with negative spins, and vice versa. For the antiferromagnetically ordered state we therefore obtain the pair of equations ! 1 N V M g lB tanh mJM ;
8:71 2 V 2 k TN g lB ! 1 N V mJM ;
8:72 M g lB tanh 2 V 2 k TN g lB where M + and M ± are the magnetizations of the two spin sub-lattices and N + = N ± is the number of metal ions in each of the sub-lattices. In the antiferromagnetic state M + = ±M ± and we obtain, in analogy with (8.67), ! 1 N V tanh M g lB mJM
8:73 2 V 2 k TN g lB and a corresponding equation for M ±. The magnetization of the sub-lattice vanishes above a critical temperature which is called the NeÂel temperature. It is analogous to the ferromagnetic case TN

1 mJ : 4 k

8:74

The NeÂel temperature is positive since we now have J < 0. In calculating the susceptibility we must dierentiate between the cases of parallel and perpendicular orientation of the external field relative to the direction of the spins, at least for temperatures smaller than TN. We first treat the case in which the external field B0 is parallel or antiparallel to the spins. The external field causes only minor changes in the magnetization of the two spin sub-lattices; these we denote by DM+ and DM ±. Instead of (8.71) and (8.72), we now obtain, with an additional field B0 1 N 1 1 gl tanh M DM g lB 2 2 B kT V Vm J
M DM B ;
8:75 0 N g2 l2B 1 N 1 1 g lB tanh M DM g lB 2 2 V kT Vm J
M DM B0 :
8:76 N g2 l2B Taking into account that M+ = ±M ± and N+ = N ± : N/2, and expanding (8.75) and (8.76) as series for small DM, B0, we find

8.7 Antiferromagnetism

1 l2B g2 N DM DM DM B0 cosh2
f 4 k T V

f

TN M
T T M s

TN DM T

213

! with

8:77

8:78

and

1 N M s g lB 2 V

8:79

where M s is the saturation magnetization of one spin sub-lattice. For temperatures above the NeÂel temperature, the magnetization of the sub-lattices vanishes and f is equal to zero. No particular direction in the crystal is any longer distinguishable and the susceptibility is isotropic: v
T l0

g2 l2B N 1 : 4 V k T TN

8:80

We thus obtain a temperature dependence similar to the Curie-Weiss law (8.70), but the critical temperature now appears with a reversed sign. At the NeÂel temperature itself, the susceptibility remains finite. For temperatures far enough below the NeÂel temperature M + (T) = M + s and we obtain vk
T l0

g2 l2B N 1 ; 4 V k T cosh2
TN =T TN

8:81

which for low temperatures can further be approximated by vk
T l0

g2 l2B N e V kT

2TN =T

T TN :

8:82

This expression for the susceptibility and the equations (8.75, 8.76) are valid only for an external field oriented parallel to the polarization of the spin sub-lattice. For the direction perpendicular to the spin orientation, the Hamiltonian (8.58) should be interpreted as a classical energy equation. In an external field, each spin sub-lattice rotates its magnetic moment by an angle in the direction of the field B0. The energy of an elementary magnet in the field B0 is then Er

1 2 g lB B0

sin 12 m J cos :

8:83

The magnitude of the second term can be derived by considering that the energy needed to reverse an elementary magnet is mJ (8.27). The equilibrium condition @Er =@ 0 leads, for small angles , to

8:84

214

8 Magnetism

g lB B0 : mJ

8:85

With the magnetization M M M 12 g lB N=V

8:86

one obtains for the susceptibility below TN the (approximately) temperature-independent value v?

g2 l2B N g2 l2B N ; 2 m J V 2 mjJjV

8:87

which is equal to the value of v at the NeÂel temperature. The overall behavior is sketched in Fig. 8.10. It should be noted that the dierence between v|| and v^ is only measurable experimentally if a single magnetic domain is present. This is not the case, for instance, in lattices with many equivalent crystallographic directions for the possible magnetic orientation. Furthermore, the characteristic temperature in the equation for the susceptibility, (8.80), is only equal to the NeÂel temperature if the exchange interaction is confined to nearest neighbor metal ions. If an additional exchange coupling J2 between next nearest neighbors exists, then TN in (8.80) is replaced by a characteristic temperature h= TN. For a simple rock salt type lattice one obtains h TN

J1 J2 : J1 J2

8:88

Thus h is larger than TN when the coupling between next nearest neighbors is antiferromagnetic and smaller than TN if the coupling is ferromagnetic. Both cases are actually observed. It should also be noted that in lattices containing several dierent kinds of transition metal ions, or transition me-

Fig. 8.10. Schematic representation of the magnetic susceptibility of an antiferromagnet. Below the NeÂel temperature TN (i.e., in the antiferromagnetically ordered state) the susceptibility differs for parallel and perpendicular orientation of the magnetic field relative to the spin axis

8.8 Spin Waves

215

tal ions in dierent valence states, the magnetic moments are not equal. Even if the coupling between the spins is antiferromagnetic, there will be a residual magnetization. This kind of magnetism is called ferrimagnetism, because is was first identified in ferrites.

8.8 Spin Waves The energy necessary to reverse the spin of a particular electron is given by the exchange interaction. This is true in both the localized and band models. In the band model, the reversal of the spin of an electron means an interband transition of an electron into the corresponding exchange-shifted band. The minimum energy necessary to flip a spin in the band model is the energy separation between the upper edge of the majority spin band and the Fermi level, the so-called Stoner gap (D in Fig. 8.6). We will now learn about another excitation, in which one spin is also reversed, but only as an average over the whole crystal. In other words, we are dealing with a collective excitation of all spins. The necessary energy is considerably smaller and may even become zero. To derive this excitation we begin again with the spin Hamiltonian (8.57) consider, however, explicitly the properties of the spin operator in (8.57). The x-, y-, and z-components of the spin operators can be represented by the Pauli spin matrices 1 1 0 1 0 1 1 0 i z x y S ; S ; S :
8:89 1 2 0 2 1 0 2 i 0 Instead of the cartesian components S x and S y, it is more convenient to use the spin reversal operators 0 1 S Sx i Sy and
8:90 0 0 0 0 x y iS :
8:91 S S 1 0 The eect of these operators on the spin states 1 0 ji and jbi is 0 1 S ji 0 ; S jbi ji ; S jbi 0 ; S ji jbi :

8:92
8:93

The operators S and S therefore switch the spin to ``+'' or ``±'', and give zero if the spin is already in the state ``+'' or ``±''. The operator S z ``prepares'' the eigenvalues in the usual way: +

±

S z ji 12 ji ; S z jbi

1 2 jbi

:

8:94

216

8 Magnetism

Armed with these equations, we can begin to rewrite the Hamiltonian of a spin lattice in terms of the new operators. For a zero external field and an exchange coupling J between nearest neighbors (index d), substitution of (8.90, 8.91) into (8.57) yields XX z H J Siz Sid 12
Si Sid Si Sid :
8:95 i

d

We assume ferromagnetic coupling between the electron spins (J > 0). In the ground state all spins are therefore oriented. Such a state is described by the product of the spin states of all atoms Q j0i jii :
8:96 i

It is immediately clear that this state is an eigenstate of the Hamiltonian (8.95), since the operators S+ S ± and S ± S+ yield zero and the S z components leave the state unaltered with the corresponding eigenvalue of S z as a prefactor PP H j0i 14 Jj0i 1 14 m J Nj0i :
8:97 i

d

A state with a reversed spin on atom j can be obtained by applying S ±j to the ground state Q j#j i Sj jin :
8:98 n

This state, however, is not an eigenstate of H because applying the opera± tors S + j S j + d inside H would shift the reversed spin to the atom j + d and create a dierent state. On the other hand, the linear combination 1 X i k rj e j#j i
8:99 jki p N j is an eigenstate. This state represents a spin wave. The eigenvalues of S zi and (S xi )2 + (S yi )2 are conserved quantities with expectation values independent of the atom i. The expectation values of S xi and S yi vanish. The spin therefore precesses around the z axis with a phase shift between atoms that is determined by the wave vector k (Fig. 8.11). We now apply H to the spin wave state and obtain

Fig. 8.11. Schematic representation of a spin wave

8.8 Spin Waves

1 X H jki p ei k rj N j

"

1 m J
N 4 #

217

1 2j#j i m Jj#j i 2

1 X J j# i j#j d i : 2 d jd

8:100

By shifting the index j in the last two terms we can also express this result as " # 1 1 X i k rd i k rd H jki mJN Jm J
e e 4 2 d 1 X i k rj p e j#j i :
8:101 N j The state jk i is therefore an eigenstate with the eigenvalue ! 1 X i k rd E E0 J m e ei k rd ; 2 d

8:102

where E0 is the energy in the ferromagnetic ground state. As we will immediately see, this result is particularly significant for small k values. When k is small, (8.102) can be approximated by E E0 12 J

P

d
k

rd 2 :

8:103

This is the characteristic dispersion relation for ferromagnetic spin waves. According to this relation, the energy required to flip a spin vanishes for small k. In Fig. 8.12 a, the dispersion relation is plotted together with the spectrum of one-electron excitations which also reverse a spin. These so-called Stoner excitations require an energy mJ for k = 0. For k = 0 there is a whole spectrum of possibilities resulting from the dispersion of the one-electron states (Fig. 8.12 b). In the region of the one-electron excitations, spin waves can decay into electron excitations. This reduces the lifetime of the spin waves and also aects the dispersion. Spin waves can be excited thermally and also by energy and momentum exchange with neutrons. Neutron scattering therefore allows an experimental determination of the dispersion curve of spin waves. The results for nickel are displayed in Fig. 8.13. The thermal excitation of spin waves has an influence on the behavior of the magnetization at low temperature. We recall that the excitation of a spin wave flips on average one spin and hence reduces the magnetic moment. The magnetization of a spin lattice thus becomes 1 1X M Ms g lB n
k ;
8:104 2 V k where n (k) is the number of excited spin waves with wave vector k. If we neglect the fact that the Heisenberg operator is actually non-linear and

218

8 Magnetism

Fig. 8.12. (a) Spin wave dispersion relation and the spectrum of single electron excitations with spin reversal in a model ferromagnet. (b) Model band structure with an exchange splitting I = mJ and a Stoner gap D

Fig. 8.13. Experimental dispersion relation for spin waves in nickel along the [111] direction [8.6]. The measurements were made at T = 295 K. The dashed line shows a dependence of the quantum energy proportional to k 2. Deviations from this line are due firstly to the exchange interaction between more distant neighbors, and secondly to the onset of one-electron excitations. The latter cause a reduction in the lifetime of the spin waves, leading to a lifetime broadening of the spectra (shaded region)

8.9 Crystalline Anisotropy

219

proceed as though the spin waves could be superposed, then the energy eigenvalues would be the same as for a harmonic oscillator P E
k n
k 12 J d
k rd 2
8:105 and the occupation statistics would likewise correspond to the harmonic oscillator. The temperature dependence of the magnetization at low temperature can be calculated as in Sect. 5.3 and we obtain M
T

M
0

T 3=2 :

8:106

This is the T 3/2 Bloch law, which replaces the exponential dependence (8.52), appropriate for a ferromagnet without spin wave excitations. The spin wave excitation is also observable in the specific heat where a T 3/2 term appears in addition to the T 3 term due to phonon excitation.

8.9 Crystalline Anisotropy Magnetization of a Specimen As demonstrated in previous sections, the basic physics of magnetism can be understood without specific reference to a crystal structure. The structure becomes important when the (average) magnetization of a specimen as function of an applied external field is considered since the magnetization depends on the orientation of the magnetic field with respect to the crystal axes. This crystalline anisotropy is caused by the spin-orbit coupling which couples the spin orientation to the orientation of the electron orbitals. Thereby, the magnetic energy of a ferromagnetic crystal depends on the orientation of the magnetization relative to the crystal axes. Although the energies associated with a rotation of the magnetization are relatively small, the resulting anisotropy is all-important. Without magnetic anisotropy, even the venerable macroscopic manifestation of magnetism, the compass needle, would not exist, and neither the possibility to store information in the orientation of magnetic moments that has become an indispensible part of today's life. The orientation of the magnetization that leads to the lowest energy is called the easy orientation and the corresponding crystal axis is the easy axis. A ferromagnetic crystal in thermal equilibrium has its magnetization along the easy axis. For hcp-cobalt e.g., this is the hexagonal c-axis. The magnetization is therefore oriented in one of the two directions parallel to the c-axis. A homogeneous magnetization of an entire specimen leads to a large external field (and to a depolarization field to be discussed later). In order to minimize the energy associated with those fields, the magnetization breaks up into two or more domains of opposite magnetization. If the crystal is heated above the Curie temperature and cooled down again,

220

8 Magnetism

(average) Magnetization M

Ms Mr

H⊥

H|| –Hc

Hc –Mr –Ms

Magnetic field H Fig. 8.14. Schematic plot of the magnetization M of a ferromagnet with a single easy axis versus the magnetic field H. Dashed line: initial magnetization starting from zero, H parallel to easy axis. Solid lines: magnetization hysteresis, H parallel to easy axis. Dash-dotted line: H perpendicular to easy axis

the number and size of the two types of domains is about equal, so that the average magnetization of the sample is nearly zero. In an external magnetic field oriented along the c-axis, the total magnetization rises by merely moving the boundaries between the domains to let one type of domain grow at the expense of the other (left insert in Fig. 8.14). Since external fields need not work against the magnetocrystalline anisotropy, the average magnetization of the sample rises steeply with the applied field and saturates at comparably small fields with only a single domain orientation surviving (Fig. 8.14). This domain type still prevails after the external field has been removed. The remaining average magnetization is called the remanence Mr. To bring the magnetization of the sample back to zero one needs to reverse the external field up to a value ±Hc which is called the coercive field. With increasing magnetic field in the reverse direction, the magnetization eventually saturates again, now in the reverse direction. In total one runs through a hysteresis loop (solid line in Fig. 8.14). The loop is symmetric if the system is symmetric with respect to the H||-axis, which is the case for typical ferromagnets. Manufactured systems that feature a polar axis are discussed in Panel VII. The area of the hysteresis loop is the energy per volume required to move the boundaries between the domains through a full cycle. The energy and thus the remanence Mr and coercive field Hc depends on nature of the material, mostly on the concentration of defects, which tend to pin the domain walls, thereby increasing the friction forces involved in their rearrangement. Materials with a large hysteresis, preferably with a remanence near saturation, are ideally suited for permanent magnets

8.9 Crystalline Anisotropy

221

and magnetic data storage media. In other technical applications, e.g. in transformer cores, one wants no remanence at all to keep the energy losses low. Perfect crystals and certain alloys (-metal, permalloy, ferrites) feature small or no remanence. A magnetization perpendicular to the easy axis in response to an external field turns the magnetization out of the easy direction (insert on the right in Fig. 8.14). Turning the magnetization away from the easy direction requires work. Accordingly, the magnetization rises but rather gradually with increasing external field. When the field is removed the magnetization inside the domains snaps back to become parallel to the c-axis. Hence, there is no remanent magnetization of the sample as a whole. Rotating the magnetization does not require work against friction forces, so that there is no significant hysteresis. Anisotropy of Cubic and Hexagonal Crystals The magnetic change of the quantitatively of the cosines

anisotropy is specific for the crystal structure. To express the energy per volume versus the orientation of the magnetization one expands the energy per volume u in terms of the power of the direction j with the crystal axes i

i cos
j; i;

8:107

and keeps the lowest and second lowest non-vanishing terms. Only even orders have nonzero coecients because of time reversal symmetry; inversion of time reverses the orientation of the spin, and hence of the magnetization, and the energy is invariant with respect to time reversal. For a cubic crystal the expansion up to fourth order would formally be ucub u2
21 22 23 u4
41 42 43 : Because of the identity X 2i 1;

8:108
8:109

i

the first term in (8.108) is constant and can be omitted. The second term can be rearranged with the help of (8.109) to read ucub

2u4
21 22 21 23 22 23 :

8:110

One sees from this result that there is no need to include mixed terms of the type 2i 2k into the formal expansion (8.108) as they are automatically included. With the fourth order expansion (8.110) the ratio of the energies along the space diagonal and the area diagonal is fixed to 4/3. To allow for a deviation from that ratio one needs to include a sixth order term. The formally simplest way to do that is by writing the anisotropy as ucub K1
21 22 21 23 22 23 K2 21 22 23 ;

8:111

222

8 Magnetism

in which K1 and K2 are the anisotropy constants. For iron K1 = 4.2104 Jm±3 and K2 = 1.5104 Jm±3 at room temperature. The easy directions are therefore 71008, the hard directions 71118. The dierence in energy between an easy and a hard direction is 1.5104 Jm±3. For nickel the constants K1 and K2 are negative (K1 = ±5.7103 Jm±3, K2 = ±2.3103 Jm±3), which makes 71118 the easy direction. For hexagonal crystals such as hcp-cobalt, the second order term in the expansion does not vanish. When the hexagonal axis is denoted by the index 3, the expansion up to forth order is formally uhex u2jj 23 u2?
21 22 u4 43 :

8:112

There is no fourth order term in 1 and 2 because of the hexagonal symmetry. The second term in (8.112) is equal to u2?
1 23 and can be integrated into the first term. The anisotropy can therefore be expressed in terms of a single angle, the angle with the c-axis uhex u2 23 u4 43

K2 cos2

K4 cos4 ;

8:113

with K2 and K4 the anisotropy constants. The negative signs are chosen to be in keeping with the conventional notation. For cobalt, the constants are K2 = 4.1105 Jm±3 and K4 = 1.0105 Jm±3. The c-axis is therefore the easy axis. Changing the orientation of the magnetization from the easy to the hard direction costs the energy 5105 Jm±3, which is 33 times more than for iron. The large energy dierence is due to fact that the second order eects do not vanish as for cubic symmetry. Domain Walls As illustrated in Fig. 8.14, a ferromagnet consists of domains in which the magnetization is oriented along one of the easy axes. The transition region in which the orientation changes from one easy orientation to another is called a domain wall. Dierent types of domain walls are distinguished, depending on the orientation of the magnetization inside the wall with respect to the orientation in the adjacent domains. Fig. 8.15 shows two types of walls between regions in which the orientation of the magnetization diers by 1808. In Fig. 8.15a, the transition from one domain to the next is by rotation of the magnetization about an axis perpendicular to the domain wall. Such a wall is called a Bloch-wall (here a 1808-Bloch-wall). Another possibility is to rotate the magnetization planar to the magnetization inside the domains as shown in the upper part of Fig. 8.15b. This type of wall is known as a NeÂel-wall (here a 1808 NeÂel-wall). Inside a NeÂel-wall, the magnetization has a nonvanishing divergence rM, while one has rM 0 inside a Bloch-wall. A nonvanishing divergence generates a magnetic depolarization field Hdep and the scalar product of that field with the magnetization M . Hdep contributes to the wall energy (see eq. (VII.1)). Inside the bulk of a magnetic material, the NeÂel-wall is therefore energetically less favored than a Bloch-wall. The situation changes

8.9 Crystalline Anisotropy

(a)

223

(b) z y x

Fig. 8.15. (a) 1808-Bloch-wall: inside the wall, the magnetization rotates around an axis perpendicular to the wall. At a surface, the Bloch-wall may convert into a NeÂel-wall in order to minimize the depolarization energy (b). In a NeÂel-wall, the magnetization rotates in the plane spanned by the magnetization inside the domains and the normal of the wall

when a Bloch-wall meets a surface. Then, the NeÂel-wall may be energetically favored since the Bloch-wall creates a divergence of the magnetic field at the surfaces and therefore costs depolarization energy (Fig. 8.15a). Bloch-walls therefore frequently convert into NeÂel-walls at a surface (Fig. 8.15b). The thickness of a domain wall results from the interplay between anisotropy energy and ferromagnetic exchange energy. Exchange energy is minimized if the angle of rotation between neighboring spins is small, hence the wall thickness large. Anisotropy energy is minimized if the volume in which the orientation of the magnetization diers from the easy axis, hence the thickness of the wall is minimal. We now consider the rotation of the magnetization inside a 1808-Bloch wall for the simple case of a primitive tetragonal structure with the c-axis as the easy axis and nearest-neighbor coupling between the spins. Since the thickness of the wall is large compared to interatomic distances the spins change orientation only little by little from one atomic plane to the next. In this case, we may interpret the Heisenberg operator (8.57) as a classical equation. The spin operators S(i) become conventional vectors, and the product between the spin operators becomes a scalar product. Since all spins within an atom plane n parallel to the wall have the same orientation a single variable, the angle fn between the spins and the c-axis suces (comp. Fig. 8.14). The angle fn varies from zero to p across the wall. In this notation the classical discrete Heisenberg equation becomes X X cos
fn1 fn KS2 cos2 fn ;
8:114 H JS2 n

n

with S, the scalar value of the spin operator and K the anisotropy constant. The terms in (8.114) correspond to the energy of an elementary cell. Because of the smallness of the changes of the angle from one cell to the next, we may write H as X 1 1 2X KS H JS2
fn1 fn 2 cos 2fn const:
8:115 2 2 n n

224

8 Magnetism

The Bloch-wall is in equilibrium if @H=@fn 0 for all planes n: @H=@fn / J 2fn fn1 fn 1 K sin 2fn 0:

8:116

We may consider fn to be a continuous variable f(n). The bracketed term (8.116) then becomes equal to the negative second derivative of f with respect to n, @2f K sin 2f: @n2 J

8:117

This is the so-called Sine-Gordon-equation. The equation is solved by firstly multiplying with @f=@n ( ) @f @ 2 f K @ 1 @f 2 K sin 2f
8:118 cos 2f 0; @n @ n2 J @n 2 @n J whereby the solvable first-order dierential equation 2 @f K cos 2f C1 @n J

8:119

is obtained. The constant C1 is determined by the condition that the derivative @f=@n must vanish deep inside the two domains, i.e. when f 0; p. It follows that 2 @f K 2K 2 sin f
1 cos 2f
8:120 @n J J Taking the square root and after integration one obtains for n
f r Z r J df J ln
tan
f=2; n
f 2K sin f 2K moreover f
n 2 tan

1

exp
n

p 2K=J

8:121

8:122

Experiments usually refer to the components of the magnetization parallel and perpendicular to the wall. These components are n p o p Mjj / cos f cos 2 tan 1 exp
n 2K=J tanh
n 2K=J; n p o p
8:123 1= cosh
n 2K=J: M? / sin f sin 2 tan 1 exp
n 2K=J The functional dependence of Mjj and M? versus n is shown in Fig. 8.16, together with the standard definition of the thickness of a wall p w
8J=K
8:124 If depolarization energy is neglected, the mathematical formalism is transferrable without alterations to the case of NeÂel-walls. The angle f is then the

Problems

225

w = (8J/K)1/2

Magnetization M/Ms

1.0

0.5

0.0

M||/Ms –0.5

M⊥/Ms

–1.0

–4

–2

0

2

4

n(2K/J)1/2

Fig. 8.16. Magnetization versus a reduced coordinate n(2K/J)1/2 perpendicular to a Blochwall. The solid and dashed lines are the components of the magnetization parallel and perpendicular to the magnetization inside the domains, respectively (8.123). The conventional definition of the wall thickness w is likewise indicated

rotation around the axis perpendicular to the magnetization inside the domains and parallel to the NeÂel-wall (Fig. 8.15b). 908-walls are obtained by replacing the argument of the cosine 2fn in (8.115) by 4fn. The formalism describes quite generally transitions from one phase to another that can be represented by single scalar parameter. The best-known case is the so-called Frenkel-Kontorova model for walls between structural domains (see e.g. [8.7]).

Problems 8.1 Calculate the diamagnetic susceptibility of the hydrogen atom using (8.12) and the ground state wavefunction w
a30 p 1=2 e r=a0 , where a0 is the Bohr radius, a0 4p h2 e0 =
me2 0:529 AÊ. 8.2 Calculate the entropy of N spins in a magnetic field using the principles of statistical thermodynamics. Describe the process of adiabatic demagnetization and discuss this method for cooling a paramagnetic salt. How much heat can one extract from the lattice in the process of adiabatic demagnetization (cf. Panel IV)? 8.3 Calculate the anisotropy energy of iron and nickel in the directions [001], [011] and [111] at 300K by using equation (8.111)! Plot the anisotropy

226

8 Magnetism

energy versus the angle to the [001]-axis. The anisotropy constants for iron and nickel are K1(Fe) = 4.2104 Jm±3, K2(Fe) = 1.5104 Jm±3 K1(Ni) = ±5.7103 Jm±3, K2(Ni) = ±2.3103 Jm±3. What are the easy and hard axes? How many of them exist? 8.4 a) Calculate the magnetization versus distance across a 908 NeÂel wall, disregarding the depolarization energy! Compare the thickness of the wall with a 1808 wall and discuss the result! b) Calculate the depolarization energy of a NeÂel wall! Does the result depend on the thickness of the wall? Would you expect the wall thickness to depend on the depolarization energy? 8.5 Why does the magnetization in the iron double-layers in Fig. VII.1 alternate between inward and outward orientation?

Panel VI

Panel VI Magnetostatic Spin Waves

In the absence of an external magnetic field, the quantum energy for spin waves in a ferromagnet vanishes for small k. This is because the dierence in spin orientation from atom to atom becomes smaller and smaller for increasing wavelength, and the exchange interaction therefore provides an ever smaller contribution to the energy. The exchange coupling eventually becomes comparable to the energy of magnetic dipoles in an external field, i.e. the dispersion of the spin waves is dependent on the magnetic field. In the following we treat such spin waves with small k values in an external field. The k value is assumed to be small compared to a reciprocal lattice vector but large compared to x/c, where x is the spin wave frequency. This condition allows us to neglect the explicit interaction with the electromagnetic field (Sect. 11.4) and to assume that r H 0

VI:1

and also of course r
H M 0

VI:2

Spin waves of this kind are called magnetostatic spin waves. They can be handled with the classical equations of motion, which relate the rate of change of the angular momentum of an electron to the torque. If the magnetic dipole moment of the electron is pi , then dpi g lB c
pi B with c : dt h

VI:3

In the following, instead of the dipole moments of single electrons, it is convenient to introduce a space- and time-dependent magnetization M (r, t), which can be constructed from a (local) average over the dipole moments per unit volume. In (VI.3) pi can be replaced by the local magnetization M (r, t). The magnetization is essentially the saturation magnetization Ms of the ferromagnet, which is oriented by the external field H0 along the z axis, with small space- and time-dependent deviations mx and my in the x and y components. We make the ansatz 0 1 mx
re ixt M
r; t @ my
re ixt A ; Ms

Panel VI

228

Panel VI Magnetostatic Spin Waves

0

hx mx e B
r; t l0 @
hy my e
H0 Ms

ixt

1

ixt

A

VI:4

and by noting that mx, my M and hx, hy H0, we obtain from (VI.3) the pair of equations hx mx j im
VI:5 im j my hy with j l0 c2 Ms B0 =
c2 B20 m l0 xcMs =
c2 B20

x2 ; x 2 ; B 0 l 0 H0 :

According to (VI.1), the two component vector h can be written as the gradient of a potential h ru ;

VI:6

where for u we insert as a trial solution a wave propagating in the y direction, i.e., u w
xei ky y :

VI:7

Application of (VI.2) then leads us to r
h m D u r m 0 ;

VI:8

from which, using (VI.5, 7), we obtain an equation resembling a wave equation for the potential 2 @ 2
1 j ky u 0 :
VI:9 @x2 A possible solution of this equation is obviously obtained when j = ±1. This condition yields a spin-wave frequency of q
VI:10 x c B20 l0 Ms B0 : The frequency is thus independent of k if the exchange coupling is completely neglected, as is the case here. It is interesting to look for solutions for special geometries of the sample. The expression (VI.7) can also be applied to the case of a slab in a B field or, simpler still, to the half space x < 0. Equation (VI.9) then has further solutions with j j ±1 when w00
x k2y w
x

VI:11

i.e., for w(x) of the form w
x A ejky jx :

VI:12

229

This solution is evidently localized at the surface of the half-space and is a surface spin wave. The condition that the normal component of B is continuous across the surface yields the eigenfrequency of this mode hx mx jx0 ;

VI:13

1 jjky j

VI:14

m ky

jky j :

We can dierentiate between the two cases ky jky j, that is, the two different directions of propagation: Case 1: ky jky j

Case 2: ky jky j

mj2; m
j 2 1 x1 c
2 l0 Ms B0 ; x2 c
12 l0 Ms B0 :

VI:15
VI:16

Fig. VI.1. Snapshot of the magnetization in a Damon-Eshbach spin wave on the two surfaces of a (thick) slab. The external magnetic field B0 points out of the page. The Damon-Eshbach waves then propagate in a clockwise direction. For smaller values of the slab thickness d, or larger wavelengths, the waves on the two surfaces interact and a coupling dispersion is obtained x = x(kyd)

Panel VI

Panel VI Magnetostatic Spin Waves

Panel VI

230

Panel VI Magnetostatic Spin Waves

Clearly, only the second case yields a positive frequency. We thus have a curious situation in which a wave exists in one direction but not in the opposite direction. This is a particularly interesting demonstration of the break-down of time-reversal invariance by a magnetic field. Corresponding solutions are obtained if the sample has the form of a thin plate with the B0 field in the plane of the plate. The spin waves then propagate in opposite directions on the two surfaces (Fig. VI.1). Because of the coupling between the two surfaces the frequency becomes dependent on ky when ky d91. These magnetic surface waves are known as ``Damon-Eshbach'' waves after their discoverers [VI.1]. They were first identified in the absorption of microwaves [VI.2]. A very nice demonstration of the unidirectional nature of Damon-Eshbach waves, and at the same time of the conservation of wave vector (including its sign) during scattering (4.28), is provided by the Raman eect (Panel III). Coupling of the light occurs in this case via the (weak) magnetooptic eect. Figure VI.2 shows the experimental setup of GruÈnberg and Zinn [VI.3]. The sample is illuminated with a laser and the Raman eect is observed in backscattering. The frequency of Damon-Eshbach waves lies in the GHz region. A spectrometer with high resolution is required, for example, a Fabry-PeÂrot interferometer. To reduce the background due to elastic diuse scattering at the sample, the beam passes through the interferometer several times (twice in Fig. VI.2). A frequency spectrum is obtained by moving the Fabry-PeÂrot mirrors relative to one another. Figure VI.3 shows a Raman spectrum for two dierent positions of a EuO sample relative to the light beam. The surface spin wave can only travel in the direction labelled qk. In the geometry shown above, one thus has
k0

kk qk :

Fig. VI.2. Experimental setup to measure Raman scattering from spin waves [VI.2]. The multiple passes of the light through the Fabry-PeÂrot spectrometer reduces the background so that very weak inelastic signals can be observed

231

Panel VI

Panel VI Magnetostatic Spin Waves

Fig. VI.3. Raman spectrum from EuO [VI.2]. According to the orientation of the sample one observes the DamonEshbach spin waves (labelled as M2 ) as a Stokes line (above ) or as an anti-Stokes line (below), while the volume spin waves appear with equal intensity in both geometries, although higher intensity is observed for the anti-Stokes line [VI.3]

Energy conservation (4.28) demands x0

x x
qk :

The associated Raman line is shifted to smaller x. We thus obtain the Stokes line, whereas the anti-Stokes line for the surface wave does not exist. For the scattering geometry sketched at the bottom of Fig. VI.3, we have
k0

kk

qk

and therefore x0

x

x
qk :

Correspondingly, only the anti-Stokes line is observed for surface waves. For the bulk wave, one observes both the Stokes and anti-Stokes lines, but curiously the anti-Stokes line has higher intensity: the number of contributing bulk waves with the same frequency is dierent for the two scattering geometries.

Panel VI

232

Panel VI Magnetostatic Spin Waves

References VI.1 R. W. Damon, J. R. Eshbach: J. Phys. Chem. Solids 19, 308 (1961) VI.2 P. GruÈnberg, W. Zinn: IFF Bulletin 22 (KFA, JuÈlich 1983) p. 3 VI.3 R. E. Camley, P. GruÈnberg, C. M. Mayer: Phys. Rev. B. 26, 2609 (1982)

Panel VII

Panel VII Magnetism in Thin-Film Systems and GMR-Eect

Magnetic Anisotropy in Thin-Film Systems Magnetic thin-film systems are of great importance in data processing and sensor technology. Moreover, they provide a fascinating playground for fundamental research where astounding discoveries have been accomplished. The versatility of magnetic phenomena in thin-film systems is largely owed to the great variety of competing anisotropies. A first source of anisotropy is the specific shape of thin films. Consider for example a homogenously magnetized thin film. If the film is magnetized perpendicular to the film plane then the jump in the magnetization M at the boundaries gives rise to a depolarizing field Hd = ±M (Hd = ±4pM in Gaussian units)*. If the film is polarized parallel to the plane then there is no depolarizing field because of the (practically infinite) lateral extension of the film. If the direction of the magnetization is turned from parallel to perpendicular, the perpendicular component builds up gradually. To calculate the energy associated with the depolarization eect one makes use of the dierential form of the magnetostatic energy density u du

0 M? dH? :

VII:1

With dH = ±dM and the angle between the orientation of the magnetization and the axis perpendicular to the film one obtains after integration 1 u 0 M2 cos2 : 2

VII:2

In Gaussian units, (VII.2) assumes the form u 2p M2 cos2 . For cobalt the depolarization energy is 1.23106 Jm±3 at room temperature, about a factor of two larger than the crystalline anisotropy energy of 5.1105 Jm±3. A Ni(100) film would have a magnetocrystalline anisotropy energy of ±2103 Jm±3 in favor of the [111] direction. The depolarization energy is 1.5105 Jm±3. The easy axis should therefore be always in the surface plane,

*

The magnetic depolarization field is the analog of the electrostatic depolarization field. In the electrostatic case, the field is caused by the polarization charge density of the surface arising from the termination of the polarization (see Ch. 11.7). In analogy, ones speaks of magnetic polarization charges although a real magnetic charge does not exist.

Panel VII

234

Panel VII Magnetism in Thin-Film Systems and GMR-Eect

if it were not for the two other sources of anisotropy, the strain-induced anisotropy and the surface and interface anisotropy. Elastic strain in thin-films arises from a mismatch between the lattice constants of a film and the substrate on which the film is deposited. If the genuine structure of the film was cubic with a 71008 axis perpendicular to the substrate then the lateral strain breaks the symmetry into a tetragonal one. The quantitative description of the strain-induced anisotropy in terms of forth rank magneto-elastic tensors becomes somewhat sophisticated because of the change in the structure and it is therefore not discussed here (see [VII.1] for details). The source of surface and interface anisotropy is the modified spin orbit coupling or the exchange coupling at the surface and the interface. The energy associated with that asymmetry is proportional to the film area, not the volume. If one still considers the energy per volume, as is conventionally done, then the surface and interface contributions to the anisotropy are proportional to the inverse of the thickness t. We consider the technically simple case of a cubic film with (100) surfaces and the rotation of the magnetization from the perpendicular orientation to the parallel orientation in the [100] zone. From (VII.2) and (8.110), we obtain the anisotropy energy 1 Ks Kint u 0 M2
VII:3 cos2 K1 cos2 sin2 : 2 t Here, is the angle between the magnetization and the surface normal, and Ks and Kint are constants describing the surface and interface anisotropy. A positive value of Ks+Kint means that the interface and surface anisotropy favor the perpendicular orientation. Beyond a critical thickness tc, the shape anisotropy prevails and the magnetization rotates into the film plane: tc 2
Ks Kint =0 M2 :

VII:4

Since the magnetization M depends on temperature the energy balance in (VII.3), and thus the orientation of the magnetization also depends on temperature. While an in-plane magnetization is the most common case, the reverse case, a magnetization perpendicular to the film plane, may also occur in epitaxially grown films because of a strain-induced anisotropy. An interesting example, may it be due to strain, may it be due to interface and surface anisotropies, is the magnetization in one and two monolayer thick iron-films deposited on W(110). The magnetization turns from parallel into perpendicular upon deposition of the second layer. On a stepped W(110) surface, the iron film nucleates at the steps. For a nominal coverage of 1.5 monolayers, the magnetization alternates between perpendicular and parallel orientation (Fig. VII.1).

235

Panel VII

Panel VII Magnetism in Thin-Film Systems and GMR-Effect

Fe W Fig. VII.1. Epitaxially grown monolayer and bilayer stripes of Fe(110) on stepped W(110) [VII.2]. The magnetic orientation changes between parallel and perpendicular to the plane

Exchange Bias In 1956, Meiklejohn and Bean discovered that the magnetic hysteresis curve of a sample of cobalt nanoparticles each coated with a cobaltous oxide shell was shifted on the H-axis after cooling to 77 K in a strong magnetic field [VII.3]. The phenomenon was attributed to the interaction between the antiferromagnetic cobaltous oxide and the ferromagnetic cobalt and was termed as exchange anisotropy by Meiklejohn and Bean. Today, in particular in connection with technical applications to be discussed shortly, the eect is usually called exchange bias. We consider the example of an antiferromagnetic substrate, e.g. NiO, which is covered with a ferromagnetic film. By cooling below the Curie temperature in a strong magnetic field, one first prepares a single domain state in the iron film. An ordered antiferromagnetic state of the NiO substrate is obtained upon further cooling below the NeÂel-temperature of the NiO substrate. The exchange coupling at the interface imposes the orientation of the magnetization in the iron film onto the first NiO layer and thereby causes a particular order in the entire NiO substrate (upper right insert in Fig. VII.2). To reverse the magnetization in the iron film requires now a higher magnetic field as its magnetization is stabilized by the exchange interaction to the NiO substrate. The hysteresis loop is therefore shifted to the left (solid line in Fig. VII.2). Above the NeÂel-temperature the spins are disordered in NiO and the magnetization curve is symmetric around H = 0 (dashed line in Fig. VII.2). We see that the exchange bias provides means for shifting the hysteresis loop back and forth on the magnetic field axis. Consider e.g. the four-layer system in Fig. VII.3. It consists of an exchange-coupled ferromagnet (ECFM) on an antiferromagnetic substrate (AF), a nonmagnetic layer (NM) and a second ferromagnetic layer (FM) on top. The FM-layer is assumed to have an in-plane easy axis. The external magnetic field is parallel to the layers. The magnetization in both the ferromagnetic top layer and the ECFM-layer changes direction if the magnetic field is cycled between large

Panel VII Magnetism in Thin-Film Systems and GMR-Eect

Panel VII

236

Fe

Magnetization M

NiO

Magnetic field H

Fig. VII.2. Hysteresis loops for the magnetization of a ferromagnetic film that is exchange-coupled to a disordered and ordered antiferromagnet substrate (dashed and solid lines, respectively). Ordering of the antiferromagnetic substrate as indicated is achieved by annealing the system above the NeÂel temperature of the substrate and subsequent cooling in a magnetic field parallel to the film plane

FM NM ECFM

Magnetization M

AF

H

Magnetic field H

Fig. VII.3. Hysteresis curve of a sandwich structure consisting of an exchange-coupled ferromagnet (ECFM) on an antiferromagnetic substrate (AF), a nonmagnetic layer (NM) and a second ferromagnetic layer (FM) on top. The hysteresis loop marked by the solid line is for magnetic fields large enough to rotate the magnetization in the ECFM-layer. For smaller fields one stays inside the small loop around zero fields (dotted line) as only the magnetization in the FM-layer changes orientation. The dash-dotted line is for an FM-top layer made of a soft magnetic material (e.g. NiFe permalloy)

237

negative and positive values. The corresponding hysteresis loop is the solid line in Fig. VII.3. If the magnetic field cycles with small amplitude, then only the magnetization in the top layer changes sign and follows the loop indicated by the dotted line. By applying small magnetic fields, one can therefore switch the sandwich between a state where the two ferromagnetic layers have the same orientation of the magnetization and where the magnetizations have the opposite direction. Both states are stable in zero magnetic fields. In this configuration, the system represents a storage device. If the ferromagnetic top layer consists of a soft magnetic material such as permalloy or -metal, the magnetization follows the dash-dotted line. Hence, for positive and negative fields the magnetization on both sides of the non-magnetic layer is parallel and antiparallel, respectively. Together with the magnetoresistance eect to be discussed in the following, a sensor for magnetic fields is obtained. Giant Magneto-Resistance (GMR-Eect) In 1988, the Giant Magneto-Resistance (GMR) eect was discovered independently by two groups. In recognition of their achievement, Albert Fert and Peter GruÈnberg were awarded with the Nobel Prize in 2007. Both groups found that the electric conductance of a layer system consisting of ferromagnetic and nonmagnetic layers would depend on the relative orientation of the magnetization in neighboring ferromagnetic layers. The resistance was smaller (larger) when the magnetization was parallel
"" (antiparallel
"#) oriented. The magnetoresistance defined as R=R
R"#

R"" =R

VII:5

amounted to 1.5 for a trilayer [VII.4] and 50 for a multi-layer system at low temperatures [VII.5]. The trilayer system of Binasch et al. [VII.4] consisted of a Fe-Cr-Fesandwich (Fig. VII.4) that was grown epitaxially on a GaAs(110)-substrate. The 12 nm thick iron films grow epitaxially with (110)-orientation so that both the easy [100]-axis and the hard [110]-axis lie in the film plane. The thickness of the chromium layer amounted to 1 nm. With that particular thickness, the magnetizations in the two iron layers assume an antiparallel orientation in the absence of an external field (see [VII.1] for the nature of that coupling]. In a strong magnetic field parallel to the [100] direction in the film plane the magnetizations in the iron films turn parallel (Fig. VII.4 right and left). The electrical resistance measured parallel to the layer is 1.5 smaller in that case. The reason for the smaller resistance is that conducting (Fermi-energy) electrons traversing the chromium layer from one iron layer into the other carry their spin orientation along. If the magnetization of both iron films points in the same direction, a spin-up electron originating in one iron layer easily finds matching states concerning its k-vector and energy in the second to continue its path without being scattered (save for a

Panel VII

Panel VII Magnetism in Thin-Film Systems and GMR-Effect

Panel VII Magnetism in Thin-Film Systems and GMR-Eect H = –H0

H = +H0

H=0

Fe Cr Fe

Fe Cr Fe

Fe Cr Fe

[100] 1.5

ΔR/R|| (%)

Panel VII

238

1.0

H || [100]

0.5

0.0 –400

–200

0

200

400

μ0 H (10−4T)

Fig. VII.4. Magnetoresistance in a three layer sandwich after Binasch et al. [VII.4]. In zero field, the magnetizations in the two iron layers are held antiparallel via interlayer coupling through the antiferromagnetic chromium. The magnetizations are forced to become parallel by applying an external field. The electrical resistance is lower for that state. This effect is called Giant Magneto-Resistance (GMR)

small interface scattering). In case of an antiparallel orientation, the spin-up states in the second layer are shifted by the exchange energy (Fig. 8.6). In general, there will be no matching states for the electron in the second iron layer. The electron is therefore scattered to loose its preferential direction, which increases the electric resistance (see also Chap. 9). Note, that the GMR-eect does not require the center layer to consist of a ferromagnetic material. In present GMR-devices the center layer is made of copper (Fig. VII.5) The trilayer system in Fig. VII.4 is not suitable as a sensor for small magnetic fields since the eect vanishes for small fields. A sensitive sensor is created in combination with the exchange anisotropy. Fig. VII.5 displays a technical realization following Paul et al. [VII. 6]. The magnetization in the upper permalloy (NiFe) layer rotates easily in an external field. Beneath the permalloy layer, lies a copper-layer sandwiched between two cobalt layers. These cobalt layers act as a spin-valve and increase the magneto-resistance eect. The orientation of the magnetization in the lower NiFe-layer is fixed via exchange coupling to the antiferromagnetic FeMn-layer. Fig. VII. 5 shows the magnetization of the entire package (solid line) together with the change of the resistance (dashed line). Due to the exchange coupling, the relation between the external field and the resistance is now linear in the field with a steep slope. Even tiny changes in the field result in measurable changes of the resistance. The high sensitivity of the sensor and the fact that it can be manufactured in small dimensions, has made

7.0 nm NiFe

8

free FM fixed FM

6

15.5 nm FeMn 3.0 nm NiFe texturing layer 5 nmTa buffer layer

4

oxidized Si-wafer

ΔR/R (%)

Magnetization M

2.0 nm Co 3.5 nm Cu 2.0 nm Co 3.0 nm NiFe

239

Panel VII

Panel VII Magnetism in Thin-Film Systems and GMR-Effect

2

0

–400

–200

0

200

Magnetic field H /Oe

Fig. VII.5. Magnetization (solid line) and magnetoresistance (dashed line) of a complex layer system (schematic after Paul et al. [VII. 6]). The magnetic field is in Oerstedt (1Oe for H is 1000/4p Am±1)

the GMR-sensor indispensable in magnetic storage devices as well as in many other technical applications.

References VII.1 H. Ibach: Physics of Surfaces and Interfaces (Springer, Berlin Heidelberg New York 2006), p. 445 . VII.2 H. J. Elmers, J. Haunschild, U. Gradmann: Phys. Rev. B 59 (1999) 3688 VII.3 W. H. Meiklejohn, C. P. Bean: Phys. Rev. 102 (1956) 1413 VII.4 G. Binasch, P. GruÈnberg, F. Saurenbach, W. Zinn: Phys. Rev. B 39 (1989) 4828 VII.5 M. N. Baibich, J. M. Broto, A. Fert, F. Nguyen van Dau, F. Petro, P. EtõÂ enne, G. Creuzet, A. Friederich, J. Chazelas: Phys. Rev. Lett. 61 (1988) 2472 VII.6 A. Paul, M. Buchmeier, D. BuÈrgler, P. GruÈnberg, J. Appl. Phys. 97 (2005) 023910

9 Motion of Electrons and Transport Phenomena

A number of important phenomena such as electrical and thermal conductivity are based on the motion of electrons in solids. The description of electron motion goes beyond our previous considerations since it involves a time-dependent SchroÈdinger equation; previously we have discussed only the time-independent SchroÈdinger equation and results for thermodynamic equilibrium (Fermi statistics, etc.). The present chapter deals with the question of how electrons in bands behave, if, for example, an external electric field is applied, so that thermodynamic equilibrium is disturbed. The simplest case is that of the stationary state, where the external forces, an electric field or temperature gradient for example, are independent of time.

9.1 Motion of Electrons in Bands and the Eective Mass In describing the motion of an electron in a solid, one is confronted with the same problem that appears when the motion of a more-or-less localized free particle is to be described from a wave theory point of view. The motion of a free electron with fixed momentum p can be described by an infinitely extended plane wave. An exactly defined value of the wave vector k, however, implies complete uncertainty about the electron's position in real space, since the plane wave extends along the entire x-axis. If, on the other hand, the electron is localized to within an interval Dx, e.g., due to a measurement of its position, then the momentum, i.e., wave vector, becomes uncertain. Mathematically, localization can be described by expressing the state of the electron as a wave packet, i.e., a linear superposition of waves with wave vector in the interval {k±Dk/2, k + Dk/2}: kDk=2

w
x; t

a
keikx

x
kt

dk ;

9:1

k Dk=2

where x(k) is determined by a special dispersion relation. As an example, Fig. 9.1 shows a wave packet in a real space representation. From the Fourier representation (9.1) one obtains the uncertainty relation of wave mechanics: Dp Dx hDk Dx h: H. Ibach, H. LuÈth, Solid-State Physics, 4th ed., DOI 10.1007/978-3-540-93804-0_9, Ó Springer-Verlag Berlin Heidelberg 2009

9:2

242

9 Motion of Electrons and Transport Phenomena

The translational motion of a wave packet may be described by the group velocity: v

@x : @k

9:3

The group velocity is the velocity of the center of gravity of the spatially localized wave packet (which is to be distinguished from the phase velocity c = x/k of a plane wave). We note that SchroÈdinger's wave mechanics already contains a dispersion x = c (k) k for a free electron, as a result of which the wave packet ``spreads out'' as a function of time, and also changes its shape, as shown in Fig. 9.1. In a crystal, electrons are described by Bloch waves, which represent spatially modulated, infinitely extended waves with wavevector k. To describe localized crystal electrons it is therefore appropriate to introduce wave packets of Bloch waves (also known as ``Wannier functions''). The localization in real space implies, via the uncertainty relation, an associated uncertainty in the momentum or k-vector. The velocity of a crystal electron in this semiclassical picture is given by the group velocity of the Bloch wave packet: 1 v rk x
k rk E
k : h

9:4

Here, E (k) is the wave-vector dependence of the energy in the band from which the electron originates. This description naturally includes the case of

Fig. 9.1. Real space representation of the wave packet describing the motion of a spatially localized free electron at times t = 0, t0, 2 t0 . . . (Re {w}: ÐÐ; |w|: ± ± ±). The center of the wave packet, i.e., in the particle picture the electron itself, moves with the group velocity v = @x/@k. The halfwidth of the envelope increases with time. As the wave packet spreads, the wavelength of the oscillations of Re {w} becomes smaller at the front and larger at the rear

9.1 Motion of Electrons in Bands and the Effective Mass

243

the free electron, for which E = h 2 k 2/2 m. From (9.4) it then follows that v =k h/m = p/m. Following the Correspondence Principle we are led to the semiclassical equations of motion for a crystal electron. A crystal electron described by a wave packet with average wave vector k in the presence of an external electric field gains, in a time, dt, an additional energy eE v d t ;

dE

9:5

where v represents the group velocity (9.4), of the wave packet. From (9.4, 9.5) it follows that: dE rk E
k dk hv dk ; h dk h k_

9:6 a

e E dt ;

9:6 b

eE :

9:6 c

This equation of motion, which for free electrons can be deduced immediately from the Correspondence Principle, states that the wave vector k of an electron in the crystal changes according to (9.6 c) in an external electric field. From the time-dependent SchroÈdinger equation, it can be shown that (9.6 c) applies quite generally to wave packets of Bloch states, provided certain conditions hold: Namely, the electromagnetic fields must not be too large compared with atomic fields, and they must be slowly varying on an atomic length and time scale. The equations (9.6) enable us to write down a semiclassical equation of motion for crystal electrons in the presence of an external field, with the influence of the atomic crystal field appearing only phenomenologically in the form of the bandstructure E (k). From (9.4) and (9.6), it follows that the rate of change of the group velocity component v i of an electron is: v_ i

1 d 1 X @2E _
rk Ei kj ; h dt j @ki @kj h

9:7 a

v_ i

1 X @2E
e E j : h2 j @ki @kj

9:7 b

This equation is completely analogous to the classical equation of motion v_ m 1
e E of a point charge
e in a field E , if the scalar mass m is formally replaced by the so-called eective-mass tensor mij. The inverse of this mass tensor 1 1 @ 2 E
k
9:8 m ij h2 @ki @kj is simply given by the curvature of E (k). Because the mass tensor mij and also its inverse (mij)±1 are symmetric, they can be transformed to principal axes.

244

9 Motion of Electrons and Transport Phenomena

Fig. 9.2 a, b. Schematic behavior of the effective mass m
k for a one-dimensional bandstructure E (k): (a) for strong curvature of the bands, i.e., small effective masses; (b) for weak curvature, i.e., large effective masses. The dashed lines denote the points of inflection of E (k)

In the simplest case in which the three eective masses in the principal axes are equal to m, we have h2 m d 2 E=dk2 :

9:9

This is the case at the minimum or maximum of a ``parabolic'' band where the dependence of E on k can be well approximated by E
k E0

h2
k2 k2y k2z : 2 m x

9:10

In the vicinity of such a critical point, the so-called eective-mass approximation is particularly useful, because here m is a constant. On moving away from this point along the band, the deviation of the E
k surface from the parabolic form (9.10) means that m depends on k. Figure 9.2 shows two one-dimensional bands E (k) with strong (a) and weak (b) curvature at the top and bottom of the bands. The eective mass is correspondingly small (a) and large (b) at these points. At the Brillouin zone boundary (top of the band), where the curvature is negative, the eec-

9.2 Currents in Bands and Holes

245

tive mass is also negative. Here it can clearly be seen that the eective-mass concept conveniently describes the eect of the periodic potential in terms of the k-dependent quantity m. It should be remarked with respect to the above description that one can still retain all the results derived in Chap. 6 for the free electron gas in metals. This is true so long as we consider only electrons in bands E (k) that can be described by the parabolic approximation (9.10). Near to the band extrema the free electron mass m is simply replaced by the eective mass m which is a constant.

9.2 Currents in Bands and Holes Since the eective mass in a band can vary over a wide range of values, such that electrons at the upper band edge move in the opposite direction to those at the bottom, the question arises of how electrons with dierent k-vectors, that is in dierent band states, contribute to an electrical current. A volume element of dk at k contributes to the particle current density jn djn v
k

dk 1 rk E
k dk 8p3 8p3 h

9:11

since the density of states in k-space is [V/(2 p )3] (or [1/(2 p )3] when related to the volume V of the crystal). We have taken into account that spin-degenerate states must be counted twice. Taken together, the electrons in a fully occupied band therefore make the following contribution to the electrical current density j :
e j 3 rk E
k dk :
9:12 8p h 1st Br:z:

Because the band is fully occupied, the integral extends over the whole of the first Brillouin zone. Thus, for each velocity v
k rk E
k=h there is also a contribution from v
k. Since the reciprocal lattice possesses the point symmetry of the real lattice (Sect. 3.2), for crystal structures with inversion symmetry one has E
k E
k :

9:13

If we denote the two possible spin states of an electron by two arrows (: and ;), then for crystal structures without an inversion center (9.13) can be generalized to E
k" E
k# :

9:14

The proof of (9.14) follows from the time-reversal invariance of the SchroÈdinger equation when the spin variable is taken into account. For simplicity, we assume spin degeneracy here, and obtain for the electron velocity associated with k

246

9 Motion of Electrons and Transport Phenomena

1 v
k r k E
k h

1 rk E
k h

v
k :

9:15

It thus follows, as a general consequence of (9.12), that the current density carried by a full band is zero: j (full band) 0 :

9:16

If we now imagine a band which is only partially filled with electrons, then an external electric field E will, according to (9.6 c), redistribute the electrons from states symmetric about k = 0 to states which are no longer symmetric about k = 0. The distribution of the occupied states is then no longer symmetric under inversion because E distinguishes a direction, and thus the current is dierent from zero j (partially filled band) j 0:

9:17

The integral now extends only over the occupied states and not over the whole Brillouin zone, so that using (9.12) and (9.16) we obtain:
e j v
k dk 8p3 k occupied
e e v
k dk v
k dk ;
9:18 3 8p 8p3 1st Br:z: k empty
e v
k dk : j 3 8p k empty

The total current calculated as an integral over the occupied states of a partially filled band may thus be formally described as a current of positive particles, assigned to the unoccupied states of the band (empty k ). These quasiparticles are known as holes, and they can be shown to obey equations of motion analogous to those derived in Sect. 9.1. Holes also behave like positive particles with regard to their dynamics in an external field. If a band is almost completely filled, then only the highest energy part in the vicinity of the maximum contains unoccupied states. In thermodynamic equilibrium electrons always adopt the lowest energy states, so that holes are found at the upper edge of the band. Near to the maximum, the parabolic approximation for E (k) applies E
k E0

2 k2 h : 2jm^j

9:19

m^ indicates that we are concerned with the eective mass at the top of the band, which is negative. Using (9.6 c), the acceleration of a hole in one of these states under the influence of an electric field is

9.3 Scattering of Electrons in Bands

v_

1 d rk E
k h dt

1 e h k_ E : jm^j jm^j

247

9:20

Here, according to (9.18), rk E and k_ are assigned to the unoccupied electronic states. The equation of motion (9.20) is that of a positively charged particle with a positive eective mass, i.e., holes at the top of a band have a positive eective mass. From the fact that a fully occupied band cannot conduct current, it immediately follows that a crystal with an absolute gap between its highest occupied and lowest unoccupied bands is an insulator. This is true, however, only for a temperature of absolute zero. Because the Fermi function is finite for E EF, even at very low temperatures, there are always at least a few thermally excited electrons in the lowest almost unoccupied band (the ``conduction band''), which produce a current flow when an electric field is applied. Thermal excitation also creates holes in the highest occupied band, the so-called ``valence band'', and these can likewise produce a current. At non-zero temperature, the current is therefore carried by both electrons and holes. This behavior is typical of semiconductors and insulators (note that the distinction between a semiconductor and an insulator is not necessarily clear-cut). How well a material conducts at room temperature, for example, depends mainly on the energetic width of the band gap over which the electrons must be thermally excited (Chap. 12). From the above, it is clear that a material with a partially filled electron band is a metal, having an essentially constant number of free carriers at all temperatures. The electrons in a partially filled band have already been treated in the framework of the potential well model (Chap. 6).

9.3 Scattering of Electrons in Bands In our treatment so far, we have neglected the important fact that electrons moving under the influence of an external field in a crystal undergo collisions, which restrict their movement. If this were not the case, there would be no electrical resistance; once created by a temporarily applied electric field, a current would continue to flow indefinitely according to the semiclassical equations of motion (9.7 b, 9.20). This phenomenon of ``superconductivity'' has indeed been observed for many materials (Chap. 10). Normal conductors, however, have a finite, often high electrical resistance. What, therefore, are the important scattering processes for electrons accelerated in external fields? Drude (1900) [9.1] assumed that the electrons scatter from the positive cores that form the periodic lattice. This model implies a mean free path between collisions of 1±5 AÊ. In obvious contradiction to this prediction, most metals are found to have a mean free path at room temperature which is about two orders of magnitude higher (Sect. 9.5).

248

9 Motion of Electrons and Transport Phenomena

The explanation of this discrepancy came with the recognition that an exactly periodic lattice of positive cores does not cause scattering. This is immediately apparent within the one-electron approximation, because Bloch waves travelling through the lattice are stationary solutions of the SchroÈdinger equation. Since ww is time independent, these solutions describe the unperturbed propagation of electron waves. These results naturally apply also to packets of Bloch waves which describe localized electrons. Deviations from this undisturbed propagation, i.e., perturbations of the stationary Bloch states can only occur in two ways: I) Within the one-electron approximation, where interactions between electrons are neglected, the only sources of electron scattering are deviations from strict periodicity in the lattice. These may be: a) defects in the lattice that are fixed in time and space (vacancies, dislocations, impurities, etc.), b) deviations from periodicity that vary in time, i.e., lattice vibrations. II) The one-electron approximation neglects interactions between electrons. Electron-electron collisions, which are not contained in the concept of a non-interacting Fermi gas, can in fact perturb the stationary Bloch states. As we will see, this eect is usually much less significant than those noted in (I). The decisive quantity for the description of an electron scattering process is the probability wk' k that the electron will be scattered from a Bloch state wk(r) to a state wk' (r) under the influence of one of the previously described imperfections. According to quantum mechanical perturbation theory, this transition probability is
wk0 k jhk0 jH 0 jkij2 j drwk0
rH 0 wk
rj2 ;
9:21 where H 0 is the perturbation to the Hamiltonian. Because of the ``Bloch character'' of wk (r) we have
0 0 0 hk jH jki dr uk0 e i k r H 0 uk ei k r :
9:22 If the perturbing potential H 0 can be written as a function of real-space coordinates, then (9.22) becomes comparable to the Fourier integral (3.6) describing diraction amplitudes from periodic structures, when
uk0 H 0 uk is identified with the scattering electron density R
r in (3.6). By comparing the calculations for diraction from static and moving scattering centers (Chap. 3 and Sect. 4.4) we can immediately draw the conclusion: If H 0
r is a potential that is constant in time, such as that of a static defect, then we expect only elastic scattering of the Bloch waves with conservation of energy. If, on the other hand, H 0
r; t is a potential that varies in time, as appropriate for the perturbation due to a lattice wave (phonon), then the scat-

9.3 Scattering of Electrons in Bands

249

tering is inelastic (Sect. 4.4). In analogy to the results of Sect. 4.4, energy conservation also applies to the scattering of conduction electrons by phonons: E
k0

E
k hx
q :

9:23

For scattering by a phonon with wave vector q, the perturbing potential H 0 naturally has a spatial dependence exp (i q r ). This means that the scattering probability (9.21) contains a matrix element (9.22) of the form:
0 0 i q r hk je jki druk0 uk ei
k k q r :
9:24 Because
uk0 uk has the periodicity of the lattice and can be expanded as a Fourier series in terms of reciprocal lattice vectors, the matrix element in (9.24) is non-zero (as in Sect. 4.3) only when k0

kqG:

9:25

To within a reciprocal lattice vector G, this relation resembles a momentum conservation law. Note that k is nothing other than the wavevector of a Bloch state, i.e. a quantum number. Only for a free electron is h k the true momentum. If we take energy conservation (9.23) and k-conservation (9.25) together, then, just as in Sect. 4.3, we see that scattering of Bloch-state electrons can be well described in the particle picture. Let us leave the one-electron approximation and proceed to the subject of electron-electron scattering. It can be shown, also in a many-body description, that energy and wavevector (quasi-momentum) conservation also apply here. For a collision between two electrons (1) + (2) ? (3) + (4), we must have E1 E2 E3 E4 ;

9:26

where Ei = E (ki) denotes the one-particle energy of an electron in a non-interacting Fermi gas. Furthermore for the corresponding k-vectors: k1 k2 k3 k4 G :

9:27

Naively, one would expect a high probability of scattering since the packing density is of the order of one electron per elementary cell and because of the strength of the Coulomb repulsion. The Pauli exclusion principle, however, to a large extent forbids scattering of this type, for the reasons detailed below. Let us assume that one electron occupies the state E1 > EF, an excited state just above the Fermi level; the second electron involved in the collision is inside the Fermi sphere with E2 < EF. For scattering to states E3 and E4, the Pauli principle demands that E3 and E4 must be unoccupied. Thus, the necessary conditions for scattering, besides (9.26), are: E1 > EF ; E2 < EF ; E3 > EF ; E4 > EF :

9:28 a

250

9 Motion of Electrons and Transport Phenomena

Fig. 9.3. Illustration in k-space of a twoelectron collision (EF is the radius of the Fermi sphere): Two electrons (1) and (2), with initial wave vectors k1 and k2, scatter from one another to final states with wave vectors k3 and k4. Their total energy and total momentum are conserved in the process. In addition, the Pauli principle demands that the electrons scatter to final states k3, k4, that were initially unoccupied (E3 > EF , E4 > EF)

From energy conservation (9.26), it then follows that E1 E2 E3 E4 > 2EF

9:28 b

E1

9:28 c

and EF
E2

EF > 0 :

If (E1±EF) < e1 (e1EF), i.e. E1 is just outside the Fermi surface (Fig. 9.3), then |E2±EF| = |e2| < e1 from (9.28 c), i.e. E2 must be only a little (*e1) below EF. Therefore only the fraction *e1/EF of all electrons may scatter with the electron in the state E1. If E1 and E2 are in the shell e1 around EF , then because of k conservation (9.27) and (9.28 b, c), E3 and E4 must also lie in the shell e1 around EF . k conservation in the form k1±k3 = k4±k2 means that the connecting lines (1)±(3) and (2)±(4) in Fig. 9.3 must be equal. Because only a fraction *e1/EF of all occupied states are allowed final states, the Pauli principle further reduces the scattering probability by a factor e1/EF. The thermal broadening of the Fermi function is of the order k T, so that the final state E1 must lie within this energy of EF , i.e. e1*k T. The temperature-dependent reduction in the cross-section for electron-electron scattering which stems from the Pauli principle can be estimated as follows: !2 kT R/ R0 :
9:29 EF Here R0 is the cross-section which would apply without the Pauli principle for a classical gas of screened point charges. Let us assume that the cross-section for the scattering of an electron from a defect in the lattice (e.g. the charged core of an impurity) is of the order R0. For both scattering partners of the electron we are concerned with screened Coulomb fields. The probability of electron-electron scattering at a tempera-

9.4 The Boltzmann Equation and Relaxation Time

251

ture of 1 K is about a factor *10±10 smaller than that of electron-defect scattering (EF/k is assumed to be about 105 K, Sect. 6.2, Table 6.1). These simple arguments again illustrate, but from a dierent viewpoint, that the Pauli principle allows electrons in solids to be treated, to a good approximation, as non-interacting, despite their high density. Therefore, in the following treatment of electrical conduction in solids we need to consider only the scattering of electrons from defects and phonons.

9.4 The Boltzmann Equation and Relaxation Time Transport phenomena, such as the flow of electric current in solids, involve two characteristic mechanisms with opposite eects: the driving force of the external fields and the dissipative eect of the scattering of the carriers by phonons and defects. The interplay between the two mechanisms is described by the Boltzmann equation. With the help of this equation one may investigate how the distribution of carriers in thermal equilibrium is altered in the presence of external forces and as a result of electron scattering processes. In thermal equilibrium, i.e. under homogeneous temperature conditions and with no external fields, this distribution function is simply the Fermi distribution derived in Sect. 6.3: 1

f0 E
k e

k

E
k EF = T

1

:

9:30

This equilibrium distribution f0 is independent of r because of the assumed homogeneity. Away from equilibrium, where we merely assume local equilibrium over regions large compared with atomic dimensions, the required distribution f (r, k, t) can be both space and time dependent: the r and k values of an electron are altered by external fields and collisions. To derive f, we first consider the eect of external fields, and then introduce the scattering as a correction. We consider the change in f during the time from t±dt to t. Under an applied external field E , an electron that is at r and k at time t, will have had the coordinates r

v
kdt

and

k

eE dt= h

9:31

at time t±dt (for e positive). In the absence of collisions, each electron with coordinates r ± v dt and k + e E dt/h at t±dt must arrive at r, k at time t, i.e., f
r; k; t f
r

v dt; k e E dt= h; t

dt :

9:32

An additional term must be added to this equation because along with the changes described by (9.31), electrons may also be scattered to or from r and k in time dt. If we express the change in f due to scattering by the term (@f=@t)s, then the correct equation is

252

9 Motion of Electrons and Transport Phenomena

f
r; k; t f
r

v dt; k e E dt= h; t

dt

Expanding this up to terms linear in dt gives @f e @f E v rr f rk f : @t h @t s

@f dt : @t s

9:33

9:34

This is the Boltzmann equation, and represents the starting point for the treatment of transport problems in solids. The terms on the left-hand side are called the drift terms, and the as yet unspecified term on the right is the scattering term. This contains all of the atomic aspects of the scattering mechanisms introduced briefly in Sect. 9.3. The generalized quantum mechanical transition probability discussed in Sect. 9.3, wk'k!|hk '|H '| ki|2 for transitions from the Bloch state wk to wk ', immediately enables us to write the scattering term in its most general form:
@f
k V dk0 f1 f
kwkk0 f
k0 1 f
k0 wk0 k f
kg :
9:35 @t s
2p3 In this equation the first term in the integrand takes account of all scattering events from occupied states k ' to unoccupied states k, while the second term includes all scattering out of k into some other state k '. If (9.35) is inserted in (9.34), it can be seen that the Boltzmann equation, in its most general form, is a complicated integro-dierential equation for determining the non-equilibrium distribution f (r, k, t). Because of this, the scattering term (9.35) is often modelled in the socalled relaxation time ansatz, which is a plausible postulate for many problems. It assumes that the rate at which f returns to the equilibrium distribution f0 due to scattering is proportional to the deviation of f from f0, i.e., @f f
k f0
k :
9:36 @t s s
k The so-called relaxation time s (k) depends only on the position of the state in k-space, which in a localized electron picture corresponds to the mean kvalue of the partial waves in the wave packet. For a spatially inhomogeneous distribution, the relaxation time s (k, r) in (9.36) will also depend on the position r. The distribution f (r, k, t) is then defined for volume elements dr which are large compared to atomic dimensions, but small compared with the macroscopic distances over which current, heat flux, etc., change significantly. The assumption behind the relaxation time model is that scattering merely serves to drive a non-equilibrium distribution back towards thermal equilibrium. The significance of the relaxation time becomes clearer if we consider the case in which an external field is suddenly switched o: If the

9.4 The Boltzmann Equation and Relaxation Time

253

external field creates a stationary non-equilibrium distribution fstat (k), and the field is then switched o, then from the moment t of switching o: @f @t

f

f0 s

:

9:37

With the initial condition f (t = 0, k) = fstat, the Boltzmann equation (9.37) has the solution f

f0
fstat

f0 e

t=s

:

9:38

The deviation of the distribution f from the equilibrium distribution f0 (k) decays exponentially with decay constant s (relaxation time). The relaxation time s is therefore the time constant with which the non-equilibrium distribution relaxes via scattering to the equilibrium state when the external perturbation is switched o. Furthermore, the Boltzmann equation allows an approximate calculation of the stationary non-equilibrium distribution which exists under the influence of an external field, e.g. an electric field E . If f does not depend on position (i.e., rr f = 0), then from (9.34, 9.36) it follows that the stationary state (i.e., @f/@t = 0) is given by e E rk f f
k f0
k=s
k ;
9:39 h e
9:40 f
k f0
k s
k E rk f
k : h This dierential equation for f (k) can be solved iteratively by initially approximating f in the
rk f -term on the right-hand side by the equilibrium distribution f0. This gives a solution of f linear in E , which can again be inserted into (9.40) to give a solution quadratic in E . Successive insertion of the solutions leads to an expression for the non-equilibrium distribution f (k) in terms of powers of the external field E . If we are only interested in phenomena that depend linearly on the external field, e.g. Ohmic conduction in solids, then we can restrict the calculation to the first approximation where f depends linearly on E , i.e. where only the equilibrium distribution f0 is considered in rkf. This gives the so-called linearized Boltzmann equation for the determination of the non-equilibrium distribution e f
k ' f0
k s
k E rk f0
k :
9:41 a h In the present approximation for small electric fields, i.e., for small deviations from thermal equilibrium (the linearized problem), (9.41 a) may be regarded as an expansion of f0 (k) about the point k: e
9:41 b f
k ' f0 k s
k E : h

The stationary distribution resulting from an external field E and including the eects of scattering (described by s ) can therefore be represented by a

254

9 Motion of Electrons and Transport Phenomena

Fig. 9.4 a, b. The effect of a constant electric field Ex on the k-space distribution of quasifree electrons: (a) The Fermi sphere of the equilibrium distribution [± ± ±, centered h. (b) The at (0, 0, 0)] is displaced in the stationary state by an amount dkx = ±e sEx / new Fermi distribution f (E(k)) only differs significantly from the equilibrium distribution f0 (± ± ±) in the vicinity of the Fermi energy (Fermi radius)

Fermi distribution shifted by e s E / h from the equilibrium position, as shown in Fig. 9.4. It is interesting to consider the eect of elastic and inelastic scattering on the approach to equilibrium in k-space. The stationary state of the distribution is represented as a displaced Fermi sphere in Fig. 9.5 (full line). If the external field is switched o, the displaced sphere relaxes back to the

Fig. 9.5 a, b. Electron scattering processes in k-space. The dashed circle represents the Fermi surface in thermodynamic equilibrium
E 0. Under the influence of an electric field Ex and for a constant current, the Fermi surface is displaced as shown by the full circle. (a) When the electric field is switched off, the displaced Fermi surface relaxes back to the equilibrium distribution by means of electron scattering from occupied states (*) to unoccupied states (*). Since the states A and B are at different distances from the k-space origin (i.e., have different energies), the relaxation back to equilibrium must involve inelastic scattering events (e.g., phonon scattering). (b) For purely elastic scattering (from states A to B ), the Fermi sphere would simply expand. When the field is switched off, equilibrium can only be achieved by inelastic scattering into states C within the dashed (equilibrium) Fermi sphere

9.5 The Electrical Conductivity of Metals

255

equilibrium distribution (dashed line). Only inelastic scattering (Fig. 9.5 a) can cause this return to equilibrium. Elastic collisions alone, e.g. from defects, cannot facilitate the return to equilibrium. Without inelastic collisions the Fermi sphere would merely expand due to the eect of elastic collisions (Fig. 9.5 b).

9.5 The Electrical Conductivity of Metals In about 1900, long before an exact theory of the solid state was available, Drude [9.1] described metallic conductivity using the assumption of an ideal electron gas in the solid. For an ideal electron gas in an external field E , the dynamics of the electrons is described by the classical equation of motion m
9:42 mv_ v D e E : s The dissipative eect of scattering is accounted for by the friction term mv D/s where v D = v±v therm is the so-called drift velocity, i.e., the additional velocity due to the field, over and above the thermal velocity v therm. Since v relaxes exponentially to the thermal velocity with a time constant s after switching o the field, s also has the meaning of a relaxation time. For the stationary case (v_ = 0) one has es E
9:43 vD m and hence the current density j in the direction of the field is j

env D nel E

e2 sn E : m

9:44

Here n is the volume density of all free electrons and the mobility l is defined as the proportionality constant between the drift velocity and the external field. In the Drude model, the electrical conductivity is therefore r j= E

e2 ns m

and the electron mobility becomes es : l m

9:45

9:46

Note that, in this simple model, all free electrons contribute to the current. This view is in contradiction to the Pauli principle. For the Fermi gas this forbids electrons well below the Fermi level from acquiring small amounts of energy, since all neighboring higher energy states are occupied. To relate the material-specific conductivity to atomically-determined features of the band structure, we consider, as in (9.2), the contribution to the current of electrons in the volume element dk. In the expressions (9.11, 9.12)

256

9 Motion of Electrons and Transport Phenomena

for the particle and electrical current densities, only the occupied states in kspace are summed. This summation, i.e., integration, over occupied states can be replaced by a much tidier sum over all states in the first Brillouin zone if one introduces the occupation probability f (k) for the states k. In analogy to (9.11), the particle current density jn is given by
1 jn 3 v
kf
kdk :
9:47 8p 1st Br:z:

Because we are confining our attention to linear eects in an external field, i.e. Ohm's law, it is sucient to insert f (k) in the linearized form (9.41 a). For an electric field E x in the x-direction, the electrical current density is
e dk v
kf
k ; j 8p3
e es
k @f0 Ex dk v
k f0
k :
9:48 8p3 h @kx For an isotropic medium and for cubic lattices, the y and z components of j vanish when the electric field points in the x-direction. In other words, the tensor relationship between current density j and electric field E reduces to a scalar relationship, jy jz 0 :

9:49

Since the integral is over the whole Brillouin zone and f0 (k) has inversion symmetry about k = 0, the integral over v x f0 vanishes. Furthermore, since @f0 @f0 hv x ; @kx @E we have jx

e2 @f0 2 E : x dkv x
ks
k 8p3 @E

The specific electrical conductivity is therefore
e2 @f0 r jx = E x : dkv 2x
ks
k 3 8p @E

9:50

9:51

9:52

The energy region over which the Fermi function f0 (E) changes rapidly has a width of about 4 k T (Sect. 6.3). It also has inversion symmetry about the point (EF , f0 (EF) = 1/2). Thus, to a good approximation, @f0 @E

d
E

EF :

9:53

This approximate solution is largely self-evident, and the derivation will not be given here.

9.5 The Electrical Conductivity of Metals

257

Using (9.53) with dk dfE dk? dfE

dE dE ; dfE jrk Ej hv
k

it follows immediately from (9.52) that
e2 v 2
k r ' 3 dfE dE x s
kd
E EF ; v
k 8p h and because of the property of the d-function in the integral
2 e2 v x
k s
kdfE : r' 3 v
k 8p h

9:54

9:55

9:56

EEF

In the general case, v (k) and s (k) vary over the Fermi surface. In (9.56) however, an average value hv 2x (k) s (k)/v (k)i EF over the Fermi surface can be taken outside the integral. For a ``Fermi sphere'', i.e., for nearly free electrons with a constant eective mass m (see below), this average value is simply equal to v
EF s
EF =3. The electrical conductivity r of a metal can thus be expressed as a surface integral over the Fermi surface E (k) = EF in k-space. Only the velocity v
EF and the relaxation time s (EF) of the electrons at the Fermi surface appear in the microscopic description. Equation (9.56) expresses precisely the fact that only electrons in the vicinity of the Fermi energy are relevant for current transport in a metal, as expected from the Pauli exclusion principle. This conclusion can also be drawn from the diagrams in Figs. 9.4 and 9.5: Electrons well below the Fermi energy are not aected by the slight stationary shift, ±(e s/ h ) E x , of the Fermi sphere in k-space. For the simple case of a conduction band of a metal (with the approximation k T EF) containing only electrons in an energy region for which the parabolic approximation is valid with a constant eective mass m, (9.56) can be evaluated further. For electrons in an exactly parabolic band (quasi-free electrons) we have v
EF hkF =m and

9:57 a

dfE 2
4pk2F :

9:57 b

EF

Furthermore, since n

2
4=3p k3F 8p3

k T EF, ; i:e:;

k3F 3p2 n :

9:57 c

It therefore follows that the electrical conductivity r and mobility l are given by

258

9 Motion of Electrons and Transport Phenomena

r'

e2 s
EF n m

9:58 a

l'

es
EF : m

9:58 b

and

These relationships are formally equivalent to those of the Drude model (9.45, 9.46). The relaxation time, which was not exactly specified in that model, is that of electrons at the Fermi level, and the eective mass m replaces the free electron mass m. The total concentration of electrons in the conduction band, which appears in the Drude model, also appears in the correct formulas (9.58 a, b). However, this is because of the formal integration over k-space (9.52) and not, as assumed in the Drude model, because all electrons contribute to charge transport. The similarity between (9.58 a, b) and (9.45, 9.46) explains why the Drude model yields satisfactory results for many purposes. It should also be remarked that for semiconductors, in which the carrier concentration n is strongly temperature dependent (Sect. 9.2, Chap. 12), the evaluation of (9.52) naturally leads to complicated averages over s (k) rather than to the expressions (9.58 a, b). To understand the temperature dependence of the resistance of metals, it suces to consider the temperature dependence of s (EF) or l, because the electron concentration n is independent of temperature. Instead of a rigorous quantum mechanical calculation of the scattering probability wk ' k (Sect. 9.3), we give here a qualitative discussion of both scattering mechanisms: phonon and defect scattering. Assuming that the two mechanisms are independent of one another, the total scattering probability is the sum of the individual scattering probabilities. The scattering probability is inversely proportional to the average free time of flight sTF of a carrier, and therefore inversely proportional to the relaxation time. It therefore follows that 1 1 1 s sph sdef

9:59

where sph and sdef are the average times between scattering from phonons and from defects, respectively. This treatment directly provides the important features of the temperature behavior of the resistivity of a metal. The number of collisions per unit time is proportional to the scattering cross-section R and to the velocity v of the particle: 1/s!Rv. For metals, v is simply the velocity at the Fermi surface v (EF) and is therefore temperature independent. For defects the cross-section R is also temperature independent. Defect scattering leads therefore to a temperature-independent component of the resistivity, Rdef . For phonon scattering, the scattering cross-section can be set proportional to the mean square vibrational amplitude hu 2 (q)i of the appropriate

9.5 The Electrical Conductivity of Metals

259

phonon (wavevector q, frequency xq ) (Chap. 5). In the classical, limiting case of high temperature, it follows from the equipartition theorem that Mx2q hu2
qi k T ;

T H

9:60

where M is the mass of the heavy ion cores. We thus obtain

kT 1 hu2
qi : sph Mx2q

9:61 a

The phonon frequency xq contains information about the elastic properties of the material. A rough estimate is obtained by replacing xq by the Debye cuto frequency xD = k H/ h (Sect. 5.3), where H is the Debye temperature. This yields MH2 for T H :
9:61 b sph T At temperatures T < H, the phonon excitation probability decreases rapidly and, together with the decreasing phonon energy, this leads to predominantly small angle scattering. GruÈneisen [9.2] has developed an exact theory for T < H, and gave the following universal expression for the phonon contribution Rph (T)!1/rph to the resistivity of metals: H=T

Rph
T A
T=H

5 0

ex

x5 dx 1
1 e x

9:62

At low temperatures, this varies as T 5.

Fig. 9.6. Electrical resistance of sodium compared to the value at 290 K as a function of temperature. The data points (*, *, ` ) were measured for three different samples with differing defect concentrations. (After [9.3])

260

9 Motion of Electrons and Transport Phenomena

Fig. 9.7. Resistivity R of pure copper and of copper-nickel alloys of various compositions. (After [9.4])

According to (9.59) we can write the resistivity R = 1/r*1/s of a metal as the sum of a temperature-independent residual resistivity Rdef (due to defects) and a part due to phonon scattering Rph (T) which is linear in temperature at high temperature: R Rph
T Rdef :

9:63

This behavior, which was first identified experimentally, is known as Matthiesen's Rule. Note that (9.63) is valid only approximately. Figure 9.6 shows the experimentally measured electrical resistance of Na at low temperature. Below about 8 K, a temperature-independent residual resistance is observed, which depends on the defect concentration of the sample. At higher temperatures, the component described by the GruÈneisen formula (9.62) becomes evident, and above 18 K Rph displays the linear dependence Rph*T. The influence of the defect concentration (nickel impurities) on the resistance of copper at moderately low temperatures is shown in Fig. 9.7. Figure 9.8 shows how the universal GruÈneisen formula (9.62) applies to a series of metals, when the resistance is plotted against reduced temperature T/H. At higher temperatures there is clearly a linear increase in resistance with temperature. For the sake of completeness, it should also be mentioned that magnetic defects can cause a quite special kind of scattering in metals that results from spin interactions. At low temperatures (T < 20 K) this leads to a minimum in R (T) instead of a constant residual resistance. This phenomenon is known as the Kondo Eect.

9.6 Thermoelectric Effects

261

Fig. 9.8. The universal curve for the reduced resistance (R/RH) as a function of reduced temperature (T/H, where H is the Debye temperature). Data points are plotted for a number of different metals

9.6 Thermoelectric Eects In calculating the electrical conductivity (9.56) using the Boltzmann equation (9.34) and the relaxation time ansatz (9.36), we assumed for simplicity a homogeneous temperature over the conductor (i.e., rr T = 0). If we relax this assumption, the distribution function f (k) is aected not only by the electric field E but also by the temperature gradient rr T = 0. The adjustment to the equilibrium distribution f0 (k) via scattering will again be described by the relaxation time postulate (9.36). For the stationary state E_ 0; @
rr T=@t 0; @f=@t 0, the non-equilibrium distribution follows from (9.34) and (9.36): e
9:64 f
k f0
k s E rk f svv rr f : h Since rr fk; T
r
@f=@Trr T, and by assuming only a small perturbation, (9.64) can be linearized in a similar way to (9.41 a), and one finds e f
k f0
k s E rk f0 h

s

@f0 v rr T : @T

9:65

To calculate the resulting electric current density in the x-direction, we insert the expression (9.65) into the relation for the current density (9.48). The first two terms in (9.65), particularly the one linear in E x, give Ohm's law, as in the calculation in Sect. 9.5 [(9.49±9.52)], so that the current density can be written as

262

9 Motion of Electrons and Transport Phenomena

jx r E x

e @f0 @T : dk s v 2x 8p3 @T @x

9:66

It is instructive to evaluate the integral with the assumptions of a spherical Fermi surface and a relaxation time that depends on energy only. Using the definition of the density of states (7.41), one obtains
1 @f0 @T :
9:67 jx r E x e dEs
Ev 2
ED
E 3 @T @x Since the derivative @f0 =@T is non-zero only in the immediate vicinity of the Fermi energy the integrands s (E) and v 2 (E) can be replaced by their average values sF and v 2F . By expanding D
E into a Taylor series around EF and by using (6.43±6.45) it can be shown that the remaining integral is proportional to the derivative of the density of states D0
EF jx r E x

p2 2 @T : ev F sF k 2 TD0
EF @x 9

9:68

In deriving (9.66) it was tacitly assumed that the Fermi energy EF can be treated as a constant. This is a good approximation for metals (Chap. 6). For semiconductors, however (Chap. 12), a temperature gradient @T/@x is associated with a considerable spatial dependence of the Fermi energy, EF (r). The derivative of the distribution f in (9.34) also brings into play the derivative of the Fermi energy @EF/@x and (9.66) must now be expressed in the general form @T 0 12 jx r E x L xx ;
9:69 @x where E 0 E e 1 rr EF
r is a generalized electric field strength, which includes the eects of the space-dependent Fermi energy. L 12 xx is a so-called transport coecient [defined by (9.66)] responsible for the fact that a temperature gradient is generally associated with an electrical current. The Boltzmann equation can be used to calculate not only electric current but also the heat flux due to electrons in an external field E and for a temperature gradient rr T. The quantity of heat transported dQ is associated with an entropy change dS, or a change in internal energy dU and particle number dn via the following thermodynamic relation (EF is the chemical potential of the electrons, i.e., Fermi energy): dQ TdS dU

EF dn :

9:70

With jE as the energy flux density and jn as the particle flux density, the heat flux density follows as jQ jE

E F jn ;
9:71 where jE = (8 p3)±1 dk E (k) v (k) f (k, r). As above, the insertion of the linearized non-equilibrium distribution (9.65) leads to a linear relation between 0 jQ , E (or E ) and rr T, as in (9.69). In general, one thus has the following

9.6 Thermoelectric Effects

263

equations for the electrical and thermal currents as a function of their origins, generalized electric field E 0 and temperature gradient rr T: j L

11

jQ L

E 0 L

21

12

E 0 L

rr T ;

22

9:72 a

rr T :

9:72 b

For non-cubic crystals the transport coecients L ij are of course tensors. Their general representation [e.g., (9.66) for L 12 xx] leads to interesting relations between the coecients, which, however, will not be pursued here. We now wish to summarize the physical behavior expressed by (9.72 a, b). An electric field or a temperature gradient causes both a thermal and an electric current; in particular, an electric field can be created by a thermal gradient. Consider a conducting loop consisting of two dierent metals A and B, which is either open, or connected only by a high resistance voltmeter (Fig. 9.9 a). The two junctions between metals A and B are at different temperatures T1 = T2 = T0. Because j = 0, we obtain from (9.72 a) (with E ' = E inside the metal):

E x
L

11

1
L

12

@T=@x K@T=@x :

9:73

The quantity K is called the absolute thermopower and is a material-specific property. We consider a one-dimensional problem in which x is the distance along the wire. The loop voltage measured by the voltmeter in Fig. 9.9 a is
1 U 0

1

2

0

E B dx E A dx E B dx 1

2

2

@T @T dx KA dx KB @x @x 2

1

T
2

KA

KB dT :

9:74

T1

Fig. 9.9. (a) Schematic arrangement for measuring the Seebeck effect. When the two junctions between metals A and B are at different temperatures
T1 6 T2 6 T0 a thermovoltage appears across the ends of the loop. (b) Adaptation for measuring the Peltier effect. A current is passed through the loop (now at constant temperature) and leads to heat transport between junctions (1) and (2)

264

9 Motion of Electrons and Transport Phenomena

This so-called thermopotential produced by the thermoelectric, or Seebeck eect, depends on the temperature dierence T2±T1 and the dierence in the absolute thermopowers KA and KB. This eect is exploited in thermocouples for measuring temperatures using essentially the same scheme as shown in Fig. 9.9 a. From (9.72 b) one can also derive the inverse eect, known as the Peltier eect. In Fig. 9.9 b the temperature is constant around the loop, i.e., @T/@x = 0. We then have jQ L

21

E

and

j L

11

E

;

9:75

and thus jQ L

21

L

11

1 j Pj ;

9:76

where P is the Peltier coecient. If we attach a battery to the conducting loop in Fig. 9.9 b, then the resulting electric current density j will be accompanied by a thermal current according to (9.76). In A the thermal current is PA j, while in B, it is PB j. Thus there must be a net heat flow of (PA±PB) j into junction (2), which must be extracted at junction (1). Point (1) becomes cooler and point (2) warmer, if PA > PB . The Peltier eect is thus a convenient way to obtain simple and easily controlled cooling.

9.7 The Wiedemann-Franz Law As mentioned in passing in Sect. 9.6, relationships between the transport coecients L ij can be derived from their explicit representations as integrals over the linearized non-equilibrium distribution f (k, r). In particular, one can derive a relationship between the electrical conductivity r and the conduction electron contribution to the thermal conductivity kE. The conductivity r is essentially equal to L 11, and kE to L 22. Making use of (9.65, 9.71), the thermal current density is found to be @f0 @T jQx dk
E EF v 2x
ks
k :
9:77 @T @x For a spherical Fermi surface, and under the assumption that s depends only on energy, we can relate this integral to the electronic specific heat, as in (9.66±9.68), and, for the thermal conductivity kE due to conduction electrons, we obtain kE 13 v 2F s
EF cv :

9:78

For a free electron gas, using (6.50), this becomes kE

p2 s
EF n k 2 T=m : 3

9:79

9.7 The Wiedemann-Franz Law

265

Table 9.1. Experimentally derived values of the Lorentz number at 0 °C, L = kE/rT, deduced from published data for electrical and thermal conductivity Metal

L (10±8 WX/K2)

Na Ag Au Cu Pb Pt

2.10 2.31 2.35 2.23 2.47 2.51

From (9.58 a), the electrical conductivity is r = e 2 s (EF) n/m, so that the quotient !2 p2 k kE =r T
9:80 3 e depends linearly on temperature. This is known as the Wiedemann-Franz law, and the factor p 2 k 2/3 e 2 is the Lorentz number L. The theoretical value of the Lorentz number is, according to (9.80), L 2:45 10 8 W X K

2

:

9:81

Table 9.1 shows a few experimental values for the Lorentz number at 0 °C; they show relatively good agreement with the value in (9.81) even for transition metals. At low temperatures (T H, where H is the Debye temperature) the value of L generally decreases strongly. For Cu at 15 K, for example, L is an order of magnitude smaller than the value in Table 9.1 at 0 °C. The reason for this deviation is that the electrical and thermal relaxation times are no longer the same at low temperatures. The dierence between the two relaxation times can be explained within a simple picture: An electric current arises due to a displacement of the Fermi sphere by an amount dk (Fig. 9.4). A thermal current, on the other hand, stems from the fact that electrons with a wave vector +kF have a dierent average temperature to electrons with ±kF. The relaxation of an electric current thus demands scattering processes with wave vector of about q = 2 kF, whereas relaxation of a thermal current requires only q-vectors of the order of q & k T/ h v F to change the energy levels of electrons near the Fermi level. At suciently high temperatures, the dierence between the scattering processes is not so important. At low temperatures, the phonons available for scattering are mostly those with small q. As a result, the thermal conductivity becomes smaller relative to the electrical conductivity and the Lorentz number L decreases with temperature.

266

9 Motion of Electrons and Transport Phenomena

9.8 Electrical Conductivity of Localized Electrons So far we have considered only transport phenomena associated with delocalized band electrons. The delocalization of band electrons is a consequence of the translational invariance of crystalline solids. In an amorphous solid, on the other hand, electrons may be either delocalized or localized. In Sect. 7.6 we have argued why electrons in the tails of the energy band extending into the forbidden gap of amorphous Si and Ge are localized, whereas the electrons in states further away from the gap remain delocalized as in an periodic solid. In this section we discuss the contribution of localized electrons to the electrical conductivity. We consider a simple model for the density of states with localized and delocalized electrons below and above a ``mobility edge'' Em, respectively (Fig. 9.10). The lower the electron energy, the stronger is the localization and the larger also is the mean spatial distance between localized electron states. In such a system the electrical conductivity depends on the relative positions of the Fermi energy EF and mobility edge Em. If the Fermi energy is above the mobility edge, then the conductivity is as in a crystalline metal with a high concentration of defects. If the Fermi energy is a few k T below the mobility edge then the conductivity is dominated by the thermally excited electrons in the states above the mobility edge. The conductivity is proportional to the concentration of electrons in the states above the mobility edge Em, hence r r0 e

k

Em EF = T

:

9:82

If the Fermi energy is below the mobility edge by more than a few k T then the electrical transport is carried by localized electrons that hop from one localized state to another via a tunneling process. This transport process is therefore known as ``hopping conduction''. Tunneling from one localized state to another requires an overlap of the wave function. Since the amplitudes of the wave functions decay exponentially the probability for a

Fig. 9.10. Electronic states of an amorphous solid (schematic). The density of states tails into the energy gap. The states are localized below the mobility edge Em and delocalized above Em. The extension of the wave function increases as the mobility edge is approached

9.8 Electrical Conductivity of Localized Electrons

267

hopping process from an atom i to an atom j depends exponentially on the distance rij between the atoms. p
rij / e

rij

:

9:83

The constant characterizes the decay of the wave function. In a hopping process, the initial state must be occupied, the final state unoccupied. Hence, the energy of the initial state must lie below the Fermi level and the energy of the final state above, so that one has Ej > Ei. The jump frequency therefore contains a Boltzmann factor, with the energy dierence between Ej and Ei in the numerator of the exponent. Thus, the probability for a jump from i to j becomes p
rij ; Ej ; Ei / e

rij

e

k

Ej Ei = T

:

9:84

The conductivity is proportional to the sum over all jump probabilities p (rij, Ej, Ei). We now consider the possible jumps into a fixed final state Ej out of a continuous distribution of initial states Ei that lie in a sphere with a radius rij < R around the final state j. A jump is possible if there is at least one state with the initial energy Ei < Ej within the sphere of radius R. In order to simplify the calculation we assume that the density of states is constant around EF . In reality this assumption is not well fulfilled (Fig. 9.10). The condition for the existence of an initial state within the sphere of radius R out of which a jump can take place is then 4p 3 R D
EF
Ej 3

Ei > 1 :

9:85

Hence, all jumps are allowed for which E < Emax Ej

3 : 4pR3 D
EF

9:86

The total jump rate and thus the conductivity is therefore proportional to r/e

R

E
max

e

k

Ej E= T

dE / e

R

e

k

3=
4pR3 D
EF T

:

9:87

1

The jump rate vanishes for large R because of the first term describing the overlap of the wave functions. The jump rate also vanishes for small R, since there are no energy terms within the sphere of radius R. In between, the jump rate has a maximum where the exponent has a minimum ! d 3 R 0:
9:88 dR 4pR3 D
EF k T The minimum is for a radius

268

9 Motion of Electrons and Transport Phenomena

Fig. 9.11. Temperature dependence of the conductivity of amorphous Si (open circles, after [9.7]). The experimental data are reasonably well represented by Mott's law with an exponent of 1/4. The data would be fitted even better with an exponent of 1/2

Rm

!1=4 9 : 4pD
EF k T

9:89

For T = 300 K, e.g., a density of states of 5 105 cm±3 and an of 107 cm±1 one calculates an optimal jump distance of 5 10±6 cm. After inserting the optimum jump distance Rm into (9.87) one obtains the temperature dependence of the conductivity r/e

T0 =T1=4

with

T0

43 : 9pD
EF k

9:90

This temperature dependence of the hopping conductivity was first derived by Mott [9.6]. It describes the temperature dependence of the conductivity of amorphous Si quite well (Fig. 9.11). An even better fit to the experimental data is obtained for an exponent 1/2 instead of 1/4. The main reason is that the density of states around the Fermi level is not constant, as assumed in the model, but increases with energy (Figs. 9.10, 7.15).

9.9 Quantum Transport in Nanostructures Characteristic Lengths The preceding sections considered electron transport in macroscopic solids. The quantum mechanical wave character of electrons showed up only in the discussion of scattering processes. The wave character of an electron is lost on the way from one electrical contact to the next since inelastic scattering

9.9 Quantum Transport in Nanostructures

269

processes shift the phase of the electron stochastically. This is dierent for transport in mesoscopic structures or in nanostructures, in particular at low temperatures. In metal and semiconductor samples with dimensions between five and a few hundred nanometers, the phase correlations between propagating electron states become important as they lead to quantum corrections in the electric conductance. Nanostructures of the required dimensions can be manufactured by lithographic methods (Panel XVIII). More and more, we encounter them also in commercial semiconductor devices. The observability of quantum eects depends on the dimensions of the conductor as well as on the number of elastic or inelastic scattering processes that occur in a given volume. In this context, one considers various characteristic length scales that can be attributed to a propagating electron. The elastic mean free path le describes the mean distance between two elastic scattering processes. In such processes the phase may shift by a fixed amount, is however not subject to stochastic variations as in inelastic scattering processes. Various partial waves of an electron have defined phase relations among each other. Elastic scattering occurs at lattice defects such as impurity atoms, dislocations or surfaces (Sect. 9.3). The elastic mean free path le can reach the order of millimeters in pure bulk copper at low temperatures so that le is determined by surface scattering and thus by the dimensions of the conductor. In metallic two-dimensional electron gases in semiconductor heterostructures (Sect.12.7), le can be as large as 10 m. Inelastic scattering of electrons is dominated by the interaction with phonons. Since the electron scatters from a time-dependent potential to loose or gain the energy of one phonon in the process the phase correlation between the electron wave before and after the scattering event is lost. Thus, the wave function of an inelastically scattered electron does not interfere with the wave function of the electron before the scattering event. The probability for inelastic scattering is described be the inelastic mean free path lin. Phonon scattering is frequently also expressed in terms of the mean time between scattering events sin. The mean free path lin and the mean time sin are related by lin vF sin
9:91 p h 2p n=m is the Fermi-velocity (Sect. 6.2). The Fermi-velocity where vF enters because only electrons at the Fermi-energy contribute to electric conduction (Sect. 9.4). A further scattering process of interest in this context is spin-flip scattering. While spin-flip scattering may be elastic, it nevertheless breaks the phase correlation. It is therefore meaningful to introduce a length that concerns only the aspect of phase coherence, the phase coherence length lF. The phase coherence length lF is equal or smaller than the inelastic mean free path lin. At low temperatures, lF may be much larger than the elastic mean free path le. This transport regime with solely phase-conserving scattering processes is called diusive transport.

270

9 Motion of Electrons and Transport Phenomena

A final important length scale is the wavelength of electrons that carry the electric current, hence the Fermi-wavelength lF = 2p/kF. The Fermi-wavelength is important since the wave nature of electrons can give rise to macroscopically observable phenomena only when the dimensions of the samples are comparable to the wavelength. For metals, lF is below 1nm (Sect. 6.2). The observation of quantum conduction therefore requires structural dimensions in that range. For quasi-metallic two-dimensional electron gases (2DEG), lF lies typically between 50 and 100nm because of the much lower density of the electron gas. Quantum eects are therefore observed already in larger structures. One-Dimensional Transport Consider a quasi one-dimensional wire with a diameter of the order of the Fermi-wavelength lF and a length Lz 0, ky > 0) of the Fermi-circle is relevant because of the fixed boundary conditions (Sect. 6.1). States with k-vectors on the kx- and ky-axes are excluded since the wave function vanishes identically there (Sect. 6.1). We see from Fig. 9.12c that the number of permitted states N is the ratio of the area of the Fermi-quadrant to the area occupied by one state p2/LxLy (spin degeneracy taken into account) N

Lx Ly 1 2 pk 4 F p2

k2 F Lx Ly 4p

1 p kF 2 Lx

1 p 1 p p kF 2 Ly 4 Lx Ly

kF 1
Lx Ly : 4 2p

9:92

The first term in the bracket is the area of the Fermi-quadrant in Fig. 9.12c, while the following terms result from the exclusion of areas along the axes and at the origin. For small cross sections, the number of states N becomes a discrete function of Lx and Ly (Lx, Ly< lF if only lF was large compared to the elastic mean free path le, that is at low temperatures where most of the phonon scattering is frozen out. The interference is observed as a small quantum correction to the conductance and is based on the existence of closed loops in elastic scattering processes (Fig. 9.18). Each elastic scattering process shifts the phase by a fixed amount. Partial waves of electrons may circulate clockwise and counter clockwise in closed loops of scattering processes as in Altshuler-Aronov-Spivakinterferences in ring structures. Depending on the type of loops and the phase shifts involved, constructive interference may occur which leads again to an enlarged backscattering that entails an enhancement of the resistance. Many similar processes with stochastically varying closed loops contribute to the finally observed increase in the resistance. The eect is called weak localization. The additional resistance caused by weak localization can be switched o if the condition for constructive interference at the starting points of the closed loops is perturbed. As in the experiments for the demonstration of the Altshuler-Aronov-Spivak-oscillations this is achieved by applying a magnetic field. The field shifts the phase dierence between the clockwise and counter clockwise circulations. Constructive interference is perturbed and the electric resistance is reduced to its classical value. This eect was first observed in the resistance of a long Li-wire with cross sections in the nanometer range as shown in Fig. 9.19. In the meantime, the eect has been demonstrated for a multitude of metallic and semiconducting systems.

a)

elastic scattering

b) 3a

3 P 2

O

Φ Q O

1

Fig. 9.18. (a) Schematic representation of diffusive transport from P to Q in which elastic scattering processes enable closed loops of trajectories in addition to various direct paths. The trajectory 3a describes a closed loop that can be circulated about clockwise and counter clockwise. The two partial waves interfere at the point O. (b) Detail of the closed loop 3a: a magnetic flux F traversing the loop shifts the phase difference between the clockwise and the counter clockwise path

9.9 Quantum Transport in Nanostructures

279

Magnetoresistance ΔR/R0 × 102

0.4

0.3

0.2

0.1

0

−200

0

200

400

600

Magnetic field H (Oe)

Fig. 9.19. Magnetoresistance DR/R of a lithium-wire (21 nm thick, 55 nm broad) measured at 0.13 K as function of a magnetic field H perpendicular to the direction of the current flow (after Dolan et al. [9.13]). Note: A magnetic field of 1Oe corresponds to 1000/4p Am±1 and thereby to a flux density B of 10±3 Vs/m2

The eect of weak localization depends strongly on temperature. For higher temperatures, the phase correlation length lF decreases because of increasing phonon scattering. The electrons loose the fixed phase in the closed loops and constructive interference is no longer possible. The eect of weak localization is also suppressed in nanostructures with small defect concentrations where ballistic transport prevails. Elastic scattering then occurs primarily at the boundaries and possible remaining eects of weak localization become size and structure dependent. Universal Conductance Fluctuations A meticulous analysis of the conductance in the hitherto described magnetotransport phenomena, from Aharonov-Bohm-eects to weak localization, reveals small irregular fluctuations as the function of the magnetic field B that look like noise upon first sight. However, these fluctuations are completely reproducible for a given sample. Furthermore the fluctuations are the more pronounced the lower the temperature is. Upon moderate annealing, the fluctuations become smaller to reappear again once the temperature is reduced (Fig. 9.20). The fluctuation pattern is dierent for dierent samples and represents a fingerprint of a specific sample thereby. The theoretical description of these universal conductance fluctuations is based on diusive transport in small sections of a conductor. We consider a conductor of length L to consist of separate small compartments of length lF in which the transport is diusive yet phase-conserving (Fig. 9.21). Hence, inside each compartment the scattering is elastic with fixed phase shifts. Among all possible quasi-classical trajectories, some closed loops exist.

280

9 Motion of Electrons and Transport Phenomena

R (Ω)

710

(a)

0,8K

705 700

5K

695

ΔG (e2/h)

690

1 (b)

0,8K

0 –1 –2

0

4

2

6

8

10

Magnetic field B (T)

Fig. 9.20. Universal conductance fluctuations measured on an InN-whisker (nano-column of 67nm diameter, distance between contacts 410nm) prepared by self-organized growth (Panel XVIII) in molecular beam epitaxy (Panel XVII). (a) Magnetoresistance vs. the magnetic field perpendicular to the column at temperatures of 0.8 and 5 K. The resistance includes a typical contact resistance of 300 O. (b) Conductance fluctuations at 0.8 K normalized to the conductance quantum e2/h calculated from the data in (a). (After BloÈmers et al. [9.14])

With a magnetic field B applied, the loops enclose a magnetic flux. Hence, upon variation of the magnetic field, the phases of clockwise and counter clockwise circulations are shifted with respect to each other and the transmission of each compartment shows characteristic fluctuations as function of the applied magnetic field. The fluctuation pattern is dierent L

(a)

lΦ

lΦ

B≠0

lΦ

Φ2 Φ1

(b)

lΦ

Φ3

lΦ B =0

Fig. 9.21. The sketch illustrates the origin of universal conductance fluctuations in a wire of length L that is a multiple of the phase coherence length lF. (a) The transport is phase coherent inside compartments of length lF. (b) Because of elastic scattering (scattering centers marked as black dots) the electrons may travel in closed loops. The magnetic fluxes F1, F2, F3 shift the phases of the wave functions of clockwise and counter clockwise circulating electrons with respect to each other

9.9 Quantum Transport in Nanostructures

281

for consecutive compartments because their defect configuration is dierent. The individual fluctuations in each compartment add up to the total fluctuations DR of the entire conductor as stochastic noise does. Hence, DR is proportional to the square root of the number of consecutive compartments, r p L DR / N / :
9:113 lF The total resistance R on the other hand is proportional to the number of consecutive compartments N. The length dependence of the fluctuations in the conductance is therefore 3=2 DR lF :
9:114 jDGj 2 / N 3=2 / L R

Change in conductance ΔGRMS (e 2/h)

The length-dependence of the conductance fluctuations has been experimentally confirmed for a sample that consisted of a series of N silver rings with N=1, 3, 10, and 30 (Fig. 9.22). The rings are connected by stripes of 75 nm width and 20 nm thickness. The conductance oscillations due to the Altshuler-Aronov-Spivak-oscillations of the frequency h/2e are independent of the number of the rings. The universal conductance fluctuations decrease with the number of rings N according to (9.115). Universal conductance fluctuations may cause considerable problems for the reproducibility of nanoscale quantum devices at low temperatures.

100

AAS-oscillations

N=4 10–1

Theory

100

101

102

Number of rings N

Fig. 9.22. Root mean square amplitude (RMS) of universal conductance fluctuations DGRMS (dashed line) and Altshuler-Aronov-Spivak(AAS)-oscillations (solid line) as measured on silver ring structures consisting of a series of N connected rings with N = 1, 3, 10, 30 (see insert). Thickness and width of the conductor are 20 nm and 75 nm, respectively. Measurements were performed in magnetic fields between 0.2 und 0.3 T at a temperature of 0.32 K. (After Umbach et al. [9.15])

282

9 Motion of Electrons and Transport Phenomena

Problems 9.1 Discuss the dierence between relaxation time, s, and free flight time, sc, using the example of the electrical conductivity of a classical gas. Assume that at time t = 0 the charged particles are moving with a velocity v 0 x in the x-direction. After switching o the electric current the particles are elastically scattered after a time sc with a non-isotropic scattering probability p (H), where H is the angle with the x-axis. Show that the mean velocity of the particles in the x-direction decreases exponentially with a relaxation time sc s= where hcos Hi is the average value of cos H over the distri1 hcos Hi bution p(H) . Compare the free flight time and the relaxation time. Under what conditions are they identical? In a solid, electrons are scattered by defects. Discuss the various types of defect with regard to the expected relation between s and sc. 9.2 Using the stationary Boltzmann equation, show that the mobility of charged particles in a classical gas is given by l

ehv 2 s
ki mhv 2 i

:

9.3 Calculate the electric field dependence of the conductivity r (E ) using the second iteration for the solution of the Boltzmann equation. In the second iteration step, as in the first, use a field-independent distribution f0. Discuss interesting applications of a material with a highly field-dependent conductivity. 9.4 Consider a semi-infinite metallic half-space with two point contacts on the surface. A magnetic field B is applied parallel to the surface and perpendicular to the line joining the point contacts. One point contact is used as a source of electrons injected into the metal, the second as a detector. Draw electron trajectories for the case where the transport is ballistic. ± At what values of B do you expect a maximum signal at the detector? ± Calculate the signal as a function of B. 9.5 Consider a semiclassical model of a cyclotron resonance experiment, where the motion of a quasi-free particle in a solid is described by the eective mass m and relaxation time s. a) Derive the cyclotron frequency xc. b) Derive the dierential equations of motion for the electron drift velocity in a static magnetic field B = (0, 0, B) and a simultaneous high-frequency (rf) electric field E = [A exp (ixt ), A exp i(xt + p/2), 0], where the associated rf magnetic field is neglected. Scattering processes are described by a frictional term mv /s.

Problems

283

c) Calculate from the current density in the x-direction the conductivity r = jx /E x, whereby Re {r} gives the damping of the electric field. d) Plot the real part of the conductivity Re {r} as a function of xc /x for the values xcs = 0.2, 1, 3 and discuss the curves. e) How can electron resonances be distinguished from hole resonances? f) A clystron yields rf radiation at a frequency of 2.41010 Hz. Maximum absorption is observed for a magnetic field B = 8.610±2 Tesla. Determine the mass ratio m/m0 of the carriers. Over what range of relaxation time and of mobility l is a resonance observable? 9.6 a) Calculate the density of states D
1
E for the electronic subband of a one-dimensional conductor following Sect. 7.5. Sketch the density of states as function of the electron energy E for a sequence of subbands as they exist in a conducting wire. b) Which scattering processes are possible in electron transport if only a single subband is occupied? What is dierent if a second subband is occupied so that the Fermi-level intersects two subbands? 9.7 Consider the ballistic transport in a two-dimensional surface electron gas (2DEG) along a nanocolumn (Fig. 9.17b) in a magnetic field along the axis of the column. Electrons may embark upon trajectories that connect the two contacts at the upper and lower end directly, or they may wind around the column. The latter motion can be separated into a propagation along the column (z-direction) and a circular path around the column (in the x,y-plane). a) Establish the Hamilton-operator H for the motion of an electron between the two contacts in a magnetic field B by considering the vector potential A and the kinetic momentum p±eA. It is useful to introduce cylinder coordinates (unit vectors e', ez) in which the vector potential A is A Bre' =2. Furthermore, we make use of the representation of the angular momentum Lz mr2 '_ for the circular movement in which r is the radius of the column. b) By using the product ansatz for the wave function w
r; 'v
z that decouples the motion along the z-axis and the circular motion one may show that the energy eigenvalues of the SchroÈdinger-equation are 2 k2z h h2 l El 2m 2mr2

F F0

2 :

Here, kz is the wave-vector of the motion along the z-axis, l the quantum number for the angular momentum, Lz, F the magnetic flux through the column, and F0 h=e the magnetic flux quantum. c) Sketch and discuss the energy eigenvalues El as function of the magnetic flux F.

284

9 Motion of Electrons and Transport Phenomena

d) Show that the transport along the column is in 1D-subbands formed by the eigenstates jli of the angular momentum and that the magnetoresistance displays oscillations with the period F0 as function of the flux F. e) In what respect do the oscillations with the period F0 as considered here dier from the Aharonov-Bohm(AB)- or Altshuler-Aronov-Spivak(AAS)oscillations in the magnetoresistance? f) What other magneto-oscillations caused by electron interferences may be superimposed on the oscillations considered here?

Panel VIII

Panel VIII Quantum Oscillations and the Topology of Fermi Surfaces

The Fermi surface of a metal is a surface defined in k-space by the relation E (k) = EF. Electrons at the Fermi surface are particularly important because only they are capable of absorbing energy in infinitesimal quantities. It is these electrons, therefore, that determine all transport properties, such as electrical conductivity (Sect. 9.5), which, as we have seen, depends on an integral over the Fermi surface. Fermi surfaces can be calculated from a known bandstructure by applying the condition E (k) = EF. Experimental methods are also available for the direct and very exact measurement of Fermi surfaces. These methods are based on the observation of quantized oscillations in a magnetic field. The origins and manifestations of quantum oscillations are not easy to understand, and their explanation will take us somewhat further afield. Free electrons in a magnetic field experience an additional force, the socalled Lorentz force. This acts perpendicular to the magnetic field and the velocity and causes a rate of change of momentum: mv_ e
vv B :

VIII:1

For electrons in the solid, we can use (9.4) to set mvv = h k and v = h±1 rk E (k). From the time-dependent variation of the momentum, we obtain the corresponding rate of change of the wave vector dk e 2 rk E
k B : dt h

VIII:2

Thus the electrons move in a plane perpendicular to the magnetic field and tangential to the surfaces of constant energy in k-space. We wish now to calculate the period of this orbit: h2 1 dk
VIII:3 T dt e B rk E
k? : Here we have introduced [rk E (k)]^, which is the component of the gradient perpendicular to the B-field. We can also write this component as dE/dk^ with k^ being the component of k perpendicular both to the B-field and to the contour line on the energy surface along which the electron moves (Fig. VIII.1). From Fig. VIII.1, we can also see that the path integral is none other than the derivative of the cross-sectional area with respect to energy

Panel VIII Quantum Oscillations and the Topology of Fermi Surfaces

Panel VIII

286

Fig. VIII.1. The Fermi-surface orbit of an electron in a solid under the influence of an applied magnetic field. The period of the orbit is proportional to the derivative of the cross-sectional area with respect to energy

dk? dS dk : dE dE

VIII:4

The period T

2 dS h eB dE

VIII:5

is thereby connected to the energy dependence of the area enclosed by the electron orbit in k-space. In general, the orbital periods are dierent for different electrons in k-space; however, for a free electron gas they are all equal. For this case, one can readily convince oneself that, since S = pk 2, dS m
VIII:6 2p 2 dE h and thus T

2pm : eB

VIII:7

Here m * is the eective mass (Sect. 9.1). For a magnetic field of 1 T (104 G), we obtain, for example, a period of T = 3.6 10±11 s. This period in k-space is also the period in real space, and we could also have derived this result for free electrons from the equality of the centrifugal and Lorentz forces (e v B = m v xc, see also Panel XV). The electron orbit is then a closed path, and the frequency xc = 2 p/T is also called the cyclotron frequency. According to our derivation, electrons under the influence of a magnetic field move on continuous paths. How can this be made consistent with the discrete k-vectors, which we have assumed up until now? The discrete values for the components of the wave vector and their uses as quantum numbers arise from the three-dimensional translational invariance. In a magnetic field, however, the SchroÈdinger equation is no longer translationally

287

invariant in the directions perpendicular to the magnetic field. In the SchroÈdinger equation, p must thus be replaced by p + e A, where B = curl A. The components of the k-vector perpendicular to the magnetic field axis (kx, ky) are therefore no longer good quantum numbers and the whole band model collapses. Fortunately, we can still make some predictions about the energy levels, provided the magnetic fields are not too large. According to the correspondence principle, the energetic splitting of two neighboring levels, En+1±En, is En1

En

2p h hx c ; T

VIII:8

where T is the period of the orbit around the cross-sectional area, and xc is the frequency [VIII.1]. The estimate of 3.610±11 s for the period allows us to estimate a dierence between energy levels of 1.110±4 eV for a magnetic field of 1 T. The existence of such discrete levels can be demonstrated via the absorption of electromagnetic radiation, clearly transitions can occur only from occupied states below the Fermi level to unoccupied states above the Fermi level (cyclotron resonance, cf. Panel XV). The interpretation of cyclotron resonances in metals is rather dicult though, because the period T depends, among other things, on the position of the cross-sectional area S which the electron path circumscribes in k-space. We now tackle the question of how k-space can be quantized although kx, ky are no longer good quantum numbers. Inserting (VIII.5) in (VIII.8), and replacing the dierential quotient dS/dE by the dierence quotient (Sn+1±Sn)/(En+1±En), we obtain Sn1

Sn 2p

eB : h

VIII:9

Hence, in a magnetic field, the areas enclosed by the electron path are quantized in k-space. Contrary to this, the states on the orbital path are degenerate. Interestingly, the dierence between the areas Sn+1±Sn is constant (for large n ) and independent of kz. The electrons are located on a concentric set of so-called Landau tubes (Fig. VIII.2). The allowed states in k-space ``condense'' onto these tubes as soon as even a minimal field is switched on. It must be remembered, however, that the distance between tubes is very small for normal magnetic fields. The total number of states, of course, does not change on ``condensation''. For each particular kz, all states which were between the tubes prior to condensation must be on the tubes after condensation. So far we have considered only a constant magnetic field. What happens when we slowly increase B ? Equation (VIII.9) tells us that the Landau tubes slowly expand, and thus successively leave the Fermi surface E (k) = EF (Fig. VIII.2) passing through a contour of contact. If the contact contour of the Fermi level is exactly between two Landau tubes, the highest occupied states lie below the Fermi level. The average energy is then lower than when

Panel VIII

Panel VIII Quantum Oscillations and the Topology of Fermi Surfaces

Panel VIII Quantum Oscillations and the Topology of Fermi Surfaces

Panel VIII

288

Fig. VIII.2. In a magnetic field, the allowed states of the electrons lie on so-called Landau tubes. These tubes are characterized by two properties: (1) The orbit of an electron in the plane perpendicular to B is around a surface of constant energy. (2) The magnetic flux enclosed between two successive tubes is constant. The axis of the tubes is only parallel to the magnetic field when the latter is directed along a principle symmetry axis of the solid. For the sake of simplicity, we show here only the tubes of circular cross section that would be obtained in the case of a free electron gas with a spherical Fermi surface at zero field. In a magnetic field, the occupied states lie on those parts of the Landau tubes that are within the sphere

the Landau tube is just leaving the Fermi surface at the contact contour. The average energy therefore oscillates. These periodic quantum oscillations are in principle observable in all solid state properties, and have in fact been observed in many. According to (VIII.9), the period of this oscillation in B is DB

2pe 2 B : SF h

VIII:10

The period DB directly measures cross-sectional areas of the Fermi surface. It is for this reason that quantum oscillations are so significant in understanding the topology of Fermi surfaces.

Fig. VIII.3. The Fermi surface of the noble metals Cu, Ag and Au make contact with the Brillouin zone boundary around the point L. Thus, perpendicular to the h111i directions for example, there are two orbits with extremal area. Perpendicular to the h110i and h100i directions there are also closed orbits that lie between the Fermi surfaces of neighboring Brillouin zones and thus enclose empty states (hole orbits). In addition, one finds open trajectories in which the electrons travel through the extended zone scheme of k-space. Such open trajectories clearly have no orbital period and it is not possible to apply the arguments derived for closed orbits

289

Panel VIII

Panel VIII Quantum Oscillations and the Topology of Fermi Surfaces

Fig. VIII.4 a, b. Original recordings of the oscillations found in the magnetic susceptibility of gold (a) As a function of magnetic field strength, (b) upon varying the direction of the magnetic field (after [VIII.3]). Such quantum oscillations can only be observed of course for a sufficiently sharp Fermi distribution
k T < hxc

The periodic oscillations of the magnetic susceptibility known as the de Haas-van Alphen eect [VIII.2] have gained particular practical importance. As an example we show some measurements on gold. In gold (as in Cu, cf. Fig. 7.12) the d-states are occupied and the Fermi level falls in the region of the sp-band. Hence the Fermi surface is approximately spherical, although it is deformed somewhat to make contact with the zone boundaries along the [111] directions. This distortion of the sphere

Panel VIII

290

Panel VIII Quantum Oscillations and the Topology of Fermi Surfaces

means that the Fermi surface is joined by a neck to the next Brillouin zone (Fig. VIII.3). For a magnetic field along the [111] direction, there are therefore two types of closed orbits along which the Landau tubes can peel o from the Fermi surface with increasing magnetic field. These are the so-called neck and belly orbits. Their cross-sectional areas determine the period of the de Haas-van Alphen oscillations. Figure VIII.4 a shows an original spectrum for this situation. The ratio of the cross-sectional areas can be read o directly by comparing the periods (1 : 29). In addition, using (VIII.9), we can calculate from the data that the cross-sectional areas are 1.51015 cm±2 and 4.31016 cm±2, respectively. With this information, one can construct an image of the Fermi surface such as that shown in Fig. VIII.3. If the angle of the magnetic field axis is varied at constant field strength, one again observes oscillations. This is because at some angles the Landau tubes touch the Fermi surface along the contact contour, while at other angles they do not (Fig. VIII.4 b). The oscillations disappear at angles where the orbit is not closed. Closed orbits with definite periods were prerequisites for the derivation of the relations (VIII.3±10).

References VIII.1 L. Onsager: Philos. Mag. 43, 1006 (1952) VIII.2 W. J. de Haas, P. M. van Alphen: Leiden Comm. 208 d, 212 a (1930) VIII.3 B. Lengeler: Springer Tracts Mod. Phys. 82, 1 (Springer, Berlin, Heidelberg 1978)

10 Superconductivity

In Chap. 9, the basic aspects of the phenomenon of electrical conductivity in metals were introduced and explained. The finite resistance of these materials originates from the fact that a real crystal always exhibits deviations from perfect lattice periodicity: phonons and defects. An infinitely high electrical conductivity is unthinkable in this description, because (1) a crystal without a certain degree of disorder is inconceivable according to the second law of thermodynamics, and (2) even in the absence of phonon and defect scattering, electron-electron scattering will still cause resistance (Sect. 9.3). However, in the year 1911, Onnes [10.1] discovered that the electrical resistance of mercury approaches an unmeasurably small value when it is cooled below 4.2 K. This phenomenon is called ``superconductivity'', and in the subsequent years many more materials were found to be superconducting when cooled to below a certain critical temperature Tc . A microscopic explanation, which, as we know from Chap. 9, cannot be obtained within the framework of a one-electron approximation, was not found for nearly half a century. It was not until shortly before 1960 that Bardeen, Cooper and Schrieer [10.2] achieved the decisive break-through and proposed the theory now named after them (BCS theory). After a short introduction to the basic phenomena of superconductivity, this chapter will give a simplified illustration of how the important properties of superconductors can be understood within the framework of BCS theory.

10.1 Some Fundamental Phenomena Associated with Superconductivity The property that gives superconductivity its name was discovered by Onnes [10.1] in mercury. Figure 10.1 shows the classical experimental results: on cooling below about 4.2 K the electrical resistance of the mercury sample collapses. It was assumed at that time to be below 10±5 X. In fact, it is fundamentally impossible to test experimentally whether the resistance is zero; one can only set an upper limit to the value of the electrical resistance, and this of course still applies to today's much improved measurement methods. The best experimental method of measuring very small resistances, which Onnes also used in addition to current-voltage measurements, is to measure the decrease of a current in a closed conducting loop. A magnetic flux H. Ibach, H. LuÈth, Solid-State Physics, 4th ed., DOI 10.1007/978-3-540-93804-0_10, Ó Springer-Verlag Berlin Heidelberg 2009

292

10 Superconductivity

Fig. 10.1. Original measurement curve for Hg with which, in 1911, the phenomenon of superconductivity was first discovered. On cooling to below 4.2 K, the electrical resistance falls below the experimental detection limit (at that time *10±5 X). (After [10.1])

through the loop is created with a magnet, and the material is then cooled to below the critical temperature Tc, so that it becomes superconducting. Removal of the magnet alters the flux through the loop, thereby inducing a current. If the ring had a finite resistance R, the current would decrease according to I
t I0 exp
Rt=L ;

10:1

where L is the self-induction of the loop. With this and similar arrangements it is possible to show that the resistance of a metal decreases by at least 14 orders of magnitude when it enters the superconducting state. Superconductivity is not confined to just a few chemical elements; the periodic table in Fig. 10.2 shows that this property is found in many elements. Both non-transition metals such as Be and Al as well as transition metals such as Nb, Mo and Zn show the eect. Semiconductors like Si, Ge, Se and Te transform to a metallic phase under high pressure and then become superconducting at low temperatures. Superconductivity may depend on the crystal structure. This is clearly seen in the case of Bi, where several of the modifications are superconducting with dierent transition temperatures, while one modification does not show the eect down to 10±2 K. A crystalline structure is not a necessary condition for superconductivity. Amorphous and polycrystalline superconducting samples, which are produced by rapid condensation onto cooled substrates, play an important role in modern research. In addition, a large number of alloys display superconductivity, with Nb3Al0.75Ge0.25, for example, having a relatively high transition temperature of 20.7 K. At present, the most fascinating superconductors are the ceramic materials, consisting, for example, of the elements Ba-Y-Cu-O. These materials can have an extremely high transition temperature in the vicinity of 100 K (Sect. 10.11). It is noticeable that the ferromagnetic materials like Fe, Co, Ni (Fig. 10.2) do not display superconductivity. It is now believed that their

10.1 Some Fundamental Phenomena Associated with Superconductivity

293

H

He

Li

Be 0.03

B

C

N

O

F

Ne

Na

Mg

Al 1.19

Si 6.7

P 4.6–6.1

S

Cl

Ar

K

Ca

Sc

Ti 0.39

V 5.3

Cr

Mn

Fe

Co

Ni

Cu

Zn 0.9

Ga 1.09

Ge 5.4

As 0.5

Se 6.9

Br

Kr

Rb

Sr

Y 0.5–2.7

Zr 0.55

Nb 9.2

Mo 0.92

Tc 7.8

Ru 0.5

Rh 325 µ

Pd

Ag

Cd 0.55

In 3.4

Sn 3.7;5.3

Sb 3.6

Te 4.5

J

Xe

Hf

Ta 4.4

W 0.01

Re 1.7

Os 0.65

Ir 0.14

Pt

Au

Hg 4.15 3.95

Tl 2.39 1.45

Pb 7.2

Bi 3.9 7.2;8.5

Po

At

Rn

Ce 1.7

Pr

Nd

Pm

Sm

Eu

Gd

Tb

Dy

Ho

Er

Tm

Yb

Lu 0.1–0.7

Th 1.37

Pa 1.3

U 0.2

Np

Pu

Am

Cm

Bk

Cf

Es

Fm

Md

No

Lw

Cs 1.5 Fr

Ba La 1.8;5.1 4.8;5.9 Ra

Ac

Fig. 10.2. The periodic table of the elements showing known superconductors (shaded ) and their transition temperatures Tc (in [K]). Dark shading means that only a high pressure phase of the element is superconducting

strong ferromagnetism is the reason for this and we will see in Sect. 10.6 that strong magnetic fields have the eect of suppressing superconductivity. It should be emphasized that, in general, the transition of a metal from its normal state to a superconducting state has nothing to do with a change of crystallographic structure; furthermore, no ferromagnetic, ferrimagnetic or antiferromagnetic transition is involved. This can be demonstrated by scattering experiments with X-rays, electrons and neutrons (Panel I). What actually occurs in the transition from the normal to the superconducting state is a thermodynamic change of state, or phase transition, which is clearly manifest in other physical quantities. The specific heat as a function of temperature, for example, changes discontinuously at the transition temperature Tc . Figure 10.3 shows the example of Al with a transition temperature of 1.19 K. The specific heat cn of a normally conducting metal is composed of a lattice-dynamical part cnl and an electronic part cne . From (6.51) we have cn cne cnl cT bT3 :

10:2

In the normal conducting state (n) cn varies smoothly at low temperatures, similar to Fig. 6.8. At the transition to the superconducting state (at Tc ) the specific heat jumps and then at very low temperatures sinks to below the value of the normal phase. Normally one assumes that at the transition to the superconducting state the lattice dynamical part cnl remains constant. A more exact analysis then shows that, for a superconductor, the electronic

294

10 Superconductivity

Fig. 10.3. Specific heat of normally conducting (cn) and superconducting (cs) aluminium. Below the transition temperature Tc , the normally conducting phase is created by applying a weak magnetic field of 300 G. (After [10.3])

part (cne*T for a normal conductor) must be replaced by a component which, well below the critical temperature, decreases exponentially cse exp
A=k T :

10:3

A further distinctive property of a superconductor is its magnetic behavior. The magnetic properties of a material that transforms to the superconducting state cannot simply be described by the Maxwell equations with the additional requirement of a vanishing electrical resistance (R ?0). Figure 10.4 A shows schematically how an ideal conductor, whose resistance is zero below a critical temperature, would behave, if it were cooled in an external magnetic field Bext, i.e. if it loses its resistance in the magnetic field. For any closed path (enclosing area S ) in a material, it must be true that
IR U curl E dS B_ S :
10:4 S

Vanishing resistance implies that the magnetic flux B S through the closed loop may not alter, i.e. that the magnetic field inside the material must be maintained both after cooling and after switching o the external field Bext. On switching o Bext in the cooled state, this requirement is satisfied because the process of switching o the field induces persistent currents inside the material, which maintain the magnetic field in the interior. If such a conductor were cooled to below Tc in a field-free space (Bext = 0), and thereafter the external field Bext was switched on, then because R = 0 the interior of the material must remain field-free, again due to the eect of the induced persistent current. After switching o Bext in the cooled state the interior of the material now remains field-free. An ideal conductor in the sense of (10.4) could thus, for Bext = 0 and T < Tc , adopt two dierent states: with and without an internal field, depending on the order of events leading to this state. Hence, if a superconductor were merely such an ``ideal conductor'', the superconducting state would not be a state in the thermodynamic sense. In fact, in the superconductor not only is

10.1 Some Fundamental Phenomena Associated with Superconductivity

295

Fig. 10.4. Magnetic behavior of an ideal conductor (A) and a superconductor (B): (A) In an ideal conductor, the final state (d ) or (g) depends on whether the sample is first cooled to below Tc before applying the magnetic field Bext, or alternatively, cooled in the presence of the field. (a ? b ) The sample loses its resistance when cooled in a field-free region. (c) Application of Bext to sample with zero resistance. (d ) Magnetic field Bext switched off. (e ? f ) Sample loses its resistance in the magnetic field. (g) Magnetic field Bext switched off. (B) For a superconductor, the final states (d) and (g) are identical, regardless of whether Bext is switched on before or after cooling the sample: (a ? b) sample loses its resistance upon cooling in the absence of a magnetic field. (c) Application of the field Bext to the superconducting sample. (d ) Bext switched off. (e ? f ) Sample becomes superconducting in the applied magnetic field Bext. (g) Magnetic field Bext switched off

B_ = 0, but also B = 0, independent of the path by which the state is reached. A superconductor behaves as sketched in Fig. 10.4 B. This eect, which represents a property independent of the vanishing resistance (R = 0), is called, after its discoverers, the ``Meissner-Ochsenfeld eect'' [10.4]. Because of the Meissner-Ochsenfeld eect, the magnetic state of a superconductor can be described as ideal diamagnetism. Persistent surface currents maintain a magnetisation M = ±Hext in the interior, and this magnetisation is exactly opposite to the applied magnetic field Hext. If an external magnetic field is applied to a superconductor at a temperature T < Tc, then a certain amount of energy is consumed to induce the supercurrents which maintain the interior of the sample magnetically field-free. If the magnetic field strength Hext is increased, then at a critical field strength Hc it is energetically more favorable for the material to convert to the normally conducting phase, in which the magnetic field penetrates the material.

296

10 Superconductivity

Fig. 10.5. Schematic phase diagram of a superconductor. The phase boundary between superconducting and normally conducting states corresponds to the critical magnetic field Hc (T)

This transition is admittedly associated with an increase of the free energy (see the specific heat in Fig. 10.3), but a strong increase of the field Hext would lead to an even higher energy expenditure in inducing the screening currents. There thus exists an upper critical magnetic field strength Hc (which is also temperature dependent), above which the superconducting phase no longer exists. A qualitative phase diagram of a superconductor as a function of temperature T and external magnetic field is shown in Fig. 10.5.

10.2 Phenomenological Description by Means of the London Equations A purely phenomenological description of superconductivity, particularly the eects described in Sect. 10.1, requires a modification of the conventional equations of electrodynamics. This description, which is not an atomistic explanation of superconductivity, was first suggested by London and London [10.5]. The vanishing resistivity, R = 0, is included in the classical equations for the motion of an electron in an external field E (9.42) by neglecting the ``friction'' ``term (m v D/s ). Thus, for a superconducting electron, one has mv_

eE :

10:5

For the current density js = ±e ns v of the superconducting electrons (density ns) the first London equation follows ns e j_s m

2

E

:

_ it follows that With this, and the Maxwell equation curl E = B, @ m curl js B 0 : @t ns e2

10:6

10:7

This equation describes the behavior of an ideal conductor
R 0, but not the ideal diamagnetism associated with the Meissner-Ochsenfeld eect, i.e. the ``expulsion'' of a magnetic field. From (10.7), as from (10.4), it merely

10.2 Phenomenological Description by Means of the London Equations

297

follows that the magnetic flux through a conducting loop remains constant. Integrating (10.7) gives an integration constant, which, if set to zero, yields the second London equation in which the Meissner-Ochsenfeld eect is correctly described curl js

ns e 2 B: m

10:8

It should again be emphasised that (10.8) was derived under two assumptions: (1) that R vanishes and (2) that the integration constant in (10.7) vanishes. To describe a superconductor in a magnetic field we now have, with the abbreviation, m kL
10:9 ns e 2 the following system of equations at our disposal: the two London equations

E

kL j_s ;

B

10:10 a

kL curl js ;

10:10 b

and, in addition, the Maxwell equation curl H js

or

curl B l0 js :

10:11

Equation (10.10) is the superconducting equivalent of Ohm's law for a normal conductor. Combining (10.11) with (10.10) yields l0 curl curl B l0 curl js B
10:12 a kL 1 l0 curl B j ; or
10:12 b curl curl js kL kL s l0 B0;
10:13 a DB kL l0 D js j 0:
10:13 b kL s For the two-dimensional problem of a semi-infinite superconductor in a vacuum under a homogeneous magnetic field B = (Bx, 0, 0), as sketched in Fig. 10.6, one obtains @ 2 Bx @z2

l0 Bx 0 ; kL

10:14 a

@ 2 js y @z2

l0 js y 0 : kL

10:14 b

From (10.11) it follows that js has the form (0, js y , 0).

298

10 Superconductivity

Fig. 10.6. Semi-infinite superconductor (z > 0) in a magnetic field that is homogeneous in the vacuum (z < 0)

The solutions of these equations, q Bx B0x exp l0 =kL z B0x exp
z=KL ; js y

j 0s y

q exp l0 =kL z j 0s y exp
z=KL

10:15 a
10:15 b

show that the magnetic field actually penetrates the superconductor. However, the field decays exponentially into the interior over the so-called London penetration depth q KL m=l0 ns e2 :
10:16 The solution (10.15 b) for js y indicates that the superconducting currents, which screen the interior of the superconductor against external fields, also decay exponentially with distance into the solid. For an order of magnitude estimate of the London penetration depth, we set m equal to the electron mass and take ns to be the atomic density, i.e., we assume that each atom provides a superconducting electron. For Sn, for example one obtains KL = 260 AÊ. An important element of the microscopic theory of superconductivity is that it is not electrons but electron pairs, so-called Cooper pairs, which are the current carriers. This can be included in the London equations if, instead of ns, one uses half of the electron density ns /2. Because the London equations describe the Meissner-Ochsenfeld eect particularly well, a microscopic theory of superconductivity should be able to provide, among other things, an equation of the type (10.10 b). This, and an explanation of the vanishing resistance at suciently low temperature (T < Tc), is the central concern of the BCS theory mentioned above. Because superconductivity is evidently a widespread phenomenon, the theory must also be suciently general; it should not hinge on one special metallic property. In the following sections the basic aspects of the microscopic theory of superconductivity will be treated in a somewhat simplified form.

10.3 Instability of the ``Fermi Sea'' and Cooper Pairs

299

10.3 Instability of the ``Fermi Sea'' and Cooper Pairs From the previously mentioned fundamental experiments on the phenomenon of superconductivity, it is clear that we are dealing with a new phase of the electron gas in a metal which displays the unusual property of ``infinitely high'' conductivity. An important contribution to our understanding of this new phase was made by Cooper [10.6] who, in 1956, recognized that the ground state (T = 0 K) of an electron gas (Sect. 6.2) is unstable if one adds a weak attractive interaction between each pair of electrons. Such an interaction had already been discussed by FroÈhlich [10.7] in the form of the phonon-mediated interaction. As it passes through the solid, an electron, on account of its negative charge, leaves behind a deformation trail aecting the positions of the ion cores. This trail is associated with an increased density of positive charge due to the ion cores, and thus has an attractive eect on a second electron. The lattice deformation therefore causes a weak attraction between pairs of electrons (Fig. 10.7 a). This attractive electronelectron interaction is retarded because of the slow motion of the ions in comparison with the almost instantaneous Coulomb repulsion between electrons; at the instant when an electron passes, the ions receive a pull which, only after the electron has passed, leads to a displacement and thereby to a polarization of the lattice (Fig. 10.7 b). The lattice deformation reaches its maximum at a distance from the first electron which can be estimated from

Fig. 10.7 a, b. Schematic representation of the phonon-induced electron±electron interaction that leads to the formation of Cooper pairs. (a) An electron (e±) travelling through the crystal lattice leaves behind a deformation trail, which can be regarded as an accumulation of the positively charged ion cores, i.e., as a compression of the lattice planes (exaggerated here for clarity). This means that an area of enhanced positive charge (compared to the otherwise neutral crystal) is created behind the electron, and exerts an attractive force on a second electron. (b) Qualitative plot of the displacement of the ion cores as a function of their distance behind the first electron. Compared with the high electron velocity v F (*108 cm/s), the lattice follows only very slowly and has its maximum deformation at a distance v F 2 p/xD behind the electron, as determined by the typical phonon frequency xD (Debye frequency). Thus the coupling of the two electrons into a Cooper pair occurs over distances of more than 1000 AÊ, at which their Coulomb repulsion is completely screened

300

10 Superconductivity

the electron velocity (Fermi velocity v F*108 cm/s) and the phonon vibration period (2 p/xD*10±13 s). The two electrons correlated by the lattice deformation thus have an approximate separation of about 1000 AÊ. This then corresponds to the ``size'' of a Cooper pair (which is also estimated in Sect. 10.7 using a dierent method). The extremely long interaction range of the two electrons correlated by a lattice deformation explains why the Coulomb repulsion is insignificant; it is completely screened out over distances of just a few AÊngstroms. Quantum mechanically, the lattice deformation can be understood as the superposition of phonons which the electron, due to its interaction with the lattice, continuously emits and absorbs. To comply with energy conservation, the phonons constituting the lattice deformation may only exist for a time s = 2 p/x determined by the uncertainty relation; thereafter, they must be absorbed. One thus speaks of ``virtual'' phonons. The ground state of a non-interacting Fermi gas of electrons in a potential well (Chap. 6) corresponds to the situation where all electron states with wave vector k within the Fermi sphere [E 0F (T = 0 K )= h 2 k 2F/2 m ] are filled and all states with E > E 0F are unoccupied. We now perform a Gedankenexperiment and add to this system two electrons [k1, E (k1)] and [k2, E (k2)] in states just above E 0F. A weak attractive interaction between these two electrons is switched on in the form of phonon exchange. All other electrons in the Fermi sea are assumed to be non-interacting, and, on account of the Pauli exclusion principle, they exclude a further occupation of states with jkj < kF . Due to phonon exchange the two additional electrons continually change their wave vector, whereby, however, momentum must be conserved: k1 k2 k01 k02 K :

10:17

Since the interaction in k-space is restricted to a shell with an energy thickness of h xD (with xD = Debye frequency) above E 0F the possible k-states are given by the shaded area in Fig. 10.8. This area and therefore the number of energy-reducing phonon exchange processes ± i.e. the strength of the attractive interaction ± is maximum for K = 0. It is therefore sucient in what follows to consider the case k1 = ±k2 = k, i.e. electron pairs with equal and opposite wave vectors. The associated two particle wave function w (r1, r2) must obey the SchroÈdinger equation h2
D1 D2 w
r1 ; r2 V
r1 ; r2 w
r1 ; r2 2m Ew
r1 ; r2
e 2E0F w
r1 ; r2 :

10:18

e is the energy of the electron pair relative to the interaction-free state
V 0, in which each of the two electrons at the Fermi level would possess h 2 k 2F/2 m. The two-particle function in this case consists of an energy E 0F = two plane waves

10.3 Instability of the ``Fermi Sea'' and Cooper Pairs

301

Fig. 10.8. Representation (in reciprocal space) of electron pair collisions for which k1 k2 k01 k02 K remains constant. Two spherical shells with Fermi radius kF and thickness Dk describe the pairs of wave vectors k1 and k2. All pairs for which k1+k2 = K end in the shaded volume (rotationally symmetric about K ). The number of pairs k1, k2 is proportional to this volume in k space and is maximum for K = 0

1 i k1 r1 1 i k2 r 2 1 p e p e 3 ei k
r1 3 3 L L L

r2

:

10:19

We note that (10.19) implies that the two electrons have opposite spin (compare Sect. 8.3). The most general representation of a two-particle state for the case of a non-vanishing interaction
V 6 0 is given by the series 1 X g
kei k
r1 r2 ;
10:20 w
r1 r2 3 L k which depends only on the relative coordinate r = r1±r2. The summation is confined to pairs with k = k1 = ±k2, which, because the interaction is restricted to the region h xD (Fig. 10.9), must obey the condition E0F

EF is of interest

302

10 Superconductivity

The quantity jg
kj2 is the probability of finding one electron in state k and the other in ±k, that is, the electron pair in (k, ±k). Due to the Pauli principle and the condition (10.21 a) we have ( k 2m
E0F hxD =h2 : Inserting (10.20) in (10.18), multiplying by exp (±i k ' r ) and integrating over the normalization volume yields 2 k2 h 1 X g
k 3 g
k0 Vkk0
e 2E0F g
k : L 0 m

10:22

k

The interaction matrix element 0 Vkk0 V
re i
k k r dr

10:23 0

0

describes scattering of the electron pair from
k; k to
k ; k and vice versa. In the simplest model this matrix element Vkk0 is assumed to be independent of k and attractive, that is, Vkk0 < 0: 8 2 2 < h k h2 k02 0 V0
V0 > 0 for EF < ; < E0F hxD Vkk0 2m 2m : 0 otherwise : (10.24) It thus follows from (10.22) that 2 2 h k 0 e 2EF g
k A ; m V0 X A 3 g
k0 L 0

where

10:25 a
10:25 b

k

is independent of k. After summing (10.25 a) over k and comparing with (10.25 b), consistency demands that 1

V0 X 1 L3 k e h2 k2 =m

2EF0

:

10:26

We denote n h2 k2 =2m EF0P and replace the sum over pair states k by the R integral over the k space (L±3 k ) dk/4p3) and keep in mind that the sum as well as the integral extends only over the manifold of states of one spin type. We have already encountered such summations in the context of exchange interaction between electrons (Sect. 8.4). With reference to Sect. 7.5 we split the integral over the entire k-space into an integral over the Fermi sphere and the energy (using (7.41) as an expression for the density of states) and obtain from (10.26)

10.3 Instability of the ``Fermi Sea'' and Cooper Pairs

1 V0

1

ZZ

2p3

dSE jgradk E
kj 2E

dE e 2E 0F

with E

h2 k2 : 2m

303

10:27a

Since the integral over the energy extends only over the narrow interval between E 0F and E 0F + h xD , the density of the free electron gas (7.41)
2m3=2 0
E F n1=2 D
E 0F
10:27b 2p2 h3 can be considered as a constant [&D (E 0F)]. Since we integrate over pair states (k, ±k), half the density of states Z (E 0F) = D (E 0F)/2 at the Fermi energy has to be taken. From (10.26) and (10.27) one then obtains: hx
D 1 0 dn :
10:28 1 V0 Z
E F 2n e D
E 0F n

0

By performing the integration we obtain 1 e 2 hxD 1 V0 Z
E 0F ln or 2 e 2 hx D e : 1 exp2=V0 Z
E 0F

10:29 a
10:29 b

For the case of a weak interaction, V0 Z
E 0F 1, it follows that e

2 hx D e

2=V0 Z
E 0F

:

10:30

There thus exists a two-electron bound state, whose energy is lower than that of the fully occupied Fermi sea (T = 0) by an amount e = E±2 E 0F < 0. The ground state of the non-interacting free electron gas, as treated in Sect. 6.2, becomes unstable when a minute attractive interaction between electrons is ``switched on''. It should be noted that the energy reduction e (10.30) results from a Gedankenexperiment in which the Fermi-sea for states with h 2 k 2/2 m < E 0F is assumed to be fixed and only the eect of the attraction between two additional electrons in the presence of the Fermi-sea is treated. In reality the instability leads to the formation of a high density of such electron pairs, so called Cooper pairs (k, ±k), via which the system tries to achieve a new lower-energy ground state. This new ground state is identical to the superconducting phase, as we shall see. In the aforegoing treatment it was important that the Pauli principle applies to both electrons. The two-particle wavefunction (10.20) was symmetric in spatial coordinates (r1, r2) under exchange of electrons 1 and 2, but the whole wavefunction including spins must be antisymmetric (the most general formulation of the Pauli principle). The spin part of the wave-function, not indicated in (10.20), must therefore be antisymmetric. The Cooper pair therefore comprises two electrons with opposite wave vectors and opposite spins
k "; k #. In this connection one often speaks of singlet pairs. It should be noted that a more complicated electron-electron coupling could lead to parallel spin pairs, so-called triplets. Models of this type have been discussed, but

304

10 Superconductivity

experimental proof of the existence of such states has not yet been found. Triplet pairs have however been found in liquid 3He. At low temperatures this system behaves like a degenerate Fermi gas.

10.4 The BCS Ground State In Sect. 10.3 we saw how a weak attractive interaction, resulting from electronphonon interaction, leads to the formation of ``Cooper pairs''. The energy reduction of the Fermi sea due to a single pair was calculated in (10.29). Such a Cooper pair must be imagined as an electron pair in which the two electrons always occupy states
k "; k #,
k0"; k0#, and so on, with opposed k-vectors and spin. The scattering of the pair from
k "; k # to
k0"; k0# mediated by Vk k' leads to an energy reduction on the formation of a Cooper pair (Fig. 10.10). Due to this energy reduction ever more Cooper pairs are formed. The new ground state of the Fermi sea after pair formation is achieved through a complicated interaction between the electrons. The total energy reduction is not obtained by simply summing the contributions (10.29) of single Cooper pairs. The eect of each single Cooper pair depends on those already present. One must thus seek the minimum total energy of the whole system for all possible pair configurations, taking into account the kinetic one-electron component and the energy reduction due to ``pair collisions'', i.e., the electron-phonon interaction. Since an excitation above E 0F is necessary, the pairing is associated with an increase in kinetic energy. The kinetic component can be given immediately: If wk is the probability that the pair state
k "; k # is occupied, the kinetic component Ekin is X wk nk ; with nk E
k E0F :
10:31 Ekin 2 k

The total energy reduction due to the pair collisions
k "; k # !
k0"; k0# can be most easily calculated via the Hamiltonian H , which explicitly takes account of the fact that the ``annihilation'' of a pair
k "; k # and the ``simultaneous creation'' of a pair
k0"; k0#, i.e. a scattering from
k "; k #

Fig. 10.10. Representation in k space of the scattering of an electron pair with wave vectors (k, ±k) to the state (k', ±k')

10.4 The BCS Ground State

305

to
k0"; k0#, leads to an energy reduction of Vkk0 (Sect. 10.3 and Fig. 10.10). Since a pair state k can be either occupied or unoccupied, we choose a representation consisting of two orthogonal states j1ik and j0ik; where j1ik is the state in which
k "; k # is occupied, and j0ik is the corresponding unoccupied state. The most general state of the pair
k "; k # is thus given by jwk i uk j0ik v k j1ik :

10:32

This is an alternative representation of the Cooper pair wavefunction (10.19). Hence wk = v 2k and 1±wk = u 2k are the probabilities that the pair state is occupied and unoccupied, respectively. We shall assume that the probability amplitudes v k and uk are real. It can be shown in a more rigorous theoretical treatment that this restriction is not important. In the representation (10.32) the ground state of the many-body system of all Cooper pairs can be approximated by the product of the state vectors of the single pairs Y jfBCS i '
uk j0ik v k j1ik :
10:33 k

This approximation amounts to a description of the many-body state in terms of non-interacting pairs, i.e., interactions between the pairs are neglected in the state vector. In the two-dimensional representation 1 0 j1ik ; j0ik
10:34 0 k 1 k one can use the Pauli matrices 0 1 0
1
2 ; rk rk 1 0 k i

i 0

k

10:35

to describe the ``creation'' or ``annihilation'' of a Cooper pair: The operator
1

2

1 r k 2
rk i rk

10:36 a

transforms the unoccupied state j0ik . into the occupied state j1ik , while
1

rk 12
rk

2

i rk

10:36 b

transforms the state j1ik into j0ik From the representations (10.34±10.36) one can deduce the following properties: r k j1ik 0 ; rk j1ik j0ik ;

r k j0ik j1ik ;

10:37 a

rk j0ik 0 :

10:37 b

± The matrices r + k and rk are formally identical to the spin operators introduced in Sect. 8.7. Their physical interpretation as ``creator'' and ``annihilator'' of Cooper pairs is however completely dierent from that in Sect. 8.7, where the reversal of a spin was described.

306

10 Superconductivity

Scattering from
k "; k # to
k0"; k0# is associated with an energy reduction by an amount Vk k '. In the simple BCS model of superconductivity (as in Sect. 10.3) this interaction matrix element Vk k ' is assumed to be independent of k, k ', i.e. constant. We relate this to the normalization volume of the crystal, L 3, by setting it equal to V0 /L 3. The scattering process is described in the two-dimensional representation as annihilation of k and creation of k '. The operator that describes the corresponding energy reduction ± is thus found to be ±(V0 /L 3) r + k ' r k. The total energy reduction due to pair collisions k ? k ' and k ' ? k is given by summing over all collisions and may be expressed in operator terminology as X1 1 V0 X H 3 V0
r r r0:
10:38 0 rk rk rk0 k L L3 0 k k 0 2 kk

kk

Since V0 is restricted to the shell h xD around E 0F, the sum over k, k ' likewise includes only pair states in this shell. In the sum, scattering in both directions is considered; the right-hand side of (10.38) follows when one exchanges the indices. The energy reduction due to collisions is given from perturbation theory as the expectation value of the operator H (10.38) in the state jfBCS i (10.33) of the many-body system hfBCS jH jfBCS i " # Y X V0 Y
u h0j v p h1j r
uq j0iq v q j1iq : k rk0 L3 p p 0 q

10:39

kk

± In evaluating (10.39), one should note that the operator r + k (rk) acts only on the state j1ik (j0ik ). The explicit rules are given in (10.37). Furthermore, from (10.34) we have the orthonormality relations

k h1j1ik

1;

k h0j0ik

We thus obtain hfBCS jH jfBCS i

1;

k h1j0ik

0:

V0 X v k u k0 u k v k0 : L3 0

10:40

10:41

kk

According to (10.31, 10.41) the total energy of the system of Cooper pairs can therefore be represented as X V0 X v 2k nk v k u k v k0 u k0 :
10:42 WBCS 2 L3 0 k kk

The BCS ground state at T = 0 K of the system of Cooper pairs is given by the minimum, W 0BCS, of the energy density WBCS. By minimizing (10.42) as a function of the probability amplitudes uk and v k we obtain the energy of the ground state W 0BCS and the occupation and non-occupation probabilities wk = v 2k and (1±wk ) = u 2k. Because of the relationship between v k and uk, the calculation is greatly simplified by setting

10.4 The BCS Ground State

p wk cos hk ; p uk 1 wk sin hk ; vk

307

10:43 a
10:43 b

which guarantees that u2k v 2k cos2 hk sin2 hk 1 :

10:43 c

The minimizing is then with respect to hk. The quantity to be minimized can be written X V0 X WBCS 2nk cos2 hk cos hk sin hk0 cos hk0 sin hk L3 0 k kk X 1 V0 X 2nk cos2 hk sin 2hk sin 2hk0 :
10:44 4 L3 0 k kk

The condition for the minimum of WBCS then reads @WBCS V0 X 2nk sin 2hk cos 2hk sin 2hk0 0 ; @hk L3 0

or

10:45 a

k

nk tan 2hk

1 V0 X sin 2hk0 : 2 L3 0

10:45 b

k

We let V0 X V0 X 0v 0 u sin hk0 cos hk0 ; k k L3 0 L3 0 k k q Ek n2k D2

D

10:46
10:47

and obtain from standard trigonometry sin 2hk tan 2hk cos 2hk

D=nk ;

10:48

2uk v k sin 2hk D=Ek ; v 2k

u2k

10:49

nk =Ek :

10:50 wk = v 2k,

of a pair state
k "; k # in the Thus the occupation probability, BCS ground state at T = 0 K is given by 0 1 1 nk 1B nk C A : 1
10:51 wk v 2k @1 q 2 2 Ek 2 2 nk D This function is plotted in Fig. 10.11. At T = 0 K (!) it has a form similar to the Fermi function at finite temperature and a more exact analysis shows that it is like the Fermi distribution at the finite critical temperature Tc. It should be noted that this form of v 2k results from the representation in terms

308

10 Superconductivity

Fig. 10.11. The BCS occupation probability v 2k for Cooper pairs in the vicinity of the Fermi energy E 0F. The energy is given as nk = E (k)±E 0F , i.e., the Fermi energy (nk = 0) serves as a reference point. Also shown for comparison is the Fermi-Dirac distribution function for normally conducting electrons at the critical temperature Tc (dashed line ). The curves are related to one another by the BCS relationship between D(0) and Tc (10.67)

of single-particle states with well-defined quantum numbers k. This representation is not particularly appropriate for the many-body problem; for example, one does not recognize the energy gap in the excitation spectrum of the superconductor (see below). On the other hand, it can be seen in the behavior of v 2k that the Cooper pairs which contribute to the energy reduction of the ground state are constructed from one-particle wavefunctions from a particular k-region, corresponding to an energy shell of D around the Fermi surface. The energy of the superconducting BCS ground state W 0BCS is obtained by inserting in WBCS ± (10.42 or 10.44) ± relationships (10.48±10.51) which follow from the minimization. The result is W0BCS

X

nk
1

nk =Ek

k

L3

D2 : V0

10:52 a

The condensation energy of the superconducting phase is obtained by subtracting from W 0BCS the energy of the normal conducting phase, P i.e., the energy of the Fermi-sea without the attractive interaction W0n jkj EC ;

12:4 a

E < EV :

12:4 b

The density in the region of the forbidden band EV < E < EC is of course zero. In an intrinsic semiconductor all ``free'' electrons in the conduction band originate from states in the valence band, and thus the concentration of holes p must be equal to the concentration of ``free'' electrons n. The situation is sketched in Fig. 12.5. If the eective masses mn and mp and therefore also the densities of states DC and DV are equal, the Fermi level EF must lie in the middle of the forbidden band. If DC and DV are dierent

426

12 Semiconductors

Fig. 12.5. (a) Fermi function f (E), density of states D (E) and electron (n) and hole (p) concentrations in the conduction and valence bands for the case of equal densities of states in the conduction and valence bands (schematic); (b) the same figure for the case of diering densities of states in the conduction and valence bands. The number of holes must again be equal to the number of electrons, and thus the Fermi level no longer lies in the middle of the gap between conduction and valence bands; its position then becomes temperature dependent

from one another, then EF shifts slightly towards one of the band edges, such that the occupation integrals (12.3) remain equal. Because the ``width'' of the Fermi function (*2 k T) is, at normal temperatures, small compared to the gap width (*1 eV), the Fermi function f (E, T) can be approximated by Boltzmann occupation statistics within the bands (E > EC and E < EV), i.e. for the conduction band: ! 1 E EF exp 1 for E EF 2 k T : kT exp
E EF =k T 1 (12.5) From (12.3 a) and (12.4 a), the electron concentration n in the conduction band follows as 3=2
2m E =k T n n e F 2p2 h3

1

p E EC e

k

E= T

dE :

12:6

EC

Substituting XC = (E±EC)/k T, we obtain the formula !1
3=2
2m EC EF n 1=2 3=2 k
T exp XC e XC dXC : n 3 2 k T 2p h

12:7

0

With an analogous calculation for the valence band, one finally obtains the expressions

12.2

2 p mnk T n2 h2

p2

2 p mpk T h2

Charge Carrier Density in Intrinsic Semiconductors

!3=2 exp

!3=2 exp

EC

EF kT

EV

!

! NC eff exp

EC

EF kT

EF EV EF NV eff exp kT kT

427

! ;
12:8 a

! :

12:8 b

V The prefactors N C eff and N eff are the well-known partition functions for translational motion in three dimensions. One sees that small concentrations of free charge carriers in semiconductors can be approximately described by Boltzmann statistics (the approximation to Fermi statistics for E±EF 2 k T). If one compares Fig. 12.5 with the potential well model of Chap. 6, the conduction band can be formally regarded as a potential well, in which the Fermi level EF lies well below ( k T) the bottom of the potential well. V The use of the so-called ``eective densities of states'' N C e and N e in (12.8) allows a further formal interpretation in which the whole conduction (valence) band can be characterized by a single energy level EC (EV) (i.e., V the band edge) with the density of states N C e (N e) (temperature dependent!). The occupation densities n and p of these bands are determined by the Boltzmann factor (with the energy in each case measured from EF). This approximation, which is often valid for semiconductors, is called the approximation of non-degeneracy. High densities of charge carriers can be created in semiconductors by means of high densities of impurities (Sect. 12.3). The approximation of non-degeneracy is then no longer valid and one speaks of degenerate semiconductors. From (12.8 a, b) the following generally valid relationship can be derived (Eg = EC±EV): !3 kT Eg =k T C V 3=2 e Eg =k T : n p Neff Neff e 4
m
12:9 n mp 2 2p h

This equation implies that for a particular semiconductor, which is completely characterized by its absolute band gap Eg and the effective masses mn and m p in the conduction and valence bands, the electron and hole concentrations behave as a function of temperature according to the law of mass action. If we further assume an intrinsic semiconductor
n p, then the intrinsic charge carrier concentration ni varies with temperature as follows !3=2 q kT Eg =2k T E =2 k T C V 2
mnmp 3=4 e g : ni pi Neff Neff e 2 2p h (12.10) Values of ni and Eg for the important materials Ge, Si and GaAs are summarized in Table 12.4.

428

12 Semiconductors

Table 12.4. Band gap Eg and the intrinsic carrier concentration ni for germanium, silicon and gallium arsenide at 300 K

Ge Si GaAs

Eg [eV]

ni [cm±3]

0.67 1.1 1.43

2.4 1013 1.5 1010 5 107

According to (12.8 a, b), the Fermi level at a particular temperature adopts the position necessary to yield charge neutrality, i.e. n p NC eff e e

k

2EF = T

EF

k

k

E C = T EF = T

e

k

NV eff
EV EC = T e NC eff

NV eff e

k

EV = T

e

k

EF = T

;

;

12:11
12:12

EC EV k T EC EV 3 C k T ln
mp =mn : ln
NV eff =Neff 4 2 2 2
12:13

If the effective densities of states and effective masses (i.e. the band curvature of the conduction and valence bands) are equal, then the Fermi level of an intrinsic semiconductor lies exactly in the middle of the forbidden band, and this is true for all temperatures. If, however, the effective densities of states in the conduction and valence bands are different, then the Fermi function lies asymmetrically with respect to the band edges EC and EV (Fig. 12.5) and the Fermi level shows a weak temperature dependence according to (12.13).

12.3 Doping of Semiconductors The intrinsic carrier concentration ni of 1.5 1010 cm±3 (at 300 K) of Si is not nearly large enough to yield the current densities necessary for practical semiconductor devices. Concentrations that are orders of magnitude higher than ni can be created by doping, i.e. by the addition of electrically active impurities to the semiconductor. Most semiconductors cannot be grown as single crystals with sufficient purity that one can observe intrinsic conductivity at room temperature. Unintentional doping, even in the purest commercially available GaAs single crystals, leads to carrier densities of about 1016 cm±3 (at 300 K), compared with a corresponding intrinsic concentration of ni = 5 107 cm±3. Electrically active impurities in a semiconductor raise the concentration of either the ``free'' electrons or the ``free'' holes by donating electrons to the conduction band or by accepting them from the valence band. These

12.3

Doping of Semiconductors

429

Fig. 12.6 a, b. Schematic representation of the eect of a donor (a) and an acceptor (b) in a silicon lattice. The valence-five phosphorus atom is incorporated in the lattice at the site of a silicon atom. The fifth valence electron of the phosphorus atom is not required for bonding and is thus only weakly bound. The binding energy can be estimated by treating the system as a hydrogen atom embedded in a dielectric medium. The case of an acceptor (b) can be described similarly: the valence-three boron accepts an electron from the silicon lattice. The hole that is thereby created in the valence band orbits around the negatively charged impurity. The lattice constant and the radius of the defect center are not drawn to scale. In reality the first Bohr radius of the ``impurity orbit'' is about ten times as large as the lattice parameter

impurities are called donors and acceptors, respectively. A donor in a Si lattice is created, for example, when a valence-four Si atom is replaced by a valence-five atom such as P, As or Sb. The electronic structure of the outermost shell of these impurities is s 2 p 3 instead of the 3s 2 3 p 2 Si configuration. To adopt the tetrahedral bonding structure of an s p 3 hybrid in the lattice, only the s 2 p 2 electrons of the valence-five atom are necessary; the excess electron in the p shell has no place in the s p 3 hybrid bond. This electron can be imagined as weakly bound to the positively charged and tetrahedrally bonded donor core, which has replaced a Si atom in the lattice (Fig. 12.6 a). A valence-five donor impurity in the Si lattice can be pictured, to a good approximation, as a positively charged monovalent core, to which one electron is bound. The electron can become dissociated and can then move ``freely'' through the lattice; i.e., on ionization, this electron will be excited from the impurity into the conduction band. The donor impurity can be described as a hydrogen-like center, in which the Coulomb attraction between the core and the valence electron is screened by the presence of Si electrons in the vicinity. To estimate the excitation and ionization energy of the extra phosphorus electron (Fig. 12.6 a), one can approximate the screening eect of the surrounding Si by inserting the dielectric constant of Si (eSi = 11.7) into the expression for the energy levels of the hydrogen atom. The energy levels for the Rydberg series of the hydrogen atom are EH n

me e4

1 n 2
4 p e0 h 2 2

12:14

430

12 Semiconductors

and for the n = 1 level, the ionization energy is 13.6 eV. For the P donor, the mass me of the free electron must be replaced by the effective mass m n = 0.3 me of a silicon conduction electron, and the dielectric constant e0 of vacuum by e0 eSi. A value for the ionization energy Ed of the donor of *30 meV results. The energy level ED of the donor electron in the bound state should thus lie about 30 meV below the conduction band edge EC . A still smaller value is obtained for germanium. Here, eGe = 15.8 and m ED ^6 meV is obtained. The situation n *0.12 me. An estimate of
EC is depicted in a bandstructure scheme in Fig. 12.7, where only the ground state of the donor is drawn. Between this ground state and the conduction band edge are a series of excited states [n > 1 in (12.14)], whose spacing decreases with increasing energy, and which finally join the continuum of the conduction band. The situation is very similar to that of the H atom, where the conduction band continuum corresponds to the unbound states above the vacuum level. The energy of the excited states can be determined, for example, from optical spectra. Figure 12.8 shows an absorption spectrum of the Sb donor in Ge. The bands below 9.6 meV correspond to excitations from the ground state to higher, excited states. The spectrum is actually more complicated than would be expected from the simple hydrogenic model; this is because the crystal field lifts the partial degeneracy of the hydrogen-like states. Above a photon energy of 9.6 meV, the electrons are excited to the continuum of the conduction band. As can be seen from the experimental example in Fig. 12.8, the simple description of the donor by a hydrogenic model allows one to estimate the order of magnitude of the ionization energy Ed. Within this model all donor impurities, such as P, As and Sb, should have the same ionization energy Ed when present in the same semiconductor host. The experimental values of Ed in Table 12.5 show, however, that the values vary somewhat from donor to donor.

Fig. 12.7. Qualitative position of the ground state levels of donors and acceptors relative to the minimum of the conduction band EC and the maximum of the valence band EV . The quantities Ed and Ea are the ionization energies of the donor and acceptor, respectively

12.3

Doping of Semiconductors

431

Fig. 12.8. Optical absorption spectrum of a Sb donor in germanium, measured at T = 9 K. (After [12.2])

Table 12.5. Ionization energies Ed for a few donor species in silicon and germanium

Si Ge

P [meV]

As [meV]

Sb [meV]

45 13

54 14

43 10

It is not surprising to find that the crude description of screening in terms of the dielectric constant of the semiconductor is inadequate to describe the finer details resulting from atomic eects. That the description by a macroscopic dielectric constant nonetheless yields good values for Ed, is because the screening leads to a wavefunction which is ``smeared out'' over many lattice constants. Inserting the dielectric constant of the semiconductor es in the formula for the Bohr radius r e0 es

h2 p mn e2

12:15

expands this radius by a factor of es (*12 for Si) compared to the (hydrogen) Bohr-radius. The bound valence electron of the donor impurity is therefore ``smeared'' over about 103 lattice sites. If a valence-three impurity atom (B, Al, Ga, In) is present in the lattice of a valence-four elemental semiconductor (Si, Ge), the s p 3 hybrid responsible for the tetrahedral bonding can easily accept an electron from the valence band

432

12 Semiconductors

Table 12.6. Ionization energies Ea for a few acceptor species in silicon and germanium

Si Ge

B [meV]

Al [meV]

Ga [meV]

In [meV]

45 11

67 11

74 11

153 12

and leave behind a hole (Fig. 12.6 b). Such impurities are called acceptors. An acceptor is neutral at very low temperature. It becomes ionized when an electron obtains sucient energy to be lifted from the valence band to the so-called acceptor level. Acceptors therefore have the charge character ``from neutral to negative'', while donors are ionized from neutral to positive. The hole that exists in the vicinity of an ionized acceptor is in the screened Coulomb field of the fixed, negative impurity, and the energy needed to separate the hole from the ion and create a ``free'' hole in the valence band can be estimated using the hydrogenic model as in the case of donors. The relationships derived for donors and acceptors are fundamentally similar except for the sign of the charge. Table 12.6 shows that the ionization energies Ea for acceptors are in fact quite close to those of donors. Semiconductors doped with donors and acceptors are called n- and p-type materials, respectively. The lowest impurity concentrations that can presently be achieved in semiconductor single crystals are of the order of 1012 cm±3. Ge with an intrinsic charge carrier concentration ni of 2.4 1013 cm±3 (at 300 K) is therefore obtainable as intrinsic material at room temperature, whereas Si (ni = 1.5 1010 cm±3 at 300 K) does not show intrinsic conductivity at room temperature. In addition to the electrically active impurities discussed here, a semiconductor may of course contain many impurities and defects that cannot be ionized as easily and thus do not aect the electrical conductivity.

12.4 Carrier Densities in Doped Semiconductors In a doped semiconductor, an electron in the conduction band can originate either from the valence band or from the ionization of a donor; likewise, a hole in the valence band may correspond either to the electron in the conduction band or to a negatively charged (ionized) acceptor. For a non-degenerate semiconductor, the occupation of the conduction and valence bands must nonetheless be governed by the Boltzmann approximation (12.8 a, b). Therefore the so-called ``law of mass action'' must also be valid for the doped semiconductor (12.9) V n p NC eff Neff e

k

Eg = T

;

12.4

Carrier Densities in Doped Semiconductors

433

in which the position of the Fermi level EF no longer appears. In comparison with an intrinsic semiconductor, the position of EF is now governed by a rather more complicated ``neutrality condition'', which also takes account of the charge on the impurities: the terms used in the following discussion are represented schematically in Fig. 12.9. The density of all available donors ND and acceptors NA is composed of the density of the neutral donors and acceptors, N 0D and N 0A, and the density of ionized donors N + D (which are then positively charged) and ionized acceptors N ±A (negatively charged). In a homogeneous semiconductor, the negative charge density n+N ±A must be compensated by an equally large positive charge density p+N + D (see Fig. 12.9). Hence, the following neutrality condition governs the position of the Fermi level EF in a homogeneously doped semiconductor: n NA p N D ;

12:16

in which ND N0D N D ;

12:17 a

NA

12:17 b

N0A

NA :

For typical impurity concentrations (1013±1017 cm±3), in which the individual donors and acceptors do not influence one another, the occupation of the donors by electrons (nD) and of acceptors by holes (pA) is given to a good approximation by nD N0D ND 1 exp
ED

EF =k T

1

;

12:18 a

pA N0A NA 1 exp
EF

EA =k T

1

:

12:18 b

Fig. 12.9. Explanation of the notation commonly used for carrier and impurity concentrations in n- and p-type semiconductors: n and p are the concentrations of ``free'' electrons and holes. The total concentrations ND and NA of donors and acceptors consist of the ± density of neutral, N 0D or N 0A, and ionized, N + D or N A, donors and acceptors, respectively. Electrons in the conduction band (density n) and holes in the valence band (density p) originate either from interband excitations or from impurities

434

12 Semiconductors

We neglect here a modification of the Fermi function (multiplication of the exponential term by 12 ), which takes into account the possibility of the capture of a single electron only, however, with two distinguishable spin states. The general case, in which both donors and acceptors are considered simultaneously, can only be treated numerically. We therefore restrict the present treatment to the case of a pure n-type semiconductor, in which only donors are available. Equations (12.8 a, 12.17 a, 12.18 a) can then be used to calculate the concentration of charge carriers. For convenience these are repeated below:

k

EC EF = T

n NC eff e ND N0D

N0D

N D

;

12:8 a

;

12:17 a EF =k T

ND 1 exp
ED

1

:

12:18 a

``Free'' electrons in the conduction band can only originate from donors or from the valence band, i.e., n N Dp:

12:19

As a further simplification we assume that the main contribution to the 2 conductivity stems from ionized donors, i.e. that N + D ni (n p = n i ). For Si 10 ±3 for example (ni = 1.5 10 cm at 300 K) this is readily fulfilled even at low doping levels. For this simple case, (12.19) is replaced by n N D ND

N0D ;

12:20

i.e. with (12.18 a) one has

!

1

n ND 1

1 exp
ED

EF =k T

:

12:21

With the help of (12.8 a), EF can be expressed via
n=NC eff e

k

EC = T

e

k

EF = T

;

12:22

to yield n

ND 1e

k

Ed = T

;

12:23

n=NC eff

where Ed = EC±ED is the energetic distance of the donor level from the conduction band edge. Expressing (12.23) as a quadratic equation for n we have n

n 2 Ed = k T e ND : NC eff

12:24

12.4

Carrier Densities in Doped Semiconductors

The physically meaningful solution is s! N D E =k T n 2ND 1 1 4 C e d Neff

435

1

:

12:25

This expression for the conduction electron concentration in n-type semiconductors contains the following limiting cases: I) If the temperature T is so low that 4
ND =NLeff e

k

Ed = T

then one has q n ND NC eff e

1

Ed =2

kT :

12:26

12:27

In this region, where a sufficiently large number of donors still retain their valence electrons, i.e. are not ionized, one speaks of the freeze-out range of carriers. The similarity between (12.27) and (12.10) should be noted: instead of the valence band quantities N V eff and EV, one now has the corresponding donor quantities ND and Ed (i.e. Ed instead of Eg). In this low-temperature regime, the electron concentration depends exponentially on the temperature T as in an intrinsic semiconductor; here, however, it is the much smaller donor ionization energy Ed that appears in place of Eg. The special case treated here of a pure n-type doping is of course rarely realized in practice. Trace quantities of acceptors are almost always present. As a consequence, the Fermi level lies below ED, and an activation energy of Ed is therefore found in most cases. II) At temperatures T, for which 4
ND =NC eff e

k

Ed = T

1;

12:28

Eq. (12.25) becomes n ND const ;

12:29

i.e. the concentration of donor electrons in the conduction band has reached the maximum possible value, equal to the concentration of donors; all donors are ionized, and one speaks of the saturation range. In a first approximation, one may still neglect electrons excited from the valence band. III) At yet higher temperatures the concentration of electrons excited from the valence band across the gap Eg increases, and eventually outweighs the electron density due to donors. In this region the n-type material behaves as an intrinsic semiconductor and one speaks of the intrinsic region of the carrier concentration. The various temperature and carrier concentration regimes are portrayed in Fig. 12.10 together with the corresponding position of the Fermi level EF .

436

12 Semiconductors

Fig. 12.10 . (a) Qualitative temperature dependence of the concentration n of electrons in the conduction band of an n-type semiconductor for two dierent donor concentrations ND0 > ND . The width of the forbidden band is Eg and Ed is the ionization energy of the donors; (b) qualitative temperature dependence of the Fermi energy EF (T) in the same semiconductor. EC and EV are the lower edge of the conduction band and the upper edge of the valence band, respectively, ED is the position of the donor levels and Ei is the Fermi level of an intrinsic semiconductor

The position of the Fermi level EF as a function of temperature can be discussed analogously to the case of an intrinsic semiconductor, but it will not be explicitly worked out here. In the freeze-out range, one may replace the valence band edge by the donor level. In the region of very high temperature, i.e. in the intrinsic region, the laws pertinent to an intrinsic semiconductor apply. For n-doped Si with a phosphorus concentration of 3 1014 cm±3, the saturation range stretches between 45 and 500 K, i.e., at room temperature all donors are ionized. Figure 12.11 shows experimental results for the electron concentration n
T, determined by Hall eect measurements, of n-doped Ge with impurity concentrations between 1013 and 1018 cm±3. The relationships sketched qualitatively in Fig. 12.10 are clearly recognizable.

12.5

Conductivity of Semiconductors

437

Fig. 12.11. The concentration n of free electrons in n-type germanium, measured using the Hall eect (Panel XIV). For the samples (1) to (6), the donor concentration ND varies between 1018 and 1013 cm±3. The temperature dependence of the electron concentration in the intrinsic region is shown by the dashed line. (After [12.3])

12.5 Conductivity of Semiconductors As was discussed more fully in Sect. 9.5, a calculation of the electrical conductivity r as a function of temperature T requires a more detailed treatment of the mobility. For a semiconductor, one must consider both the electrons in the lower conduction band region (concentration: n, mobility: ln) and the holes at the upper valence band edge (p, lp). The current density j in an isotropic semiconductor (non-tensorial conductivity r) is therefore

438

12 Semiconductors

j e
n ln p lp E :

12:30

In contrast to a metal, where only electrons at the Fermi edge need be considered, i.e. l = l (EF) (Sect. 9.5), the mobilities ln and lp in a semiconductor are average values for the electron and hole occupied states in the lower conduction band and upper valence band, respectively. In non-degenerate semiconductors, Fermi statistics can be approximated by Boltzmann statistics in this region. Within the framework of this approximation, the averaging, which will not be carried out in more detail, yields the following expression ln

1 hs
kv 2
ki e: m hv 2
ki n

12:31

Here v
k is the velocity of an electron in an electric field E at the point k in reciprocal space, and s (k) is its relaxation time (a more exact definition is given in Sect. 9.4). For holes, the quantities in (12.31) are taken at corresponding points in the valence band, and the effective mass mn of the electrons is replaced by that of holes. Instead of deriving a rigorous solution of the Boltzmann equation and an exact further treatment of (12.31), we restrict ourselves in the present case, as we did for metals (Sect. 9.5), to a more qualitative discussion of the scattering processes in semiconductors. In this respect, electrons and holes behave in a qualitatively similar way. After considerable simplification, (12.31) yields a proportionality between the mobility and the relaxation time (l!s). For metals, this proportionality holds exactly, see (9.58 b). Because s is also proportional to the average time between collisions, it follows that 1 / hviR ; s

12:32

where R represents the scattering cross section for electrons and holes at a scattering center. In contrast to the case of metals (Sect. 9.5), hvi is to be considered as a thermal average (according to Boltzmann statistics) over all electron or hole velocities in the lower conduction band or upper valence band, respectively. Because of the validity of Boltzmann statistics in semiconductors, we have p hvi / T :
12:33 If we now consider scattering from acoustic phonons, we can estimate the cross section Rph, as in the case of metals (Sect. 9.5), from the square of the average vibrational amplitude hu2
qi of a phonon
q; xq , i.e. for temperatures T H (H is the Debye temperature), we have (Sect. 9.5) M x2q hu2
qi k T ;

12:34 a

12.5

Conductivity of Semiconductors

Rph T :

439

12:34 b

Using (12.32, 12.33), one then arrives at the following estimate lph T

3=2

:

12:35

In addition to the usual scattering from phonons considered here, the scattering in piezoelectric semiconductors (e.g. III±V and II±VI compounds) may contain substantial contributions from phonons that are associated with a polarization (piezoelectric scattering). Charge carriers can also be scattered from optical phonons of higher energy. In this case the description becomes extremely complicated, since the relaxation time approximation (Sect. 9.4) loses its validity. A further important source of scattering in semiconductors is scattering from charged defects (ionized donors or acceptors). A carrier moving past a point-like charged defect experiences a Coulomb interaction, and the scattering cross section Rdef for this ``Rutherford scattering'' is Rdef / hvi

4

;

12:36 p where the thermal average hvi / T is assumed for the velocity. Equation (12.36) follows from a classical or quantum mechanical treatment of the scattering process (see introductory textbooks on mechanics or quantum mechanics). Because the total scattering probability must also be proportional to the concentration Ndef of impurities, it follows from (12.32, 12.33, 12.36) that 1 / Ndef =T 3=2 ; sdef

12:37

and for the mobility, provided the scattering is due only to charged defects, one thus has ldef / T 3=2 :

12:38

The reciprocal of the total mobility for scattering from defects and phonons is given by the sum of the reciprocal mobilities in (12.35) and (12.38), i.e. the qualitative behavior shown in Fig. 12.12 results. Figure 12.13 shows the experimentally measured dependence l(T) for the electron mobility in n-Ge, as determined from Hall effect and conductivity measurements; for the purest crystals (ND^1013 cm±3), l(T) approaches the theoretically expected dependence for pure phonon scattering (12.35). With increasing donor concentration ND, the additional contribution from impurities (12.38) becomes evident (see also Fig. 12.12). Figure 12.14 shows that the characteristic trend of the mobility in Fig. 12.12 also manifests itself in the temperature dependence of the conductivity in the region of carrier saturation, where n(T) is approximately constant (Figs. 12.10, 12.11). In this region r(T) shows a maximum, while in the regions of intrinsic conductivity (high T ) and in the freeze-out range

440

12 Semiconductors

Fig. 12.12. Schematic temperature dependence of the mobility l for a semiconductor in which scattering from phonons and charged impurities occurs

Fig. 12.13. Experimentally determined temperature dependence of the mobility l of free electrons. For the samples (1) to (6), the donor concentration ND varies between 1018 and 1013 cm±3. The samples are the same as those used for the measurements in Fig. 12.11. (After [12.3])

(low T), the exponential dependence of the carrier concentration n(T) (Fig. 12.11) dominates the weak temperature dependence of the mobility. The experimental results of Figs. 12.11, 12.13 and 12.14 were all obtained from the same Ge samples [numbered from (1) to (6)], so that the conductivity r can be calculated directly from n(T) and l(T).

12.5

Conductivity of Semiconductors

441

Fig. 12.14. Experimentally measured conductivity r of n-type germanium as a function of temperature. For the samples (1) to (6), which were also used for the measurements in Figs. 12.11 and 12.13, the donor concentration ND varies between 1018 and 1013 cm±3. (After [12.3])

So far the discussion of the conductivity of semiconductors was concerned merely with the ohmic behavior at relatively low electric fields E where the carrier drift velocity v D is proportional to the electric field and the mobility l = v D/E is a constant. In modern semiconductor devices with dimensions in the sub-micrometer range electric fields are frequently in excess of 105 V/cm and Ohm's law is no longer valid since the average drift

442

12 Semiconductors

Drift velocity vD (cm/s)

velocity v D is no longer proportional to the field strength. According to experiment and theoretical calculations, the proportionality v D!E remains valid up to fields of about 2 103 V/cm for the important semiconductors Si, Ge, GaAs, etc. (Fig. 12.15). For higher fields v D eventually saturates at a velocity v S &107 cm/s for the indirect semiconductor Si, and similarly for Ge. The energy that is continuously transferred to the carriers by the electric field is lost essentially via phonon scattering processes and is thus converted to heat. Scattering due to optical phonons is particularly ecient in this energy range. The carriers are accelerated in the external electric field along the energy band profiles E
k, until they reach the energy (referred to EF) of optical phonons with high density of states (about 60 meV in Si, 36 meV in GaAs). These phonons are then eciently excited and any further energy gain of the carriers is immediately lost to phonons; the drift velocity saturates as a result. The optical phonons excited in this process are thermalized to low-energy acoustic phonons. A peculiar behavior is observed in direct semiconductors such as GaAs, InP, GaN. These semiconductors display a negative dierential conductivity r @j=@ E en@v D =@ E < 0 for higher electric fields (Fig. 12.15). In the low field regime (< 103 V/cm) electrons have a high mobility because of the low eective mass of 0.068 m0 (for GaAs) in the C-minimum. As the electrons

Electrons Holes

Electric field strength (V/cm)

Fig. 12.15. Carrier drift velocity v D at 300 K as a function of electric field E. The data for Si and GaAs are from a compilation (Sze [12.4]) of experimental results on highly pure, crystalline samples. The curve for GaN is calculated by means of Monte Carlo simulations. (After Gelmont et al. [12.5])

12.6

The p±n Junction and the Metal/Semiconductor Schottky Contact

443

are accelerated to higher kinetic energies eective phonon scattering into the side minima at L and X sets in. Electrons in these minima possess a higher eective mass. Their mobility is therefore lower, and the average drift velocity of the whole ensemble of conduction electrons is thereby reduced. As a consequence, the drift velocity v D passes through a maximum with increasing field strength and eventually saturates at a lower value. The saturation value is then similar to that of Si. With even further increasing field strength, above 3 105 V/cm, the electrons in the side valleys of the band structure with high eective mass are accelerated and the drift velocity v D would again increase proportional to the field strength albeit with much lower mobility than in the low-field regime (< 103 V/cm). In the range of extremely high fields, above some 105 V/cm this eect is, however, superimposed by the onset of the avalanche breakthrough. The accelerated electrons gain so much energy that they excite more and more electrons from the valence into the conduction band. The conductivity of the semiconductor increases abruptly, avalanche-like, by the multiplication of the number of free carriers. This eect is also used in modern devices. It is remarkable that the indirect semiconductor Si has a similar saturation velocity at field strengths above 3 104 V/cm as the indirect semiconductor GaAs (Fig. 12.15). Hence, the mobility advantage of GaAs with respect to Si at low fields is lost in small devices in which rather high fields occur. A further remarkable aspect of Fig. 12.15 is the high drift velocity of the wide band gap semiconductor GaN. Because of its additional high thermal stability GaN is well suited for applications in the area of fast ``hightemperature'' devices. Furthermore, the large band gap energies (> 3 eV) of the group III-nitrides in general (GaN, AlN, AlxGa1±xN) enable high breakthrough voltages (up to 100 V) and this class of material is employed in fast high-power devices.

12.6 The p±n Junction and the Metal/Semiconductor Schottky Contact Modern solid state physics is closely associated with the development of semiconductor devices, i.e. solid state electronics. The operation of almost all semiconductor devices relies on phenomena that are due to inhomogeneities in semiconductors. Inhomogeneous concentrations of donor and acceptor impurities cause particularly interesting conductivity phenomena, which enable the construction of semiconductor devices. The most important building blocks in semiconductor devices are the p±n junction and the metal/semiconductor contact. In a p±n junction, we have a semiconductor crystal which is p-type on one side, and n-type on the other (Fig. 12.16). In the ideal case (which cannot, of course, be practically realized), the transition from one zone to the other would take the form of a step function.

444

12 Semiconductors Fig. 12.16 a±e. Schematic representation of a p±n junction in thermal equilibrium: (a) a semiconductor crystal doped on one side with acceptors
NA and on the other side with donors
ND ; (b) band scheme for the n and p sides for the imaginary case of total decoupling of the two sides. EA and ED indicate the ground states of the acceptors and donors; EF is the Fermi level; (c) band scheme of the p±n junction when the two sides are in thermal equilibrium with one another. The transition from the p to the n doping is assumed to be abrupt. The position of conduction and valence band edges are denoted E pC and E pV deep in the p region, and E nC and E nV deep in the n region. VD is the diusion voltage. In the region of the p± n junction, a so-called macropotential V
x is induced; (d) the fixed space charge R
x in the region of the p±n junction due to the ionized impurities; (e) qualitative behavior of the concentrations of acceptors NA, donors ND, holes p and free electrons n. The intrinsic carrier concentration is ni and pp and pn denote the hole concentrations deep in the p and n regions, respectively (and similarly for np and nn). Considered here is the frequently occurring case in which almost all of the donors and acceptors in the interior of the crystal are ionized

In practice, doping inhomogeneities can be created using a variety of techniques. For example, acceptor impurities can be diused into one region while donors are diused into another. The dopant atoms can also be implanted as ions: the ions of the required dopant elements are ``fired'' into the semiconducting material with high kinetic energy (using high electric fields). In the following we will consider the conduction behavior of a p±n junction, consisting for example of a Si crystal, which is doped in the left half with acceptors (e.g. B, Al, Ga) and in the right half with donors (e.g. P, As, Sb). We begin by considering this inhomogeneously doped semiconductor in thermal equilibrium, i.e. without an externally applied voltage (Fig. 12.16).

12.6

The p±n Junction and the Metal/Semiconductor Schottky Contact

445

The p±n Junction in Thermal Equilibrium Let us first of all imagine that the p- and n-type halves of the crystal are isolated from one another (Fig. 12.16 b), such that the Fermi levels in the two regions lie at different points on the common energy scale. In reality, however, we are concerned with one and the same crystal which simply has an abrupt doping junction. The Fermi level, i.e. the electrochemical potential, must therefore be common to both crystal halves at thermal equilibrium. In the transition zone between the n and p regions there must therefore be a so-called band bending, as shown in Fig. 12.16 c. Within the present semiclassical description, the situation in the transition layer is described by a positiondependent macropotential V(x), which reflects the bending of the band structure. This description is possible because the potential V(x) changes only slightly over a lattice parameter. According to the Poisson equation, the macropotential V(x) corresponds to a space charge R(x) @ 2 V
x @x2

R
x : e e0

12:39

For the limiting case T^0, where, deep inside the crystal, EF lies either near the acceptor level (p-type region) or near the donor level (n-type region), one can understand the origin of the space charge from the following qualitative argument: The bending of the bands in the transition region has the effect that acceptors in the p region are pushed below the Fermi level, i.e. are occupied by electrons, whereas in the n region donors are lifted above the Fermi level, i.e. are unoccupied and thus positively charged. The space charge that results from (12.39) thus consists of ionized acceptors and donors that are fixed in space and give rise to a charged double layer across the jump in the doping profile. In the case of carrier freeze-out shown in Fig. 12.16 (T^300 K, EF between the impurity levels and the middle of the forbidden band), the space charge stems from the fact that the charge of the fixed donors and acceptors in the vicinity of the doping jump is no longer compensated by the mobile electrons and holes of the conduction and valence bands. One therefore speaks of a space-charge region where R(x)=0. The concentrations of charge carriers and impurities associated with this space-charge region are represented in Fig. 12.16 e. Well ± outside the space-charge zone, the donors (N+ D if charged) or acceptors (NA) are compensated by equally large electron (nn) or hole (pp) concentrations. The subscripts n, p indicate whether the electrons and holes are situated in the n or p regions. These carriers correspond to the type of doping in the respective regions and they are denoted majority carriers. Because the electrons and holes are ``freely'' mobile, electrons diffuse into the p region and holes into the n region. There they are called minority carriers and their concentrations are denoted by np (electrons) and pn (holes). In thermal equilibrium, the law of mass action (n2i = np) must be fulfilled at each point. For the concentration of majority carriers (electrons in the n region, nn, or holes in the p region, pp), it follows from the arguments in Sect. 12.3 that

446

12 Semiconductors

nn

NC eff

pp

NV eff

exp

exp

ECn

EF kT EVp kT

EF

! ;

12:40 a

:

12:40 b

!

Furthermore we have n2i

nn pn

C NV eff Neff

exp

ECn

EVn kT

! :

12:41

The diusion voltage VD ± the dierence between the maximum and minimum of the macropotential V(x) (Fig. 12.16 c) ± which is built up in thermal equilibrium, is thus related to the carrier density by eVD

EVn

EVp k T ln

pp nn : n2i

12:42

At low temperature in the carrier freeze-out regime it is evident that p jeVDj*Eg (Fig. 12.16 c). Here, EVn and EV are the valence band edges in the n and p regions. The state of a semiconductor as represented in Fig. 12.16 b±e must be understood as a steady state, because the concentration profiles of ``free'' carriers as in Fig. 12.16 e imply diusion current (electrons diusing from right to left and holes from left to right). On the other hand, a space charge as in Fig. 12.16 d is associated with an electric field E (x) and therefore with drift currents of electrons and holes. We represent the corresponding (charge) current densities as: @n @p diff diff diff j Dp j n j p e Dn ;
12:43 @x @x j drift e
n ln plp E x : j drift j drift n p

12:44

Here Dn and Dp denote the diffusion constants for electrons and holes, respectively. In (dynamic) thermal equilibrium, the currents exactly compensate one another. In the p and n regions electron-hole pairs are continually created due to the finite temperature, and subsequently recombine. The total current density obeys j diff j drift 0

12:45

and thus the separate contributions of the electrons and holes must vanish individually, i.e. for electrons it follows from (12.43±12.45) that Dn where

@n @V
x nln ; @x @x

E x

@V=@x is used.

12:46

12.6

The p±n Junction and the Metal/Semiconductor Schottky Contact

447

If, instead of considering, as in (12.40), the space-charge concentration far outside the space-charge layer where E nC and E pV are constant, we consider it in the space-charge zone itself, then the conduction band edge is of course described by [E pC ± eV(x)] and the concentration of the electrons is position dependent with ! p E eV
x E F C n
x NC ;
12:47 eff exp kT from which it follows that @n e @V n @x k T @x

12:48

or, by substituting into (12.46), Dn

kT e

ln :

12:49

This so-called Einstein relation between carrier diffusion constant and mobility is valid whenever diffusion currents and drift currents are carried by one and the same type of carrier. A relation analogous to (12.49) also applies of course for holes, since the total hole current must vanish too. A rigorous treatment of the p±n junction is not simple because, in the Poisson equation (12.39), the exact form of the space-charge density R
x depends on the interplay of diusion and drift currents [which in turn depends on V(x)]. For the ``abrupt'' p±n boundary treated here, the following approximate solutions can be given; they are known as the Schottky model of the space-charge zone. If we imagine that the zero of the x-axis in Fig. 12.16 is at the junction between the n and the p regions, where the donor (ND) and the acceptor (NA) concentrations abruptly meet, then for the space charge we have the general relations R
x > 0 e
N D R
x < 0

n p

e
NA n

p

in the n-region ;

12:50 a

in the p-region :

12:50 b

The position-dependent concentrations n
x and p
x of ``free'' charge carriers adjust themselves of course according to the respective distances of the conduction and valence band edges from the Fermi level (Fig. 12.16 c). Although this distance changes slowly and monotonically over the entire space-charge zone, the Fermi function and therefore the occupation in an energy region *2 k T (300 K)^0.05 eV, which is small compared to the band gap, changes from approximately zero to its maximum value. If one neglects the so-called transition zone of the Fermi function, then the concentration N + D of charged donors not compensated by free electrons, and the corresponding concentration of charged acceptors N ±A, can be

448

12 Semiconductors

approximated by a step function (Fig. 12.17 a), i.e. the space-charge density becomes 8 0 for x < dp > < eNA for dp < x < 0
12:51 R
x eN for 0 < x < dn > D : 0 for x > dn . With this piecewise constant space-charge density, the Poisson equation, for example for the n region (0 < x < dn) d 2 V
x ' dx2

eND e e0

12:52

can be readily integrated. The calculation for the p region is of course completely analogous. For the electric field E x (x) and the potential V
x in the n region of the space charge zone, one obtains (Fig. 12.17 b, c) e E x
x ND
dn x
12:53 e e0 and V
x Vn
1

eND
dn 2e e0

x2 :

12:54

Outside the ``Schottky space-charge zone'', the potentials are Vn(?) in the n region and Vp(±?) in the p region (Fig. 12.17c). One notes the inverted form of the band edges EV (x) and EC (x) (Fig. 12.16c) compared with the potential energy [E(x)=±eV(x)]. Within the Schottky model, the lengths dn and dp give the spatial extent of the space-charge zone in the n and p regions, respectively. From charge neutrality it follows that ND dn NA dp ; and the continuity of V
x at x = 0 demands e
ND dn2 NA dp2 Vn
1 Vp
1 VD : 2 e e0

12:55

12:56

If the impurity concentrations are known, one can thus calculate the spatial extent of the space-charge layer from the diffusion voltage VD and the difference between the positions of the band edges in the p and n regions. From (12.55) and (12.56) it follows that

dn

2 e e0 VD NA =ND 1=2 ; e NA ND

12:57 a

dp

2 e e0 VD ND =NA 1=2 : e NA ND

12:57 b

12.6

The p±n Junction and the Metal/Semiconductor Schottky Contact

449

Fig. 12.17 a±c. The Schottky model for the space-charge zone of a p±n junction (at x = 0). (a) Spatial variation of the spacecharge density R
x produced by the ionized acceptors
NA and donors
ND . The real form of the curve (dashed) is approximated by the rectangular (full line) form; (b) behavior of the electric field strength Ex (x); (c) the potential V
x in the region of the p±n junction

Since diffusion potentials are typically of the order of Eg, that is about 1 eV, impurity concentrations of 1014±1018 cm±3 result in a space-charge zone of size dn or dp between 104 and 102 AÊ. The electric field strength is therefore between 104 and 106 V/cm in such space charge zones. The Biased p±n Junction ± Rectification If a time-independent external electrical voltage U is applied to a p±n junction, thermal equilibrium is destroyed, and the situation in the p±n junction can be described as a stationary state in the vicinity of thermal equilibrium. Because of the depletion of free carriers (depletion zone), the space-charge zone between ±dp and dn has a considerably higher electrical resistance than the region outside the p±n junction. As a result, the potential drop across the space-charge zone accounts for nearly all of the externally applied voltage U. Thus the band scheme of Fig. 12.16 and the form of the potential in Fig. 12.17 c do not alter except in the region of the space-charge zone; elsewhere, EC (x), EV (x) and V
x are constant and therefore remain horizontal. The potential drop across the space-charge zone, instead of being equal to the diffusion voltage VD (at equilibrium: U = 0 V), now has the value Vn
1 Vp
1 VD U :
12:58 Here U is taken to be positive when the potential on the p side is raised relative to the n side. The externally applied voltage now influences the size of

450

12 Semiconductors

the space-charge zone, since the quantity VD in (12.57) is now replaced by VD ±U. One thus has dn
U dn
U 0
1

U=VD 1=2 ;

12:59 a

dp
U dp
U 0
1

U=VD 1=2 :

12:59 b

In thermal equilibrium, the drift and diffusion currents of electrons are equal and opposite, and the same is true for the hole currents. If an external voltage U is applied, then equilibrium is destroyed. Let us consider, for example, the balance in the electron currents: we are concerned on the one hand with the drift currents of the minority carriers coming from the p region (where electrons are the minority carriers), which are drawn across into the n region by the diffusion voltage VD. Because these minority carriers are continually generated in the p region by thermal excitation, this current is called the generation current, I gen n . For a sufficiently thin space-charge zone and a sufficiently small recombination rate in this region, each electron coming from the p region that finds its way into the field of the spacecharge zone will be drawn from this into the n region. This effect is largely independent of the value of the diffusion voltage and therefore also of the external voltage. The diusion current of electrons from the n region, where the electrons are majority carriers, into the p region (called the recombination current I rec n ) behaves dierently. In this direction the electrons are moving against the potential threshold of the diusion voltage. The fraction of electrons which can overcome the potential threshold is determined by the Boltzmann factor exp [± e (VD±U)/k T ], and is therefore strongly dependent on the externally applied voltage U. The following relations describe the electron currents In through a p±n junction with an externally applied voltage U: Inrec
U 0 Ingen
U j 0 ; Inrec / e

k

e
VD U= T

12:60

;

12:61

which together yield Inrec Ingen e

k

e U= T

;

12:62

and therefore a total electron current of In Inrec

Ingen Ingen
e

k

eU= T

1 :

12:63

The same analysis applies to the hole currents Ip, so that for the characteristic of a p±n junction one obtains ! e U I
U
Ingen Ipgen exp 1 :
12:64 kT

12.6

The p±n Junction and the Metal/Semiconductor Schottky Contact

451

Fig. 12.18. Schematic representation of the current voltage (I±U) characteristic of a p±n junction, together with the corresponding circuit. The maximum current in the reverse direction is given by the sum of the generation currents for electrons and holes

The extremely asymmetric form of this typical rectifying characteristic for the two polarities can be seen in Fig. 12.18. gen To derive a quantitative value of the saturation current ±(I gen n +I p ) in the reverse bias direction, a rather more exact treatment of the stationary state in the presence of a dc voltage U is necessary. It follows from the treatment above that the disturbance of thermal equilibrium is due largely to a change in the diusion currents, while the influence of the external voltage U on the drift currents can, to a good approximation, be neglected. In the framework of the so-called diusion current approximation, it is sucient to consider only the diusion currents under the influence of the voltage U. If we now consider a p±n junction biased in the forward direction (Fig. 12.19), the carrier concentration rises in the space-charge region, as can be seen from Fig. 12.19 b. In this situation, the law of mass action n p = n 2i is no longer fulfilled. The Fermi levels well outside the space-charge zone are dierent by exactly the applied voltage U, corresponding to an energy ±e U (Fig. 12.19 a). In the space-charge zone, which is no longer in thermal equilibrium, a true Fermi level can no longer be defined. If, as is assumed here, the stationary state is close to thermal equilibrium, then it remains possible to describe the situation approximately with Boltzmann statistics. However, instead of a single Fermi level, two so-called quasi Fermi levels, for electrons (dotted line in Fig. 12.19 a) and for holes (dashed line in Fig. 12.19 a), must be introduced. Further details of this approach are beyond the scope of this treatment. Using the approximation that recombination of electrons with holes can be neglected in the space-charge zone, it is sucient to consider the change in the diusion current density at the edges of the space-charge zone, i.e. at x = ±dp and x = dn. Here the calculation is particularly easy. We restrict ourselves to the treatment of hole diusion current densities j di p , because the calculation for electrons is analogous. For the diusion current at x = dn, it follows from (12.43) that @p diff j p
x dn e Dp :
12:65 @x xdn

452

12 Semiconductors

Fig. 12.19 a±c. Forward- and reverse-biased p±n junctions (non-equilibrium state). (a) Band scheme in the presence of an external voltage +U or ±U. The Fermi levels E pF and E nF in the p and n regions are shifted with respect to one another by e U. In the region of the p±n junction, the equilibrium Fermi level (± ±) splits into so-called quasi Fermi levels for electrons ( ) and for holes (± ± ±); (b) spatial variation of the concentration of holes p and electrons n in a biased p±n junction (full line) and without bias at thermal equilibrium (± ± ±). The lengths ±dp and dn give the range of the space charge zone in thermal equilibrium, i.e. without bias voltage. The carrier concentrations deep in the p and n regions are denoted pp , np and pn , nn , respectively; (c) spatial variation of the hole concentration p
x in a forward biased p±n junction in the region outside the thermal equilibrium space-charge zone
x > dn . (Enlarged from Fig. 12.19 b for forward bias)

12.6

The p±n Junction and the Metal/Semiconductor Schottky Contact

453

As will be shown in the following, diffusion theory yields a simple relationship between the concentration gradient @p=@x and the increase in the hole concentration at x = dn. The resulting hole concentration p
x dn (Fig. 12.19 b) at x = dn, due to the applied bias U, follows from Boltzmann statistics as ! VD U p
x dp pp exp e ;
12:66 kT p
x dn pn exp
e U=k T :

12:67

Here dn and dp are the widths of the space-charge zone in thermal equilibrium (U = 0 V). The increased hole concentration leads to increased recombination in the n region, which results in a larger electron current. Far into the n region, the current is thus carried by electrons and far into the p region by holes. The continuity condition implies that the hole concentration in a volume element can only change if holes flow in or out, recombine or are thermally created. The greater the amount by which the hole concentration exceeds the equilibrium concentration pn, the higher is the recombination rate. With an average lifetime sp for a hole, the continuity relation for the non-equilibrium carriers is @p @t

1 div j diff p e

p

pn sp

:

12:68

In the stationary case considered here, @p=@t must be equal to zero and from (12.65, 12.68) we have @p @2p Dp 2 @t @x

p

pn sp

0;

12:69 a

and thus @2p 1
p 2 @x Dp sp

pn :

12:69 b

Solution of this differential equation yields the diffusion profile p
12:70 p
x exp
x= Dp sp : p Here Lp = Dp sp is the diffusion length for holes. This is the distance over which the hole concentration decreases from a certain value, e.g. p
x dn in Fig. 12.19 c, by a factor 1/e. From (12.70) and referring to Fig. 12.19 c, we obtain @p p
x dn pn ;
12:71 @x xdn Lp

454

12 Semiconductors

where, in the case of an externally applied voltage, we have from (12.67) p
x dn

pn pn exp
e U=k T

1 :

12:72

From (12.65, 12.71, 12.72), we finally arrive at the hole diffusion current density due to the externally applied voltage U: e Dp diff jp pn exp
e U=k T 1 :
12:73 Lp xdn Analogous calculations can be carried out for the diusion current carried by electrons, and the total current density flowing through the p±n junction is simply the sum of these two components. As shown above, it is not necessary to consider the drift currents. Their components from the p and n regions are, within the present approximation, unchanged from their thermal equilibrium values and serve merely to compensate the equilibrium part of the diusion current, i.e. ! e Dp e Dn eU j
U pn np 1 :
12:74 exp Lp Ln kT We have thus expressed the generation currents appearing in (12.64) in terms of the diffusion constants and diffusion lengths of electrons and holes, and the minority carrier concentrations pn and np. Figure 12.20 shows an experimentally measured current-voltage characteristic I (U) of a p±n junction. The form of the curve sketched qualitatively in Fig. 12.18 for a rectifier is clearly recognizable. When an external voltage U is applied to a p±n junction, the spatial extent of the space-charge zone dn from (12.59), and thus also the charge stored in the space-charge zone, are altered Qsc ' e ND dn
UA :

12:75

This relation is valid within the framework of the above ``Schottky approximation'' for the p±n junction, where A is the cross-sectional area of the junction (perpendicular to the current flux) and ND is the concentration of donors as above. A p±n junction thus has a voltage-dependent ``space-charge capacitance'' Csc: dQsc d dn
U : e ND A
12:76 Csc dU dU From (12.59 a) and (12.57 a) it follows that 1=2 d 1 2 e e0 VD NA =ND 1 ; dU dn
U 2V e
NA ND 1 U=VD D

12:77

12.6

The p±n Junction and the Metal/Semiconductor Schottky Contact

455

Fig. 12.20. Example of a current-voltage characteristic for a silicon p±n junction. Reverse voltages and currents are given as negative values. (From the advanced lab. course of the II. Physics Institute of the RWTH Aachen)

and so the space-charge capacitance (12.76) can be written Csc

1=2 A NA ND 2 e e e0 : 2 NA ND
VD U

12:78

The relationship (12.78) implies that C2sc

1 VD

U

;

12:79

which explains why a measurement of space-charge capacitance as a function of external voltage is often used to determine the impurity concentrations.

456

12 Semiconductors

Fig. 12.21. Experimentally determined relationship between the space-charge capacitance and the reverse voltage (indicated by negative values) for the Si p±n diode discussed in Fig. 12.19. (From the advanced lab. course of the II. Physics Institute of the RWTH Aachen)

Figure 12.21 shows experimental results for space-charge capacitance as a function of external voltage. The Metal/Semiconductor Schottky Contact Because of its rectifying function ± similar to the p±n junction ± the metal/ semiconductor contact was used as a device already at the beginning of the 20th century with the advent of microelectronics. When a metal is evaporated onto a clean semiconductor surface under good vacuum conditions, mostly an electronic band scheme as in Fig. 12.22 is established in the case of n-doping. The reason is found in the existence of electronic interface states that are formed at the metal/semiconductor interface. Their spatial extension is limited to a few atomic layers around the interface and their energetic distribution is fixed with respect to the conduction and valence band edges of the semiconductor. These interface states, sometimes called MIGS (metal-induced gap states) originate from the Bloch waves in the metal. Bloch waves are extended states in the metal that can not abruptly end at the interface, they must tail into the semiconductor, even in the energy range of the forbidden band, where no electronic bulk states exist on the semiconductor side. In the energy range of the forbidden band these tails of the Bloch states (MIGS) must therefore be mathematically represented by a superposition (Fourier series) of bulk-wave functions of the conduction and valence band, respectively. The energetic band of interface states (MIGS) has thus more conduction-band character (close to the conduction-band edge) or more valence band character (close to the valence-band edge) depending on the percentage of the respective bulk states that constitute the MIGS. Conduction band states are negatively charged when occupied by electrons and neutral in the unoccupied state (acceptor-like); valence band states, however have a donor-like charging character, i.e. positive when empty and neutral in the occupied state. Thus, a neutrality level exists

12.6

Metal

The p±n Junction and the Metal/Semiconductor Schottky Contact

457

n-Semiconductor

Interface states

Fig. 12.22. Electronic band scheme of a metal/semiconductor (n-doped) junction; pinning of the Fermi-level EF in interface states near the neutrality level causes the formation of a Schottky-barrier efSB and a depletion space charge layer within the semiconductor. VD is the ``built-in'' diusion voltage. (a) In thermal equilibrium, (b) under external bias U

within the band of interface states, which separates the more acceptor-like states in the upper part from the more donor-like states in the lower part of the band. When the Fermi energy EF crosses the band of interface states just at the neutrality level, the interface states as a whole are neutral. Slight deviations of EF from the neutrality level cause interface charge within the MIGS: negative if EF lies higher in energy than the neutrality level, positive for EF below the neutrality level. The band bending within the semiconductor in Fig. 12.22 is thus determined by a charge balance between negative charge Qis in the interface states and the positive space charge QSC originating from the ionized bulk donor states in the depletion layer. For atom area densities at the interface of some 1014 cm±2 electronic interface state densities can reach a similar order of magnitude. Typically, these states are distributed over an energy range of 0.1 to 1 eV within the forbidden band. Interface densities of states per energy can thus easily amount to 1015 (eV)±1 cm±2. Such a high density of interface states will practically fix (pin) the Fermi level very close to the neutrality level (Fermi-level pinning). Larger deviations of EF from the neutrality level would cause too high a charge density within the interface that can not be compensated by the space charge

458

12 Semiconductors

within the semiconductor. Changes of the space charge QSC by variation of doping or by means of external electric fields thus can shift the Fermi level within the band of interface states with respect to the neutrality level only by amounts of 10±2 to 10±3 eV. The Schottky barrier (Fig. 12.22) is therefore a quantity that is characteristic for a particular metal-semiconductor junction. Within certain limits it is, of course, slightly aected by atomistic details of the interface structure and morphology. From a comparison of Fig. 12.22 a with Fig. 12.16 b it is evident that a Schottky barrier at a metal-semiconductor junction can be described in a simplifying fashion as one half of a p±n junction, where the p-type semiconductor is replaced by the metal. Obviously, one can interchange the situation; the n-side of the p±n junction can be replaced by a metal and a Schottky barrier in the p-doped semiconductor with hole depletion results. In a pdoped semiconductor EF is close to the valence band edge EV deep in the bulk (Fig. 12.22). The band curvature in the space charge region of the Schottky contact on p-doped material is thus inverse to that of an n-type semiconductor. Under the condition of ideal pinning of EF Schottky barriers for electrons and holes in n- and p-type material of the same semiconductor sum up to the band gap energy. As in a p±n junction the depletion space-charge region in a Schottky contact exhibits a resistance. An external bias produces a voltage drop essentially across the space-charge zone (Fig. 12.22 b). Apart from this spatial range, i.e. within the metal and deep in the semiconductor the voltage drop is negligible and thermal equilibrium is nearly achieved. There, Fermi energies EF can be defined, the energetic dierence of which corresponds to an externally applied voltage. Within the Schottky barrier space-charge region quasi-Fermi levels can be defined similarly as for p±n junctions. The mathematical description of the space-charge region below a metalsemiconductor junction is analogous to a p±n junction. The thickness of the Schottky contact space charge region in thermal equilibrium, e.g., is obtained from (12.57 a) for the p±n junction with the assumption ND NA (much higher metallic conductivity as compared with the p-type semiconductor) as 2 e e0 VD 1=2 d :
12:80 e ND Similarly, the capacity of a metal-semiconductor junction as a function of external bias can be obtained from (12.78) as A 2 e e e0 ND 1=2 ;
12:81 C 2 VD U where A is the area of the contact. The rectifying properties of a p±n junction are analogously found on a metal-semiconductor Schottky contact, as is evident from Fig. 12.22. Electron transport from the metal into the semiconductor requires that the

12.7

Semiconductor Heterostructures and Superlattices

459

carriers overcome the Schottky barrier efSB, while in the inverse direction electrons can penetrate the metal from the semiconductor side without any barrier for an external bias jUj > fSB .

12.7 Semiconductor Heterostructures and Superlattices Using modern epitaxial methods, such as molecular beam epitaxy (MBE, Panel XVII) or metal organic chemical vapor deposition (MOCVD, Panel XVII), it is today possible to deposit two different semiconductors on one another in a crystalline form. These semiconductors will generally have different electronic properties, and in particular different band gaps. Such layer structures play a particularly important role in devices made from III±V semiconductors such as GaAs, InP, etc. It is also significant that using such epitaxial methods, ternary and quaternary alloys of the type AlxGa1±xAs or GaxIn1±xAsyP1±y can be deposited, whose band gaps lie between those of the corresponding binary compounds. By controlled variation of the composition x in AlxGa1±xAs, the electronic bandstructure can be continuously adjusted between that of GaAs and that of AlAs. At the composition x = 0.45, the alloy changes from a direct-gap semiconductor (like GaAs) to an indirect-gap semiconductor (like AlAs) (Fig. 11.13). Figure 12.23 plots the band gap energies at 300 K for the most important binary and elemental semiconductors against the lattice constant. This plot is of particular interest because, as one might expect, it is possible to

Fig. 12.23. Band gap Eg of some important elemental and binary compound semiconductors plotted against the lattice parameter at 300 K. The right-hand scale gives the light wavelength k corresponding to the band gap energy. The connecting lines give the energy gaps of the ternary compounds composed of various ratios of the corresponding binary materials

460

12 Semiconductors

produce particularly good and defect-free epitaxial layers from semiconductors whose lattice constants match. From Fig. 12.23 it can be seen that both band gap and lattice parameter change when one chooses a composition for epitaxy which lies between two binary semiconductors. It can easily be seen that the epitaxy of Ge on GaAs, and vice versa, leads to particularly good lattice matching, and that the alloy system AlGaAs allows a variation of the band gap between 1.4 and 2.2 eV, whereby it is expected that the extremely good lattice matching of the two components GaAs and AlAs should lead to excellent crystalline quality in growing one semiconductor on another. CdTe and HgTe are also an excellent pair of semiconductors which can be grown on one another largely free from defects. The structure consisting of layers of two different semiconductors grown epitaxially on one another is called a semiconductor heterostructure. The width of the transition regions between the two semiconductors can be as little as one atomic layer if a suitable epitaxial method (MBE, MOCVD) is used. In such a heterostructure the band gap changes over distances of atomic dimensions. What does the electronic bandstructure of such a semiconductor heterostructure look like (Fig. 12.24)? Two important questions need to be answered:

Fig. 12.24 a±c. Band schemes (one-electron energies plotted in real space) for a heterostructure formed from semiconductors I and II. (a) Semiconductors I and II are assumed to be isolated; vI and vII are the electron anities, i.e., the energy between the vacuum energy Evac and the lower conduction band edge EC . (b) Semiconductors I and II are in contact, but not in thermal equilibrium because the Fermi levels EF on the two sides have not equalized. DEC and DEV are the band discontinuities in the conduction and valence bands, respectively. (c) In thermal equilibrium, the Fermi energies EF in I and II must be identical. Since the band discontinuities DEC and DEV are predetermined, band bending must occur in the two semiconductors

12.7

Semiconductor Heterostructures and Superlattices

461

a) How are the valence band edges EV and conduction band edges EC to be ``lined up''? This question addresses the so-called band discontinuity or band offset DEV (Fig. 12.24 b). b) What band bending occurs in the two semiconductors I and II to the left and right of the junction (Fig. 12.24 c)? In nearly all cases it is possible to treat these two questions separately and independently of one another, because the relevant phenomena involve different energy and length scales. Matching of the two bandstructures takes place within an atomic distance. Interatomic forces and energies are decisive for this process and the electric fields are of the order of the atomic fields (0108 V/cm). The band bending, on the other hand, takes place over hundreds of AÊngstroms, so that in thermal equilibrium the Fermi level has the same value on both sides of the semiconductor interface, and is determined deep inside each semiconductor by the doping level (Fig. 12.24 c). As was the case for the p±n junction, the decisive condition is that no net current flows in the heterostructure at thermal equilibrium, see (12.45). The band bending in semiconductors I and II is, as in the p±n junction, associated with space charge, and the space-charge field strengths are of the order of 105 V/cm. The most important material-related parameters of a semiconductor heterostructure are therefore the valence and conduction band discontinuities, DEV and DEC . The classical, but nowadays revised, assumption was that in the ideal case the two bandstructures of the semiconductors line up such that the vacuum energy levels Evac match one another. This gave a conduction band discontinuity DEC equal to the dierence in electron anities Dv (Fig. 12.24) DEC vI

vII Dv :

12:82

The electron affinity v , which is the difference between the vacuum energy and the bottom of the conduction band, is a theoretically well-defined quantity in the bulk of a material. It is determined, however, with the aid of surface experiments, in which the bulk value of v can be strongly altered by surface dipoles (e.g. due to the different atomic coordination at the surface). For the interface between two semiconductors v cannot be related in a simple way to the bulk quantities. Band offsets are meanwhile well explained by models in which the electronic bands in ideal, abrupt semiconductor heterostructures are lined up so that no atomic dipoles are created, e.g. due to electronic interface states (similar to MIGS, p. 428) or charge transfer in the chemical bonds at the interface [12.6, 12.7]. A detailed theoretical treatment of these models requires a microscopic description of the electronic properties of the few atomic layers at the semiconductor junction. This is beyond the scope of the present book. We therefore treat the band discontinuities DEC and DEV as phenomenological quantities, which may be determined experimentally. A few well-established values are listed in Table 12.7 [12.7]. From a knowledge of the valence band discontinuity DEV and the band gap

462

12 Semiconductors

Table 12.7. Compilation of a few experimentally determined valence band discontinuities DEV. The semiconductor named first is the substrate, on which the second semiconductor is deposited, generally as a thin strained layer. (After [12.7]) Heterostructure

Valence band Heterodiscontinuity structure DEV [eV]

Valence band Heterodiscontinuity structure DEV [eV]

Valence band discontinuity DEV [eV]

Si-Ge AlAs-Ge AlAs-GaAs AlSb-GaSb GaAs-Ge GaAs-Si GaAs-InAs GaP-Ge GaP-Si GaSb-Ge GaSb-Si

0.28 0.86 0.34 0.4 0.49 0.05 0.17 0.80 0.80 0.20 0.05

0.33 0.15 0.64 0.57 0.0 0.0 1.75 1.55 1.30 1.20 0.85

1.1 1.40 1.25 1.03 0.95 0.85 0.83 0.74 0.85 0.7

InAs-Ge InAs-Si InP-Ge InP-Si InSb-Ge InSb-Si CdS-Ge CdS-Si CdSe-Ge CdSe-Si CdTe-Ge

CdTe--Sn ZnSe-Ge ZnSe-Si ZnSe-GaAs ZnTe-Ge ZnTe-Si GaSe-Ge GaSe-Si CuBr-GaAs CuBr-Ge

energies of the two semiconductors, the conduction band discontinuity DEC can of course easily be determined. The calculation of the space-charge zones is performed in complete analogy to the calculations for a simple p±n junction (Sect. 12.6), except that the positive and negative space-charges now occur in two dierent semiconductor materials I and II with dierent dielectric constants eI and eII. The corresponding quantities for a p±n heterojunction are depicted in Fig. 12.25. The simplest description is again within the framework of the Schottky model, in which the space charges ±e N IA and e N II D are assumed to be constant over their respective space-charge zones d I and d II. The Poisson equation (12.39, 12.52) can once again be integrated piecewise in semiconductors I and II. It is important to remember that the diusion voltage VD is now partitioned between two dierent semiconductors, i.e. divided into V ID and V II D VD V ID V II D :

12:83

The same is true for an external voltage applied across the p±n heterojunction: U U I U II :

12:84

To match the two solutions of the Poisson equation at the interface
x 0, the continuity of the dielectric displacement must be considered e0 eI E I
x 0 e0 eII E II
x 0 :

12:85

In analogy to (12.57) the thicknesses of the space-charge zones in semiconductors I and II are given by the formulae

12.7

Semiconductor Heterostructures and Superlattices

463

Fig. 12.25. Band scheme of a semiconductor heterojunction; semiconductor I with dielectric function e I is p-doped with an acceptor concentration N IA, semiconductor II with a dielectric function e II is n-doped with a donor concentration N II D. The space-charge zones have thicknesses d I and d II; the diusion voltages associated with the space-charge zones are V ID and V II D. DEV is the valence band discontinuity. Such a heterojunction consisting of a p-type semiconductor with a small band gap and an n-type semiconductor with a large band gap is also called a p±N heterojunction (small p for the small band gap, large N for the large band gap)

1=2 2NDII e0 eI eII
VD U d ; eNAI
eI NAI eII NDII I 1=2 2NA e0 eI eII
VD U II d : eNDII
eI NAI eII NDII I

12:86 a
12:86 b

Appearing here, in addition to the terms in (12.57), is the externally applied voltage U. The ratio of the voltage drops in the two semiconductors is V ID V II D

UI NDII eII : U II NAI eI

12:87

For the case of a simple p±n junction (eI eII ) in thermal equilibrium (U = 0), equation (12.86) reduces of course to (12.57). Of particular interest are heterojunctions between two dierent semiconductors with the same doping, so-called isotypic heterojunctions (e.g. n±N in Fig. 12.24 c). In this case, because of the continuity conditions for the Fermi level, an accumulation space-charge zone for electrons is created on the side of the semiconductor with a smaller forbidden gap, which leads to an extremely large increase in local electron concentration. This is true even when this side of the heterostructure is only very weakly doped, i.e. almost intrinsic (Fig. 12.26 a). The high concentration of free electrons in this spacecharge zone (semiconductor II) is compensated by a depletion space-charge zone in semiconductor I. This has a strong positive space-charge as a result of the high concentration of ionized donors. These donors have given up their valence electrons to the energetically more favorable potential well in the accumulation zone of semiconductor II. In this way the high density of free electrons is spatially separated from the ionized impurities from which

464

12 Semiconductors

Fig. 12.26. (a) Modulation-doped heterojunction consisting of a heavily n-doped semiconductor I with a large band gap and a weakly (or nearly intrinsic) n-doped semiconductor II with a small band gap (N±n heterojunction); (b) band scheme of a modulation-doped composition superlattice; the layers of the semiconductor I are in each case highly ndoped, while the layers of type II are weakly doped or nearly intrinsic

they originate. Impurity scattering, which is an important source of electrical resistance at low temperature, is therefore strongly reduced for this free electron gas. In a homogeneously doped semiconductor, an increase of the carrier concentration requires a simultaneous increase of the doping level, thus leading to increased impurity scattering, which in turn reduces the conductivity. This necessary correlation of higher impurity scattering with increasing carrier concentration does not occur for heterostructures such as that shown in Fig. 12.26. This type of ``one-sided'' doping in a heterostructure is called ``modulation doping''. Electron mobilities of a modulation-doped AlxGa1±xAs/GaAs heterostructure are shown in Fig. 12.27. If the electron mobility were governed by scattering from ionized impurities (ID) and phonons (P) in the same way as in homogeneously doped GaAs, then there would be a characteristic limit resulting from these processes, decreasing at higher and lower temperature. A maximum in the mobility of about 4 103 cm2/Vs would be obtained for a donor concentration of ND of 1017 cm±3 at about 150 K. The experimentally determined mobilities of modulation-doped structures (shaped region) show, however, no reduction in the mobility at low temperature. The variation of the mobility in the shaded region is due to dierences in the perfection of the heterojunction achieved by dierent authors. At temperatures below 10 K, extremely high mobilities of up to 2 106 cm2/Vs are achieved commonly. Best state-of-heart values are around 107 cm2/Vs. The increase in mobility can be further enhanced if an undoped AlxGa1±xAs layer with a thickness of about 100 AÊ is placed between the highly n-doped AlGaAs and the weakly doped GaAs during epitaxy. In this way, scattering processes at impurities in the immediate vicinity of the semiconductor junction are eliminated. For n-doping concentrations in AlGaAs of about 1018 cm±3, typical thicknesses of the electron enrichment layer are in the region 50±100 AÊ. The free electrons are confined here in a narrow triangular potential well in the

12.7

Semiconductor Heterostructures and Superlattices

465

Fig. 12.27. Temperature dependence of the electronic mobility in a quasi 2 D electron gas in modulation-doped AlGaAs/ GaAs structures; the shaded region represents a great many experimental data. For comparison the mobility curves of homogeneously doped GaAs with donor concentrations ND = 4 1013 cm±3 and ND = 1017 cm±3 are also shown (dashed). The limiting values of the mobility are determined by the following mechanisms: scattering from ionized impurities (ID) ( ); phonon scattering (P) (± ±); piezoelectric scattering (PE) (± ±). (After [12.8])

z direction (perpendicular to the heterojunction) (Fig. 12.26 a). They can move freely only in the direction parallel to the heterostructure. The wavefunction of such an electron thus has Bloch-wave character only parallel to the heterostructure; perpendicular to it (along z), one expects quantum effects like those for electrons in a potential well (Sect. 6.1). One speaks of a two-dimensional electron gas (2 DEG). Similar eects to those in the simple modulation-doped heterostructure (Fig. 12.26 a) appear if one epitaxially grows two heterostructures that are mirror images of one another, or even a whole series of layers of semiconductors I and II with dierent band gaps (Fig. 12.26 b). A series of so-called ``quantum wells'' are then formed in the bandstructure, in which the free electrons of the conduction band accumulate. Such a structure is shown in Fig. 12.26 b; it is called a composition superlattice, because the crystal lattice has superimposed on it an artificially created structure of potential wells with larger periodicity. One continues to speak of a modulation-doped superlattice when, as in Fig. 12.26 b, only semiconductor I with the larger band gap is heavily n-doped, while semiconductor II with the smaller gap is lightly doped. The free electrons in the quantum wells of semiconductor II are again separated from the donor impurities in semiconductor I from which they originate. Impurity scattering is strongly reduced and perpendicular to the superlattice direction (z axis), extremely high mobilities are found at low temperatures as is evident in Fig. 12.27. The band bending shown in Fig. 12.26 b, positive in semiconductor I and negative in semiconductor II, corresponds to the sign of the space charge in each region. An unambiguous relationship between these quantities is given

466

12 Semiconductors

by the Poisson equation (12.39). If the quantum wells in Fig. 12.26 b are suciently narrow, i.e. their extension in the z direction is smaller than or on the order of 100 AÊ, then quantization eects become evident in the z direction for the thin space-charge zone (Fig. 12.26 a). This so-called z quantization can be described straightforwardly using the time-independent SchroÈdinger equation for a crystal electron as in Fig. 12.26 a and b. The electron is ``trapped'' in one direction (along the z axis), while it is free perpendicular to this direction. The potential V is then a function only of z, and with three eective mass components mx, my , mz , the following SchroÈdinger equation applies 2 h 1 @2 1 @2 1 @2 2 e V
z w
r E
w
r :
12:88 2 mz @z 2 mx @x2 m y @y With an ansatz of the form w
r uj
zei kx xi ky y uj
zei kk r ;

12:89

equation (12.88) can be separated into two independent differential equations h2 @ 2 e V
z uj
z ej uj
z ;
12:90 2 mz @z2 and

2 @ 2 h 2 mx @x2

2 @ 2 i kx xi ky y h Exy ei kx xi ky y : e 2 2 m y @y

12:91

The solutions of (12.91) are energy eigenvalues that correspond to the unimpeded motion of an electron perpendicular to z Exy

2 2 h h2 2 h2 2 kx ky k : 2 mx 2 my 2 mk k

12:92

For the determination of ej in (12.90), the exact form of the potential V
z must be known. The existence of the space charge means of course that V
z depends on the density of free electrons and ionized donor cores; i.e., the probability density juj
zj2 is included in the potential via the electron density. Equation (12.90) must thus be solved self-consistently. In a simple approximation, however, V
z is described by a rigid square-well potential (as in Sect. 6.1) for the case of quantum wells (Fig. 12.26 b), or by a triangular potential for the case of a simple modulation-doped heterostructure (Fig. 12.26 a). If for the square-well potential one assumes in addition infinitely high potential walls, the electron wavefunctions are simple standing waves in the z direction and, as in Sect. 6.1, the eigenvalues ej are given by ej '

2 p2 j2 h ; 2 mz d2z

j 1; 2; 3 . . . ;

12:93

12.7

Semiconductor Heterostructures and Superlattices

467

where dz is the width of the potential well in the z direction. The total energy eigenvalues for such electron states quantized in the z direction Ej
kk

2 k2k h ej 2 m k

12:94

are described by a family of discrete energy parabolas along kx and ky, socalled subbands (Fig. 12.28 b). These two-dimensional (2 D) subbands have a constant density of states D (E) = dZ/dE, as can easily be demonstrated. In analogy to Sect. 6.1 one notes that in the 2 D reciprocal space of wave numbers kx and ky, the number of states dZ in a ring of thickness dk and radius k is given by dZ

2pk dk
2p2

:

12:95

Since dE = h 2 k dk/mk, one obtains a density of states

Fig. 12.28 a±c. Quantization of a quasi 2 D electron gas in a triangular potential well, as occurs in the strong accumulation zone at a heterojunction
z 0. (a) Behavior of the conduction band edge EC (z); EF is the Fermi level. e1, e2, . . . are the energy levels resulting from the quantization of the one-electron states along z; (b) energy parabolas of the subbands, plotted against the wave vector kx in the plane of free propagation perpendicular to z; (c) density of states of the quasi 2 D electron gas reflecting its quantization into subbands

468

12 Semiconductors

h2 const ; D dZ=dE mk =p

12:96

with spin degeneracy accounted for by the factor 2. The total density of states D (E) of all subbands is therefore a superposition of constant contributions, or a staircase function as in Fig. 12.28 c. Sharp parabolic subbands as in Fig. 12.28 only appear when the eigenvalues ej (12.93) are sharp energy levels. This is the case for a single potential well in the conduction band, or when, in a superlattice, the neighboring potential wells are so far apart that the wavefunctions of the individual potential wells do not overlap. If the distance between the potential wells is so small (less than 50±100 AÊ) that significant overlap between the wavefunctions exists, then this leads to a broadening of the bands. The broadening is completely analogous to that of the individual atomic energy levels of atoms in a crystal (Sect. 7.3). Figure 12.29 shows the theoretically expected broadening for subband energies e1, e2, . . . for the case of a rectangular superlattice, in which the width of the potential wells dz corresponds to the spatial separation of two heterojunctions. One sees that the energetically lowest subband e1 is noticeably broadened for a periodicity of less than 50 AÊ, and splits o as a band. For the higher subbands, the broadening begins at even larger distances between the potential wells. The broadening of the subbands and, in particular, the dependence of the subband energies on the spatial width of the potential wells is clearly seen in photoluminescence experiments. Photoluminescence spectroscopy is

Fig. 12.29. Energy states of electrons confined in the rectangular potential wells (inset) of the conduction bands of a composition superlattice; the potential wells have a width dz which also corresponds to their distance from one another. For the calculation, an electronic eective mass of m * = 0.1 m 0 was assumed. The heavy lines in the shaded regions are the results for single potential wells with the corresponding widths dz; potential wells in a superlattice with suciently small separation lead to overlap of wavefunctions and therefore to a broadening into bands (shaded region). (After [12.9])

12.7

Semiconductor Heterostructures and Superlattices

469

an important optical method for characterizing semiconductor heterostructures and superlattices. It is essentially the reverse of an optical absorption experiment: The semiconductor structure is illuminated with monochromatic laser light of photon energy above the band edge, thus creating electron± hole pairs. These occupy the subbands of the conduction or valence bands of the semiconductor or the corresponding excitonic states (Sect. 11.11). In the case of direct gap semiconductors (Sect. 12.1), the recombination of the free electrons with the holes is associated with strong luminescence, which, for sharply defined subbands, is monochromatic and corresponds, apart from the exciton binding energies (Sect. 11.11), to the energetic separation of the sub-bands for electrons and holes. The experiment has to be performed at low temperatures in order to observe the small energy broadening of the subband structure (e1, e2, . . . ). The low temperature is also the reason why the subband excitons are stable and radiative recombination occurs from the excitonic electron-hole states. Figure 12.30 shows a photoluminescence spectrum taken from an AlGaAs/GaAs multilayer structure at a temperature of 2.7 K. The layer structure consists of four GaAs quantum wells of diering thicknesses (20, 30, 60, 100 AÊ) embedded between barriers of Al0.3Ga0.7As. The four dierent quantum-well widths give rise to four sharp luminescence lines at dierent photon energies in the range 1.55±1.75 eV. Since the sub-bands are characterized by the fact that an integral number of half electron wavelengths must more or less fit into the quantum well, narrower quantum wells yield subbands in the valence and conduction bands that lie further apart and thus have higher energy transitions in the photoluminescence. Of course, an exact theoretical analysis of the relationship between luminescence energy and quantum-well width must take into account the Coulomb attraction between the excited electron-hole pairs. This means that the energy dierence between electron and hole subbands diers from the energy of the emitted photon by the amount of the exciton binding energy. Since local variations in the width of the quantum well lead to a spread in the spectral position of the emitted photoluminescence line, high

Fig. 12.30. Photoluminescence spectrum of an MBE-grown multiple quantum well structure of Al0.3Ga0.7As/GaAs taken at 2.7 K. The various emission lines result from electron±hole recombination processes in quantum wells of dierent thicknesses (20±100 AÊ). The bandstructure
Ec ; Ev of the layer structure is indicated showing the correspondence of the quantum wells to the emission lines. (After [12.7])

470

12 Semiconductors

resolution photoluminescence spectroscopy is particularly well suited to measuring spatial variations in the layer thickness of quantum well layers. Besides the compositional superstructures considered so far, there is a further type of semiconductor superlattice, the so-called doping superlattice. Here the superlattice structure consists of one and the same semiconductor, but the material is periodically and alternately n and p doped. In principle it is equivalent to a periodic sequence of p±n junctions (Sect. 12.6). Because quasi intrinsic (i regions) exist between each n and p zone, these structures also have the name ``nipi structures''. The production of such lattices is also carried out using epitaxy (MOCVD, MBE, etc., Panel XVII). During the growth process, the p and n doping sources are switched on alternately. The interesting properties of nipi superlattices manifest themselves in the position-dependent electronic bandstructure (Fig. 12.31). Because of the periodic sequence of n- and p-doped regions, the conduction and valence bands must alternately approach the Fermi level. This leads to a periodic modulation of the band edges with position. Excited free electrons (thermal and non-equilibrium) are found in the minima of the conduction band, while excited holes are spatially separated and gather in the maxima of the valence band. This spatial separation of electrons and holes is responsible for the fact that the collision rate between these two particles is drastically reduced. One interesting property which results is an extremely long recombination lifetime for electrons and holes. This is clearly manifest when electron-hole pairs are created by irradiation with light. A photocurrent can exist for considerably longer in such a nipi structure than in a homogeneously doped semiconductor. Another interesting property of doping superlattices concerns the band gap. In spite of the considerable spatial separation of electron and hole

Fig. 12.31 a±c. Schematic bands of a doping (nipi) superlattice, in which one and the same semiconductor material (e.g. GaAs) is alternately n- and p-doped. (a) Qualitative sketch of the structure; (b) band scheme in thermal equilibrium; (c) band scheme under strong excitation of electron±hole pairs to above their thermal equilibrium densities

12.7

Semiconductor Heterostructures and Superlattices

471

states, there is nonetheless a certain overlap of the wavefunctions in the transition region (i region). This results in the possibility of optical transitions in absorption and emission. As a consequence of the band modulation one thus observes optical transitions at quantum energies below the band edge of the homogeneously doped semiconductor (Fig. 12.32). Nipi structures have an eective band gap E e q , which can be adjusted in a controlled way by the respective n and p doping levels. In the simplest approximation one assumes, as for a p±n junction (Sect. 12.6), that all impurities are ionized, and applies the Schottky approximation with a rectangular spacecharge distribution. Because of the relationship between band bending and space-charge density [described by the Poisson equation (12.39)], it is immediately clear that a reduction of the space charge results in a decrease of the band bending and therefore a flattening out of the band modulation. The eective band gap becomes larger (Fig. 12.31). The space charge consists of ionized donors (positive) and electrons in the n region, and of ionized acceptors (negative) and holes in the p region. Suciently energetic excitation of electrons and holes, e.g. by irradiation with light, reduces the space charge and also the band modulation. In nipi superlattices, the eective band gap is dependent on the density of optically excited non-equilibrium carriers. Thus the eective band gap can be optically altered. This may be demonstrated in a photoluminescence experiment (Fig. 12.32), in which the emission due to recombination of optically excited electrons and holes is observed as a function of laser excitation power [12.11]. In a GaAs nipi superlattice with a p and n doping of about 1018 cm±3 and a translational period of about 800 AÊ, the band edge luminescence line at low excitation

Fig. 12.32. Photoluminescence spectra of a GaAs nipi superlattice, which was deposited by metal organic molecular beam epitaxy (MOMBE) on a GaAs wafer with (100) orientation, p-doping due to carbon, n-doping due to Si. The spectra were taken with dierent excitation powers and a photon energy of 1.92 eV at 2 K. (After [12.11])

472

12 Semiconductors

power appears slightly above 1.3 eV (Fig. 12.32), whereas the band gap in homogeneously doped GaAs at 2 K is about 1.5 eV. With increasing excitation power the luminescence line shifts to a higher energy, approaching the region of the GaAs band edge, as one would expect for a decrease in the band modulation. Because of their completely new properties which are not present in homogeneous semiconductors, heterostructures and superlattices have opened up a new dimension in the field of microelectronics. Devices based on new concepts are being realized both in the area of very fast circuits and in optoelectronics. This whole domain is a rapidly developing field with great promises for the future [12.12].

12.8 Important Semiconductor Devices Modern information technology is based on integrated semiconductor circuits (IC) that are used for data processing (logic), data storage (memory) and data transfer in networks, e.g. glass fiber networks, where optoelectronic devices such as detectors and optical emitters (light emitting diodes, LEDs, and lasers) are the fundamental elements. While more than 90% of the semiconductor ICs are fabricated on silicon wafers, the major material base for optoelectronic devices are the III±V semiconductors, and particularly GaAs. The reason is that the elemental semiconductor silicon permits the highest density of integration, i.e. the smallest size of devices, while the much stronger coupling of electronic transitions to the electromagnetic field in the case of direct band gap III±V semiconductors is essential for optoelectronic devices. Of all active devices, transistors are the most important ones for data processing in logic and memory circuits as well as for power electronics. Transistors are three-port devices, i.e. essentially switches, in which an input signal at one contact controls the resistance between two other contacts. Simultaneously, transistors possess amplifying properties for current and/or voltage. The essential optoelectronic devices, such as detectors, light emitting diodes and lasers, on the other hand, are two-port devices (diodes) that feature a current flow between two contacts only. Devices can be distinguished further by another criterion: Depending on the transport mechanism, be it by only one type of carriers, electrons or holes, or by both types of carriers, devices are called unipolar or bipolar. According to this criterion two classes of transistors exist, so-called bipolar transistors and the field effect transistors (FETs) which have unipolar character. In this sense laser devices and LEDs where the light emission originates from the recombination of electrons and holes are also bipolar devices.

12.8

Important Semiconductor Devices

473

The Bipolar Transistor The classical bipolar transistor, invented by Bardeen, Brattain and Shockley at the Bell Laboratories (USA) in 1947, consists of two oppositely biased pn-junctions (Fig. 12.33 a). Accordingly there are both, npn- and pnp-transistors; in npn devices the current is essentially carried by electrons, while in the pnp

Emitter

Base

Collector

Fig. 12.33. Basic layout and function of an npn-bipolar transistor. (a) Layout of the transistor together with the external circuitry in the so-called common-base configuration; the space charge regions of the forward-biased emitter (E)-base (B) junction and the reversebiased base (B)-collector (C) junction are shaded. (b) Schematic plot of the currents involved in the function of the transistor. The large shaded arrow depicts the electron current from the emitter to the collector via the base. A small portion of the current is diverted into the base. This current pattern is essential for the performance of the transistor. The directions of the currents (IE, IC, IB, etc.) are drawn according to engineer's convention. (c) Electronic band scheme E(x) along the coordinate x from the emitter to the collector, with an emitter-base voltage UEB and a base-collector voltage UBC applied. ECE, EVE, and ECC, EVC are conduction and valence band edges in the emitter (E) and the collector (C) regions, respectively. EFE and EFC are the quasi-Fermi levels in the emitter and collector regions, respectively. The electron-hole recombination process in the base region (which is detrimental to the performance) is indicated by dashed arrows

474

12 Semiconductors

arrangement holes are the main carrier type. Nevertheless, both carrier types contribute to the device performance, as is expressed by the term ``bipolar'' transistor. In Fig. 12.33 a the scheme of an npn-transistor together with its external circuitry is shown: the first n+p-junction (high n doping, medium p doping) is biased in the forward direction, such that the p-doped base region is flooded by a high concentration of electrons from the n+-emitter region through the narrow, low-resistance n+p space-charge zone. The electrons injected from the emitter into the base region are minority carriers there, and have, therefore, a high tendency to recombine with holes, which represent the majority carriers in the base region. However, in an efficient bipolar transistor the base region is small compared to the recombination length and the major part of the emitted electrons reaches, without recombination the adjacent base-collector junction (biased in the reverse direction). As is seen from the band scheme in Fig. 12.33 c these excess electrons are accelerated by the spatially extended electric space-charge field of the reverse-biased pn junction into the collector region. For a sufficiently narrow base region the collector current IC is smaller than the emitter current IE but by only a tiny amount, namely by the current IBn which is lost due to the recombination with holes (majority carriers in the base) (Fig. 12.33 b). The collector current IC is mainly determined by the forward bias UEB between emitter and base and therefore also by the base current IB. The collector current IC is thus essentially controlled by the base current IB, while the reverse bias at the base-collector junction has only a negligible effect on the current IC. The external current IB into the base consists of three contributions: The portion IBn originates from recombination of holes with electrons being transferred from the emitter region. The hole current (majority carriers in the base) diffuses into the emitter via the valence band barrier. The third contribution is due to holes that are thermally generated within the collector region and are accelerated into the base by the strong space-charge field between base and collector (Fig. 12.33b). For the different current contributions the following relations therefore result: IE IEn IEp ;

12:97 a

IC ICn ICp ;

12:97 b

IB IE

IC IEp IBn

ICp :

12:97 c

Since the base current IB is typically below 1% of the collector current IC the collector current, which flows as an emitter-base current through the base region into the collector, is approximately represented by the relation for a p±n junction (12.74) as IC IE A

eDn nB exp
eUEB =k T Ln

1 :

12:98

Here, A is the current-carrying area of the transistor, Dn the diffusion constant of electrons in the base region, nB their equilibrium concentration

12.8

Important Semiconductor Devices

475

therein, and Ln the electronic diffusion length in the p-doped base. Since the diffusion length Ln is related to the diffusion time sn according to p Ln = Dn sn , the ratio Dn /Ln can be considered as a diffusion velocity of electrons in the base. The collector and emitter current (12.98) can therefore be interpreted as a product of the number of electrons injected into the base and their diffusion velocity. This diffusion velocity thus determines predominantly the speed of the transistor. The exponential increase of the collector current Ic with base-emitter voltage UEB is plotted in Fig. 12.34 b. This plot is usually called the transfer characteristics. The so-called output characteristics IC(UCE) are shown in Fig. 12.34 c. They represent essentially the behavior of the reverse-biased base-collector p±n junction, since the base-emitter resistance is small. The output characteristic is therefore the reverse bias currents of a p±n junction, controlled in magnitude by the emitter-base voltage UEB.

Fig. 12.34. (a) Layout of a planar bipolar transistor. The dierently doped emitter, base, and collector regions are shaded according to the concentration of dopants, with black denoting the highest concentration. The space-charge layers E/B and B/C are drawn as unshaded. The top view on the metallic emitter (E) and base (B) contact in the inset indicates the position of the cross section through the layer structure along AA'. (b) Input characteristic of a bipolar transistor (after Tietze and Schenk [12.13]). (c) Output characteristics of a bipolar transistor with emitter-base voltage UEB as a parameter. An important figure of merit of a transistor is the derivative of the collector current IC with respect to the emitterbase voltage, the transconductance gm = @IC/@UEB. (After Tietze and Schenk [12.13])

476

12 Semiconductors

Depending on the dierent applications, bipolar transistors can be used in connection with three circuitry configurations [12.13]. The common base configuration in which the base is at ground potential was used in the considerations to Fig. 12.33. There, the collector output current IC is always smaller than the input current IE by the (small) amount IBn (IBn IC). Nevertheless, significant voltage and power amplification can be achieved since the input circuit of the transistor contains the low-resistance emitterbase p±n junction biased in the forward direction, while the output current IC (&IE) flows through the high resistance of the base-collector p±n junction biased in the reverse direction. This permits the use of a high load resistance in the output circuitry with large voltage drop. More frequently used is the emitter configuration where the emitter contact of the transistor is at ground potential. In this configuration, the base current IB, small in comparison with IE and IC, controls the output collector current IC. The current amplification of this configuration is obvious. Apart from current amplification the parameters known as transconductance gm @IC =@UEB and emitter eciency c = @IEn/@IE are the principle figures of merit of a bipolar transistor. The emitter eciency indicates what percentage of the total emitter current IE is carried by the majority carriers rather than by holes from the base region. In order to increase the speed of the transistor one has to enhance the conductance of the base region, i.e. the doping level of the base. This, on the other hand, increases the back current of holes IEp into the emitter and thus causes a decrease of the emitter eciency c. A way out of this problem is provided by modern hetero-bipolar transistors (HBTs), where the emitter region is formed by a semiconductor layer of a wide band gap material deposited epitaxially on the base-collector system formed by lower band gap materials (e.g., AlGaAs on GaAs). Given a significant valence band oset (Sect. 12.7) this valence band barrier reduces the back-stream of holes from the base into the emitter, despite a large p-doping of the base. Similar concepts are realized by using low band gap semiconductors as the base material in connection with emitter layers possessing a larger band gap. Field Eect Transistors (FET) A field effect transistor (FET) is essentially a resistor that is controlled by an external bias voltage. Its architecture is rather simple. A FET consists of a current channel with two contacts, the source and the drain, and a third contact, the gate, which is separated from the current channel by an insulating barrier. The gate contact can therefore be biased with respect to the conducting channel. Depending on the polarity and magnitude of the gate voltage more or less charge is induced in the channel, and the channel conductance is thereby modified. Since only one type of carriers is controlled by the external bias the FET is a unipolar device. There are three main types of FETs (Fig. 12.35), which are distinguished according to the nature of their channels and gate barriers. The most important FET, which is the

12.8

Important Semiconductor Devices

477

Fig. 12.35. Schematic layout and electronic band schemes for the three most important types of field eect transistors (FET). The figure displays the cross section perpendicular to the wafer surface below the metallic gate electrode. The symbols S, G, and D denote source, gate, and drain, respectively. (a) MOSFETs (metal-oxide-semiconductor FET) can only be realized on a Si basis with SiO2 as gate oxide. The conducting channel and its length are denoted by ch and L, respectively. For technological reasons the metallic gate electrode is fabricated from highly degenerate doped polycrystalline Si (poly Si). (b) MESFETs (metal semiconductor FET) are preferentially realized on III±V semiconductor basis, e.g., GaAs. (c) HEMTs (high electron mobility transistor) preferentially realized on III±V semiconductor heterostructures, e.g., AlGaAs/GaAs; the conducting channel is formed by a two-dimensional electron gas (2 DEG) that is connected to the source and drain contacts by highly n+-doped regions. The band schemes are plotted for the case of zero gate voltage (UG = 0) (upper panel) and for positive (a) and negative (b,c) gate voltages UG, for MOSFETs and MESFETs and HEMTs, respectively (lower panel); the (quasi-) Fermi level, the conduction band edge, the valence band edge, and the intrinsic energy level are denoted as EF , EC, EV, and Ei, respectively

basis for all highly integrated silicon circuits, be it logic or memory circuits, is the MOSFET (metal oxide semiconductor FET). The schematic cross section in Fig. 12.35 a displays the essential features: Source and drain regions are formed by highly n+-doped wells that are generated by ion implantation in a moderately p-doped wafer. The two n+ wells are therefore separated by

478

12 Semiconductors

a p-type region. For any applied voltage between source and drain either one of the two p±n junctions is biased in the reverse direction allowing only a small current between source and drain. The p-type region between the n+-source and drain is separated from the metallic gate (G) contact by a very thin gate oxide (SiO2). A bias voltage applied to the gate gives rise to a large electric field across the gate oxide layer that in turn causes a band bending in the underlying semiconductor. For a sufficiently positive gate voltage UG the initial p-region (at UG = 0) below the gate is inverted (Ei < EF) to become an n-accumulation layer. The two source and drain n+-wells are thence connected by a conductive n-accumulation channel. The transistor has switched from ``off '' to ``on''. The performance of a MOSFET depends essentially on the perfection of the gate SiO2 layer and its interface to the underlying Si channel. Any residual trap defect states in the oxide or at the Si/SiO2 interface would be detrimental to the performance since the charge influenced by the gate voltage would merely reside in the defects rather than aecting the inversion channel. Since only Si is able to form thin, but nevertheless tight and stoichiometrically almost ideal oxides, with atomically smooth interfaces to the Si substrate MOSFETs can be fabricated only on Si wafers. III±V semiconductors such as GaAs, while being superior to Si with regard to electron mobility and thus device speed, do not form perfect oxide overlayers. Even if a high performance of the insulator were granted, the interface between the GaAs substrate and the insulating epilayer exhibits such a high density of interface traps (partially due to non-stoichiometry) that MOSFET structures based on GaAs are very ineective. The MESFET (metal semiconductor field eect transistor) is therefore the most common FET on III±V compounds (Fig. 12.35 b). A highly resistive, intrinsic (i) or semi-insulating GaAs (achieved by doping with Cr) with the Fermi level EF located near the midgap position serves as the substrate on which a thin, crystalline ndoped GaAs layer is epitaxially deposited or generated by ion implantation. Due to its high free electron concentration arising from ionized donors the lower conduction band edge in this epilayer lies close to the Fermi level EF and a conducting n-channel is formed that is separated from the metallic gate by the Schottky barrier below the metal/GaAs junction (Sect. 12.6). Since in this metal/GaAs junction the Fermi level is pinned near midgap at the interface, the electronic bands are bent upwards with respect to the conducting n-channel. The metallic gate is thus separated from the n-channel by a depletion region of high resistance. In contrast to the p-channel, source and drain contacts are highly conductive due to a local high n+ doping below the metallization layer. Thus, a conductive channel between source and drain exists for UG = 0 in the arrangement of Fig. 12.35 b. This channel can be pinched o by applying a negative voltage UG to the gate because the negative bias lifts the Fermi level EF of the metallic gate with respect to EF in the i-GaAs. Since on the other hand EF is pinned near midgap (fB = const) at the interface between the gate electrode and the p-channel the entire band

12.8

Important Semiconductor Devices

479

scheme is lifted by the applied bias voltage UG, and the channel becomes depleted of electrons and thus highly resistive. Hence, the transistor switches from ``on'' to ``o '' when subjected to a suciently high negative gate voltage UG. The performance depends sensitively on the thickness of the ndoped layer as compared with the extension of the Schottky depletion space-charge layer (typically 50 nm) under the gate metal contact. Complementary to the ``normally on''-MESFET described above, the ``normally o '' MESFET is designed to possess a thin n-GaAs channel with a thickness comparable to the extension of the Schottky depletion layer. A suciently high positive gate bias bends the electronic bands below the metal gate downwards and opens the channel; the transistor switches to the ``on'' state only under this positive gate bias. Since semiconductor heterostructures of high quality can be produced by modern epitaxy techniques such as MBE and MOCVD (panel XVII) the MESFET concept has been extended to a heterostructure FET, the so-called HEMT (high electron mobility transistor), which is extremely fast (20± 300 GHz) and exhibits very low noise (Fig. 12.35 c). Its major fields of application are therefore radar and satellite communication. As a ``heterostructure MESFET'' the HEMT is switched by a Schottky barrier, separating the metal gate contact electrically from the conducting channel. The conduction channel, however, is a modulation-doped 2DEG at the interface of an AlGaAs/GaAs heterostructure in this case (Sect. 12.7). The high electron concentration of typically 2 1012 cm±2 in the 2DEG originates from donors in the n+-AlGaAs barrier that are spatially separated from the 2DEG. The conducting 2DEG channel is thus free of ionized scattering centers which results in low noise and high carrier mobility. A possible modification that exists for all three types of FETs is to invert the type of doping (from p to n). These ``inverted'' FETs exhibit the same transistor functions, albeit with inverted external bias (plus to minus). Holes rather than electrons then carry the transistor function. Holes have higher eective masses than electrons, their mobility is lower and therefore p-channel FETs are slower than their n-channel analogues. Nevertheless, nearly all advanced silicon ICs consist of combinations of p- and n-channel MOSFETs (CMOS = complementary MOS). The combination of both transistor types allows the realization of logic gates that carry current only within the switching period between two bit-operations. CMOS circuits, therefore, consume less power, which is of significant advantage in the ever-increasing integration density. FETs show amplification since very small gate currents induce sucient charge on the gate such that much larger source-drain currents are controlled. Since the resistance of the SiO2 layer in the case of the MOSFET is much higher than the resistance of the Schottky depletion space-charge layer under the gate of a MESFET or a HEMT, gate currents in MOSFETs are lower than in MESFETs and HEMTs. Characteristic figures of merit for a FET are its transconductance g (the ratio between drain current and the applied change

480

12 Semiconductors

in the gate voltage) and the gate capacity Cg. The ratio between transconductance and gate capacity determines the cut-o frequency fmax = g/Cg, up beyond which the power amplification drops below 1. In order to improve the high-frequency performance of a FET, its gate capacity should be decreased and the highest possible transconductance should be achieved. Fast, high-performance HEMTs in the material system GaInAs/InP reach transconductances g of about 600 mS/mm and upper cut-o frequencies fmax&300 GHz at channel lengths of 0.1 lm [12.14]. Typical source-drain current characteristics (ISD vs. USD) of FETs, in particular of MOSFETs, are shown in Fig. 12.36, with the gate voltage UG as a parameter. For small USD, where the inversion space-charge zone along the channel is essentially not aected by a change in USD, the current ISD is nearly proportional to the applied voltage USD (quasi-ohmic behavior). Increasing source-drain voltage USD causes a significant potential drop along the channel within the semiconductor, while the potential on the metallic gate contact remains constant. The voltage drop between the metallic gate contact and the channel (perpendicular to the direction of the channel) thus increases along the channel. This causes a decrease of the channel width (12.80) along the channel, which results in a saturation of ISD for voltages USD > 2 V. The dependence of the saturation current ISD on the gate voltage UG diers for short- and long-channel transistors. In short channels (Fig. 12.36 a), high electric fields of the order of 104 to 105 V/cm are reached

Fig. 12.36. Source-drain current (ISD) vs. voltage (USD) characteristics of Si MOS-field effect transistors (MOSFETs): ISD(USD) curves are plotted with the gate voltage UG as a parameter. (a) Short-channel MOSFET with gate length Lg = 0.6 lm and gate width 5 lm. (b) Long-channel MOSFET with gate length Lg = 10 lm and gate width 5 lm (after MuÈhlho and McCaughn [12.15])

12.8

Important Semiconductor Devices

481

and the carriers are accelerated up to their saturation velocity v s (Fig. 12.15). Consequently, the current ISD grows proportionally with the charge induced on the gate and is thus proportional to UG (Fig. 12.36a). In the case of long channels, one has to consider the fact that the potential difference between gate and channel varies along the channel. In the saturation limit (high source/drain voltage) the gate may be positively biased with respect to the channel near the source, however, still negatively biased with respect to the channel near the drain. As a consequence, the channel is quenched to a high resistance near the drain. A more positive bias on the gate therefore changes not only the carrier concentration locally but also reduces the length where the channel is eectively quenched. In that case a nearly quadratic dependence of the source-drain current ISD on the gate voltage results (Fig. 12.36 b). Similar current-voltage characteristics ISD (USD) as discussed here for MOSFETs are also found for MESFETs and HEMTs.

Semiconductor Lasers The performance of optoelectronic devices such as photodetectors, solar cells, light emitting diodes (LED) and lasers is based on the interaction of the electromagnetic light field with electronic excitations in the semiconductor. Three different interaction processes exist: (i) an absorption of light quanta by an excitation of electrons from the valence band into the conduction band, or between electronic defect levels within the forbidden band, (ii) an inverse process, the stimulated emission, in which the incident photon stimulates an electron to be de-excited from a state of higher energy into a state of lower energy, and (iii) the spontaneous emission of light. Both, absorption and stimulated emission depend linearly on the strength of the electric field E
x of the electromagnetic wave (Sect. 11.10). The stimulated emission is coherently coupled with the light field so that the emitted photon is in phase with the stimulating electromagnetic wave. In contrast, spontaneous emission is not coherently coupled to the light field. All three types of interactions are used in photoelectric devices: For photodetectors and solar cells the absorption process is essential. Light emitting diodes (LED) utilize spontaneous emission, while lasers are based on stimulated coherent emission. In all three processes energy conservation is obeyed hx E2

E1 ;

12:99

with hx the photon energy and E2 and E1 the energies of the excited and ground state, respectively. Under stationary illumination with light the transition rates must compensate each other. With A21 as the probability for spontaneous emission and B21 and B12 the probabilities for stimulated emission and absorption, respectively, the stationary state is described by n_ 2

B21 n2 jE
xj2

A21 n2 B12 n1 jE
xj2

n_ 1 0 ;

12:100

482

12 Semiconductors

where n1 and n2 are the occupation numbers of the ground state and the excited state, respectively. Apart from a pre-factor the coefficients B21 and B12 are equal to the square modulus of the transition matrix element |xij|2 for stimulated emission and absorption (11.93) and are therefore equal to each other (11.93). The ratio of the stimulated and spontaneous emission rates is n_ 2stim =n_ 2spon

B21 jE
xj2 : A21

12:101

Since laser action requires an excess of stimulated emission processes, a laser is built as a standing-wave resonator for the wavelength to be emitted. Thereby, a high electric field within the lasing medium is generated. Furthermore, the rate of stimulated emission must exceed that of absorption in a laser. Neglecting spontaneous emission because of (12.101) at high light fields E
x and using the equality B21=B12 one obtains from (12.100) the following laser condition: n_ 2

n2

n1 B21 jE
xj2 < 0 i:e: n2 > n1 :

12:102

This condition describes the inversion of the occupation (population) statistics (see Problem 11.8). In thermal equilibrium, just the opposite would hold: the occupation of the excited states is less than the occupation of the ground state. Population inversion is achieved by ``pumping'' into the excited state. In a semiconductor laser a convenient method for pumping is to bias a p±n junction in the forward direction and to flood the space-charge region with non-equilibrium electrons and holes. In writing (12.100±12.102) it was assumed that the final states of the electronic transitions were unoccupied, i.e. their probability to be empty was ``one''. While this assumption is correct for an ensemble of single atoms in a gas laser, where the occupation of an excited state results from depopulation of the ground state the laser condition has to be modified for the valence band (EV) and the conduction band states (EC) of a semiconductor laser. Here, the transition rates are proportional to the density of occupied initial and the density of empty final states. The condition for population inversion in a p±n junction biased in the forward direction thus follows as B21 DC
EC DV
EV f
EC 1 B12 DV
EV DC
EC f
EV 1

f
EV f
EC < 0 :

12:103

In (12.103) the occupied and empty energetic regions of the conduction and valence band, respectively, are represented by sharp energy levels EC and EV, the integrals over the corresponding energetic ranges (*kT) are approximated by constant densities of states DC (EC) and DV (EV), respectively. f (E) is the Fermi distribution function, which can not be approximated by the Boltzmann distribution at high doping levels. Because B21 = B12 (12.103) gives: f
EC 1

f
EV > f
EV 1

f
EC > f
EV :

f
EC

12:104 a
12:104 b

12.8

Important Semiconductor Devices

483

The occupation probabilities can be approximated by Fermi functions with E nF, E pF as quasi-Fermi levels in the n- and p-region, respectively (Fig. 12.37) f
EC 1 exp
EC

EFn =kT

1

;

12:105 a

f
EV 1 exp
EV

EFp =kT

1

:

12:105 b

Hence, the condition for population inversion becomes E nF

E pF > EC

EV Eg :

12:106

For laser operation, the quasi-Fermi levels in the n- and p-doped region must energetically be separated from each other by more than the band gap energy Eg. The p- and n-type regions, therefore, have to be doped deep into degeneracy, in order to reach population inversion by an externally applied forward bias U = (E nF±E pF)/e (Fig. 12.37 a, b). The current through the p±n junction thus defines the onset of laser action. The emitted light power plotted versus current density through the p±n junction increases slowly due to spontaneous emission, until population inversion is reached at a certain threshold current density and laser action starts. At this point stimulated emission becomes the determining mechanism (Fig. 12.38). Threshold

EC

EC

EC

Fig. 12.37. Electronic band schemes E(x) of pn-semiconductor laser structures along a direction x perpendicular to the layer structure: (a) Degenerately doped p++n± ± junction without external bias (thermal equilibrium); (b) same p++n± ± junction with maximum bias U in forward direction; (c) double-heterostructure pin junction of pAlGaAs/i-GaAs/n-AlGaAs with maximum bias U in forward direction. EnF , EpF are the quasi-Fermi levels in the n- and p-region, respectively; EC and EV are conduction and valence band edges

484

12 Semiconductors

Emitted power P7 (mW)

current density is thus the major figure of merit of a semiconductor laser; the lower it is, the more effectively the laser performs. Too high threshold current densities cause too much energy dissipation (Joule heating) which, aside from making the laser less efficient, reduces the lifetime of a laser considerably. An important breakthrough leading to the commercialization of semiconductor lasers was the invention of the double heterostructure laser. Figure 12.37 c shows the electronic band scheme of such a laser, in this case an AlGaAs/GaAs/AlGaAs heterostructure. A lowly doped or intrinsic (i)GaAs layer is inserted into a p±n junction between two p- and n-doped wide band gap AlGaAs regions. In spite of the low p- and n-type doping in the AlGaAs regions on both sides the quasi-Fermi levels in the active (i)-GaAs region are located within the conduction and valence band of the GaAs layer under strong forward bias. Population inversion is thus easily achieved without employing highly doped, degenerate semiconductors and the high current densities that accompany the use of degenerate semiconductors. The active iGaAs region is flooded with non-equilibrium electrons and holes, which are confined to the active region by the conduction and valence band discontinuities, respectively. This eect, which causes enhanced light emission is called ``electrical confinement''. Additionally, this structure provides an ``optical confinement'', since for the wavelength of the emitted light (which corresponds to the GaAs band gap) the refractive index of the active GaAs region exceeds that of the adjacent AlGaAs layers (see Problem 11.9). The light originating

Metal Metal

active region

Current I (mA)

Fig. 12.38. Emission characteristics at room temperature T = 300 K of an AlGaAs/ GaAs/AlGaAs double-heterostructure laser: the emitted light power is plotted as a function of the current I through the laser; Ith is the threshold current where laser action begins. Inset: Schematic layer structure of the laser with emitted radiation (hm). (After Kressel and Ackley [12.16])

12.8

Important Semiconductor Devices

485

from stimulated emission in the GaAs is therefore totally reflected at the AlGaAs layers; it remains in the active GaAs channel, and is focused and concentrated. The schematic representation of a double heterostructure laser device (inset in Fig. 12.38) shows that the active GaAs channel (resonator) is spatially confined by the two AlGaAs layers on the top and bottom of the GaAs layer, and laterally by a metal stripe deposited into an opening in the SiO2 mask. The metal contacts the semiconductor layer structure only within this stripe whereby the electric field and the current flow is laterally limited to the width of the stripe. The optical resonator, i.e. the active GaAs channel (Fabry±PeÂrot interferometer) requires eective semi-transparent mirrors at its front and back side, through which the light is emitted or reflected. In the simplest case these mirrors are realized by cleavage planes of the GaAs wafer along (110). Typical lengths of these active channels range between 100 and 1000 lm. The emitted light power as a function of the external current (Fig. 12.38) slowly increases at lower currents due to spontaneous emission. In this current regime the amplification is too low to overcome losses in the resonator. At a certain threshold current Ith the amplification of the device matches the resonator losses and laser action starts, and the output light power increases abruptly. An important figure of merit of a semiconductor laser is thus a threshold current as low as possible (or threshold current density) arising from low losses in the resonator. With increasing temperature the electrical confinement of the laser deteriorates, since carriers populate higher energy states because of a less sharp Fermi edge. The threshold current increases and the laser performs less eciently. Since Boltzmann statistics are approximately valid, the threshold current Ith depends exponentially on the working temperature T: Ith / exp
T=T0 :

12:107

A further figure of merit of a semiconductor laser is the critical temperature T0, which should be as high as possible, so that the laser shows a slow increase of the threshold current with working temperature T. Typical values of T0 are close to 100 oC for double-heterostructure lasers. In the double-heterostructure lasers (DHL) considered so far, the vertical extension of the active channel, i.e. the thickness of the embedded GaAs layer is much higher than 200 AÊ. Carriers in the active zone occupy quantum states of a macroscopic 3D crystal. Further improvement of the laser performance is achieved by incorporating into the active zone even thinner layers (thickness 100 AÊ) of a semiconductor with a lower band gap than that of GaAs, e.g., InGaAs. Since InxGa1±xAs is not latticematched to GaAs these interlayers are highly strained. They can only be grown without dislocations up to a particular critical thickness. Due to their smaller band gap, i.e. their band osets with respect to GaAs both in the conduction and valence bands, these thin InGaAs interlayers act as

486

12 Semiconductors

quantum wells for electrons as well as for holes. The electronic states in the conduction and in the valence band are quantized perpendicular to the layer sequence. The density of states within these layers for each subband is constant and the superposition for all sub-bands is step-like (Fig. 12.28 c). Carriers that occupy the lowest possible energy states are thus even more spatially confined and on even sharper energy levels than in the double heterostructure laser. These so-called quantum-well lasers exhibit even better confinement and therefore lower threshold currents and larger critical temperatures T0.

Problems 12.1 Silicon crystallizes in the diamond structure with a lattice constant a = 5.43 AÊ. a) How many atoms does the cubic elementary cell contain? b) Phosphorus atoms incorporated on Si sites act as donors. Calculate the ionization energy of such a donor impurity within the framework of the simple hydrogenic model (dielectric constant eSi = 12). c) Calculate the radius r0 of the first Bohr orbital. What is the probability of finding the electron in its ground state within a sphere of radius 2 r0? How many Si atoms are located within such a sphere? d) Discuss the validity of the hydrogenic model and explain its shortcomings. e) At what impurity concentration does interaction between the donor centers become important? The related impurity band conductivity is assumed to correspond to an average donor separation of 4 r0. 12.2 The eective mass of electrons at the lower conduction band edge of a semiconductor is three times higher than that of holes at the upper valence band edge. How far is the Fermi energy EF located from the middle of the forbidden band in the case of intrinsic conduction. The band gap energy Eg must exceed 8 k T ; why is this a prerequisite for the calculation? 12.3 A semiconductor with a band gap energy Eg of 1 eV and equal hole and electron eective masses me mh m0 (m0 is free electron mass) is pdoped with an acceptor concentration of p = 1018 cm±3. The acceptor energy level is located 0.2 eV above the valence band edge of the material. a) Show that intrinsic conduction in this material is negligible at 300 K. b) Calculate the conductivity r of the material at room temperature (300 K), given a hole mobility of lp = 100 cm2/Vs at 300 K. c) Plot the logarithm of the hole concentration, ln p, versus reciprocal temperature 1/T for the temperature range 100 to 1000 K. 12.4 Consider the electronic bandstructure of a typical direct-gap III±V semiconductor like GaAs with a high-mobility, sharp conduction band

Problems

487

minimum at C and a broad side minimum at somewhat higher energy (cf. Fig. 12.4). a) Discuss qualitatively the dependence of the average drift velocity of free electrons on the strength of an externally applied electric field taking into account scattering into the side valley of the conduction band. b) Give a similar discussion of an indirect-gap semiconductor such as Si, where only the broad side minimum of the conduction band is occupied (Fig. 7.13). 12.5 Calculate the Hall coecient RH for an intrinsic semiconductor in which electric current is carried by both electrons and holes. a) Discuss the temperature dependence of the Hall coecient RH (T) of the intrinsic semiconductor, when hole and electron mobilities lp and ln are assumed to be equal. b) In an experimental measurement of the Hall voltage, reversing the sense of the magnetic field yields a dierent magnitude for this quantity. Explain the origin of this eect. 12.6 Consider the process of photoconductivity in semiconductors. Concentrations of electrons and holes above those of thermal equilibrium are produced from defect sites or from the valence band by means of photoionization. Write down the rate equations for the direct recombination of electron± hole pairs for the cases of (a) intrinsic conduction and (b) n- or p-doping. Calculate the stationary photocurrent at constant illumination and the time dependence of the photocurrent after the illumination is switched o. 12.7 Explain the operation of a solar cell in which a p±n junction is illuminated. Assume a closed circuit containing an external resistance R. Make qualitative sketches of the current±voltage relationships with and without incident light. What is the minimum frequency which the light must have? What is the theoretical eciency as a function of the frequency of the light? How can the current±voltage characteristic be used to obtain the photoelectrically generated power? Discuss the various parameters that influence the eciency. Why is it advantageous to combine several p±n junctions of semiconductors with dierent band gaps using thin-film technology? 12.8 Small-gap semiconductors such as InAs (Eg = 0.35 eV), and InSb (Eg = 0.18 eV) usually exhibit surface Fermi level pinning within the conduction band (approximately 100 meV above the lower conduction band edge EC for InSb). Plot qualitatively the band scheme (band energy versus spatial coordinate) in the vicinity of a metal contact to such a semiconductor that is highly n-doped. What is the electrical resistance behavior for both bias directions?

488

12 Semiconductors

12.9 Calculate the transconductance gm =
@ISD/@UG as a function of gate capacity Cg and gate length Lg for a field eect transistor (MOSFET, MESFET or HEMT, Sect. 12.8). Note that even without an external gate bias (UG = 0) a ``built-in'' band bending under the gate with a threshold voltage U0 is present. For short-channel transistors one can assume in a simple approximation that the carrier velocity in the channel is constant and equal to the saturation velocity v s for high field strength (Fig. 12.15). The sourcedrain current ISD consists of the 2-dimensional (2D) carrier density n2D which is induced in the channel by the action of the gate bias UG. a) Using Fig. 12.15, estimate the transit time for carriers under the gate for a short channel AlGaAs/GaAs HEMT with gate length Lg = 100 nm. b) What gate capacity can be reached in these transistors for a transconductance gm = 150 mS?

Panel XIV

Panel XIV The Hall Eect

To separately determine the carrier concentration n and the mobility appearing in the conductivity = n e , one measures both the conductivity and the Hall eect. A current I is passed through a crystal sample and a magnetic field (magnetic induction B) is applied normal to the current. Using two contacts placed opposite to one another (perpendicular to I and B), a so-called Hall voltage UH can be measured (open circuit measurement, IH = 0). This is shown schematically in Fig. XIV.1. Since measured in the absence of current, the Hall voltage UH which builds up in the sample in the y direction is exactly compensated by the Lorentz force on an electron, which also acts in the y direction. The Lorentz force on an electron moving in the x direction with velocity v x is: Fy

e
v By

ev x B

eE y

eE y 0 :

XIV:1

Here E y = UH/b is the so-called Hall field. Assuming that the current is carried exclusively by electrons (n-type semiconductor or metal), we have jx I=
b d

n ev x

XIV:2

Fig. XIV.1. Schematic set-up for a Hall effect measurement. B: magnetic induction; i: current through the sample; UH: Hall voltage. The dashed lines are the paths which electrons and holes would follow in the absence of a compensating circuit for UH and with a current flow (I=0). For IH = 0, the carriers are forced to move in straight lines (parallel to x) due to the build-up of the Hall voltage UH

Panel XIV

490

Panel XIV The Hall Eect

and it thus follows that

E y

UH b

1 jx B ne

1 IB : n e bd

XIV:3

The quantity RH = ±(ne)±1 is called the Hall constant. It can be determined from measurements of UH, i and B via the relation UH RH I B=d :

XIV:4

The sign of RH gives the type of carrier (a negative sign corresponding to electrons) and its absolute value gives the carrier concentration n. If the current in a semiconductor is carried by both electrons (concentration: n, mobility: n) and holes (p, p), then an analogous calculation gives the following expression for the Hall constant (Problem 12.5) RH

pm2p

nm2n

e
pmp nmn 2

:

XIV:5

Fig. XIV.2 a, b. Temperature dependence of the Hall constant RH for p-type (a) and n-type silicon (b). For p-type with a boron concentration of 2 1017 cm±3 intrinsic conductivity sets in at temperatures in the vicinity of 1300 K. The curve in part (a) would then go through zero and finally convert to the intrinsic branch of (b) [XIV.1]

491

Figure XIV.2 shows experimentally determined values of the Hall constant RH for boron-doped p-silicon (a), and arsenic-doped n-silicon (b). Because the Hall constant gives the reciprocal carrier concentration in units of the elementary charge e, the shape of the curve in a logarithmic plot is similar (at least in the temperature region 33±500 K) to a typical curve of the carrier density for semiconductors (see e.g. Fig. 12.10). The gradients in the region 33±50 K are governed by the ionization energies of the acceptors and donors (12.27). The steeply rising section of the curve in Fig. XIV.2 b at about 103 K reflects the intrinsic conductivity due to electron-hole pair creation. The dierent signs of RH in Fig. XIV.2 a, b correspond to the dierent kinds of carriers in the p- and n-doped material.

Reference XIV.1 F. J. Morin, J. P. Maita: Phys. Rev. 96, 29 (1954)

Panel XIV

Panel XIV The Hall Effect

Panel XV

Panel XV Cyclotron Resonance in Semiconductors

The eective masses of electrons
m n and holes
mp in semiconductors can be determined by cyclotron resonance. A crystal sample is placed in a variable, static magnetic field B and the absorption of a high-frequency alternating field is measured as a function of B. Electrons in the static magnetic field move in k-space on surfaces of constant energy in a plane perpendicular to B and around the magnetic field axis (Panel VIII). In real space there is also a closed orbit. For crystal electrons, however, this orbit, like the k-space orbit, is not simply a circle (Fig. XV.1). Absorption of the high frequency alternating field occurs when the orbital frequency is exactly equal to the period xc (xc = ±e B/mn ). Orbits in k-space which enclose an extremal area (maximum or minimum) are especially important since the number of states per frequency interval is particularly high at these points. The high-frequency absorption then has a clear maximum, and for the interpretation of the data one only needs to consider ``extremal orbits''. As examples of cyclotron resonance in semiconductors we consider Si and Ge. In a semiconductor, electrons and holes are found in the vicinity of the conduction band minimum and valence band maximum, respectively. As shown in Sect. 12.1, the surfaces of constant energy around the conduction band minimum have the form of ellipsoids with rotational symmetry around either the [100] or [111] directions. For an arbitrary orientation of the magnetic field, there is a dierent extremal orbit for each ellipsoid pair along a particular [100] or [111] axis. For silicon there are three dierent values corre-

Fig. XV.1. Classical description of cyclotron resonance for electrons with an effective mass mn : On a stable orbit around the magnetic field axis, the centrifugal force and the Lorentz force are in equilibrium. In general, the high frequency field E HF is maintained at a constant frequency and the magnetic field B is varied

493

sponding to the three dierent [100] axes, and for germanium there are four, one for each of the dierent [111] directions in space (Fig. XV.2 a). If the magnetic field is orientated in a symmetry plane, these numbers are reduced. In Fig. XV.2 b the cyclotron resonance spectra of Dresselhaus et al. [XV.1] are shown. The magnetic field was in the (110) plane. Under these condi-

Fig. XV.2. (a) Surfaces of constant energy near the minimum of the conduction band for Si (left) and Ge (right). Electrons move on these surfaces along closed paths perpendicular to the magnetic field. The frequencies of the various orbits for a particular magnetic field are generally different. When the energy surfaces take the special form of ellipsoids, the frequencies are the same for all electrons on one ellipsoid. This, however, is unimportant for the observability of cyclotron resonance, since in each case it is the extremal orbit (here the orbit with the largest cross-sectional area) that leads to a clear maximum in the rf absorption. For an arbitrary orientation of the magnetic field there are three different extremal orbits for Si and four for Ge. (b) Cyclotron resonance absorption for Si (left) and Ge (right) with the magnetic field oriented in the (110) plane and angles of 308 and 608 respectively to the [100] direction (magnetic flux density measured in Gauss: 1 G = 10±4 T = 10±4 Vs/m2). In both cases, two of the extremal paths are equal for symmetry reasons, such that only two (three) remain distinct. The two valence bands at C with their different curvatures show up in the form of the peaks labeled ``light'' and ``heavy'' holes. For the observation of cyclotron resonance low temperatures are necessary. The electron-hole pairs were created by irradiation with light. (After [XV.1])

Panel XV

Panel XV Cyclotron Resonance in Semiconductors

Panel XV

494

Panel XV Cyclotron Resonance in Semiconductors

tions, two of the ellipsoid pairs have the same orientation with respect to the magnetic field and the number of absorption maxima for electrons is reduced from three (four) to two (three) for Si (Ge). Cyclotron resonance is also observed for holes. The direction of their orbit, however, is opposite to that of electrons. It is thus possible to distinguish between electrons and holes by using a circularly polarized high-frequency field incident along the axis of the B field. Electrons and holes then absorb, according to the direction of their orbit, only right or left circularly polarized radiation. In the absorption spectra (Fig. XV.2 b), it can be seen that two maxima are assigned to holes. The interpretation here is dierent from the case of electrons. Hole states are found at the valence band maximum at the G point of the Brillouin zone. In a (simple) treatment, one would expect only spherical energy surfaces on the grounds of the symmetry of the Brillouin zone, that is to say only one cyclotron frequency. As discussed in Sect. 12.1, however (see also Figs. 12.3, 12.4), the band structure at the valence band maximum is rather more complicated: there are both ``light'' and ``heavy'' holes. Cyclotron resonance can only be observed if the carriers are able to complete a large number of closed orbits around the magnetic field prior to suering collisions with phonons or impurities. This is possible when the relaxation time (of the order of the mean time between collisions) is large compared to the inverse cyclotron frequency x ±1 c . Cyclotron resonance is therefore only observed in pure and highly perfect crytals at low (liquid-He) temperature.

Reference XV.1 G. Dresselhaus, A. F. Kip, C. Kittel: Phys. Rev. 98, 368 (1955)

Panel XVI

Panel XVI Shubnikov-de Haas Oscillations and Quantum Hall Eect

Precise semiconductor heterostructures and superlattices can be prepared by using atomically controlled epitaxy (Sect. 12.7). Such structures allow the confinement of free conduction electrons in quasi-two-dimensional (2D) quantum-well structures with typical vertical dimensions between 20 and 100 AÊ. Thereby, quasi-2D electron gases (2DEG) are generated that exhibit highly interesting physical eects, in particular in externally applied strong magnetic fields. An electron gas in a 2D quantum well is confined in one direction z, perpendicular to the hetero-interface or to the layer sequence in a superlattice. Electrons are free to move about only in the x,y-plane perpendicular to the z-direction. Accordingly, the energy eigen-values of an electron within the 2DEG are given as (Sect. 12.7): Ej
kk

2 2 h h2 2 kx k y "j ; 2mx 2m y

j 1; 2; . . .

XVI:1

where mx and m y are the eective mass components for a free motion in the x,y-plane. The discrete eigen-values that result from the quantization in the zdirection are denoted by "j (12.90). For a rectangular quantum well of thickness dz (Sect. 6.1) with infinitely high barriers, e.g., "j correspond to standing electron waves in a potential box (12.93). "j '

2 p2 j2 h ; 2mz dz2

j 1; 2; 3; . . . :

XVI:2

Equation (XVI.2) thus describes a set of discrete energy parabolas along kx and ky , the so-called subbands (Sect. 12.7). Application of a strong magnetic field B perpendicular to the x,y-plane of free-electron movement further decreases the dimensionality of the electron gas. The electrons are forced into cyclotron orbits perpendicular to the B-field (Panel XV). The cyclotron frequency (frequency of circulation) oc

eB mk

XVI:3

is determined by the balance between the Lorentz force and the centrifugal force. mk is the eective mass of the electrons parallel to the orbital movement (for isotropy in the x,y-plane: mx =m y = mk ). Since an orbital movement can

Panel XVI

496

Panel XVI Shubnikov-de Haas Oscillations and Quantum Hall Eect

be decomposed into two linear harmonic oscillations perpendicular to each other, the quantum-mechanical energy eigenvalues of the orbits are those of a harmonic oscillator with eigenfrequency xc. The magnetic field B therefore causes a further quantization of the subbands with single particle energies: Ej;n;s "j
n 12 hoc sgB B :

XVI:4

The last term accounts for the two spin orientations in the magnetic field in which s = 1 is the spin quantum number, B the Bohr magneton and g the LandeÂ factor of the electron. The magnetic-field-induced quantization (XVI.4) has already been derived for the free electron gas of a metal by a somewhat dierent method in Panel VIII. In both cases the B-field-induced quantization into so-called Landau levels (energetic separation hxc ) leads to a splitting of the continuous energy parabolas (subbands) into discrete energy eigenvalues (Fig. XVI.1 b). Because of the 2D-dimensionality of the bands the density of states at vanishing magnetic field (B = 0) is a step function (Fig. 12.28 c) for each particular subband. In a finite field B=0 this continuous function splits into a series of -like peaks that are separated

Fig. XVI.1 a±c. Qualitative illustration of the quantization of a 2D electron gas in an external magnetic field B (perpendicular to the (x, y) plane of free-electron propagation). (a) Energy parabola of the first subband (12.92) of a free 2D electron gas along kx. A further quantization in the form of Landau states (points) appears upon application of an external magnetic field; (b) density of states D in the first subband of the 2D electron gas, without a magnetic field (dashed line) and with an external magnetic field (solid lines), xc = ±eB/mk is the cyclotron frequency of the electron orbits perpendicular to the magnetic field B; (c) representation of the Landau splitting n 12 hoc in the (kx, ky) plane of the reciprocal space

497

from each other by the energy hoc . The quantum states ``condensate'' into sharp Landau levels. Since the number of states is conserved in the condensation, a -like Landau level must contain exactly the number of states that were originally, at B = 0, distributed over the energy range between two neighboring Landau levels, i.e. the degeneracy of a Landau level amounts to NL ho c D 0 ;

XVI:5

where D0 is the state density of the subband at B = 0. As opposed to (12.96) the spin degeneracy is lifted in the magnetic field and consequently the density of states is a factor of 2 smaller than in (12.96):
XVI:6 D m=2p h2 : 0

k

Thus the degeneracy of a Landau level is NL eB=h 2:42 1010 cm 2 T

1

B:

XVI:7

A Landau level with an energy below the Fermi level is occupied with NL electrons at suciently low temperature. A variation of the external magnetic field changes the energetic separation between the Landau levels, as well as their degree of degeneracy (XVI.5). With increasing magnetic field strength, the Landau levels shift to higher energies and finally cross the Fermi energy EF; the Landau levels are emptied and the corresponding electrons occupy the next lower Landau level. This becomes possible because of the increased degree of degeneracy (XVI.7). In the case of a sharp Fermi edge at a suciently low temperature, the electron system reaches its lowest free energy each time when a Landau level has just crossed the Fermi level. With increasing B-field the free energy increases again, until the next Landau level is emptied. As a consequence, the free energy oscillates as a function of the external magnetic field, and so do the material constants, such as the conductivity (Shubnikov-de Haas eect) and the magnetic susceptibility (de Haas-van Alphen eect). The de Haas-van Alphen eect has been of considerable importance in studies of the topology of Fermi surfaces in metals (Panel VIII). The quantization of states in a magnetic field also gives rise to the quantum Hall eect in semiconductors with 2D-electron gases (2DEG). Since its discovery by Klaus von Klitzing (Nobel prize 1985) the quantum Hall eect [XVI.1] has become an important tool to characterize heterostructures in semiconductor physics. Moreover, the quantum Hall eect had an important impact on the development of the physics of nanostructures in general. The experimental arrangement for the observation of the quantum Hall eect is similar to that of the classical Hall eect (Panel XIV): a Hall voltage UH is measured perpendicular to the current through the sample at two opposite contacts. Unlike in the classical Hall-eect, however, the current is carried by a 2DEG in a semiconductor heterostructure, e.g., in a modulation-doped AlGaAs/GaAs heterostructure. The magnetic field B is oriented normal to the current flow and also normal to the plane of the 2DEG

Panel XVI

Panel XVI Shubnikov-de Haas Oscillations and Quantum Hall Effect

Panel XVI

498

Panel XVI Shubnikov-de Haas Oscillations and Quantum Hall Eect

(insert in Fig. XVI.2 and Fig. XVI.5 c). In order to ensure a sharp Fermi edge in the highly degenerate 2DEG the measurement is performed at low temperature. When the magnetic field B is increased the Hall resistance rH = UH/I varies stepwise, with steps at those B values where a sharp Landau level crosses the Fermi energy (Fig. XVI.2a). A simultaneous measurement of the magnetoresistance Rxx (!UL/I) parallel to the current flow via a pair of contacts placed along the direction of the current yields a sequence of sharp resistance peaks each time when in the Quantum Hall eect rH jumps from one plateau to the next, i.e. where a Landau level crosses the Fermi energy EF . For B values in between, Rxx is negligible, at least for higher magnetic fields. These resistance oscillations are the Shubnikov-de Haas oscillations of a 2DEG. The experimentally observed values of the Hall resistance at those magnetic fields where Landau levels cross EF are derived directly from the relation for the classical Hall eect (Panel XIV). From (XIV.3) one obtains rH

UH B B ; nde eN2D I

XVI:8 a

where N2D is the two-dimensional carrier density of the 2DEG which, of course, amounts to multiples of the degree of degeneracy NL (XVI.7) in a magnetic field B. The Hall resistance at Landau level crossing EF are thus obtained as:

Fig. XVI.2. (a) Quantum Hall effect measured at 4 K for the quasi-2D electron gas of a modulation-doped AlGaAs/GaAs heterostructure; 2D electron density N = 4 1011 cm±2, electronic mobility = 8.6 104 cm2/Vs. The Hall resistance RH = UH /I was measured as a function of the magnetic field B using the arrangement shown in the inset; (b) Shubnikov-de Haas oscillations of the magnetoresistance Rxx, measured as indicated in the inset via UL/I as a function of the external magnetic field B. The numbers denote the subbands and the arrows indicate the spin direction relative to the B field (after [XVI.2])

rH

B NL e

h 1 ; e2

1; 2; 3; . . .

499

XVI:8 b

(XVI.8 b) describes correctly single discrete points of the experimental curve in Fig. XVI.2 a, but the characteristic plateaus in the Hall resistance are not at all explained. In order to understand the causes for the existence of plateaus a more profound consideration of the transport in a DEG in the presence of magnetic fields is necessary. In a strong magnetic field, electrons in the 2DEG are forced into cyclotron orbits. Undisturbed, closed orbits, however, are possible only in the interior of the sample (Fig. XVI.3). In that

B low

Scattering

Fig. XVI.3. Explanation of the so-called edge channels for electrons when a magnetic field B is applied perpendicular to the plane of a 2D electron gas (2DEG). (a) A strong magnetic field B perpendicular to the 2DEG causes quantization of the electronic states into Landau levels (n = 1, 2, 3, . . .), which correspond to closed cyclotron orbits in the interior of the sample. At the sample boundaries y1 and y2 orbiting is interrupted by elastic reflection from the surface. The increased spatial confinement entails a strong enhancement of the energy of the Landau levels, which eventually cross the Fermi energy EF . (b) Under the condition of ballistic current flow the chemical potentials R and L of the right and left edge channels are different and determine the potentials of the corresponding right and left contacts. (c) With increasing magnetic field B the splitting between the Landau levels increases, while the upper Landau level approaches the Fermi level EF . Electronic states near EF in the interior of the sample become available for scattering processes and the left and right edge channels communicate by these scattering processes

Panel XVI

Panel XVI Shubnikov-de Haas Oscillations and Quantum Hall Effect

Panel XVI

500

Panel XVI Shubnikov-de Haas Oscillations and Quantum Hall Eect

case, the orbital energies are those of the undisturbed Landau levels (XVI.4). Electrons near the boundaries of the sample on the other hand are hindered to complete a full cyclotron orbit. In the simplest case of an elastic mirror reflection at the boundary the electron path becomes a sequence of partial circles (skipping orbits). The combination of cyclotron orbits and surface scattering in the skipping orbits amounts to an additional spatial confinement of the electrons (Fig. XVI.4). By virtue of the uncertainty principle, a stronger confinement is equivalent to a higher kinetic energy. Near the boundaries of the sample the energies of the Landau level are therefore bent upwards and eventually even cross the Fermi level EF at y1 and y2 near the sample surface (Fig. XVI.3 a). Crossing the Fermi level means that one has metallic conduction. Thus, a Landau level that cannot contribute to the electrical conductance in the bulk of the material (since its energy is deep below the Fermi level) does contribute to the conductance at the surface, in the so-called edge channels. The edge channels possess a further important property. Transport in these states is quasi-ballistic, even in macroscopic samples containing impurities. When a carrier in an edge channel is scattered from a defect S (Fig. XVI.4) its trajectory is redirected into the forward direction by the Lorentz force of the strong magnetic field. The total current in the forward direction is therefore not reduced by the presence of impurities and transport in edge channels is therefore quasi-ballistic, i.e. without resistance, regardless of the presence of impurities. The two edge channels on either side are electrically isolated from each other provided that the Landau levels in the interior of the sample are more than a few kBT below the Fermi energy EF . Because of the quasi-ballistic transport in the channels, electrons within one channel are at the same potential. For an electron current flow from left to right this potential is the potential L of the left contact, while electrons in the right ``backwards'' edge channels are at the potential of the right contact R (Fig. XVI.5). The dierence in the potential is the applied voltage multiplied by the electron charge L

R eV :

XVI:9

Sample boundary

Fig. XVI.4. Schematic trajectory of a carrier in an edge channel that undergoes an elastic scattering process on a defect atom S. The magnetic field is oriented perpendicular to the 2DEG. The 2DEG is assumed to be confined by the sample boundary. The scattering processes at the boundary are assumed to be elastic

501

Fig. XVI.5. (a) Ballistic electron transport in edge channels that are generated by quantization in a spatially limited 2 DEG due to a strong magnetic field B perpendicular to the 2DEG. Under the assumption of negligible inelastic scattering between left (L) and right (R) channels the chemical potentials L and R of the left and right channels equal those of the left and right electrical contacts. (b) Conduction through edge channels in a 2 DEG in the presence of two electrical contacts 1) and 2) for measuring the Shubnikov-de Haas oscillations in a strong magnetic field. Inelastic scattering (i.s.) between left and right channels causes a potential difference between the contacts. (c) Conduction through edge channels in a 2 DEG with two opposite contacts 1) and 2) for measuring the quantum Hall effect

The net electric current carried by the left and right (1D) edge channels is the dierence between the contributions from both contacts (see also Sect. 9.9, (9.96)): I

nc
L X n1

eD
1 n
Ev n
EdE :

XVI:10

R

The sum runs over all occupied Landau levels n (up to a maximum occupied ±1 ±1 is the 1D level nc), which cross EF as edge channels, D(1) n = (2p) (dEn/dkx) ±1 density of states of the n-th edge channel, while v n = h (dEn/dkx) is the electron velocity within this channel. The n-th edge channel thus contributes to the current an amount e In
L h

R

e2 V: h

XVI:11

The quantum Hall eect is measured as the resistance between left and right edge channels via two contacts perpendicular to the current flow (Fig. XVI.5 c). According to (XVI.11) each channel contributes an amount of e2/h to the total conductance, i.e. h/e2 to the Hall resistance. This is exactly

Panel XVI

Panel XVI Shubnikov-de Haas Oscillations and Quantum Hall Effect

Panel XVI

502

Panel XVI Shubnikov-de Haas Oscillations and Quantum Hall Eect

the quantum (XVI.8 b) by which the resistance is stepwise enhanced each time a further Landau level crosses the Fermi energy and is thus depleted of electrons. The Shubnikov-de Haas eect is explained in a similar way. In this case, the magneto-resistance is measured along the path of the current via two contacts arranged along the edge channels (Fig. XVI.5 b). As long as the Landau levels in the interior of the sample are suciently far away from EF, no voltage drop occurs, because of the ballistic transport. At a particular magnetic field one of the Landau levels in the interior of the sample reaches the Fermi level EF and electronic states for scattering between the left and right edge channel become available. Scattering between the forth and back channels induces a resistance along the channel direction. Hence, at these particular magnetic fields a peak-like increase of the resistance is observed (Fig. XVI.2 b). In this interpretation, both quantum Hall eect and Shubnikov-de Haas oscillations are attributed to quasi-onedimensional carrier transport in edge channels [XVI.4]. The step-like change of the Hall resistance rH can be determined experimentally with an accuracy of 10±7 on samples of dierent structure and from dierent groups [XVI.1]. The measurement of quantum Hall eect is therefore presently used for a very precise determination of the fine structure constant.

e2 0 c 1 : 137 h 2

XVI:12

If, on the other hand, is assumed to be known ( is determined by a large number of independent precise experiments) the quantum Hall eect allows the introduction of a standard for the resistance unit ``Ohm''. It should finally be mentioned that the quantum Hall eect has the same physical origin as a number of other phenomena related to 1D transport in mesoscopic systems and nanostructures. The fact that edge channels with their 1D conductance (induced by the high magnetic field) each contribute an amount of e2/h to the total conductivity can directly be transferred to other types of 1D conductance channels. The only requirement is that the width of the channels is comparable with the Fermi wavelength kF of the electrons and that the transport is quasi-ballistic, i.e. that the sample dimensions (wire length) are smaller than the mean free path of the carriers. It was, for example, shown that short 1D channels (induced by two metal gates evaporated on the sample) within a 2D electron gas at a modulation-doped AlGaAs/GaAs heterostructure (Sect. 12.7) show a step-like variation of their electrical conductance with varying gate voltage. The channel conductance increases by quanta of 2e2/h when the channel width is increased by a positive bias on the metal gate contacts on top [XVI.5]. The conductance quantum amounts to 2e2/h because of spin degeneracy (see Sect. 9.9).

503

References XVI.1 K. von Klitzing, G. Dorda, M. Pepper: Phys. Rev. B 28, 4886 (1983) XVI.2 M. A. Paalonen, D. C. Tsui, A. C. Gossard: Phys. Rev. B 25, 5566 (1982) XVI.3 H. LuÈth: Solid Surfaces, Interfaces and Thin Films (Springer, Berlin Heidelberg 2001) 4th edition, p. 419 XVI.4 M. Janûen, O. Viehweger, U. Fastenrath, J. Hajdu: Introduction to the Theory of the Integer Quantum Hall Eect (VCH, Weinheim 1994) XVI.5 B. J. van Wees, H. van Houten, C. W. J. Beenakker, J. W. Williamson, L. P. Kouwenhoven, D. van der Marel, C. T. Foxon: Phys. Rev. Let. 60, 848 (1988)

Panel XVI

Panel XVI Shubnikov-de Haas Oscillations and Quantum Hall Effect

Panel XVII

Panel XVII Semiconductor Epitaxy

In modern semiconductor physics and device technology, thin crystalline layers are playing an ever increasing role. Of particular interest are multilayer structures, for example, multiple layers of AlGaAs and GaAs, or layers of GaInAs on an InP substrate. Such systems enable one to study novel phenomena such as the quantum Hall eect (Panel XVI), and, at the same time, are the basis for the production of fast transistors and semiconductor lasers. Semiconductor layer structures are almost invariably produced by means of epitaxy. This is a method that nowadays allows extremely precise control of the growth ± so precise that single layers of atoms can be reliably deposited under favorable conditions. Samples for use in fundamental research are most commonly produced by Molecular Beam Epitaxy (MBE), a process in which semiconductor layers are deposited epitaxially on a substrate in an ultra-high-vacuum chamber [XVII.1, 2] (Fig. XVII.1). The principle behind the method is simple: a substance such as Ga or Al is evaporated and the vapor deposited on a substrate such as GaAs. Ultra-high-vacuum (UHV) systems with base pressures in the 10±8 Pa range are used to prevent contamination and to ensure well-defined conditions, both in the molecular beam and at the surface of the substrate. One can estimate that, at a pressure of 10±8 Pa, it will take a few hours for a newly prepared surface to become covered with a monolayer of adsorbates, even if every impinging gas molecule sticks to the surface. Such UHV chambers are made of stainless steel, and the extremely low pressures of less than 10±8 Pa (corresponding to a molecular mean free path of some meters) are maintained by ion-getter pumps or turbomolecular pumps. In an ion-getter pump, gas atoms are ionized by high electric fields and then adsorbed onto appropriately charged active metal films (e.g. Ti) ± this latter process being known as ``gettering''. The pumping action of a turbomolecular pump relies on the momentum exchange between gas molecules and the blades of a rapidly rotating turbine. The UHV chamber that comprises the main part of an MBE machine (Fig. XVII.1) is equipped with an internal cryoshield cooled by liquid nitrogen. This serves to trap stray atoms and molecules, thereby further reducing the background pressure. The substrate material, e.g. a GaAs wafer, onto which an AlGaAs layer is to be deposited, is mounted on a rotating substrate holder. During growth the substrate must be maintained at a temperature of about 500±600 °C in order to ensure a suciently high mobility of the imping-

505

Panel XVII

Panel XVII Semiconductor Epitaxy

Fig. XVII.1. Schematic illustration of a UHV chamber for molecular beam epitaxy (MBE) of III±V semiconductor layers (viewed in section from above). (After [XVII.3])

ing atoms or molecules (Ga, As4, Si, etc.) on the surface. The atoms or molecules to be incorporated into the growing crystal originate from a so-called effusion source in which the starting material, e.g. solid Ga and As for GaAs epitaxy, is vaporized from boron-nitride crucibles by electrical heating. Mechanically driven shutters, controlled from outside, can open and close the individual eusion cells, thereby switching the corresponding molecular beams on and o. The growth rate of the epitaxial layer is determined by the particle flux in the molecular beam, which, in turn, is controlled by varying the temperature of the crucible. To obtain a particular sequence of well-defined layers with atomically sharp boundaries, as is required for a composition superlattice (Sect. 12.7), the crucible temperature and the shutter-opening times must be regulated by a computer program. This is particularly necessary for the epitaxial growth of ternary or quaternary alloys such as Al0.55Ga0.45As with a fixed composition. Homoepitaxy of GaAs layers on a GaAs substrate does not demand any precise regulation of the molecular flux. In this case, nature herself provides a helping hand: stoichiometric growth of GaAs is possible even for a non-stoichiometric beam composition. The growth rate is determined solely by the rate of arrival of Ga atoms. At a substrate temperature of between 500 and 6008C, arsenic atoms only stick to the surface when sucient numbers of Ga atoms are present on the growing surface; the sticking coefficient for As approaches one for a Ga excess on the surface and is close to zero when Ga is underrepresented. Thus GaAs epitaxy occurs optimally for an excess of arsenic. For a deeper understanding of the GaAs growth in MBE, it is also

Panel XVII

506

Panel XVII Semiconductor Epitaxy

important to know that the arsenic molecular beam produced by evaporation of solid arsenic consists mostly of As4 molecules, which must be dissociated into As atoms by the thermal energy of the hot substrate surface before they can be incorporated in the growing layer. This dissociation process is sometimes carried out thermally in hot graphite ``cracker'' cells, which leads to better layer quality. Important dopants in III±V MBE are Si for n and Be for p doping. These materials are also evaporated from eusion cells which can be switched o and on in a controlled way by the opening and closing of shutters. As shown in Fig. XVII.1, an MBE system is normally also furnished with an electron gun and a fluorescent screen for the observation of diraction patterns (Reflection High Energy Electron Diraction, RHEED). Diraction patterns provide information about the crystallographic structure of the growing surface. An ionization pressure gauge is also included to measure both the chamber pressure and the pressure in the molecular beams. The MBE system shown in Fig. XVII.1 is of the type frequently employed for the epitaxy of III±V and II±VI semiconductors. Si MBE [XVII.4] is carried out in similar systems, but the Si molecular beam is not produced by thermal evaporation from eusion cells, but rather by electron bombardment of a solid Si target, which thereby becomes so hot that it evaporates. The decisive advantage of MBE over other epitaxial methods which work at higher presssure is the fast switching time between dierent sources. This provides a straightforward method of obtaining sharp doping and composition profiles. A typical growth rate is 1 mm/h, which corresponds to about 0.3 nm/s, or one monolayer per second. The time needed to switch between dierent sources should therefore be well below one second. Such short switching times are more dicult to achieve using the second important epitaxial method, Metal Organic Chemical Vapor Deposition (MOCVD) [XVII.5]. Here growth takes place in a reactor, whose whole gas volume must be exchanged on switching from one source to another. Compared to MBE, MOCVD has the interesting advantage for industrial applications that the sources can be easily controlled by gas flow regulators. Furthermore the gas phase sources allow almost continuous operation of the system. We will discuss the principles of MOCVD processes using GaAs epitaxy as an example. We are concerned here with the deposition of solid GaAs from gas phase materials containing Ga and As. The molecule AsH3 and the metal organic gas trimethylgallium [TMG = Ga(CH3)3] are frequently used. The overall reaction, which takes place via several complicated intermediate steps, can be written Ga
CH3 3 gas AsH3 gas ! GaAssolid 3CH4 gas :

XVII:1

AsH3 is fed directly from a gas bottle via a gas regulating valve into the quartz reactor (Fig. XVII.2 a). The metal organic component TMG is in a bulb, and its vapor pressure is controlled by a temperature bath. Hydrogen (H2) flows through this bulb and transports the TMG to the reactor. Another gas line allows the whole system to be flushed with H2. The

507

Panel XVII

Panel XVII Semiconductor Epitaxy

Fig. XVII.2 a, b. Schematic illustration of an apparatus for metal organic chemical vapor deposition (MOCVD) of III±V semiconductor layers. (a) General overview; (b) quartz glass reactor (typical length 50 cm); the susceptor, which holds the wafer to be epitaxially coated, is heated during growth to 700±1200 K. (After [XVII.6])

components which are not consumed in the reaction, and the reaction products, are pumped out at the end of the reactor through a decomposition oven, to eliminate the dangerous excess AsH3. The pumping system also allows the reactor to be operated at low pressure (so-called low pressure MOCVD). With this method the switching time between dierent sources can be reduced and most of the advantages of MBE obtained. Besides the sources for the growth of the base material (AsH3 and TMG) other gas lines are needed for the doping gases, such as SiH4, (C2H5)2Te, (C2H5)2Mg for Si, Te or Mg doping. For the growth of ternary and quaternary III±V alloys further gas lines are also necessary. These supply metal organic materials such as trimethylaluminium (CH3)3Al, trimethylantimony (CH3)3Sb, trimethyl-indium (CH3)3In and others. For the growth of phosphoruscontaining materials such as InP and GaP, the hydride phosphine PH3 is used. Figure XVII.2 b shows a possible design for a flux reactor. The wafer on which the films are to be deposited, the so-called graphite susceptor, is

Panel XVII

508

Panel XVII Semiconductor Epitaxy

held at a temperature between 600 and 8008C during growth. Heating takes place by radiation, direct electrical current or microwave heating. Compared with MBE, the growth process in MOCVD is considerably more complicated. A stream of gas flows over the growing layer, and from this stream the reaction components diuse to the surface. Both at the surface and in the gas phase dissociation reactions take place, e.g. AsH3 is dissociated by collision in the gas phase as well as on the surface itself. After the required surface reactions have occurred, e.g. the incorporation of the dissociated As into the growing crystal lattice, the reaction products such as CH4 are again transported away from the surface by the gas stream. MOCVD growth is therefore largely determined by transport to and from the surface and by surface reaction kinetics. This is seen clearly if one plots the rate of growth in the MOCVD process as a function of the substrate temperature (Fig. XVII.3). The result is a typical curve in which the fall-o at lower temperatures has the form exp (±Ea /k T), since the rate is kinetically limited by surface reactions. Typical activation energies, Ea, in this region are around 1 eV per atom. The temperature range in which this kinetically limited region occurs depends on the source material. For the relatively stable TMG, the exponential decrease is observed at temperatures below 850 K, but for the more easily dissociated triethyl-gallium [TEG, (C2H5)3Ga] it occurs below 700 K. For temperatures above the kinetically limited region, the growth rate shows a plateau whose height depends on the conditions influencing diusion to and from the substrate (e.g. the flow velocity in the reactor). At still higher temperatures, another decrease in the growth rate is observed (Fig. XVII.3). It is probable that the reasons for this

Fig. XVII.3. Growth rates of GaAs layers during metal organic chemical vapor deposition (MOCVD) from the starting materials AsH3 and trimethyl-gallium (TMG) or triethylgallium (TEG); GaAs wafer orientation (100). The gas flow velocities v and the partial pressures PTEG , PTMG , PAsH3 are given. The total pressure in each experiment is 104 Pa. (After [XVII.7])

509

are not inherent to the process. A likely cause is the loss of reactants from the gas stream due to deposition on the reactor walls. By clever process control in low pressure MOCVD, and by using specially designed valves, very short switching times can now be achieved. Thus, even with MOCVD it is possible to produce atomically sharp heterojunctions between two semiconductors. A third modern epitaxial method, so-called Metal Organic MBE (MOMBE), also called CBE (Chemical Beam Epitaxy), combines the advantages of MBE and MOCVD [XVII.8]. As in MBE, a UHV system serves as the growth chamber (Fig. XVII.1). The source materials, however, are gases, as in MOCVD, and these are fed through lines with controlled valves into the UHV chamber. Inside the chamber, specially constructed admission systems (capillaries) serve to form the molecular beams, which are directed at the surface of the substrate to be coated. For the growth of GaAs, one might use, for example, AsH3 and triethylgallium [(C2H5)3Ga, TEG]. In a MOCVD reactor, collisions in the gas above the hot substrate surface lead to a significant predissociation of the AsH3, but this does not occur here because of the very low background pressure. In MOMBE, the AsH3 must therefore be thermally dissociated in the inlet capillary. All metal organic epitaxy processes suer from the presence of carbon impurities, which originate in the decomposition of the metal organics. The carbon is most frequently incorporated at As lattice positions and leads to p conduction (although it can also be incorporated as a donor at Ga sites). Carbon inclusion becomes stronger the lower the pressure used for epitaxy. Thus in MOMBE, GaAs layers with low levels of p doping can only be achieved using TEG, whereas in MOCVD it is also possible to use TMG.

References XVII.1 M. A. Herman, H. Sitter: Molecular Beam Epitaxy, 2nd ed., Springer Ser. Mater. Sci., Vol. 7 (Springer, Berlin, Heidelberg 1996) XVII.2 E. H. C. Parker (Ed.): The Technology and Physics of Molecular Beam Epitaxy (Plenum, New York 1985) XVII.3 A. Y. Cho, K. Y. Cheng: Appl. Phys. Lett. 38, 360 (1981) XVII.4 E. Kasper, H.-J. Herzog, H. DaÈmbkes, Th. Richter: Growth Mode and Interface Structure of MBE Grown SiGe Structures, in Two-Dimensional Systems: Physics and New Devices, ed. by G. Bauer, F. Kuchar, H. Heinrich, Springer Ser. SolidState Sci., Vol. 67 (Springer, Berlin, Heidelberg 1986) XVII.5 Proc. ICMOVPE I, J. Crystal Growth 55 (1981); Proc. ICMOVPE II, J. Crystal Growth 68 (1984) W. Richter: Physics of Metal Organic Chemical Vapour Deposition: FestkoÈrperprobleme 26, 335 (Advances in Solid State Physics 26) ed. by P. Grosse (Vieweg, Braunschweig 1986) XVII.6 H. Heinecke, E. Veuho, N. PuÈtz, M. Heyen, P. Balk: J. Electron. Mater. 13, 815 (1984) XVII.7 C. Plass, H. Heinecke, O. Kayser, H. LuÈth, P. Balk: J. Crystal Growth 88, 455 (1988) XVII.8 H. LuÈth: in Surf. Science 299/300, 867 (1994)

Panel XVII

Panel XVII Semiconductor Epitaxy

Panel XVIII

Panel XVIII Preparation of Nanostructures

Studies on electronic transport in nanostructures require samples that are appropriately downscaled in their dimensions. For quantum transport as described in Sect. 9.9, e.g., cross sections in the range between 10 and 100nm are necessary. Suitable structuring techniques, for metals as well as for semiconductors, have been developed in the context of microelectronics, where they are used for the fabrication of highly integrated circuits on silicon wafers. One common method for the preparation of 3-dimensional nanostructures on a substrate begins with the deposition of the desired material on a large area substrate wafer, e.g. silicon, GaAs, or sapphire (Al2O3). Deposition of metals is frequently performed by evaporation from electrically heated tungsten or graphite crucibles or by sputter-deposition. Crystalline growth of the deposited epilayer is possible if the growing film is latticematched to the substrate. For ordered crystal growth, the substrate is typically heated in order to aord sucient surface mobility to the deposited atoms. Growing crystalline epilayers is called epitaxy. Epitaxy techniques such as MBE (Molecular Beam Epitaxy) or MOVPE/MOCVD (MetalOrganic Vapour Phase Epitaxy/MetalOrganic Chemical Vapour Deposition), (Panel XVII) are employed in particular for growing crystalline semiconductor layers and multilayer systems, e.g. of GaAs/AlGaAs, InGaAs/InP or Si/Ge on convenient substrates. Deposition of polycrystalline layers, amorphous layers or crystalline epilayers and multilayer systems thus enables the nanostructuring in one, namely the direction perpendicular to the substrate surface. For film growth rates of 1mm/h (i.e. 0.3nm/s), layer thicknesses below 1nm and atomically sharp interfaces are easily achieved. In order to machine 3D nanostructures an additional lateral structuring of the layer systems is necessary. This is achieved by lithography (greek: oB=stone, q'=write). Lateral structuring down into the 100nm range is performed via optical lithography, i.e. by the use of illumination techniques with visible and UV light. Nanostructuring down to the 5-10nm scale presently requires electron beam (e-beam) lithography in electron optical columns. Optical and e-beam lithography are similar insofar as a photoresist is irradiated. The irradiation changes the chemical and structural properties of the resist such that its solubility in an organic solvent is modified. In optical lithography the irradiation of the resist is performed through a patterned mask, whether by contact illumination or by optical projection.

511

The desired pattern is thus transferred as a whole to the resist in parallel, i.e. in a single illumination step. Electron beam lithography, on the other hand, is a serial illumination technique, where a focused electron beam is scanned computer controlled over the resist film whereby the beam writes the pattern into the resist step-by-step. For this purpose, a high-precision electron microscope column is used, similarly as in a scanning electron microscope. In comparison with optical lithography, electron beam lithography is much more costly and time consuming. For industrial applications, present research aims therefore at replacing electron beam lithography by parallel illumination techniques with light of extremely short wavelength. An example is the so-called extreme UV (EUV) lithography, which uses coherent radiation pulses of soft X-ray lasers. The current most advanced laser of that type is based on the amplification of the spontaneous emission in a plasma of Ag-ions [XVIII.1]. A spatially coherent beam is generated by amplification in a second Ag-plasma. The output emission line with a wavelength of 13.9nm (h = 89.2eV) corresponds to the 4d-4p transition of nickel Ni-like Ag ions.

Fig. XVIII.1. Schematic presentation of important lithographical structuring techniques. The illumination steps for metal etching (3) and for the lift-off process (2) are performed in parallel in optical lithography by exposure through masks (as shown) or by projection, or alternatively in series by scanning electron beam lithography. A negative photoresist becomes insoluble in the illuminated areas while a positive resist, there, is soluble in the subsequent development step

Panel XVIII

Panel XVIII Preparation of Nanostructures

Panel XVIII

512

Panel XVIII Preparation of Nanostructures

In order to transfer lateral structures of the irradiated photoresist into semiconductor layer systems or onto a wafer, several etching processes are applied. The most important transfer methods are compiled in Fig. XVIII.1. In case of metal structuring on a wafer two techniques are commonly used, direct metal etching and the so-called lift-o process. In metal etching (left column in Fig. XVIII.1), patterns are etched into the metal film which has been deposited in advance by evaporation or sputtering (step 1). The metal film with a typical thickness of 100 nm is then spin-coated in a centrifuge with an organic photoresist (often PMMA=poly-methyl metacrylate) (step 2). In direct metal etching, a so-called negative resist is used, in which the locally illuminated areas ± be it by means of light through a mask or by an electron beam (step 3) ± exhibit a decreased solubility in the subsequent development process (step 4). The decreased solubility of the resist in the illuminated areas arises from irradiation induced polymer formation. In the development process (step 4) an organic solvent removes the non-illuminated areas of the resist layer. The remaining resist structures then protect the underlying metal film against metal etching (step 5). Depending on the requirements concerning edge sharpness the etching itself is performed by wet chemistry in solution (HCl, H2O2 etc.) or by ion bombardment in a plasma discharge (O2), sometimes in combination with more or less chemically reactive species (HF, HBr). The latter technique, called Reactive Ion Etching (RIE), is performed in vacuum chambers (RIE chamber, Fig. XVIII.2). After the metal etching, nanostructures consisting of metal and the resist on top remain on the substrate. In the last final step 6, the resist caps are removed by heating in an oven and the desired metal nanostructures are found on the wafer. Since III-V semiconductors and metals exhibit similar etching properties, the hitherto described method is not well suited for the generation of metal-

reactor

grounded anode reactive Ions (plasma)

etching gas

water cooled cathode impedance matching network

Pump

≈

RF-generator

Fig. XVIII.2. Scheme of a set-up for Reactive Ion Etching (RIE). The plasma discharge with reactive ions commonly runs in a low-pressure vacuum vessel as reactor

513

lic nanostructures on III-V semiconductor substrates. For this purpose, the so-called lift-o process is preferred. The III-V wafer surface is covered with a positive resist (step 1). This type of resist is chemically modified by illumination, be it by light or by an electron beam, such that the illuminated areas become more soluble (breaking of polymer bonds). Subsequently the positive resist is illuminated by light or by electron beam radiation (step 2). After development, i.e. the removal of the resist in the illuminated areas (step 3) the wafer is covered by a structured resist film. The subsequent deposition of metal covers the resist and the open wafer areas equally (step 4). In the lift-o process the metal-covered resist structures are now removed in a solvent (step 5) and only the metal structures remain on the wafer, similar as in the direct metal etching process. Positive resists can also be used in order to transfer patterns directly into the semiconductor wafer. After the illumination of the resist (step 2) and removal of the illuminated areas (step 3) only one etching process (step 4), mostly by RIE, is used to generate the required pattern of holes or nanostructures extending from the wafer surface like a mesa (Spanish: table). In the last fifth step, the resist remaining on top of the mesas is removed. This structuring method is extremely useful in order to prepare three-dimensional quantum boxes (dots) based on semiconductor multiple heterostructures. An epitaxially deposited layer stack with two energetic barriers for electrons, e.g. of AlAs embedded in GaAs, creates a two-dimensional quantum confinement by means of the two energetic barriers (Sec. 12.7). Confinement in the third direction, i.e. formation of the quantum dot, is achieved by lithographic structuring of nanoscale mesa-like columns. All structuring methods for nanostructures presented so far start with macroscopic solids and/or solid films and use lithographic techniques to machine the nanoscale structures into the solid (top-down approach). In recent years, so called bottom-up techniques have gained interest, in which the self-organization principle of nature, as we know it from crystal growth, is successfully applied. Under adequate physical and chemical conditions, nanostructures grow by self-organization without the use of complex and cost-intensive lithographic techniques. An example is the chemical self-organization of organic nanoparticles and fiber structures. Particularly in semiconductor physics, the self-organized epitaxial growth of semiconductor whiskers (wires, columns) has gained importance for the study of quantum transport and for future device applications. After deposition of metallic nanoparticles with dimensions of 10-100nm on a semiconductor wafer these particles act as crystallization nuclei and local catalysts in the subsequent epitaxial growth of whiskers both in MBE and in MOVPE (MOCVD, panel XVIII). In the MOVPE process, the metallic nuclei locally enhance the catalytic decomposition of the gaseous precursors and induce epitaxial growth under special growth conditions only on the nuclei. This leads to whisker growth; 10 to 100nm thick nanocolumns with lengths up to several micrometers grow. In the case of III-nitrides, whisker growth occurs

Panel XVIII

Panel XVIII Preparation of Nanostructures

Panel XVIII

514

Panel XVIII Preparation of Nanostructures

Fig. XVIII.3. Scanning electron microscopy image of an arrangement of GaN whiskers grown by molecular beam epitaxy on a Si(111) substrate (a) and of one single whisker which has been removed from the substrate and is placed on a new Si/SiO2 host substrate (b). Electron beam lithographically structured markers (bright spots) were deposited in advance on the host substrate. The whisker is electrically contacted by metal contacts (large bright areas) that are also prepared by electron beam lithography. (After Calarco et al. [XVIII.2])

(a)

(b) 5µm

in MBE under nitrogen rich conditions even without the use of metallic nuclei (Fig. XVIII.3a). After removal of the nanocolumns from the substrate in an ultrasonic bath they can be spread on a high resistive host substrate (SiO2 etc.), electrically contacted by lithography (Fig. XVIII.3b) and subsequently used for the study of quantum transport. For eventual applications in quantum electronics, an ordered growth of semiconductor nanocolumns with respect to thickness, length and local arrangement is desirable. This can be achieved by depositing metal dots of homogeneous thickness on well-defined sites on the wafer. Well-ordered arrangement of nanocolumns can also be achieved by selective growth through mask holes, which are deposited on the wafer in advance. As an example, Fig. XVIII.4 shows ordered selective growth of GaAs columns with a diameter of about 150nm on GaAs(111). The mask con(a)

(b)

Fig. XVIII.4. Ordered selective growth of GaAs nanocolumns on a masked GaAs(111) substrate (scanning electron microscopic images). (a) HSQ (hydrogen silesquioxane) mask prepared on a GaAs(111) wafer by electron beam lithography; (b) GaAs nanocolumns (diameter approx. 180 nm) grown in metal-organic vapor phase epitaxy (MOVPE, panel XVII) by use of the HSQ mask in a). (After Klinger et al. [XVIII.3])

515

sisting of an inorganic negative resist (HSQ = Hydrogen Silesquioxane) was fabricated by electron beam lithography. The GaAs columns were grown in MOVPE at a growth temperature of 750oC using AsH3 and TMG (Trimethyl Gallium) as precursors. Once more, it should be emphasized that the selective growth is essential as is possible preferentially in MOVPE, where the non-reactive surface of the mask does not catalytically dissociate the precursors and therefore does not allow GaAs growth. Growth of semiconductor columns was meanwhile demonstrated in MBE, MOVPE, and in MOCVD for the important semiconductors Si, SiGe, and GaAs, InAs, GaN, InN and ZnO. Hence, interesting new developments are expected that may lead to a semiconductor-based quantum electronics.

References XVIII.1 M. Nishikino, M. Tanaka, K. Nagashima, M. Kishimoto, M. Kado, T. Kawachi, K. Sukegawa, Y. Ochi, N. Hasegawa, Y. Kato: Phys. Rev. A 68, 061802 (2003) XVIII.2 R. Calarco, M. Marso, R. Meijers, Th. Richter, N. Aykanat, T. Thillosen, T. Stoica, H. LuÈth: NanoLetters 5 (2005) 981 XVIII.3 V. Klinger, J. Wensorra (Research Centre JuÈlich 2007): priv. commun.

Panel XVIII

Panel XVIII Preparation of Nanostructures

References

Chapter 1 1.1 1.2 1.3 1.4

L. Pauling: The Nature of the Chemical Bond, 3rd edn. (Cornell Univ. Press, Ithaca, NY 1960) S. GoÈttlicher: Acta Cryst. B 24, 122 (1968) Y. W. Yang, P. Coppens: Solid State Commun. 15, 1555 (1974) S. P. Walch, W. A. Goddard, III: Surf. Sci. 72, 645 (1978)

Further Reading Ballhausen, C. J., Gray, H. B.: Molecular Orbital Theory (Benjamin, New York 1964) Cartmell, E., Fowles, G. W. A.: Valency and Molecular Structure, 2nd edn. (Butterworths, London 1961) Coulson, C. A.: Valence, 2nd edn. (Oxford Univ. Press, Oxford 1961) Hartmann, H.: Theorie der chemischen Bindung (Springer, Berlin Heidelberg 1954) Pauling, L.: Die Natur der chemischen Bindung (Chemie-Verlag, Weinheim 1964) Philips, J. C.: Covalent Bonding in Crystals, Molecules and Polymers (The Univ. of Chicago Press, Chicago 1969) Slater, J. C.: Quantum Theory of Molecules and Solids (McGraw-Hill, New York 1963) Vinogradov, S. N., Linell, R. H.: Hydrogen Bonding (Van Nostrand-Reinhold, New York 1971)

Chapter 2 2.1 2.2

K. Urban, P. Kramer, M. Wilkens: Phys. Bl. 42, 373 (1986) T. B. Massalski (ed.): Binary Alloy Phase Diagrams, 2nd edn. (American Society for Metals, Metals Park, Ohio 44073, 1990) A database is available under the name TAPP of ES Microwave, 2234 Wade Court, Hamilton, OH 45013, USA

Further Reading Burzla, H., Thiele, G. (eds.): Kristallographie ± Grundlagen und Anwendungen (Thieme, Stuttgart 1977), insbesondere: Burzla, H., Zimmermann, H.: ``Symmetrielehre'', Bd. I

H. Ibach, H. LuÈth, Solid-State Physics, 4th ed., DOI 10.1007/978-3-540-93804-0_BM2, Ó Springer-Verlag Berlin Heidelberg 2009

518

References

Hamermesh, M.: Group Theory and Its Application to Physical Problems (Addison-Wesley/Pergamon, London Paris 1962) Heine, V.: Group Theory in Quantum Mechanics (Pergamon, London 1960) Koster, G. F., Dimmock, J. O., Wheeler, R. G., Statz, H.: Properties of the 42 Point Groups (MIT Press, Cambridge, MA 1963) Streitwolf, H.: Gruppentheorie in der FestkoÈrperphysik (Akademische Verlagsges., Leipzig 1967) Tinkham, M.: Group Theory and Quantum Mechanics (McGraw-Hill, New York 1964) Vainshtein, B. K.: Fundamentals of Crystals: Symmetry and Methods of Structural Crystallography, Springer Ser. Modern Crystallography, Vol. 1 (Springer, Berlin Heidelberg 1994)

Chapter 3 3.1 3.2 3.3 3.4 3.5

W. Marshall, S. W. Lovesey: Theory of Thermal Neutron Scattering (Clarendon, Oxford 1971) L. D. Landau, E. M. Lifschitz: Lehrbuch der theoretischen Physik, Bd. VIII: ``Elektrodynamik der Kontinua'' (Akademie Verlag, Berlin 1874) p. 436 . J. B. Pendry: Low Energy Electron Diraction (Academic, London 1974) S. Kugler, L. Pusztai, L. Rosta, P. Chieux, R. Bellissent: Phys. Rev. B48, 7685 (1993) Y. Waseda: The Structure of Non-Crystalline Materials (McGraw-Hill, New York 1981)

Further Reading Bacon, G. F.: Neutron Diraction, 3rd edn. (Oxford Univ. Press, Oxford 1975) Dachs, H. (ed.): Neutron Diraction, Topics Curr. Phys., Vol. 6 (Springer, Berlin Heidelberg 1978) Kleber, W.: EinfuÈhrung in die Kristallographie, 16. Aufl. (Verlag Technik, Berlin 1983) Lovesey, S., Springer, T. (eds.): Dynamics of Solids and Liquids by Neutron Scattering. Topics Curr. Phys., Vol. 3 (Springer, Berlin Heidelberg 1977) Pinsker, Z. G.: Dynamical Scattering of X-Rays in Crystals, Springer Ser. Solid-State Sci., Vol. 3 (Springer, Berlin Heidelberg 1978) Sellin, A. (ed.): Structure and Collisions of Ions and Atoms, Topics Curr. Phys., Vol. 5 (Springer, Berlin Heidelberg 1978) Shull, C. G.: Early Developments of Neutron Scattering, Rev. Mod. Phys. 67, 753 (1995) Ziman, J. M.: Models of Disorder (Cambridge University Press, Cambridge 1979)

References

519

Chapter 4 4.1 4.2 4.3 4.4 4.5 4.6

M. Born, R. Oppenheimer: Ann. Phys. (Leipzig) 84, 457 (1927) G. Leibfried: In Handbuch der Physik, Vol. 7/1 (Springer, Berlin Heidelberg 1955) p. 104 G. Dolling: In Inelastic Scattering of Neutrons in Solids and Liquids, Vol. II (Intern. Atomic Energy Agency, Vienna 1963) p. 37 R. F. S. Hearman: Advances in Physics 5, 323 (1956) W. A. Brantley: J. App. Phys. 44, 534 (1973) G. Simmons, H. Wang: Single crystal elastic constants and calculated aggregate properties; A Handbook, 2nd edn., Cambridge, USA (MIT Press, Cambridge 1971)

Further Reading Bak, T. A.: Phonons and Phonon Interactions (Benjamin, New York 1964) Bilz, H., Kress, W.: Phonon Dispersion Relations in Insulators, Springer Ser. Solid-State Sci., Vol. 10 (Springer, Berlin Heidelberg 1979) Born, M., Huang, K. H.: Dynamical Theory of Crystal Lattices (Clarendon, Oxford 1954) Leibfried, G., Breuer, N.: Point Defects in Metals I, Introduction to the Theory, Springer Tracts Mod. Phys. Vol. 81 (Springer, Berlin Heidelberg 1977) Ludwig, W.: Recent Developments in Lattice Theory, Springer Tracts Mod. Phys., Vol. 43 (Springer, Berlin Heidelberg 1967) Maradudin, A. A., Montroll, E. W., Weiss, G. H.: ``Theory of Lattice Dynamics in the Harmonic Approximation'' in Solid State Physics, Advances and Applications, ed. by H. Ehrenreich, F. Seitz, D. Turnbull (Academic, New York 1971) Suppl. 3 Wallis, R. F. (ed.): Lattice Dynamics (Plenum, New York 1965)

Chapter 5 5.1 5.2 5.3 5.4 5.5 5.6

G. Dolling, R. A. Cowley: Proc. R. Soc. London 88, 463 (1966) American Institute of Physics Handbook, 3rd edn. (McGraw-Hill, New York 1972) pp. 4±115 Wei Chen, D. L., Mills: Phys. Rev. B 36, 6269 (1987) H. Ibach: Phys. Status Solidi 31, 625 (1969) R. W. Powell, C. Y. Ho, P. E. Liley: NSRDS-N 13S8 (1966) R. Berman, P. G. Klemens, F. E. Simon, T. M. Fry: Nature 166, 865 (1950)

Further Reading Rosenberg, H. M.: Low Temperature Solid-State Physics (Clarendon, Oxford 1963)

520

References

Chapter 6 6.1 6.2 6.3 6.4 6.5

A. Sommerfeld, H. Bethe: Elektronentheorie der Metalle, Heidelberger Taschenbuch, Bd. 19 (Springer, Berlin Heidelberg 1967) Landolt BoÈrnstein, Neue Serie III/6 (Springer, Berlin Heidelberg 1971) C. A. Bailey, P. L. Smith: Phys. Rev. 114, 1010 (1959) N. F. Mott: Cdn. J. Phys. 34, 1356 (1956); Nuovo Cimento 7 (Suppl.), 312 (1958) H. B. Michaelson: J. Appl. Phys. 48, 4729 (1977)

Further Reading Grosse, P.: Freie Elektronen in FestkoÈrpern (Springer, Berlin Heidelberg 1979)

Chapter 7 7.1 7.2 7.3 7.4 7.5 7.6 7.7 7.8

W. Shockley: Electrons and Holes in Semiconductors (Van Nostrand, New York 1950) L. P. Howard: Phys. Rev. 109, 1927 (1958) B. Segall: Phys. Rev. 124, 1797 (1961) R. Courths, S. HuÈfner: Phys. Rep. 112, 55 (1984) H. Eckhardt, L. Fritsche, J. Noke: J. Phys. F 14, 97 (1984) F. Herman, R. L. Kortum, C. D. Kuglin, J. L. Shay: In II±VI Semiconducting Compounds, ed. by D. G. Thomas (Benjamin, New York 1967) T. H. Upton, W. A. Goddard, C. F. Melius: J. Vac. Sci. Technol. 16, 531 (1979) H. Haberland (ed.): Clusters of Atoms and Molecules I and II, Springer Series in Chem. Phys. 52, 56 (Springer, Berlin Heidelberg 1994)

Further Reading Ashcroft, N. W., Mermin, N. D.: Solid State Physics (Hold, Rinehart and Winston, New York 1976) Brillouin, L.: Wave Propagation in Periodic Structures (Academic, New York 1960) Callaway, J.: Energy Band Theory (Academic, New York 1964) Harrison, W. A.: Pseudopotentials in the Theory of Metals (Benjamin, New York 1966) Herrmann, R., Preppernau, U.: Elektronen im Kristall (Springer, Berlin Heidelberg 1979) Jones, H.: The Theory of Brillouin-Zones and Electronic States in Crystals (North-Holland, Amsterdam 1962) Loucks, T. L.: Augmented Plane Wave Method (Benjamin, New York 1967) Madelung, O.: Introduction to Solid-State Theory, Springer Ser. Solid State Sci., Vol. 2 (Springer, Berlin Heidelberg 1978)

References

521

Skriver, H. L.: The LMTO Method, Springer Ser. Solid-State Sci., Vol. 41 (Springer, Berlin Heidelberg 1984) Wilson, A. H.: The Theory of Metals, 2nd edn. (Cambridge Univ. Press, London 1965)

Chapter 8 8.1 8.2 8.3 8.4 8.5 8.6 8.7

A.S. Arrat, in F.A.C. Bland, B. Heinrich (eds.): Ultrathin Magnetic Structures, Vol. I (Springer, Berlin 1994) p.7 J. F. Janak: Phys. Rev. B 16, 255 (1977) J. Callaway, C. S. Wang: Phys. Rev. B 7, 1096 (1973) P. Weiss, G. Foex: Arch. Sci. Natl. 31, 89 (1911) P. Weiss, R. Porrer: Ann. Phys. 5, 153 (1926) H. A. Mook, D. McK. Paul: Phys. Rev. Lett. 54, 227 (1985) H. Ibach: Physics of Surfaces and Interfaces (Springer, Berlin, Heidelberg, New York 2006), p. 38

Further Reading Chakravarty, A. S.: Introduction to the Magnetic Properties of Solids (Wiley, New York 1980) Crangle, J.: The Magnetic Properties of Solids (Arnold, London 1977) Ibach, H.: Physics of Surfaces and Interfaces (Springer, Berlin, Heidelberg, New York 2006) Moriya, T.: Spin Fluctuations in Itinerant Electron Magnetism, Springer Ser. Solid-State Sci., Vol. 56 (Springer, Berlin Heidelberg 1985) White, R. M.: Quantum Theory of Magnetism, Springer Ser. Solid-State Sci., Vol. 32 (Springer, Berlin Heidelberg 1983) see also Mattis, D. C.: The Theory of Magnetism I and II, Springer Ser. Solid-State Sci., Vols. 17, 55 (Springer, Berlin Heidelberg 1985, 1988)

Chapter 9 9.1 9.2 9.3 9.4 9.5 9.6

9.7

P. Drude: Ann. Phys. (Leipzig) 1, 566 (1900) E. GruÈneisen: Ann. Phys. (Leipzig) (5) 16, 530 (1933) D. K. C. McDonald, K. Mendelssohn: Proc. R. Soc. Edinburgh, Sect. A 202, 103 (1950) J. Linde: Ann. Phys. (Leipzig) 5, 15 (1932) J. M. Ziman: Principles of the Theory of Solids (Cambridge Univ. Press, London 1964) N. F. Mott: Phil. Mag. B19, 835 (1984) N. F. Mott: in The Physics of Hydrogenated Amorphous Silicon Vol. II, ed. by J. D. Joannopoulos and G. Luckowsky, Topics in Applied Physics, Vol. 56 (Springer, Berlin Heidelberg 1984) p. 169 B. Ruttensperger, G. MuÈller, G. KroÈtz: Phil. Mag. B68, 203 (1993)

522

References

9.8. B.J. van Wees, H. van Houten, C.W.J. Beenacker, J.W. Williamson, L. P. Kouwenhoven, D. van der Marel, C.T. Foxon: Phys. Rev. Lett. 60, 848 (1988) 9.9. K. Hansen, E. Laegsgaard, I. Stensgaard, F. Besenbacher: Phys. Rev. B 56, 2208 (1997) 9.10. Y. Aharonov and D. Bohm: Phys. Rev. 115, 485 (1959) 9.11. R. A. Webb, S. Washburn, C. P. Umbach, R. B. Laibowitz: Phys. Rev. Lett. 54, 2696 (1985) 9.12. J. Wesorra, M. Lepsa, M. Indlekofer, Ch. BloÈmers, S. Heiderich, Th. SchaÈpers, H. LuÈth : unveroÈentlicht 9.13. G.J. Dolan, J.C. Licini, D.J. Bishop: Phys. Rev. Lett. 56, 1493 (1986) 9.14. Ch. BloÈmers, Th. SchaÈpers, T. Richter, R. Calarco, H. LuÈth, M. Marso: Appl. Phys. Lett. 92, 132101 (2008) 9.15. C.P. Umbach, C. Van Haesendonck, R.B. Laibowitz, S. Washburn, R.A. Webb: Phys. Rev. Lett. 56, 386 (1986) Further Reading Blatt, F. J.: Physics of Electronic Conduction in Solids (McGraw-Hill, New York 1968) Busch, G., Schade, H.: Vorlesungen uÈber FestkoÈrperphysik (BirkhaÈuser, Basel 1973) Madelung, O.: Introduction to Solid-State Theory, Springer Ser. Solid-State Sci., Vol. 2 (Springer, Berlin Heidelberg 1978) Nag, B. R.: Electron Transport in Compound Semiconductors, Springer Ser. Solid-State Sci., Vol. 11 (Springer, Berlin Heidelberg 1980) Smith, A. C., Janak, J. F., Adler, R. B.: Electronic Conduction in Solids (McGraw-Hill, New York 1967) Ziman, J. M.: Electrons and Phonons (Clarendon, Oxford 1960)

Chapter 10 H. K. Onnes: Akad. van Wetenschappen (Amsterdam) 14, 113, 818 (1911) 10.2 J. Bardeen, L. N. Cooper, J. R. Schrieer: Phys. Rev. 108, 1175 (1957) 10.3 N. E. Phillips: Phys. Rev. 114, 676 (1959) 10.4 W. Meissner, R. Ochsenfeld: Naturwissensch. 21, 787 (1933) 10.5 F. London, H. London: Z. Phys. 96, 359 (1935) 10.6 L. N. Cooper: Phys. Rev. 104, 1189 (1956) 10.7 H. FroÈhlich: Phys. Rev. 79, 845 (1950) 10.8 N. N. Bogoliubov: Nuovo Cimento 7, 794 (1958) 10.9 J. Hinken: Supraleiter-Elektronik (Springer, Berlin Heidelberg 1988) 10.10 V. V. Schmidt (eds. P. MuÈller, A. V. Ustinov): The Physics of Superconductors (Springer, Berlin Heidelberg 1997) 10.11 P. L. Richards, M. Tinkham: Phys. Rev. 119, 575 (1960) 10.12 I. Giaever, K. Megerle: Phys. Rev. 122, 1101 (1961) 10.1

References

523

10.13 E. Maxwell: Phys. Rev. 86, 235 (1952); B. Serin, C. A. Reynolds, C. Lohman: Phys. Rev. 86, 162 (1952); J. M. Lock, A. B. Pippard, D. Schoenberg: Proc. Cambridge Phil. Soc. 47, 811 (1951) 10.14 V. L. Ginzburg, L. D. Landau: Soviet Phys.-JETP (USSR) 20, 1064 (1950) siehe auch V. L. Ginzburg: Nuovo Cimento 2, 1234 (1955) 10.15 A. C. Rose-Innes, E. H. Rhoderick: Introduction to Superconductivity (Pergamon, Oxford 1969) p. 52 10.16 R. Doll, M. NaÈbauer: Phys. Rev. Lett. 7, 51 (1961) 10.17 B. S. Deaver Jr., W. M. Fairbank: Phys. Rev. Lett. 7, 43 (1961) 10.18 T. Kinsel, E. A. Lynton, B. Serin: Rev. Mod. Phys. 36, 105 (1964) 10.19 J. Schelten, H. Ullmeier, G. Lippmann, W. Schmatz: in Low Temperature Physics ± LT 13, Vol. 3, ed. by K. D. Timmerhaus, W. J. O'Sullivan, E. F. Hammel (Plenum, New York 1972) p. 54 10.20 J. G. Bednorz, K. A. MuÈller: Z. Phys. B 64, 189 (1986) 10.21 M. K. Wu, J. R. Ashburn, C. J. Tornq, P. H. Hor, R. L. Meng, L. Gao, Z. J. Huang, Y. Q. Wang, C. W. Chu: Phys. Rev. Lett. 58, 908 (1987) 10.22 J. R. Cooper, S. D. Obertelli, A. Carrington, J. W. Loran: Phys. Rev. B 44, 12 086 (1991) 10.23 R. WoÈrdenweber: Private Mitteilung (ISI, Forschungszentrum JuÈlich) 10.24 H. Maeda, Y. Tanaka, M. Fukutomi, T. Asano: Jpn. J. Appl. Phys. Lett. 27, L 209 (1988) 10.25 Z. Z. Sheng, A. M. Hermann: Nature 332, 55 (1988) 10.26 R. Hott, H. Rietschel, M. Sander: Phys. Bl. 48, 355 (1992) 10.27 B. Kabius: Private Mitteilung (IFF, Forschungszentrum JuÈlich) 10.28 S. J. Hagen, T. W. Jing, Z. Z. Wang, J. Horvath, N. P. Ong: Phys. Rev. B 37, 7928 (1988) 10.29 J. Zaanen, A. T. Paxton, O. Jepsen, O. K. Anderson: Phys. Rev. Lett. 60, 2685 (1988) 10.30 Ching-ping S. Wang: Electronic Structure, Lattice Dynamics, and Magnetic Interactions, in High Temperature Superconductivity, ed. by J. W. Lynn, Graduate Texts Contemp. Phys. (Springer, Berlin Heidelberg 1990) p. 122 10.31 H. Takagi, S. Uchida, Y. Tokura: Phys. Rev. Lett. 62, 1197 (1989) 10.32 Y. Zhang, Y. Tavrin, M. MuÈck, A. I. Braginski, C. Heiden, T. Elbert, S. Hampson: Physiol. Meas. 14, 113 (1993) 10.33 J. Fink, E. Sohmen: Phys. Bl. 48, 11 (1992) 10.34 C. Politis, V. Buntar, W. Krauss, A. Gurevich: Europhys. Lett. 17, 175 (1992) Further Reading Buckel, W.: Supraleitung, 5. Aufl. (VCH, Weinheim 1993) De Gennes, P. G.: Superconductivity of Metals and Alloys (Addison-Wesley, Reading 1992) Huebener, R. P.: Magnetic Flux Structures in Superconductors, Springer Ser. Solid-State Sci., Vol. 6 (Springer, Berlin Heidelberg 1979)

524

References

Kuper, Ch. G.: An Introduction to the Theory of Superconductivity (Clarendon, Oxford 1968) Lynn, J. W. (ed.): High Temperature Superconductivity, Graduate Texts Contemp. Phys. (Springer, Berlin Heidelberg 1990) Lynton, E. A.: Superconductivity (Methuen's Monographs on Physical Subjects, London 1964). (Deutsche UÈbersetzung: Bibliographisches Institut, Mannheim 1966) Rickayzen, G.: Theory of Superconductivity (Wiley, New York 1965) Rose-Innes, A. C., Rhoderick, E. H.: Introduction to Superconductivity (Pergamon, Braunschweig 1969) Schmidt, V. V. (eds. P. MuÈller and A. V. Ustinov): The Physics of Superconductors (Springer, Berlin Heidelberg 1997) Stolz, H.: Supraleitung (Vieweg, Braunschweig 1979) Tinkham, M.: Introduction to Superconductivity, 2nd edn., (McGraw-Hill, New York 1996)

Chapter 11 11.1 11.2 11.3 11.4 11.5 11.6 11.7 11.8 11.9 11.10 11.11 11.12 11.13

B. Schrader, W. Meier: Raman/IR Atlas organischer Verbindungen, Bd. 1 (VCH, Weinheim 1974) L. H. Henry, J. J. Hopfield: Phys. Rev. Lett. 15, 964 (1965) T. P. Martin: Phys. Rev. B 1, 3480 (1970) M. Hass, B. W. Henri: J. Phys. Chem. Sol. 23, 1099 (1962) G. Frank, E. Kauer, H. KoÈstlin: Phys. Bl. 34, 106 (1978) J. C. Phillips: in Solid State Physics, Vol. 18, ed. by F. Seitz, P. Turnbull (Academic, New York 1966) G. W. Gobeli, H. Y. Fan: in Semiconductor Research, 2nd Quarterly Report, Purdue Univ. (1956) E. J. Johnson: in Semiconductors and Semimetals, Vol. 3, ed. by R. K. Willardson, A. C. Beer (Academic, New York 1967) p. 171 H. Ehrenreich, H. R. Philipp: Phys. Rev. 128, 1622 (1962) M. D. Sturge: Phys. Rev. 127, 768 (1962) H. LuÈth: Solid Surfaces, Interfaces and Thin Films, 4th edn. (Springer, Berlin Heidelberg New York 2001) J. Geiger, K. Wittmaack: Z. Phys. 195, 44 (1966) H. Ibach: Phys. Rev. Lett. 24, 1416 (1970)

Further Reading Abeles, F. (ed.): International Colloquium on Optical Properties and Electronic Structure of Metals and Alloys (North-Holland, Amsterdam 1966) Cho, K. (ed.): Excitons, Topics Curr. Phys., Vol. 14 (Springer, Berlin Heidelberg 1979) FroÈhlich, H.: Theory of Dielectrics (Clarendon, Oxford 1958) Geiger, J.: Elektronen und FestkoÈrper (Vieweg, Braunschweig 1968) Greenaway, D. L., Harbeke, G.: Optical Properties and Band Structure of Semiconductors (Pergamon, Oxford 1968)

References

525

Haken, H., Nikitine, S. (eds.): Excitons at High Densities, Springer Tracts Mod. Phys., Vol. 73 (Springer, Berlin Heidelberg 1975) Mitra, S. S., Nudelman, S. (eds.): Far Infrared Properties of Solids (Plenum, New York London 1970) Nakajima, S., Toyozawa, Y., Abe, R.: The Physics of Elementary Excitations, Springer Ser. Solid-State Sci., Vol. 12 (Springer, Berlin Heidelberg 1980) Nudelman, S., Mitra, S. S. (eds.): Optical Properties of Solids (Plenum, New York 1969) Willardson, R. K., Beer, A. C. (eds.): Semiconductors and Semimetals, Vol. 3, Optical Properties of III±V-Compounds (Academic, New York 1968)

Chapter 12 12.1 12.2 12.3 12.4 12.5 12.6 12.7

12.8 12.9 12.10 12.11 12.12 12.13 12.14 12.15 12.16

J. R. Chelikowsky, M. L. Cohen: Phys. Rev. B 14, 556 (1976) J. H. Reuszer, P. Fischer: Phys. Rev. 135, A 1125 (1964) E. M. Conwell: Proc. IRE 40, 1327 (1952) S. M. Sze: Physics of Semiconductor Devices, 2nd edn. (Wiley, New York 1969) B. Gelmont, K. Kim, M. Shur: J. Appl. Phys. 74, 1818 (1993) H. LuÈth: Solid Surfaces, Interfaces and Thin Films, 4th edn. (Springer, Berlin Heidelberg 2001) G. Margaritondo, P. Perfetti: The Problem of Heterojunction Band Discontinuities, in Heterojunction Band Discontinuities, Physics and Device Applications, ed. by F. Capasso, G. Margaritondo (NorthHolland, Amsterdam 1987) p. 59 H. MorkocË: Modulation-doped AlxGa1±xAs/GaAs Heterostructures, in The Technology and Physics of Molecular Beam Epitaxy, ed. by E. H. C. Parker (Plenum, New York 1985) p. 185 L. Esaki: Compositional Superlattices, in The Technology and Physics of Molecular Beam Epitaxy, ed. by E. H. C. Parker (Plenum, New York 1985) p. 185 A. FoÈrster: Private Mitteilung (ISI, Forschungszentrum JuÈlich) H. Heinecke, K. Werner, M. Weyers, H. LuÈth, P. Balk: J. Crystal Growth 81, 270 (1987) F. Capasso (ed.): Physics of Quantum Electron Devices, Springer Ser. Electron. Photon., Vol. 28 (Springer, Berlin Heidelberg 1989) U. Tietze, Ch. Schenk: Halbleiterschaltungstechnik (Springer, Berlin Heidelberg 1983) K. Schimpf, M. Sommer, M. Horstmann, M. Hollfelder, A. van der Hart, M. Marso, P. Kordos, H. LuÈth: IEEE Electron Device Letters 18, 144 (1997) H.-M. MuÈhlho, D.V. McCaughan: MOS Transistors and Memories, in Handbook of Semiconductors, Vol. 4, ed. by T.S. Moss, C. Hilsum (North-Holland, Amsterdam 1993) p. 265 H. Kressel, D.E. Ackley: Semiconductor Lasers, in Handbook of Semiconductors, Vol. 4, ed. by T.S. Moss, C. Hilsum (North Holland, Amsterdam 1993) p. 725

526

References

Further Reading Allan, G., Bastard, G., Boccara, N., Lanoo, M., Voos, M. (eds.): Heterojunctions and Semiconductor Superlattices (Springer, Berlin Heidelberg 1986) Bauer, G., Kuchar, F., Heinrich, H. (eds.): Two-dimensional Systems: Physics and New Devices, Springer Ser. Solid-State Sci., Vol. 67 (Springer, Berlin Heidelberg 1986) Brauer, W., Streitwolf, H. W.: Theoretische Grundlagen der Halbleiterphysik (Akademie-Verlag, Berlin 1976) Buchreihe: Halbleiter-Elektronik, Bd. 1±20, ed. by W. v. Heywang, R. MuÈller (Springer, Berlin Heidelberg) Capasso, F., Margaritondo, G. (eds.): Heterojunction Band Discontinuities, Physics and Device Applications (North-Holland, Amsterdam 1987) Chang, L. L., Ploog, K. (eds.): Molecular Beam Epitaxy and Heterostructures, NATO ASI Ser. E, No. 87 (Martinus Nijho, Dordrecht 1985) Kelly, M.J.: Low-Dimensional Semiconductors, Materials, Physics, Technology, Devices (Clarendon Press, Oxford 1995) Lanoo, M., Bourgoin, J.: Point Defects in Semiconductors I and II, Springer Ser. Solid-State Sci., Vols. 22, 35 (Springer, Berlin Heidelberg 1981, 1983) Madelung, O.: Grundlagen der Halbleiterphysik, Heidelberger Taschenbuch, Bd. 71 (Springer, Berlin Heidelberg 1970) Nizzoli, F., Rieder, K.-H., Willis, R. F. (eds.): Dynamical Phenomena at Surfaces, Interfaces and Superlattices, Springer Ser. Surf. Sci., Vol. 3 (Springer, Berlin Heidelberg 1985) Parker, E. H. C. (ed.): The Technology and Physics of Molecular Beam Epitaxy (Plenum, New York 1985) Reggiani, L. (ed.): Hot-Electron Transport in Semiconductors, Topics Appl. Phys., Vol. 58 (Springer, Berlin Heidelberg 1985) Seeger, K.: Semiconductor Physics, 4th edn., Springer Ser. Solid-State Sci., Vol. 40 (Springer, Berlin Heidelberg 1988) Shklovskii, B., Efros, A. L.: Electronic Properties of Doped Semiconductors, Springer Ser. Solid-State Sci., Vol. 45 (Springer, Berlin Heidelberg 1984) Shockley, W.: Electrons and Holes in Semiconductors (Van Nostrand, Princeton 1950) Spenke, E.: Elektronische Halbleiter (Springer, Berlin Heidelberg 1965) Sze, S. M.: Physics of Semiconductor Devices, 2nd edn. (Wiley, New York 1969) Ueta, M., Kanzaki, H., Kobayashi, K., Toyozawa, Y., Hanamura, E.: Excitonic Processes in Solids, Springer Ser. Solid-State Sci., Vol. 60 (Springer, Berlin Heidelberg 1986) Yu, P. Y., Cardona, M.: Fundamentals of Semiconductors, 3rd edn. (Springer, Berlin, Heidelberg 2001)

Index

A

Absolute thermopower, 263 Absorption coefficient, 71, 376 Absorption of electromagnetic radiation, 374 Acceptors, 429 Acoustic branch, 90 Adiabatic approximation, 83, 135 – demagnetization, 131, 225 Aharanov-Bohm-effect, 273 ff. Alloys, 36 ff. Altshuler-Aronov-Spivak-oscillations, 273 ff. Amorphous – materials, 21, 56, 71, 138, 181, 266 – phases, 180 Angle resolved photoemission spectroscopy, 184 ff. Anharmonic effects, 121 Anisotropy, magnetic, 219 ff., 233 ff. Anomalous absorption, 78–80 – transmission, 78–80 Antibonding orbital, 4 Antiferromagnetism, 211–215 Anti-Stokes lines, 108 f., 231 Antisymmetrization, 197 Atomic beams, 73 ff. – scattering factor, 65 ff. Atom motion, 83 ff. Auto-correlation, 54 Avalanche breakthrough, 443

BCS coherence, 324 ff. – excitation spectrum, 312 ff. – ground state, 304 ff. – occupation probability, 307 – theory, 291, 304 ff. Beer’s law, 379 Benzene, 156 Bipolar – devices, 472 – transistor, 473 Bloch’s T3/2 law, 219 – theorem, 161 ff. Bloch-wall, 222 ff. Bloch waves, 161 ff. Body-centered cubic lattice, 33 Bogoliubov equations, 317 Bohm-Staver relation, 405 Bohr magneton, 192 Boltzmann equation, 126, 251 ff. Bonding orbital, 4 Bose statistics, 117 ff. Bottom-up approach, 513 Bragg equation, 62 ff. Bragg-Williams approximation, 39 Bravais lattices, 24 Brillouin scattering, 93, 111 – zone, 63 ff. Bulk modulus, 103, 123, 156 Burgers vector, 46

B

C

Ballistic transport, 268 ff., 500 f. Band discontinuity – of conduction band, 461 – of valence band, 461 Band gap, 163 ff., 419 ff. Bandstructures, 173 ff. – experimental determination, 187 Base, 473 – current, 474 Basis vectors, 23

C60, 8 Carrier freeze out, 435 – drift velocity vD, 441 – saturation, 435 Cauchy relation, 105 Causality principle, 403 Cesium chloride structure, 10, 35, 77 Chandrasekhar limit, 158 Charge carrier density in semiconductors, 424 ff., 432 ff.

Index

528

Chemical bonding, 1 ff. – potential, 41, 145 Clausius-Mossotti relation, 387 Cluster calculations, 181 CMOS (complementary MOS), 479 Coercive field, 220 Coherence of the BCS groundstate, 325 ff. Coherence length of a Cooper pair, 325 ff. Collector, 473 – current, 473 Common base configuration, 476 – tangent, 42 Composition superlattice, 464 ff. Condensation energy density (superconductivity), 324 Conductance – one dimensional, 272, 502 Conduction band, 419 Cooper pairs, 299 ff. – tunneling of, 362 ff. – wavefunction, 301 ff. Coordination number, 31 ff. Coulomb potential, 10 Coupling constants, 85 Covalent bonding, 4 ff. Critical current (superconductivity), 321 ff. Critical exponent, 207 – magnetic field, 296, 324, 329 – points of the bandstructure, 178 ff. Crystal classes, 27 ff. – structures, 31 ff. Crystalline anisotropy, 219 ff. Cubic crystals (elastic constants), 103 Curie temperature, 207 Cut-off frequencies, 480 Cyclotron resonance, 282, 492 ff. D

Damon-Eshbach waves, 229 Debye cut-off frequency, 118 ff. – model of specific heat, 118 ff. Debye-Scherrer method, 69 Debye temperature, 119 – of superconductors, 320 Debye-Waller factor, 105 Degeneracy and group theory, 28 ff. d-electrons, 2, 14, 175 ff., 206 De Haas-van Alphen effect, 289 Density of states, 115 ff. – for electrons, 177 ff. – of ferromagnets, 196, 205 – of free electron gas, 138

– non-crystalline solids, 179 ff. – for phonons, 116 Depolarization field, 219, 222, 233 Devices, 472 ff. Diamagnetism, 191 ff., 295 Diamond structure, 34 Diatomic linear chain, 86 ff. Dielectric energy losses of electrons, 400 ff. – function, 372 ff. – modes, 379 – properties, 371 ff. – susceptibility, 373 Diffraction experiments, 72 ff. – theory, 51 ff. Diffusion current approximation, 451 – length, 453 – voltage, 446 Diffusive transport, 269 ff. Diode characteristics, 153, 455 Dipole interaction, 16 Direct transitions, 394 Dislocations, 46 Dispersion relation, 88 ff., 381, 404 Domains, 71, 219 ff. Donors, 429 ff. Doped semiconductors, 432 ff. Doping superlattice, 470 Double heterostructure laser, 484 Drude conductivity, 255, 258 Dynamical matrix, 86 Dynamics of atoms, 83 ff. Dynamic scattering, 52 E

Easy axis, 219 Edge dislocation, 47 Effective band gap, 471 – charge, 377 – density of states, 427 – mass, 196, 241 ff., 399, 422 ff. Einstein relation, 447 Elastic – constants, 98 ff. – isotropy, 103 – modules, 98 – properties of crystal, 94 Elastic scattering, 53 – of electrons in bands, 254 Electrical conductivity of metals, 255 ff. – of semiconductors, 424 ff. Electrical confinement, 485 Electrical susceptibility, 107, 373 Electron affinity, 9, 461

Index Electron-defect scattering, 250 ff., 258 Electronegativity, 11 Electron-electron scattering, 250 Electron energy loss spectroscopy, 402 – energy shells, 2 Electronic bandstructure, 159 ff. – examples, 173 ff. – nearly free electron approximation, 163 ff. – tight binding approximation, 167 ff. Electron-phonon scattering, 336, 396 Elementary mesh, 73 Emitter, 472 – configuration, 476 – current, 474 – efficiency, 476 Energy gap – in semiconductors, 178, 420 ff. – in superconductors, 308 ff. Entropy, 17, 40, 262 Epitaxial films, 234 Epitaxy, 459, 479 Equation of motion – of atoms, 85 – for crystal electrons, 242 Ewald sphere, 60 EXAFS, 71 Exchange anisotropy, 235 Exchange bias, 235 ff. Exchange hole, 201 – interaction, 199 ff. – splitting, 202 Excitation spectrum – superconductor, 308 ff. Excitons, 398 Expansion coefficient, 123 ff. F

Fabry-Perot interferometer, 230, 485 Face-centered cubic lattice, 31 Fermi distribution, 144 ff. – energy, 145 – gas, 146 ff. Fermi level for different doping, 433 – of heterostructures, 459 ff. – pinning, 457 – for p-n junction, 443 ff., 445 ff. Fermi sphere, 141, 175 – surface, 174, 250, 290 Ferroelectrics, 387 ff. Ferromagnetism, 201 ff. Field effect transistors, 476 ff. Fine structure constant, 502

529

Fixed boundary conditions, 136 Fluxoid, 330 Flux quantization, 331 ff. – tubes, 338 – vortex, 340 Flux quantum, 275, 331 ff., 368 Forbidden band, 164 ff., 179, 420 Form anisotropy, 233 ff. Fourier transform, 53, 389 – spectroscopy, 415 Free-electron gas, 136 ff., 389 ff. – two-dimensional, 465 ff., 477 Free energy – defects, 46 – enthalpy, 39 – of vibrations, 122 Frenkel – defect, 45 – exciton, 398 Friedel oscillations, 182 Friedel’s rule, 59 Fro¨hlich interaction, 299 Frustrated total reflection, 383 Fullerenes, 8 G

Gap energy (superconductivity), 316 Generation current, 450 Giant magneto resistance, 237 ff. Ginzburg-Landau theory, 336 GMR-effect, 237 ff. Gru¨neisen formula, 259 – number, 124 Group – III-nitrides, 443 – velocity, 127, 242 H

H2, H2+ molecules, 4 ff., 198 Hall effect, 489 ff., 497 ff. Harmonic approximation, 85 – oscillator, 116, 377 ff. Heat reflecting window, 390 Heisenberg Hamiltonian, 199, 209, 223 Helium atom scattering, 73 f. HEMT (high electron mobility transistor), 477 Hexagonal close packing, 32 High-temperature superconductors, 340 ff. Holes, 245 ff., 424 ff. Hopping conduction, 266 sp3 Hybridization, 7, 18, 176, 423

Index

530

Hydrogen bonding, 15 – model for impurities, 430 – molecular ion, 5 Hysteresis, 220 f., 235 f. I

Ideal conductor, 294 III-V semiconductors, 423 ff., 459, 478 ff. Impurities in semiconductors, 440, 465 Indirect semiconductor, 421, 442 – transitions, 394, 443 Inelastic scattering, 93 ff. – of electrons in bands, 254 ff. – tunneling, 359 ff. Infrared-active phonon, 89, 377 Infrared spectroscopy, 414 ff. Instability of the Fermi sea, 299 ff. Interband transitions, 390 ff. Interface – energy (superconductivity), 336 – states, 456 Interface anisotropy, 234 Internal energy of free electron gas, 146 Interstitial site, 45 Intrinsic semiconductors, 424 ff. Inversion, 478 – symmetry, 25 Ionic bonding, 9 ff. – structure, 35 Ionization energy, 9 – of donors and acceptors, 429 ff. Irreducible representation, 29 ff. Isotope effect – in superconductors, 320 f. J

Joint density of states, 395 ff. Josephson effect, 362 ff. – junction, 363 K

Kinematic diffraction theory (scattering theory), 52 ff. Kondo effect, 260 Kramers-Kronig relations, 374 L

Landau levels, 287 ff., 496 ff. Laplace equation, 157, 382 Laser, 405, 472, 481 Lattice, 22 ff. – defects, 45 – plane separation, 61 ff.

Laue – condition, 59 – method, 70 T3 Law, 120 T3/2 Law, 219 Law of mass action for charge carrier concentrations, 432, 445 Layer crystal, 345 LCAO, 157, 167, 182 Left-handed materials, 408 ff. Lift-off process, 511 ff. Light sources, 185, 414 Linear combination of atomic orbitals (LCAO) method, 157, 168, 182 Liquid structure factor, 55, 68 Liquidus, 38 Lithography, 510 ff. Local field, 385 ff. Localized electrons, 266 ff. Local modes, 104 London equations, 296 ff., 328 – penetration depth, 298 Longitudinal effective mass, 422 – waves in solids, 379 ff. Lorentz Force, 286, 492, 500 Lorentz number, 265 Low energy electron diffraction (LEED), 72 Low-temperature experiments, 131 ff. Lyddane-Sachs-Teller relation, 382 M

Madelung constant, 11 Magnetic anisotropy, 219 ff., 233 ff. – domains, 219, 222 Magnetic dipole moment, 192 – flux quanta, 275, 331 ff., 368 – – tubes, 338

– susceptibility, 194 ff., 213, 289 – – of an antiferromagnet, 213

Magnetism, 191 ff. – at surfaces, 223, 229 ff. Magnetization curve, 220, 236 ff., 337 – definition, 192 Majority charge carriers, 445 Many electron theory, 191 Mass tensor, 243 Matrix representation, 28 ff. Matthiesen’s rule, 260 Mean field approximation, 39, 209 Mean free path, 127 f., 247, 269 ff. Meissner-Ochsenfeld effect, 295, 324 ff. Meissner phase, 337 MESFET (metal semiconductor field effect transistor), 477 Metallic bonding, 13 ff.

Index Metal organic chemical vapor deposition (MOCVD), 459, 505 ff. Metal organic molecular beam epitaxy (MOMBE), 509 Metamaterials, 410 ff. Microbridge, 362 MIGS (metal-induced gap states), 456 Miller indices, 60 f. Minority charge carriers, 445 Miscibility gap, 38, 43 Mixing entropy, 39 Mobility – edge, 266 – in metals, 255 ff. – in semiconductors, 424 ff., 437 ff. Modulation doping, 464 f. Moire´ topography, 79 Molecular beam epitaxy (MBE), 459, 504 ff. Molecular orbitals, 4 ff. Momentum conservation and energy uncertainty of a Cooper pair, 303 – in photoemission, 186 ff. – in scattering, 92, 127 MOSFET (metal oxide semiconductor field effect transistor), 477 Motion of electrons and transport phenomena, 241 ff. Mott’s law, 268 Mott transition, 150 ff. Mott-Wannier exciton, 400 Multiphonon processes, 121 N

Ne´el temperature, 212 Nee´l-wall, 222 ff. Negative differential conductivity, 442 Negative index materials, 408 ff. Nernst calorimeter, 132 Neutrality level, 456 ff. Neutron diffraction, 75 ff. – stars, 158 ff. nipi superlattices, 470 Non-crystalline solid, 179 ff. Nondegenerate semiconductors, 432 ff. Nonlinear conductivity, 282 Normal coordinates, 19 Normal mode vibrations of a molecule, 30 Novel optical materials, 407 ff. O

One-electron approximation, 135 ff. Optical – branch, 88 – confinement, 484

531

Optoelectronic devices, 472 Orbital, 4 ff. – angular momentum, 192 Orbit of electrons, 286 ff., 492 Oscillations – de Haas-van Alphen, 289 – Shubikov-de Haas, 495 ff. Oscillator – harmonic, 85, 116 ff., 377 ff., 404 Output characteristics, 475 Overlap, 172 – integral, 5, 197 P

Pair – correlation function, 55 f. – wavefunction, 197 ff., 305 Paramagnetism, 191 ff. Parity, 29 Partial dislocation, 47 Patterson function, 54 Pauli matrices, 199, 215 – paramagnetism, 195 ff. – principle, 6, 142, 250 Peltier effect, 263 Penn model, 405 Periodic table, 1 ff. Periodic boundary conditions, 114, 138 Permalloy, 221, 236 ff. Phase coherence length, 269 ff. Phase diagrams, 36 ff. Phonon, 91 ff. – decay, 126 – exchange, 300 – spectroscopy, 91 ff. Photocurrent, 470 Photoemission spectroscopy, 186 ff. Photoluminescence, 468 ff. Photonic crystals, 412 Photoresist, 510 ff. Piezoelectric effect, 130, 388 Plasmons, 389 f., 401 Plastic deformations, 47 p-n junction, 443 ff. Point – defects, 45 – groups, 27 ff. – Scho¨nflies symbols, 28 – symmetry, 25 ff. Poisson – equation, 150 ff., 445 ff. – number, 103 Polaritons, 381 Polarizability, 377 ff., 387

Index

532

Polarization, 373 ff. – catastrophe, 387 ff. Population inversion, 405, 482 Powder method, 69 Q

z Quantization, 466 ff., 495 Quantization of magnetic flux, 329 ff. Quantum Hall effect, 495 ff. – oscillations, 273 ff. – well lasers, 471 – wells, 495 Quantum transport, 268 ff., 273, 279 Quasi – electrons, 313 – Fermi level, 451 – harmonic approximation, 123 – holes, 313 – momentum, 93 – particles, 312 R

Raman-active phonon, 110 Raman scattering, 107 ff. – from spin waves, 231 Rayleigh scattering, 108 Reactive ion etching (RIE), 512, 513 Reciprocal lattice, 57 ff. Recombination, 451 – current, 450 Reduced zone scheme, 163, 175 Reduction to first Brillouin zone, 163 Reflection high energy electron diffraction (RHEED), 505 – symmetry, 25 Reflectivity, 375, 384 ff. Refractive index, 374, 407 Relaxation time, 126, 251 ff. Remanence, 220 Representation of a group, 29 Residual resistivity, 260 Resistivity – electrical, 247 ff. – – amorphous solids, 266 – – semiconductors, 414 ff.

– thermal, 124 ff. Resonant Raman scattering, 110 ff. Reststrahlen (residual radiation), 384 Reverse bias, 451 Richardson-Dushman formula, 155 ff. Ritz method, 17, 168 Rotating crystal method, 69 Rotation axes, 25

S

Scattering conditions, 58 – density, 53 – of electrons in bands, 247 ff. – vector, 53 Scho¨nflies symbols, 28 Schottky – barrier, 458 – contact, 443 ff. – defect, 46 Screw dislocation, 47 Seebeck effect, 263 Selection rules, UPS, 189 ff. Semiconductor, 419 ff. – epitaxy, 504 ff. – heterojunction, 460 – heterostructures, 459 ff. – superlattice, 459 ff. Shubnikov-de Haas oscillations, 495 ff. Shubnikov phase, 337 ff. Sine-Gordon equation, 224 Singlet state, 198 Slater determinant, 327 Sodium chloride structure, 9 ff. Solid solution, 48 Solidus line, 37 Sound – velocity, 100, 116 – waves, 94, 100 Space charge capacitance, 454 – groups, 27 – zone, 454 Specific heat of free-electron gas, 145 ff. – of atom variations, 118 ff. – of superconductors, 293 Spin operator, 193, 209, 215, 305 Spin-orbit coupling, 219 Spin-orbit splitting, 421 Spin valve, 238 Spin waves, 215 ff. – magnetostatic, 227 ff. Split ring resonators, 410 Spontaneous emission, 481 Square-well model for metals, 136 ff. Stars and Fermi gas, 158 ff. Stereographic projection, 27 Stimulated emission, 481 Stokes lines, 109, 231 Stoner criterion, 203 – gap, 205, 218 Stoner-Wohlfart model, 201 ff. Strain, 95 Stress tensor, 98 Structure analysis, 67 ff. – factor, 64 ff.

Index Subbands, 467 Superconducting quantum interference device, (SQUID), 347, 366 Superconductivity, 291 ff. – coupling constants, 320 Superconductors, elemental, 293 – oxide, 340 ff. – type II, 333 ff. Supercurrent, 295, 321 ff. Superlattices, 73, 459 ff. Superstructure, 73 Surface waves, 157, 230, 382 ff. – magnetic, 230 ff. Susceptibility – antiferromagnetic, 214 – electric, 107, 373, 497 – magnetic, 192 ff., 207, 214 Symmetry, 25 ff. – points, 64 Synchrotron radiation, 185 T

Thermal conductivity – via electrons, 264 – via phonons, 124 ff. Thermal energy, 118 ff. – expansion, 121 ff. – properties, 113 ff. Thermoelectric effects, 261 ff. Thermionic emission, 152 ff. Thomas-Fermi screening length, 151, 405 Threshold current density, 485 Total reflection, 384, 390, 417 ff. Transconductance, 476, 480 Transfer characteristics, 475 Transistor, 472 ff. Transition temperature – high Tc superconductors, 344 ff. – magnetic, 209 ff. – in superconductors, 291 ff. Transport coefficients, 263 – phenomena, 124 ff., 251 ff. Transverse effective mass, 422 – waves in solids, 90, 379 ff. Triplet state, 198 Tunnel barriers, 356 ff. – diode, 357, 360 – spectroscopy, 360 Tunneling experiment, 352 ff. – of Cooper pairs, 362 ff. – of electrons, 352 ff. – process, 352 Two-dimensional density of states – for electrons, 156, 467 – for phonons, 129

533

Two-dimensional electron gas, 156, 182, 467, 499 Two-dimensional lattice, 22 Two-dimensional Schro¨dinger equation, 466 U

UHV (ultra high vacuum) system, 504 – technology, 504 Ultraviolet photoemission spectroscopy (UPS), 184 ff. Umklapp process, 128 Universal conductance fluctuations, 279 ff. V

Valence band, 176, 178, 419 ff. Van der Waals bonding, 15 f., 19 Van Hove singularity, 115, 177, 395 Virtual phonons, 300 Voigt’s notation, 98 Volume expansion coefficient, 122 W

Wave packet, 125, 241 ff. Weak localization, 278 ff. Weissenberg method, 69 Wiedemann-Franz law, 264 ff. Wigner-Seitz cell, 64 Work function, table of, 155 Wurtzite lattice, 35 X

X-ray – diffraction, 59 ff. – interferometry, 78 ff. – photoemission spectroscopy (XPS), 184 ff. – topography, 78 ff. X-ray lasers, 511 Y

Young’s modulus, 103 Z

Zero point energy, 113 – entropy, 17 Zinc blende structure, 35 Zone melting, 45

Table of Constants Quantity

Symbol

Value

SI Unit

Velocity of light in vacuum Permeability of vacuum Permittivity of vacuum Proton rest mass Electron rest mass Elementary charge Planck's constant Planck's constant Flux quantum Sommerfeld fine-structure constant Rydberg-constant Bohr magneton Avogadro's number Atomic mass unit

c l0 = 1/e0 c 2 e0 = 1/l0 c 2 mp me e h h = h/2 p U0 = h/2 e = l0 ce 2/2 h

2.997925 4p 8.854188 1.672649 9.109534 1.602189 6.626176 1.054589 2.067851 7.297351

108 m s±1 10±7 Vs/Am 10±12 As/Vm 10±27 kg 10±31 kg 10±19 As 10±34 J s 10±34 J s 10±15 J A±1 10±3

R? = l 20 me e 4 c 3/8 h 3 lB = e h/2 me NA mu = 1 u = (10±3 kg mol±1)/NA k

1.097373 9.274078 6.022045 1.660566

107 m±1 10±24 Am2 1023 mol±1 10±27 kg

1.380662

10±23 J K±1

Quantity

Symbol

Value

SI Unit

Energy equivalent of the Hertz Frequency equivalent of the electron volt Energy equivalent of the reciprocal meter Wave-number equivalent of the electron volt Energy equivalent of the Kelvin Temperature equivalent of the electron volt

E [Hz] = (1 Hz) h m [eV] = 1 eV/h

6.626176 2.417970

10±34 J 1014 Hz

E [m±1] = (1 m±1) hc

1.986478

10±25 J

r [eV] = 1 eV/hc

8.065479

105 m±1

E [K] = (1 K) k T [eV] = 1 eV/k

1.380662 1.160450

10±23 J 104 K

Boltzmann's constant

Equivalent Values